With examples and clear explanation throughout, this stepbystep approach makes quantum theory of plasmons accessible t
548 112 10MB
English Pages 320 [325] Year 2020
Table of contents :
Contents
Preface
1 Introduction and Description of Contents
2 Physics of Metals – Preliminaries
2.1 Definition of a Metal
2.2 Scheme of the Fermi Liquid Theory
2.2.1 Phenomenological Theory of a Fermi Liquid
2.2.2 Outline of the Microscopic Theory of a Normal Fermi Liquid
3 Quasiclassical Description of Plasmons in the Bulk Metal
3.1 Random Phase Approximation Theory of Plasmons of Pines and Bohm
3.2 Screening of the Coulomb Interaction in Metals
4 Plasmon Excitations in NanometreSized Metallic Particles
5 Damping of Plasmons in Metallic Nanoparticles
5.1 Damped Plasmonic Oscillations in Metallic Nanospheres in Dielectric Surroundings
5.2 Attenuation of Dipole Surface Plasmons with Exact Inclusion of the Lorentz Friction
5.3 Comparison of Surface Plasmon Oscillation Features Including Lorentz Friction with the Experimental Data and Simplified Mie Approach
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
6 Plasmon Photovoltaic Effect
6.1 Semiclassical RPA Approach to Plasmons in Large Metallic Nanospheres
6.2 Damping of Plasmons in Large Nanospheres
6.2.1 Radiation from Dipole Surface Plasmons – Lorentz Friction for Plasmons
6.3 Transfer of Sunlight Energy to a Semiconductor Mediated by Surface Plasmons through the Channel of Dipole Coupling in the NearField Regime
6.3.1 Fermi Golden Rule for Band Electron Transitions due to Coupling with Plasmons
6.3.2 Plasmon Damping Rate due to NearField Coupling with SemiconductorBand Electrons
6.3.3 Transfer of Light Energy via the Plasmon Channel
6.4 Experimental Demonstration of the Proximity Constraints of the Plasmon Effect
6.5 Calculation of the Matrix Element for the Fermi Golden Rule Expression (6.37)
7 PlasmonInduced Efficiency Enhancement of Solar Cells Modified by Metallic Nanoparticles: Material Dependence
7.1 PlasmonMediated Photoeffect: Probability of Electron Interband Excitation Due to Plasmons
7.2 Damping Rate for Plasmons in a Metallic Nanoparticle Deposited on a Semiconductor
7.3 Efficiency of the Light Absorption Channel via Plasmons for Various Materials
8 Numerical Simulation of Plasmon Photoeffect
8.1 Lorentz Friction Channel for Energy Losses of Surface Plasmons in a Metallic Nanoparticle
8.2 Fermi Golden Rule for Probability of Electron Interband Excitation due to Plasmons in a Metallic Nanoparticle
8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL
8.4 Comparison with Experiment
8.5 Conclusions
9 Plasmon–Polaritons in Metallic Nanoparticle Chains
9.1 Plasmon Oscillations in Metallic Nanospheres
9.2 Radiative Properties of a Metallic Nanosphere in a Chain
9.3 Calculation of the Radiative Damping of a Plasmon–Polariton in a Chain
9.4 Plasmon–Polariton SelfModes in a Chain Propagation
9.5 The SelfFrequencies and Group Velocities of Plasmon–Polaritons in a NanoChain
9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy
9.7 Collective PlasmonWaveType Propagation along a NanoChain; NearFieldZone Approximation
9.7.1 NearFieldZone Approximation of the Dipole Interaction in a Chain
9.7.2 Medium and FarField Corrections to the NearField Dipole Interaction
9.7.3 Nonlinear Corrections to the Lorentz Friction
9.7.4 Nonlinear Correction to the Radiation Losses of Plasmon–Polariton in a NanoChain
10 Plasmon–Polariton Kinetics in a Metallic NanoChain Located in Absorbing Surroundings
10.1 Plasmon Oscillations in a Single Metallic Nanosphere Including Damping
10.2 Radiative Properties of Plasmon–Polaritons in a Metallic NanoChain Embedded in a Dielectric Medium
10.3 Plasmon–Polariton SelfModes in a Chain in Dielectric Surroundings
10.4 Damping of Surface Plasmons in a Single Metallic Nanoparticle Deposited on a Semiconductor Substrate
10.5 Plasmon–Polariton Dynamics in a Metallic Chain Deposited on a Semiconductor
11 Plasmons in Finite Spherical Ionic Systems
11.1 Fluctuations of the Charge Density in a Spherical Electrolyte System
11.2 Model Definition
11.3 Solution of RPA Plasmon Equation: Volume and Surface Plasmon Frequencies in a Spherical Finite Ion System
11.3.1 Ionic Surface Ion Plasmon Frequencies for an Electrolyte Nanosphere Embedded in a Dielectric Medium with ε1 > 1
11.4 Damping of Plasmon Oscillations in Ionic Systems
11.4.1 Exact Inclusion of the Lorentz Damping
11.5 Derivation of Plasmon Frequencies for a Finite Electrolyte System
11.5.1 Volume Ionic Plasmons
11.5.2 Surface Ionic Plasmons
12 Plasmon–Polaritons in a Chain of Finite Ionic Systems; Model of Saltatory Conduction in Myelinated Axons
12.1 Plasmon–Polariton Propagation in Linear Periodic Ionic Systems
12.2 Plasmon–Polariton Model of Saltatory Conduction: Fitting the Kinetics to the Axon Parameters
12.3 Soft Plasmonics Application: The Role of Grey and White Matter in Information Processing in the Brain
12.3.1 Possible Link with the Topological Model of a Neuron Web
References
Index
Q UA N T U M NA N O  P L A S M O N I C S
With examples and clear explanation throughout, this stepbystep approach makes the quantum theory of plasmons accessible to readers without a specialized training in theory. A fully analytical formulation offers an opportunity for further development of the research and applications. The theory is focused on the random phase approximation description of plasmons in metallic nanostructures, previously defined for the bulk metal only. Particular attention is paid to the large damping of plasmons in nanostructures, including electron scattering and Lorentz friction losses; a quantum description of the plasmon photovoltaic effect is presented and there is an indepth analysis of plasmon–polariton kinetics in metallic nanochains. Suitable for students in the fields of plasmonics, optoelectronics, and photonics and for researchers active in the fields of photovoltaics, optoelectronics, nanoplasmonics, and nanophotonics, the book should also be useful for researchers in soft plasmonics since it includes applications to electrosignalling in neurons. w i t o l d a . jac a k is Associate Professor at Wrocław University of Science and Technology. He is a theoretical physicist active in the fields of nanoplasmonics, quantum mechanics, decoherence in quantum dots, quantum information, and communication.
Q UA N T U M NA N O  P L A S M O N I C S W I TO L D A . JAC A K Politechnika Wroclawska, Poland
University Printing House, Cambridge CB2 8BS, United Kingdom One Liberty Plaza, 20th Floor, New York, NY 10006, USA 477 Williamstown Road, Port Melbourne, VIC 3207, Australia 314–321, 3rd Floor, Plot 3, Splendor Forum, Jasola District Centre, New Delhi – 110025, India 79 Anson Road, #06–04/06, Singapore 079906 Cambridge University Press is part of the University of Cambridge. It furthers the University’s mission by disseminating knowledge in the pursuit of education, learning, and research at the highest international levels of excellence. www.cambridge.org Information on this title: www.cambridge.org/9781108478397 DOI: 10.1017/9781108777698 © Cambridge University Press 2020 This publication is in copyright. Subject to statutory exception and to the provisions of relevant collective licensing agreements, no reproduction of any part may take place without the written permission of Cambridge University Press. First published 2020 A catalogue record for this publication is available from the British Library. ISBN 9781108478397 Hardback Cambridge University Press has no responsibility for the persistence or accuracy of URLs for external or thirdparty internet websites referred to in this publication and does not guarantee that any content on such websites is, or will remain, accurate or appropriate.
Contents
Preface
page ix
1
Introduction and Description of Contents
2
Physics of Metals – Preliminaries 2.1 Definition of a Metal 2.2 Scheme of the Fermi Liquid Theory 2.2.1 Phenomenological Theory of a Fermi Liquid 2.2.2 Outline of the Microscopic Theory of a Normal Fermi Liquid
17 17 22 22
Quasiclassical Description of Plasmons in the Bulk Metal 3.1 Random Phase Approximation Theory of Plasmons of Pines and Bohm 3.2 Screening of the Coulomb Interaction in Metals
35
4
Plasmon Excitations in NanometreSized Metallic Particles
41
5
Damping of Plasmons in Metallic Nanoparticles 5.1 Damped Plasmonic Oscillations in Metallic Nanospheres in Dielectric Surroundings 5.2 Attenuation of Dipole Surface Plasmons with Exact Inclusion of the Lorentz Friction 5.3 Comparison of Surface Plasmon Oscillation Features Including Lorentz Friction with the Experimental Data and Simplified Mie Approach 5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
59
3
1
26
35 39
63 71
77 83
v
vi
6
7
8
9
Contents
Plasmon Photovoltaic Effect 6.1 Semiclassical RPA Approach to Plasmons in Large Metallic Nanospheres 6.2 Damping of Plasmons in Large Nanospheres 6.2.1 Radiation from Dipole Surface Plasmons – Lorentz Friction for Plasmons 6.3 Transfer of Sunlight Energy to a Semiconductor Mediated by Surface Plasmons through the Channel of Dipole Coupling in the NearField Regime 6.3.1 Fermi Golden Rule for Band Electron Transitions due to Coupling with Plasmons 6.3.2 Plasmon Damping Rate due to NearField Coupling with SemiconductorBand Electrons 6.3.3 Transfer of Light Energy via the Plasmon Channel 6.4 Experimental Demonstration of the Proximity Constraints of the Plasmon Effect 6.5 Calculation of the Matrix Element for the Fermi Golden Rule Expression (6.37) PlasmonInduced Efficiency Enhancement of Solar Cells Modified by Metallic Nanoparticles: Material Dependence 7.1 PlasmonMediated Photoeffect: Probability of Electron Interband Excitation Due to Plasmons 7.2 Damping Rate for Plasmons in a Metallic Nanoparticle Deposited on a Semiconductor 7.3 Efficiency of the Light Absorption Channel via Plasmons for Various Materials
97 101 104 105
109 109 113 116 120 124 133 134 138 140
Numerical Simulation of Plasmon Photoeffect 8.1 Lorentz Friction Channel for Energy Losses of Surface Plasmons in a Metallic Nanoparticle 8.2 Fermi Golden Rule for Probability of Electron Interband Excitation due to Plasmons in a Metallic Nanoparticle 8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL 8.4 Comparison with Experiment 8.5 Conclusions
150
Plasmon–Polaritons in Metallic Nanoparticle Chains 9.1 Plasmon Oscillations in Metallic Nanospheres 9.2 Radiative Properties of a Metallic Nanosphere in a Chain 9.3 Calculation of the Radiative Damping of a Plasmon–Polariton in a Chain
179 181 186
155 158 163 173 176
190
Contents
9.4 Plasmon–Polariton SelfModes in a Chain Propagation 9.5 The SelfFrequencies and Group Velocities of Plasmon–Polaritons in a NanoChain 9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy 9.7 Collective PlasmonWaveType Propagation along a NanoChain; NearFieldZone Approximation 9.7.1 NearFieldZone Approximation of the Dipole Interaction in a Chain 9.7.2 Medium and FarField Corrections to the NearField Dipole Interaction 9.7.3 Nonlinear Corrections to the Lorentz Friction 9.7.4 Nonlinear Correction to the Radiation Losses of Plasmon–Polariton in a NanoChain 10 Plasmon–Polariton Kinetics in a Metallic NanoChain Located in Absorbing Surroundings 10.1 Plasmon Oscillations in a Single Metallic Nanosphere Including Damping 10.2 Radiative Properties of Plasmon–Polaritons in a Metallic NanoChain Embedded in a Dielectric Medium 10.3 Plasmon–Polariton SelfModes in a Chain in Dielectric Surroundings 10.4 Damping of Surface Plasmons in a Single Metallic Nanoparticle Deposited on a Semiconductor Substrate 10.5 Plasmon–Polariton Dynamics in a Metallic Chain Deposited on a Semiconductor 11 Plasmons in Finite Spherical Ionic Systems 11.1 Fluctuations of the Charge Density in a Spherical Electrolyte System 11.2 Model Definition 11.3 Solution of RPA Plasmon Equation: Volume and Surface Plasmon Frequencies in a Spherical Finite Ion System 11.3.1 Ionic Surface Ion Plasmon Frequencies for an Electrolyte Nanosphere Embedded in a Dielectric Medium with ε1 > 1 11.4 Damping of Plasmon Oscillations in Ionic Systems 11.4.1 Exact Inclusion of the Lorentz Damping 11.5 Derivation of Plasmon Frequencies for a Finite Electrolyte System 11.5.1 Volume Ionic Plasmons 11.5.2 Surface Ionic Plasmons
vii
195 198 202 210 211 215 221 225 231 233 237 240 246 249 252 253 255 261
262 263 267 270 270 271
viii
Contents
12 Plasmon–Polaritons in a Chain of Finite Ionic Systems; Model of Saltatory Conduction in Myelinated Axons 12.1 Plasmon–Polariton Propagation in Linear Periodic Ionic Systems 12.2 Plasmon–Polariton Model of Saltatory Conduction: Fitting the Kinetics to the Axon Parameters 12.3 Soft Plasmonics Application: The Role of Grey and White Matter in Information Processing in the Brain 12.3.1 Possible Link with the Topological Model of a Neuron Web References Index
276 279 284 293 296 303 313
Preface
Plasmonics in metallic nanostructures is a rapidly developing area with various prospective applications in photovoltaics and nanooptoelectronics. The most popular approach to plasmonics is based on the classical Fresnel problem for the propagation of electromagnetic waves with boundary conditions imposed on the Maxwell equations by the presence of metallic components. The typical solution for such a boundary problem uses the dielectric functions of both the dielectric and the metallic materials as prerequisites. The dielectric function of the metallic component is assumed to take the form of the Drude model with the parameters usually adjusted to experimental data extracted from bulk or thinfilm measurements. However, this approach is not sufficient for metallic nanostructures because the dielectric functions of bulk metals and thin films differ significantly from that of a metallic nanocomponent. The strong size and shape dependences of plasmon excitations in metallic nanoparticles are caused by quantumtype effects not included in a phenomenological Drude–Lorentz approach and go beyond the classical determination of light scattering and absorption achieved by solving the Maxwell–Fresnel equations. In the present treatise, we demonstrate that the quantum properties of plasmons are of high importance for nanometrescale metallic components and strongly influence plasmonassisted phenomena not accounted for by the conventional electrodynamic model. We present the random phase approximation (RPA) theory of plasmons in metallic nanoparticles and detail the development of this theory for nanoplasmonic applications in plasmonmediated photovoltaics and optoelectronics. This theory may be helpful for improving popular models of plasmonic effects based on the Mie approach and on numerical solutions of the Maxwell equations, e.g., within the COMSOL system. We describe how to upgrade conventional electrodynamic models by including quantum effects suitably due to the nanometrescale metallic components of various plasmonic systems. This treatise presents a completely developed, mostly analytical, quantum approach to plasmons in metallic nanostructures that can be directly applied ix
x
Preface
to specific situations, such as plasmonics for photovoltaics, plasmon–polaritons in metallic arrays, and plasmons and plasmon–polaritons in ionic soft matter. To ensure completeness we present selfcontained descriptions in each chapter, allowing for independent reading of the chapters. Though each chapter uses formalisms developed in the preceding chapters, a short overview of the most important information and derivations is provided in each chapter foreword, repeating and summarizing the previous derivations as necessary. Thus, the reader can begin at any arbitrary point in the book. Furthermore, the analytical formulation of the theory provides the opportunity for immediate further development and applications by readers.
1 Introduction and Description of Contents
In this introductory chapter a description of the aims of the monograph and its contents is given. The main results are briefly stated in the context of previous publications and knowledge. The applications of nanoplasmonics presented in the book are outlined.
The publication of this book is intended to meet the considerable recent interest in subdiffraction light manipulation by plasmon excitations in nanoscale metallic components [1]. The related rapid development of the new field of nanoplasmonics overlaps with nanophotonics and newgeneration optoelectronics [1–6]. From the quantum physics point of view, metallic nanoparticles are quite different from semiconductor quantum dots (QDs) [7] despite their similar spatial confinement sizes. In a nutshell: QDs are manufactured nanometresized quantum wells that are relatively shallow and do not possess the singularities present in Coulomb confinement. Quantum dots are typically located in semiconductor surroundings and are able to trap conductionband electrons, valenceband holes, or excitons from the surrounding material. They localize electrons in discrete quantum states analogous to those of atoms, though without the limitation caused by the instability of the atomic nucleus. Quantum dots can thus be filled with several carriers, electrons or holes; however, this is limited in practice by the depth of the QD well. The analogy between QDs and ordinary atoms can be somewhat misleading owing to the strong dephasing of states in QDs by collective excitations in the surroundings (mostly phonons). This dephasing occurs because the energy scales of the trapped carriers in QDs and of the collective phonon excitations in the surrounding crystal are similar. Hence, the decoherence of QD states (hybridization with collective band excitations) is, by several orders of magnitude, larger than that in atoms [8]. Nevertheless, the concept of a QD is physically straightforward and allows for easy and efficient numerical modelling based upon an elementary quantum mechanics scheme for a small number of particles.
1
2
Introduction and Description of Contents
For metallic nanoparticles the situation is different and is related to the much more complicated physics of metals. The typical situation for metals is a deep Fermi sea of nearly free electrons with a welldefined Fermi surface even at high temperatures; the Fermi energy in metals, of the order of 104 K, greatly exceeds the melting temperature. The theory of metals was developed for bulk metals in the 1960s by the application of advanced methods for multiparticle systems, mostly in terms of the Green function approach [9]. The quantum degeneracy of the dense Fermi liquid of electrons in metals (actually the degeneracy of the Landau quasiparticles, which are stable on the Fermi surface [9]) makes a finite metal sample confined at the nanoscale a quantum system very different from a QD lowpopulated with band carriers in semiconductors. In metals, the crystalline positive ion background that is essential for the definition of the related quantum states causes an additional complication. There have been many successful attempts to describe the excitations in metals using quantum statistical physics and manybody theory methods [9–11] or a quasiclassical phenomenological approach [12, 13]. Besides the lowenergy excitations near the Fermi surface in metals (i.e., the electrons that can be expressed in terms of socalled Landau quasiparticles [9, 11]), there exist also collective highenergy excitations involving all the electrons simultaneously, not just those located close to the Fermi surface. For a bulk metal, an efficient theory for these highenergy collective excitations of electrons in metals was developed in 1952, within the random phase approximation (RPA) approach, by Pines and Bohm [14, 15]; these highenergy collective excitations were called plasmons. Owing to the large energy difference between plasmons and the Landau quasiparticles close to the Fermi surface, plasmons do not interact with the Landau quasiparticles, although all the electrons collectively create plasmons. Thus, plasmons cannot be excited just by lowenergy electrons, as the plasmon energy in a bulk metal is typically of the order of 10 eV, exceeding even the Fermi energy, which is usually of the order of 7−8 eV. The plasmon energy is thus of a scale similar to that of ultraviolet (UV) photons, and so plasmons can be excited by sufficiently hard electromagnetic radiation. However, in confined metallic nanoparticles the energies of plasmons are considerably lower [17–21], and in noble metals (Au, Ag, Cu) they fit with the visible photon energies. This observation sparked the nanotechnology revolution related to the modification and control of visible light by plasmons in metallic nanostructures [1–6] whose spatial size is much lower than the wavelength of light, referred to as subdiffraction light manipulation. It should be noted that plasmas and their excitations were the subject of interest early in the twentieth century [18] and since then have been investigated in relation to highenergy plasmas of charged particles (mostly protons) in stellar kernels, tokamaks, galaxy ion clouds, and the ionosphere. This interest has been stimulated also by the development of overhorizon radar and
Introduction and Description of Contents
3
antiradar technology, which has been accelerated in recent years by achievements in metamaterial construction (such as an ‘invisibility cloak’) allowing control over light in a manner different from ordinary reflection and refraction. The main objective of this book is to present an effective theory of plasmons in metallic nanoparticles that is as analytical as possible, allowing universal applications that are not restricted to previously studied numerical models. The numerical methods developed in the 1980s for ab initio approaches to plasmons in metallic clusters were limited to approximately 300 electrons (owing to the high numerical complexity of the solution of the Kohn–Sham equations) [19, 20]. In view of these problems, insights into the plasmonics of metallic nanoparticles were confined to phenomenological approaches; these approaches used experimentally aided modelling [22] of the dielectric function in the solution of the classical Fresnel–Maxwell equations for the boundary problem of a metallic nanoparticle with spherical geometry and an incident planar wave. The analytical solution of this problem is known as the Mie approach [17, 18] and results in formulae for the scattering and extinction cross sections for light incident on a metallic sphere. However, the Mie approach uses a phenomenological dielectric function for the metal as a prerequisite to model light absorption in the metallic nanoparticle (according to the conventional Drude–Lorentz model) [17]. The same approach is used for the numerical solution of the Maxwell equations with boundary conditions in the COMSOL system (which is not limited to spherical geometry); this utilizes the finite element method to solve the Maxwell equations. The COMSOL calculus includes the plasmon dynamics only phenomenologically, via a predefined dielectric function of the metallic compound. However, recognition of the plasmon properties of metallic nanoparticles is not available in either of the aforementioned approaches, which is a significant drawback. Therefore, progress in the description of plasmon excitations in metallic nanoparticles within a microscopic framework, preferably in an analytical form, may have considerable significance for improving upon the very popular Mietype and COMSOL methods. Upgrading these classical methods may consist in a better declaration of the dielectric functions of the objects under study, since these functions are prerequisites for both the Mie and COMSOL calculus. The modelling of dielectric functions at the nanoscale is a source of certain discrepancies between the numerical solutions and experiments because a predefined dielectric function is usually supported by experimental data that come from bulk metals or thin films, rather than from nanoscale particles. Thus, theoretical insights into the properties of plasmons at the nanoscale that include quantum effects are necessary to improve the conventional numerical models. This can be done via the development of a microscopic quantum model for surface and volume plasmons in metallic nanoparticles using the RPA approach [16] for finite nanoscale geometries [23], in a generalization of the Pines–Bohm theory [14–16].
4
Introduction and Description of Contents
We will demonstrate this approach in the present text and describe an analytical description of all the multipole modes (for spherical symmetry) for surface and volume plasmons within the RPA model that agrees well with experimental observations. Surface plasmons in a metallic nanoparticle correspond to the translational collective oscillation modes of all the electrons in the nanoparticle when the charge fluctuations that are not compensated by the static positive ion jellium occur only on the nanoparticle surface. This condition is in contrast with volume plasmons, which are compressionaltype modes with charge density varying along the nanoparticle radius. Remarkably, the surface plasmons in nanoparticles have resonance energies lower than the energy of the bulk plasmons, i.e., hω ¯ p = h¯ ne2 /(mε0 ) (n is the electron density in the metal, e and m are the electron charge and mass, and ε0 is the dielectric constant); for √ the simplest case, that of dipoletype surface plasmon oscillations, hω ¯ p / 3 (the Mie energy). However, the volume plasmons in ¯ 1 = hω nanoparticles have resonance energies higher than those in the bulk. Neither type of plasmon excitation – the surface or the volume plasmons – occurs in the bulk metal (although for a halfspace √ geometry there are surface plasmons at the socalled Ritchie frequency, ωp / 2 [5]). The essential difference between the RPA Pines–Bohm model for bulk metals [16] and the RPA theory for metallic nanoparticles consists in the explicit definition, in the latter theory, of the finite rigid jellium (defining the shape of the nanoparticle) [23]. In the RPA Pines–Bohm theory, the infinite jellium in the bulk is renormalized out via an ideal compensation with a uniform longwavelength coherent electron fluctuation (i.e., a uniform plasmon mode with momentum q = 0). For a finite nanoparticle, however, such a renormalization is impossible because of the absence of translational invariance and the presence of quantum numbers that are different from momentum quantum numbers for the plasmon excitations, owing to the explicit presence of the jellium rim. The quantum dynamics equation in the Heisenberg representation determines the selfmodes for collective local charge density fluctuations [16, 23]. The gradient operator in the kinetic energy term produces Dirac delta singularities on the rim of the jellium; these arise from the derivative of the Heaviside step functions defining the jellium border. Because these singularities are located on the edge of the nanoparticle, they allow separation of the surface and volume plasmon components in the dynamics equation [23]. However, a mutual dependence of the two types of excitation is visible within the RPA approach. Moreover, the problem of the socalled spillout of the electron liquid beyond the rim of the jellium can also be considered in the RPA theory. Nevertheless, the spillout appears to be on the scale of the Thomas–Fermi length [19] and is thus unimportant for nanoparticles with a radius larger than about 5 nm, though for smaller nanoparticles
Introduction and Description of Contents
5
(of size 2−3 nm) the spillout considerably dilutes the electron density inside the cluster and redshifts the resonance plasmon frequencies, which are proportional to the square root of the charge density [19–21]. Surface effects such as spillout and Landau damping [20] (the latter corresponds to the decay of plasmons into a pair of quasiparticles distant from the Fermi surface and thus unstable) become less important for larger nanoparticle sizes, and for nanospheres with radii larger than 5 nm these surface effects are negligible [20]. The reduction in the role of spillout (which makes the surface fuzzy and perturbs the surface modes) for particles larger than a few nanometres in radius supports the usability of the RPA approach in a quasiclassical way: it is a sufficiently accurate quantum approach at this nanoparticle size [23] as it allows the separation of volume and surface local electron density fluctuations. In ultrasmall nanoparticles [19], mixing of the surface and volume excitations occurs for up to approximately 60 electrons, when shell effects cease to contribute [19, 21]; for larger nanoparticles the separation between the surface and volume excitations improves for greater numbers of electrons [23] and is almost ideal for nanospheres with radii larger than approximately 5 nm. The quantum dynamics equation (the Heisenberg equation for the secondorder time derivative of the local electron density operator [16, 23]) has a complicated form owing to the presence of the finite jellium. However, after making the RPA simplification, including a quasiclassical averaging of the kinetic energy according to the socalled fivethirds Thomas–Fermi formula [16]), this quantum dynamics equation describes a plethora of plasmon modes in the nanoparticle [16], many more than the single volume mode of the bulk metal [16]. An important advantage of the RPA model developed in this book is the possibility of including dissipation effects such as those due to electron scattering on other electrons, on phonons, on admixtures and defects or on the boundary of the nanoparticle. The resulting shift in the plasmon resonance caused by the scattering damping of plasmons scales as 1/a, where a is the radius of a nanoparticle [24], which agrees with experimental observations for the radius range 5 < a < 10 nm (for Au in a vacuum), where electron scattering energy dissipation dominates other damping channels [25]. Nevertheless, plasmon oscillations are also damped by radiation, an effect that increases with the electron number in a nanoparticle and leads to pronounced crossover in the size dependence of the plasmon attenuation and the related resonance shift for nanosphere radii a of 10−12 nm (for Au in vacuum, in general the crossover depends on the metal and the dielectric surroundings). At nanoparticle sizes corresponding to this crossover, the decrease in the plasmon damping as 1/a changes to a strong increase proportional to a 3 [26], the a 3 dependence is related to the fact that all the electrons participate in plasmon oscillations and their radiation properties; this is true even for surface plasmons.
6
Introduction and Description of Contents
Thus, the contribution of all the electrons in a nanoparticle is manifested by the volume factor a 3 , which causes a similar scaling in the radiative damping of plasmons resulting from the socalled Lorentz friction [26], i.e., the energy loss of oscillating charged particles due to the radiation of electromagnetic waves. For a sufficiently large number of electrons inside the nanosphere, the Lorentz friction losses dominate other channels of plasmon damping. The large radiation energy loss expressed by the Lorentz friction damping initially grows with a 3 , as mentioned above [27], but then saturates at approximately a ∼ 50 nm (for Au in vacuum) and gradually decreases for larger nanoparticles. This behaviour is identified and described in this text. Such behaviour reveals that the inclusion of Lorentz friction considerably changes the plasmon oscillation regime: the oscillations are not of the harmonicoscillator type because the Lorentz friction is proportional to the thirdorder time derivative rather than the firstorder time derivative as is the case for the ordinary friction of a harmonic oscillator. The harmonic oscillator model appears to be incorrect for plasmons in large metallic nanoparticles, and many simplified harmonic models of plasmons that are popular in the literature are misleading. In particular, the overdamped regime typical for harmonic damped oscillators, which would terminate plasmon oscillations within the harmonic model at approximately 57 nm, for Au in vacuum, does not reflect reality. The solution of the thirdorder dynamic differential equation is different from that for a harmonic oscillator, and the relationship between the frequency and damping of a harmonic oscillator,
ω02 − 1/τ 2 (which defines the overdamped regime when the expression under the square root is negative), is not valid for plasmons. Beyond the harmonic model the relationship between frequency and damping also has an analytical form, which has been derived and which allows us to describe plasmon behaviour precisely. The exact solution of the Lorentz friction problem for plasmons in metallic nanoparticles [26] gives very good agreement with experiment, with respect to the size dependence of plasmon resonances in metallic nanospheres. This result provides more precise modelling of metal dielectric functions, for specific sizes of nanostructure configurations, that includes plasmon damping and has also been applied to modify numerical studies using COMSOL and Mietype calculation schemes [28, 22, 29], in both cases these schemes use predefined dielectric functions for the systems analysed. The results have been confirmed experimentally for Au and Ag nanoparticles. The RPA theory of plasmons in metallic nanoparticles and their radiative properties is useful for modelling the socalled plasmonaided photovoltaic (PV) effect. The damping of the plasmons changes radically when another electrical system is located near a metallic nanoparticle with plasmons; such a system could be a semiconductor substrate with a band electron system. In such a case, the
Introduction and Description of Contents
7
semiconductor substrate receives an extremely strong flow of energy from the plasmons to the band electrons, which corresponds to plasmon damping greatly exceeding the Lorentz friction losses in the dielectric surroundings. This new and strong channel of energy transfer can be described by applying the Fermi golden rule to the quantum interband electron transitions induced by the nearfield radiation of plasmons in a metallic nanoparticle deposited on a semiconductor substrate [30]. The mediation by plasmons in the energy harvesting of a photoactive semiconductor layer results in significant modification of the ordinary photoeffect. This phenomenon is of high practical importance in view of the current rapid development of photovoltaics; in 2015, the total power of all PV solar cell installations worldwide was approximately 250 GW, whereas the total power produced by conventional coal or gas energy plants was approximately 29 GW in Poland. There could be an increase in the efficiency of solar cells (particularly thinfilm solar cells and organic ‘plastic’ cells) by several per cent due to mediation by plasmons in metallic nanoparticles deposited on the cell surfaces (metallic coverings with low densities, ∼ 108−10 /cm2 and thus low costs and easy accessibility for industry technology) [31]. This could have a large economic impact in the field of renewable energy sources [32–36]. In Au, Ag, and Cu nanoparticles with radii a ∼ 10−50 nm the photoeffect efficiency is enhanced, in laboratory setups of photodiodes, by a factor 2−10 owing to energy transfer from the incident photons to the semiconductor substrate via plasmons in the deposited metallic components [31–36]. However, in solar cells the efficiency of the photoeffect is only one factor amongst many other factors that define the final total efficiency of a cell, and a large increase in photoeffect efficiency causes a more modest increase in the total efficiency of a solar cell. Through the quantum calculus of the Fermi golden rule scheme, we can demonstrate [30] that the nearfield coupling of the dipole mode of the surface plasmons in metallic nanoparticles deposited on top of a semiconductor is very efficient, i.e., this coupling effect causes a strong increase in the probability of interband transitions compared with the ordinary photoeffect, in which the planewave photons interact directly with the band electrons. The advantage of the result obtained via the Fermi golden rule approach is its analytical form (which is similar to the formula for the ordinary photoeffect in a semiconductor, though the calculus for plasmon mediation is much more complicated; however, it is analytically attainable [30]). The analytical form of this approach allows for the analysis of various competing mechanisms, and leads to an expression for the photoeffect efficiency increase due to plasmons in solar cells. The related calculations explicitly demonstrate that the absence of translational invariance for a nanoparticle coupled in a nearfield zone with a semiconductor substrate removes the constraints imposed by the momentum conservation rule.
8
Introduction and Description of Contents
Thus, in addition to the vertical interband transitions (conserving the electron momentum plus the negligible photon momentum) found in the ordinary photoeffect, all indirect interband transitions between arbitrary electron momenta are available, which strongly enhances the probability of interband transition. The momenta of incident photons with energies beyond the forbidden energy gap are negligible compared with the momenta of the Bloch states of the band electrons in a semiconductor, which results in a constraint to ‘vertical’ interband transitions in the ordinary photoeffect. This constraint is removed when the translational symmetry is violated for a small metallic nanoparticle. The coupling of the plasmon dipole in the nearfield regime allows all skew interband transitions, enhancing the total probability of interband excitations of carriers in the semiconductor substrate. This effect favours smaller metallic nanoparticles but, conversely, larger nanoparticles have larger dipoles (in proportion to the electron number), which also enhances the transition probability. The resulting tradeoff of these opposing tendencies defines the optimal size for a metallic nanoparticle to increase the photoeffect efficiency. Moreover, the type of nanoparticle deposition used plays an important role. Though problematic from a technological perspective, a convenient deposition method is the complete embedding of the metallic nanoparticles into the semiconductor layer. The theory has been developed to allow analysis of the aforementioned size tradeoff and of the role of the nanoparticle deposition method on the photodiode surface. Energy transfer through the coupling of the subphoton near field (i.e., the near field on a length scale 10−100 times smaller than the photon wavelength) with the surface plasmon dipoles is very efficient. This high efficiency results in high damping of the plasmons, much higher than the radiative damping due to Lorentz friction and the damping due to electron scattering [23], and elucidates the very strong plasmonic PV effect that is observed experimentally. The prospects for largescale utilization of this effect in industry and commercial photovoltaic devices depend on the practical deposition methods for nanoparticles on cell surfaces, which usually reduce the net effect as too high a density of metallic particles results in inconvenient interference reflection effects of the metallic nanocover. Nevertheless, at low surface concentrations of the metallic nanoparticles, the theoretically determined resonance curves agree very well with the experimental results [30, 31, 33]. Another experiment elucidated by the theory concerns a twolayer structure of Si–ZnO nanopillars, consisting of a thick layer of pSi covered with nZnO vertical nanorods with diameters ranging from 200 to 300 nm and heights of approximately 1000 nm [30]. When the top of the structure was covered with silver nanoparticles (with radii of 5, 20, or 50 nm), the photoresponse doubles. This increase is caused in part by ZnO subgap transitions but also by the Si substrate; this is revealed by the characteristic size dependence. This proves that the range of the
Introduction and Description of Contents
9
plasmonic effect is at least 1 micrometre, which makes the effect convenient for thinlayer solar cell technology [34–36]. Multicrystalline Si solar cells sparsely covered with nanoparticles have recently shown very good agreement with the predictions of the theory; the gains in efficiency have reached 5.6% for Au nanoparticles and 4.8% for Ag nanoparticles, whereas, for CIGS (copper indium gallium diselenide) cells, gains of 1.2% (Au) and 1.4% (Ag) have been achieved [31]. Many other, even greater, experimental results have been reported. However, as mentioned, an excessive concentration of metallic covering diminishes the efficiency of solar cells (owing to screening and reflection effects). The successful theoretical RPA description of plasmons in a single metallic nanoparticle and the recognition of their radiative properties allows for the development of the RPA model for interacting systems (arrays) of metallic nanoparticles, in particular for metallic nanochains that could serve as lowloss plasmon–polariton wave guides for the desired miniaturization of optoelectronics. Plasmon–polaritons are collective wavetype modes of surface plasmons hybridized with an electromagnetic wave propagating, with almost lossless kinetics, along a periodic chain of metallic nanoparticles. They are analogous to the surface mode of plasmon propagation along a metal–insulator interface, also called a plasmon–polariton [1, 5]. The change in the configuration of the electromagnetic field near the metal– insulator interface around a metallic wire is utilized in highfrequency microwave techniques (e.g., in singlewire Goubau transmission lines [37]). This effect raises an interesting issue for similar propagation along discrete metallic nanochains [38–43] – experiments confirm the lossless propagation of dipole collective wavetype oscillations in the range of several micrometres [39, 40] with group velocity at least 10 times lower than c (the velocity of light). The latter property allows for a reduction in the diffraction constraints [38] that severely limit the miniaturization of the optonanoelectronics, where the wavelengths of photons with energies typical for the nanoelectronics scale (meV) greatly exceed the dimensions of the nanoscale electronic elements (because of the high value of c), precluding miniaturization. The transformation of the electromagnetic signal into a plasmon–polariton, which has the same frequency but a 10 times (at least) shorter wavelength, allows the avoidance of diffraction limits. This is promising for future nanoscale plasmon optoelectronics [5, 38, 42]. An analysis has been developed of the plasmon–polariton kinetics inhmkujkj metallic nanochains using a farreaching analytical formulation of the RPA theory [44–46] (which has made significant progress in comparison with numericalonly studies [41, 43]). This analytical formulation allows the precise identification of various factors that were previously resistant to insight within complex numerical approaches [42, 43]. These factors are related to detailed identification of how the damping and the group velocity of plasmon–polaritons depend on the material and geometry parameters.
10
Introduction and Description of Contents
In particular, it has been demonstrated that the accurate inclusion of all terms in the dipole interaction in the near, medium, and farfield zones, together with retardation effects (frequently neglected in the literature), leads to ideal compensation of the Lorentz friction in each nanosphere in a chain by the radiation energy income from the remaining nanoparticles in the chain [46]: thus the propagation of plasmon–polaritons in the chain is radiatively lossless. Taking into account that the Lorentz friction in a large metallic nanosphere, with radius > 12 nm, for Au in vacuum, greatly exceeds the electron scattering energy losses (i.e., the irreversible dissipation of plasmon energy into Joule heating due to scattering from electrons, phonons, admixtures, defects, and boundaries), a metallic nanochain behaves as an almost lossless ideal wave guide for plasmon–polaritons [46]; this agrees with experimental observations [39, 38] and indicates possible applications in subdiffraction plasmonoptoelectronics due to the low group velocity (and wavelength) of plasmon–polaritons. The RPA model developed for plasmon–polaritons [46] shows that this ideal compensation of the Lorentz friction occurs only inside the light cone (on which the plasmon–polariton phase velocity equals the velocity of light); outside the light cone the damping of plasmon–polaritons is strengthened to values above the Lorentz friction scale (this damping outside the light cone increases steadily with increasing plasmon–polariton wave number for longitudinal plasmon–polariton polarization, when the dipoles oscillate along the chain direction, and increases stepwise for transverse polarization [47, 45]). On the light cone (in one dimension there are only two points in the Brillouin zone for a periodic chain – the light cone here is a triangle as a function of the chain separation), a logarithmic singularity of the dynamics equation occurs [45]. This singularity is caused by constructive interference of the radiation from the nanospheres in the chain in the farfield zone and occurs only for transverse polarizations of the plasmon–polaritons; it causes a similar divergence at all orders in the perturbation series for the dispersion [45]. The logarithmic perturbative divergence in the dispersion of the plasmon–polaritons in turn causes a hyperbolic singularity in the group velocity for transversely polarized plasmon–polaritons, which is observed in many numerical simulations presented in the literature (in a numerical solution of the dynamics, a certain kind of perturbative solution is linked with an unavoidable truncation of the exact infinite Green function series, which produces a numerical artefact that has been erroneously interpreted as superluminal propagation). The aforementioned error has been explained in detail and is not present in an exact solution of the dynamic equation for plasmon–polaritons obtained using a special nonperturbative method (i.e., by separate solution of the nonlinear problem at approximately 20,000 points of the Brillouin zone by a Newtontype
Introduction and Description of Contents
11
procedure) which allows for determination of the dispersion and the damping of the plasmon–polaritons beyond any perturbative step [45]. This solution has revealed the precise removal of the ‘perturbative’ singularity in the group velocity (which is hyperbolic for transverse polarizations) via its truncation at the velocity of light in the dielectric surroundings, which agrees with Lorentz invariance. Other singularities in the group velocity of the plasmon–polariton were also identified for both polarizations; these singularities occur also on the light cone, are of logarithmic character, and are caused by constructive interference in the mediumfield zone in the dynamics equation for plasmon–polaritons [45] (again manifesting themselves at any perturbation order, these singularities correspond to the derivative with respect to the wave number of the mediumfieldzone contribution to the selffrequency, which is logarithmically divergent at the light cone). Via the exact nonperturbative solution, it was demonstrated that these group velocity singularities (without any dispersion singularities) are excluded and truncated exactly at the velocity of light. This analysis elucidates the misleading interpretations of numerical approximate simulations as being due to artefacts caused by the perturbative approach. An interesting analogy might be drawn: in quantum field theory, singularities occur at any order of the perturbation series but these singularities can be removed by renormalization procedures. Hence, the problem analysed above of plasmon–polariton dynamics is actually an example of explicitly performed renormalization via the exact solution of the highly nonlinear singular problem, regularized by Lorentz invariance. In a similar manner, the problem of the numerically observed longrange plasmon–polariton modes close to the light cone is explained. In contrast with the explanation in the literature, of an extraordinary mode with lowered damping, the longerrange modes can be identified with a local increase in the group velocity for a thin wave packet close to the truncation singularity; this gives a range of propagation several times longer at the same level of damping. By analysis of the convergence of an appropriate series related to the radiation effects in the chain, the small impact of the finiteness of the chain on the plasmon–polariton kinetics was demonstrated and thus the usability of the infinitechain results for finitelength periodic structures (even 10 periodic elements in the chain yield almost the same plasmon–polariton behaviour as an infinite chain, owing to the very quick convergence of the radiation series, except for those series resulting in singularities but these types of series do not occur in finite chains). The theory developed for plasmon–polaritons in a metallic nanochain demonstrates the propagation of a collective surface plasmon mode with the whole electromagnetic field compressed along the chain (which agrees with COMSOL simulations and nearfield scanning optical microscopy (SNOM)) [39, 40]. Owing to the incommensurability of photon wavelengths and the wavelengths of
12
Introduction and Description of Contents
plasmon–polaritons with the same energies, any mutual perturbation of both these excitations is precluded; thus the detection, excitation, or perturbation of plasmon– polaritons by free photons is not possible, which makes plasmon–polaritons immune to electromagnetic perturbations. Moreover, the lossless subdiffraction plasmon–polariton mode controlled by the chain parameters might be able to sense nanodeformations due to strain in various mechanical constructions. This could be done by the use of elastic substrates with metallic nanochains simply pasted onto the strained elements, stepwise changing the regime of the plasmon–polariton kinetics, which are very sensitive to small changes in nanoparticle separation due to length deformation of the substrate. This effective microscopic RPAtype theory of plasmons and plasmon–polaritons in metallic nanostructures creates an opportunity for the development of similar approaches for other (ionic) charged multiparticle systems. The plasmon and plasmon–polariton RPA theory of metallic nanostructures has been applied to ionic plasmons and plasmon–polaritons in finite electrolyte systems (confined by the dielectric membranes that are frequently found in biocell organization) [48]. This generalization involves the following steps. (a) The accommodation of the RPA model defined for a finite quantum degenerate Fermi liquid of electrons in a metal to a Boltzmanntype nondegenerate liquid of ions (fermions or bosons) requires substitution of the socalled 5/3 Thomas–Fermi formula for a degenerated electron gas by a classical estimation of the average kinetic energy according to the Maxwell–Boltzmann distribution; simultaneously, the Fermi velocity must be substituted by the Boltzmann average velocity of ions. These changes introduce a specific temperature dependence that is absent in the metallic RPA model. (b) The core element of the ionic theory of plasmons is the introduction of an auxiliary fictitious twocomponent ‘jellium’ for a binary electrolyte. In any electrolyte, ions of both signs are dynamical components of the system, unlike in metals, where the positive jellium in the form of the crystalline lattice defines a stiff shape for the nanoparticle. Nevertheless, by modelling the Hamiltonian for a binary electrolyte, a fictitious jellium with two components whose charges mutually cancel can be introduced without any change in the total energy. For sufficiently small local charge excitations in the electrolyte, the twocomponent fictitious jellium model allows for a description of plasmon excitations that is in analogy with that for metals, in the form of two mutually coupled ionic excitations. This model admits the classification of volume and surface ionic plasmons (compressional and translational modes, respectively) with various polarizations for spherical symmetry and the estimation of their energy and damping in analogy to that for metallic nanoparticles. Because ions have larger masses than electrons and typically have lower concentrations in electrolytes compared with the free electron concentrations in metals, the characteristic plasmonic size scale (defined
Introduction and Description of Contents
13
as the size of a finite system with maximal plasmon radiation) is on the scale of micrometres for ions rather than the nanometre scale of electrons in metals, and the plasmon frequency is strongly reduced by many orders of magnitude depending on the ion concentration and the ion mass and charge. All the elements of the RPA model generalized to finite ion systems have counterparts in metals, including the characteristic and typical behaviours of surface and volume plasmons (however, the latter exhibit a temperature dependence for ions that is absent for electrons in metals). There are similar radiation effects, including a Lorentz friction loss that is larger than ordinary scattering losses (for ions it depends on the temperature in a quite different way than that for the electron archetype owing to the substitution of the practically temperatureindependent Fermi velocity of metals by the temperaturedependent averaged velocity of the ions in an electrolyte). In addition to the plasmon excitations in a separated single finite electrolyte system, a theory of ionic plasmons on finite periodic ionic systems with ionic plasmon– polaritons was developed [49]. In analogy to plasmon–polaritons in metallic nanochains, similar properties were described for ionic plasmon–polaritons in periodic ionic microchains. The wave guide kinetics of plasmon–polaritons in ionic chains was analysed with respect to a wide range of ion parameters and confinement scales including overlap with additional specific vibrational and rotational excitations of the electrolyte’s solvent molecules (of water). The plasmon–polariton model of a chain of finite electrolyte systems was next applied to the original explanation for socalled saltatory conduction in myelinated axons. The intention was to explain using ionic plasmon–polariton kinetics the unknown and mysterious mechanism of the quick and efficient nervous signal transduction observed in periodically myelinated axons in neurons of the peripheral nervous system and in the white matter of the brain and spinal cord [50, 51]. The standard cable model [52] (originated by William Thomson in the nineteenth century) describes well the diffusiontype kinetics of the ionic electrical signal along the dendrites and nonmyelinated axons (in the grey matter in the central nervous system). According to the cable theory, the velocity of a signal depends on the conductivity of the innerneuron cytoplasm and on the capacity across the cell membrane between the inner and outer cytoplasm; it is stiffly confined, and reaches at most 1−3 m/s. This signal velocity is too low for the transduction of nerve signals over longer distances; moreover, in myelinated axons, which are periodically wrapped with a white lipid called myelin, the action potential somehow jumps between the consecutive socalled Ranvier nodes separating the segments wrapped with the myelin sheath. In this way, the signal accelerates and the velocity reaches the 100−200 m/s required for proper signalling and functioning of the body. The mechanism of these jumps is unknown, having been researched for a long time
14
Introduction and Description of Contents
without progress, and is phenomenologically designated ‘saltatory conduction’. It is agreed [50, 51] that the myelin sheath is crucial for saltatory conduction: the myelin is much thicker than would be needed for isolation only; moreover, any deficit in the thickness of the sheaths results in severe demyelination diseases such as multiple sclerosis, manifesting itself in slowing saltatory conduction and motor dysfunction. Myelin is produced for neurons in the peripheral nervous system by Schwann cells, whereas in the central nervous system oligodendrocytes produce the necessary myelin [51, 50]. Remarkably, the length of myelinated sectors is typically 100 μm and, as mentioned above, the myelinated sectors are separated by very short nonmyelinated fragments called Ranvier nodes [51, 53]. In the Ranvier nodes spikes of the action potential form, according to a wellknown mechanism, on a time scale of a few milliseconds [50], but the mechanism by which the ignition signal jumps to the neighbouring Ranvier nodes cannot be explained by any accepted model based on the cable theory. We proposed an original assumption, that saltatory conduction in neurons periodically wrapped with the thick myelin sheath has an ionic plasmon–polariton character. We then obtained a satisfactory prediction for the signal velocity at realistic parameters for the electrolyte of the neuron cytoplasm. The model achieved good consistency with the various features of saltatory conduction observed in myelinated axons [49], including the following. (a) A high group velocity for the plasmon–polariton wave packet in agreement with the velocity observed in myelinated axons and real electrolyte parameters inside the axon. (b) There is an absence of radiative damping of the plasmon–polaritons and the reduction of attenuation to the level of only ohmic losses (lower than those for ordinary conduction); with only low energy supplementation (which occurs at the Ranvier nodes) a forced undamped plasmon–polariton mode can propagate without deformation over arbitrary long distances. (c) The energy supplementation takes place residually, at the generation of action potential spikes on consecutive Ranvier nodes, according to a known [50] mechanism. This mechanism employs ion channels across the unmyelinated axon cell membrane at the Ranvier node. It is the final phase of a cycle during which steady conditions are restored, and so an external energy supply is needed to actively transfer ions (Na+ and K+ ) across the cell membrane against the concentration gradient. The energy is supplied by the ADP/ATP mechanism in the cell and residually also covers the ohmic losses (ultimately transferred to Joule heat) of plasmon–polaritons. (d) The wave nature of saltatory conduction is confirmed by the observation that axon ignition is maintained even if the axon is broken into two separate pieces located near each other (this property is impossible to explain within the cable theory or on the basis of other electricalcurrenttype mechanisms but fits reasonably well with properties of plasmon–polaritons, which can propagate either along a continuous fibre or along a discontinuous chain) [50]. That plasmon–polaritons have a wave nature also agrees well with the observed oneway direction of propagation when an axon is initiated from the
Introduction and Description of Contents
15
synapse or axon hillock and twoway propagation when a passive neuron is ignited from its centre. The plasmon–polariton mechanism is also consistent with the observation that axon firing continues even if several Ranvier nodes are damaged and inactive [50]. (e) The model gives a temperature dependence that is typical for ionic plasmon–polaritons, and it also gives the dependence of the plasmon– polariton group velocity on the cross section of the thin inner cord of the axon. The role of myelin, different other than giving insulation, is explained by the plasmon–polariton model (a sufficiently thick myelin sheath is required to build the dielectric tunnel around the inner cord needed for the formation of a plasmon– polariton; decreasing the thickness of this myelin tunnel results in the deceleration of plasmon–polariton propagation, which is actually observed in multiple sclerosis) [50]. (f) The model is also consistent with the exclusive property that plasmon– polaritons cannot be ignited, perturbed, or detected by electromagnetic waves (since photons with low energies identical to those of ionic plasmon–polaritons do not interact with plasmon–polaritons), and therefore, plasmon–polariton signalling is immune to electromagnetic perturbations (note that ordinary current conduction in the grey matter can be detected by electromagnetic means (encephalography) and can even be perturbed electromagnetically, but signalling in the white matter cannot). Application of plasmon and plasmon–polariton effects in ionic systems opens a new field, that of the soft plasmonics of confined electrolytic systems in relation to biomatter organization and its functionality. The example presented above illustrates the usefulness of the developed RPA model of plasmons and plasmon–polaritons. Author contributions In this treatise the original results of the author with coauthors are utilized with permission of the coauthors and the publishers. To be specific: in Chapter 4, reference [23]; in Chapter 5, references [26–28]; in Chapters 6 and 7, references [30, 31]; in Chapter 8, references [145, 159]; in Chapter 9, references [44–46]; in Chapter 10, reference [47], in Chapters 11 and 12, references [48, 49]. The references are listed below. [23] J. Jacak, J. Krasnyj, W. Jacak, R. Gonczarek, A. Chepok, and L. Jacak, ‘Surface and volume plasmons in metallic nanospheres in semiclassical RPAtype approach; nearfield coupling of surface plasmons with semiconductor substrate’, Phys. Rev. B 82, 035418, 2010 (with permission from APS). [26] W. A. Jacak, ‘Lorentz friction for surface plasmons in metallic nanospheres’, J. Phys. Chem. C 119(12), 6749–6759, 2015 (author reuse in the book with permission from the American Chemical Society). [27] W. A. Jacak, ‘Sizedependence of the Lorentz friction for surface plasmons in metallic nanospheres’, Opt. Express 23, 4472–4481, 2015 (author reuse in the book with permission from the Optical Society).
16
Introduction and Description of Contents
[28] K. Kluczyk and W. Jacak, ‘Dampinginduced size effect in surface plasmon resonance in metallic nanoparticles: comparison of RPA microscopic model with numerical finite element simulation (COMSOL) and Mie approach’, J. Quant. Spectrosc. Radiat. Transfer. 78, 168, 2016 (with permission from Elsevier for the author reuse in the book). [30] W. Jacak, E. Popko, A. Henrykowski, E. Zielony, G. Luka, R. Pietruszka et al., ‘On the size dependence and the spatial range for the plasmon effect in photovoltaic efficiency enhancement’, Sol. Energy Mater. Sol. Cells 147, 1, 2016 (with permission from Elsevier for author reuse in the book). [31] M. Jeng, Z. Chen, Y. Xiao, L. Chang, J. Ao, Y. Sun, et al., ‘Improving efficiency of multicrystalline silicon and CIGS solar cells by incorporating metal nanoparticles’, Materials 8(10), 6761–6771, 2015 (with permission from MDPI for unrestricted use and reproduction as an open access publication). [44] W. Jacak, ‘On plasmon polariton propagation along metallic nanochain’, Plasmonics 8, 1317, 2013. DOI: 10.1007/s1146801395288 (with permission for author reuse from Springer Nature). [45] W. Jacak, ‘Exact solution for velocity of plasmon–polariton in metallic nanochain’, Opt. Express 22, 18958, 2014 (author reuse in the book with permission from the Optical Society). [46] W. Jacak, J. Krasnyj, and A. Chepok, ‘Plasmon–polariton properties in metallic nanosphere chains’, Materials 8, 3910, 2015 (with permission from MDPI for unrestricted use and reproduction as open access publication). [47] W. Jacak, ‘On plasmon polariton propagation along metallic nanochain’, Plasmonics 8, 1317, 2013 (with permission for author reuse from Springer Nature). [48] W. Jacak, ‘Plasmons in finite spherical electrolyte systems: RPA effective jellium model for ionic plasma excitations’, Plasmonics, 2015. DOI: 10.1007/s1146801500646 (with permission for author reuse from Springer Nature). [49] W. Jacak, ‘Propagation of collective surface plasmons in linear periodic ionic structures: plasmon polariton mechanism of saltatory conduction in axons’, J. Phys. Chem. C 119(18), 10015, 2015 author (reuse in the book with permission from the American Chemical Society). [145] K. Kluczyk, C. David, J. Jacak, and W. Jacak, ‘On modeling of plasmoninduced enhancement of the efficiency of solar cells modified by metallic nanoparticles’, Nanomaterials 9, 3, 2019. DOI: 10.3390/nano9010003 (with permission from MDPI for unrestricted use and reproduction as open access publication). [159] K. Kluczyk, C. David, and W. Jacak, ‘On quantum approach to modeling of plasmon photovoltaic effect’, J. Optical Soc. America B 34, 2115, 2017 (author reuse in the book with permission from the Optical Society).
2 Physics of Metals – Preliminaries
A concise description of the theory of metals in the normal bulk state is given. The concept of Landau quasiparticles close to the Fermi surface is briefly described. A microscopic formulation of the normal Fermi liquid theory in terms of the kinetic equation and Green function approach is sketched.
2.1 Definition of a Metal Using singleelectronband Bloch theory the Schr¨odinger equation in a periodic potential can be solved. The periodicity corresponds to a crystal lattice. A periodic potential in a crystal lattice can be expressed as follows: V (r) = V (r + an ).
(2.1)
with an = n1 a1 + n2 a2 + n3 a3 , where the Bravais vectors ai , i = 1,2,3, span the elementary crystal lattice cell and an is an arbitrary lattice vector, i.e., a linear combination of the three basis vectors ai defining the unit cell, with integer coefficients ni . The choice of the vectors ai is sometimes ambiguous for a particular periodic crystal structure, which can result in different socalled Bravais webs; these are, however, equivalent [54]. The Schr¨odinger equation for an electron in a periodic crystalline potential thus attains the form h¯ 2 ∇ 2 (r) + V (r)(r) = E(r). (2.2) 2m This equation is invariant with respect to translations in the crystal lattice, and so the wave functions (r) and (r + an ) satisfy the same equation as each other.1 Hence, for nondegenerate states, −
(r + an ) = eiα(an ) (r).
(2.3)
1 Because ∇ = ∇ r r+an .
17
18
Physics of Metals – Preliminaries
In the case of degeneracy of the states for a particular energy E, a wave function with a shifted argument can be expressed as a linear combination of unshifted wave functions which span the degenerate subspace of the Hilbert space. Owing to the unitarity of the related representation one can diagonalize the coefficient matrix, obtaining phase factors as the diagonal elements, which resolves the problem to one that is analogical to the case of no degeneracy. It is easy to see that α(a1 + a2 ) = α(a1 ) + α(a2 ),
(2.4)
since the sum of lattice vectors is also a lattice vector. Next, taking into account the uniqueness of the solution of Eq. (2.4) in the form of a linear function, we get α(an ) = k · an,
(2.5)
where k is associated with the energy E of the stationary state and with the corresponding wave function; hence both Ek and k (r) are assigned by k (this mapping E → k is singlevalued, but its inverse is in general multivalued). The phase factor eik·an is invariant with respect to the translation of the vector k by an arbitrary vector of the form, km = m1 K1 + m2 K2 + m3 K3,
(2.6)
where mi are integers, and a2 × a3 , a1 · (a2 × a3 ) a3 × a2 K2 = 2π , a1 · (a2 × a3 ) a1 × a2 K3 = 2π . a1 · (a2 × a3 )
K1 = 2π
(2.7)
Indeed, we see that eik·an = ei(k+km )·an . The vectors Ki , i = 1,2,3, define the socalled reciprocal lattice for a crystal and its elementary cell is the domain for the vectors k. The vectors k forming the elementary cell of the reciprocal lattice thus enumerate the phase factors caused by translations of the wave functions in the Bravais lattice. These kvectors enumerate the stationary states of an electron in a periodic potential. There exist as many different stationary states as the kvectors that are available. The number of available kvectors in the elementary cell of the reciprocal lattice is finite, because of the discrete structure of k caused by the normalization condition for the wave functions k (r) (which is similar to that for the stationary states of a free particle with momentum p = hk, ¯ with periodic Born–Karman conditions imposed [55]).
2.1 Definition of a Metal
19
The translation properties of a stationary wave function for an electron in a crystal are thus defined by the vectors k taken from an elementary cell in the reciprocal lattice: k (r + an ) = k (r)eik·an .
(2.8)
One can rewrite the wave function as follows: k (r) = eik·r u(r) (taking advantage of the fact that eik·r = 0). By virtue of the formula (2.8) we see that u(r + an ) = u(r).
(2.9)
The periodic function u(r) is called a Bloch function and its periodicity property is referred to as the Bloch theorem. One can notice that the factor eik·r is the unnormalized eigenfunction of the momentum operator, with eigenvalue hk. ¯ Hence, one can say that the Bloch function periodically modulates the momentum states of an electron. The latter momentum states are, however, not arbitrary as for a free particle: in a crystal hk ¯ can attain only values corresponding to the kvectors from the single elementary cell of the reciprocal lattice. This difference is expressed in the term ‘pseudomomentum’ that is used for hk ¯ in a crystal rather than ‘momentum’, the term used for a free particle. The Bohr–Karman periodic conditions allowing for normalization of the wave function k (r) = eik·r u(r) confined to a box with volume V = L1 · (L2 × L3 ) (this box can be oriented along the Bravais lattice vectors ai ) are the same for the pseudomomentum as for the ordinary momentum: ki = 2πli /Li , where li are integers. Hence, one can assess the total number of kvectors in an elementary cell of a reciprocal lattice, by dividing the volume of this cell, vo = K1 · (K2 × K3 ) = (2π)3 /v (here v = a1 · (a2 × a3 ) is the volume of an elementary cell in the corresponding Bravais lattice) by the kvector density; this equals the volume of the parallelepiped falling at a single k in the Bohr–Karman discretization, (2π)3 (2π)3 = . L1 L2 L3 V The result of this division gives the number of possible kstates, N = 2V /v (the factor 2 accounts for additional possibility of two distinct orientations of the spin of an electron). One can conclude that the number of stationary states of an electron in a crystal is equal to double the number of elementary Bravais cells in the volume of the crystal sample, 2V /v. In order to better reflect a particular crystal symmetry, instead of the elementary cell in a reciprocal lattice one can select the Wigner–Seitz cell, which has the same volume as the elementary cell but is symmetrical according to the point group of the crystal. The Wigner–Seitz cell is defined by the planes perpendicular to all
20
Physics of Metals – Preliminaries
reciprocal lattice vectors that can be drawn from a selected node in this lattice, when these planes divide the lattice vectors at their centres [54]. The Wigner–Seitz cell contains a set of vectors k equivalent to those of the elementary reciprocal cell and is called the first Brillouin zone. The mapping Ek → k is usually not onetoone because the mapping k → Eki is multivalued; this is denoted by an additional index i enumerating ‘energy bands’. In each band there is the same number of different kstates – the number of states in the elementary cell of a reciprocal lattice or, equivalently, in the first Brillouin zone. This number (including spin) equals twice the number of Bravais elementary cells in the crystal sample. In each Bravais elementary cell there is the same complex of atoms with the same number of collectivized electrons. If only one electron in each Bravais cell is collectivized then we have a halffilled single band; if two electrons are collectivized in each Bravais cell then the single band is completely filled. When three electrons are collectivized per cell then one and a half bands are full in the crystal (because each state in a band may be occupied by only a single electron, since electrons are fermions). The following distinct situations are possible. The lastfilled band is separated from the next band by an energy gap, either large or small; alternatively, the succeeding bands overlap in some region of the first Brillouin zone. If the last band is completely filled and the gap to the next empty band is large then the crystal is insulating. If the gap to the next empty band is small (compared with kB T , where kB = 1.38×1023 J/K is the Boltzmann constant and T is the temperature in kelvins) then we have a semiconductor crystal. If the last band is halffilled, which happens when there is an odd number of collectivized electrons in each Bravais cell, then the crystal is a metal. In the case of an overlap between the last completely filled band and the next empty band, the crystal is a socalled semimetal [54]. Metals are thus characterized by a halffilled last band, and electrons can hop to empty kstates in this band when the crystal is subject to an external electric field. In this field the halffilled band will be reorganized in such a manner that an electric current will flow in the crystal. The related nonzero conductivity is thus a result of the specific filling of bands with electrons. In the case of a completely filled band any reorganization of the electrons, enabling a current, is blocked by the energy gap to the next empty band. A large gap blocks the current even at a strong electric field – this is an insulator. In semiconductors, where the gap is small, the temperature ‘chaos’ allows for a small proportion of the electrons in the completely filled band (called the valence band) to hop to the originally empty conduction band. This small amount of electrons at the bottom of the conduction band gives a small current if there is an applied electric field. Turning back to the case of a metal, we note that a halffilled band still contains a huge number of electrons, the number of elementary Bravais cells in the crystal
2.1 Definition of a Metal
21
sample. The latter number is of the order of Avogadro’s number (6.02 × 1023 ) for a crystal sample with mass equal to the atomic mass number (in grams) of the metal element. The Fermi sphere (the ground state in momentum space) of so huge a number of electrons has a large radius pF , the Fermi radius.2 The Fermi energy (the energy of the uppermost electrons) εF = pF2 /(2m) is typically of the order of 104 −105 K (in units where the Boltzmann constant kB = 1) and is thus much larger than room temperature or melting temperature (the melting temperature for a crystal corresponds to the thermal decomposition of the ion web; the energy of the hot electrons on the Fermi surface cannot, however, be used to melt the crystal because these electrons are not able to lose their energy since the lowerenergy states are completely filled by other electrons). The Fermi momentum and energy may thus be found from the relation (2π)3 4πpF3 = N. (2.10) 2 3 V In a metal the Fermi surface accommodates itself to the crystal isoenergy surfaces in the Brillouin zone, and only in an idealized case does it have the shape of a sphere. When the Fermi surface crosses the borders of the first Brillouin zone, it must be perpendicular to these borders (as is required by timereversal symmetry) [12]. In such a case the whole ‘Fermi ball’ spills out beyond the borders of the first Brillouin zone and partly fills the second (and then the third) Brillouin zone. The shapes of the Fermi surfaces for various crystalline symmetries are known in detail for all metals, both experimentally and theoretically [12]. Despite the fact that the true Fermi surface in a real metal is strongly deformed and complicated, the idealized isotropic spherical model is frequently helpful. The electrons in a crystal interact strongly with the background ions and with each other; thus the singleelectron gas model is a very crude approximation to a real electroninteracting Fermi liquid. Interactions also modify to some extent the picture of the Fermi surface: the sharp ideal Fermi surface at T = 0 K is blurred due to interactions, but the expressions given above for the Fermi energy and the Fermi momentum still hold (according to the Luttinger theorem [9]). The existence of a free Fermi surface beyond which are empty states in the band can be thus identified with the definition of a metal in its normal phase. Because of the large depth of the Fermi sea, greatly exceeding the temperature and energy of an applied electric or magnetic field, the majority of experimentally available
2 In the idealized spherically symmetrical case fermions fill the discrete kstates one by one starting from zero (the origin of the first Brillouin zone); the energy of an electron in the gas model is h¯ 2 (kx2 + ky2 + kz2 )/(2m)
and the ground state corresponds to a filled sphere in kspace with radius given by pF /h¯ = ( kx2 + ky2 + kz2 )F .
22
Physics of Metals – Preliminaries
thermal and galvanomagnetic phenomena in metals involve only electrons located very close to the Fermi surface. The deeply located electrons are usually passive in thermal and transport effects because their excitation requires too high an energy. An exception is provided by plasmon effects, to which all electrons contribute, including those located deep below the Fermi surface. The description of the interacting Fermi liquid of electrons in metals, including the electron–electron Coulomb interaction and the interaction of the electrons with the ion background, was the subject of intensive studies in the second half of the twentieth century. Very precise methods have been developed within the Green function approach to metals [9] (earlier investigations were in terms of the kinetic equation method [56, 57], which has been proved to be equivalent to the Green function picture [9, 10, 58]). The exceptional precision of the microscopic theory of a Fermi liquid is linked with the existence, for metals, of a small parameter expressed as the ratio of the temperature and the energy of the experimentally accessible electric and magnetic field values, with respect to the Fermi energy, large in metals. This small parameter ensures the quick convergence of all perturbation series with respect to the interaction, which results in the exceptionally high accuracy of metal models. In the case of semiconductors the Fermi energy is small and the small parameter identified above disappears; this means that the semiconductor description is less accurate and less predictable than that for metals (in semiconductors the widths of the bands and of the interband gaps are important instead) [59]. 2.2 Scheme of the Fermi Liquid Theory 2.2.1 Phenomenological Theory of a Fermi Liquid The phenomenological theory of a normal Fermi liquid,3 formulated by Landau [56, 60, 61, 13] is based on the assumption that the ground state and low lying excited states in a multiparticle Fermi liquid in its socalled normal phase may be mapped onetoone onto the welldefined Fermi surface of the gas of electrons and the excited free electrons beyond this surface, without interaction. In this way one can introduce the powerful concept of quasiparticles – excited states low lying in energy – for a strongly interacting multielectron system. The concentration of these quasiparticles can be expressed in terms of the concentration of their noninteracting partners; thus the change in concentration is δn(p) = n(p) − n0 (p). At T = 0, n0 (p) corresponds here to the sharp Fermi surface for a noninteracting electron gas (at higher temperatures the Fermi surface is blurred on the scale of kB T , as shown in Fig. 2.1). 3 Not superconducting and not magnetic.
2.2 Scheme of the Fermi Liquid Theory
23
T = 0K
T > 0K energy
Figure 2.1 Oneparticle distribution function for a fermion gas, f (ε) = 1 (the Fermi–Dirac function). For T = 0 K the chemical potential e(ε−μ)/kB T +1 μ = εF ; at temperatures T > 0 K but small in comparison to εF /kB (kB is the Boltzmann constant) the Fermi surface blurs and also μ shifts slightly [13].
Next, Landau introduced an effective Hamiltonian for quasiparticles in order to derive a kinetic equation of Boltzmann type. This effective Hamiltonian has the form εp δn(p) + Tr Tr fpp δn(p)δn(p ), (2.11) H = Tr p
p,p
s a 0 0 + fpp · σ expresses the effective interaction of quasiparwhere fpp = fpp σ σ σ ticles, additionally including the spin structure; σ 0 and σ are the unit 2 × 2 matrix and the vector of Pauli matrices, respectively, which together span the spin structure δn(p) = δns (p)σ 0 + δna (p) · σ , and εp = vF (p − pF ), vF = pF /m∗ , where m∗ is the effective mass of a quasiparticle. The singlequasiparticle energy can be thus written as ε˜ p = εp + T r p fpp δn(p ) and, assuming that the density (concentration) of quasiparticles varies in time and space, one can derive a Boltzmanntype kinetic equation, {˜ε,δn} + ∂δn/∂t = I [δn] (here {,} denotes a Poisson bracket).4 Keeping only the linear terms in the above equation, we obtain, ∂δn ∂εp ∂δn ∂ Tr p fpp δn(p ) ∂n0 + − = I [δn]. (2.12) ∂t ∂p ∂r ∂r ∂p
ˆ ˆ − εF ) (for n0 (εp ) = − pF ) = −vF pδ(ε Taking into account that ∂n0 /∂p = −pδ(p 1 − (εp − εF ), where is the Heaviside step function) and assuming that δn = ˆ for Fourier space–time components e−iω+iq·r , we get δ(ε − εF )ν(p), pF2 ˆ = pˆ · q d fpˆ pˆ ν(pˆ ), Tr (2.13) (ω − vF pˆ · q)ν(p) (2π h) ¯ 3
4 Let us note that the effective Hamiltonian for quasiparticles depends in an implicit manner on the temperature
via the temperaturedependent quasiparticle density – thus this Hamiltonian is of a phenomenological, not a microscopic, character.
24
Physics of Metals – Preliminaries
where d = sin d dφ is the differential in spherical coordinates;5 the collision integral, on the righthand side of Eq. (2.12), does not contribute in the case ωτ
1, where τ ∼ T −2 is the mean intercollision time for quasiparticles, since the damping of quasiparticles is proportional to square of the separation from the Fermi surface and is zero on the Fermi surface itself [13]. The kinetic equation for quasiparticles in metals (2.13), called the Landau kinetic equation, allows the identification of the energy ω(q) of the socalled zeroth sound, of spin waves, and of Landau damping as well as the expression of parameters for these effects in terms of Landau amplitudes, i.e., the coefficients in the decomposition of fpˆs(a) pˆ (see the text below Eq. (2.11)). In the isotropic case this function depends only on the angle between the versors pˆ and pˆ , which admits the following decomposition in the Legendre polynomial basis: s(a) Pl (pˆ · pˆ ). The coefficients in this decomposition of the fpˆs(a) l (2l + 1)fl pˆ = quasiparticle interaction are the Landau amplitudes. Utilizing the definition of the group velocity, v = ∂ ε˜ /∂p, one can express the total flow of the quasiparticle mass (taking into account that the number of quasiparticles agrees with the number of bare noninteracting electrons) as follows: d 3p ∂ ε˜ d 3p n(p)p = m n(p) . (2.14) 3 3 (2π h) (2π h) ∂p ¯ ¯ Using the expression for the quasiparticle energy (see the paragraph after (2.11)) one can rewrite the change in flow induced by a variation δn of the quasiparticle density (taking the variation of both sides of Eq. (2.14)): p ∂ε(p) d 3p d 3p δn(p) δn = 3 3 (2π h) m (2π h) ∂p ¯ ¯ (2.15) 3 d p d 3p ∂ + Tr Tr fpp n(p)δn(p ). (2π h) (2π h) ¯ 3 ¯ 3 ∂p Now using integration by parts in the second term on the righthand side, and exchanging in this term the notations p and p , we finally obtain d 3p p ∂ε(p) d 3p δn δn = 3 3 (2π h) m (2π h) ∂p ¯ ¯ (2.16) 3 ∂ d p d 3p fpp n(p )δn(p). − Tr Tr (2π h) (2π h) ∂p ¯ 3 ¯ 3 Owing to the arbitrariness of δn(p) we get p d 3 p ∂n(p ) ∂ε(p) f . = − Tr Tr pp m ∂p (2π h) ∂p ¯ 3 5 The reader should note that here refers to a spherical coordinate.
(2.17)
2.2 Scheme of the Fermi Liquid Theory
ˆ For n(p) = 1 − (p − pF ), we have ∂n/∂p = −pδ(p − pF ); thus 1 pF 1 d f s (cos ϑ) cos ϑ, = ∗+ m m (2π h) ¯ 3
25
(2.18)
giving for the effective mass m∗ = m(1 + F1 ).
(2.19)
Here we employed decomposition in the Legendre polynomial basis, f s (cos ϑ) = s l (2l + 1)Pl (cos ϑ)fl and 1 pF m ∗ s d Fl = fl . Pl (cos ϑ) cos ϑ = δl,1, 4π 2l + 1 2π 2 h¯ 3 The Landau kinetic equation (2.13) allows analysis of the collective excitations in a normal Fermi liquid. For spinless excitations (when δn does not depend on the spin) the kinetic equation (2.13) can be rewritten in the form d ˆ = k · v F (ϑ)ν(pˆ ) , (2.20) (ω − k · v)ν(p) 4π where Tr f = (2π 2 h¯ 3 /(pF m∗ ))F (pˆ · pˆ ). Using the notation s = (ω/(vF k)) we obtain d (s − cos )ν(,ϕ) = cos (2.21) F (cos ϑ)ν(,ϕ ). 4π The above equation can be solved for specific forms of F (cos ϑ), where cos ϑ = pˆ · pˆ . For F = F0 = const., owing to the absence of any dependence on the angle ϑ under the integral, we get ν = const. ×
cos , s − cos
and substitution into (2.21) gives F0 π cos sin d = 1. 2 0 s − cos
(2.22)
(2.23)
After integrating we obtain s s+1 1 . ln −1= 2 s−1 F0
(2.24)
This equation has a real solution for s, i.e., for the zero sound velocity, when F0 > 0. For −1 < F0 < 0 the solution is complex and corresponds to damping – the socalled Landau damping. For F0 ≤ −1 the complex solution is unstable; the normal Fermi liquid loses its stability as the ground state of interacting fermions (this instability was described by Pomeranchuck [62]). The sound identified above
26
Physics of Metals – Preliminaries
as a spinless collective mode arising from the interaction of Landau quasiparticles is called the ‘zero sound’. The zero sound corresponds to oscillations or deformations of the quasiparticle density on the Fermi surface without any change in the volume of the Fermi sphere – thus without any density fluctuation in position space. This is the difference from ordinary acoustic sound, which corresponds to fluctuations of the density in position space and is linked with oscillations of the Fermi sphere size (the Fermi sphere radius depends on the particle density). The zero sound is a collective excitation which can propagate in a Fermi liquid even at T = 0 K, whereas ordinary sound does not propagate at zero temperature (at zero temperature, phonons, the carriers of ordinary sound, disappear). In analogy to the zero sound in the Fermi liquid, spin waves corresponding to fluctuations of the spin part of the quasiparticle density on the Fermi surface may also occur; the velocity of spin waves is governed by the spin part of the Landau interaction function [10, 9, 13]. The Landau theory of the normal Fermi liquid, though based on phenomenological assumptions, agrees very well with experimental observations of electrons in metals (some generalizations towards inclusion of the Coulomb interaction and its screening by positive ion background in a crystalline lattice were developed by Silin [57]). The most important aspect of the Landau theory is the introduction of quasiparticles and of their effective interaction, expressed by the Landau function and different from the Coulomb interaction of electron charges, the latter interaction having been largely included in the definition of quasiparticles. The notion of quasiparticles and their effective interaction found complete confirmation in the microscopic theory of the normal Fermi liquid, which was developed next. Worth emphasizing is the fact that the Landau theory of quasiparticles is not of a perturbation character and thus is applicable for strongly interacting electron systems, such as electrons in metals. The confirmation of this theory using Green function formalism requires the exact summation of an infinite perturbation series and thus is independent of the perturbation scheme and demonstrates in detail the structure of quasiparticles and their effective interaction [58, 9, 63, 64]. It is surprising that electrons in metals are quasiparticles on the Fermi surface and are actually different from ordinary free electrons (they also have a different effective mass). These quasiparticles interact residually in a way that is quite distinct from that of strongly interacting ordinary electrons. The quasiparticle picture in metals agrees perfectly with experiment. 2.2.2 Outline of the Microscopic Theory of a Normal Fermi Liquid The fundamental assumption of the Fermi liquid theory is the existence of a welldefined Fermi surface for noninteracting fermions at T = 0 K. The interaction can
2.2 Scheme of the Fermi Liquid Theory
27
Figure 2.2 Graphical presentation of the Dyson equation. The mass operator is built from all multiline graphs which cannot be cut across a single line; the thin lines represent the zeroth (bare – without interaction) Matsubara Green functions; the thick lines represent the full Matsubara Green functions with the interaction included.
be switched on via a mass operator and vertex functions conveniently expressed in terms of Matsubara Green functions (of imaginary time) [9, 11]. Next, assuming that the mass operator is a continuous and smooth, i.e., differentiable, function of its own parameters (momentum and energy or the Matsubara frequency after an analytical continuation) near the Fermi surface, a socalled ‘normal’ metal can be defined. With the above conditions one can develop the mass operator up to linear terms (the imaginary part of the mass operator is of second order in the momentum with respect to the Fermi surface). Such a development of the mass operator allows for the definition of Landau quasiparticles as poles of a retarded singleparticle Green function. Poles of a twoparticle retarded Green function define collective excitations: the zero sound and spin waves. An important achievement of the microscopic Fermi liquid theory is the expression of the Landau amplitudes (the Legendre components of the quasiparticle interaction, in the isotropic case) as an appropriate limit of the vertex function for Matsubara Green functions. The advantage of the Matsubara functions is the inclusion of zero and nonzero temperatures simultaneously in the same formalism. The mass operator is defined by the Dyson equation for the Matsubara Green function (see Fig. 2.2), G(k,iων ) = G 0 (k,iων ) + G 0 (k,iων )(k,iων )G(k,iων ).
(2.25)
Then (taking into account that G 0 = 1/(iων − εk ), εk = p2 /2m − μ, where μ is the chemical potential and p = h¯ k; iων is the Masubara frequency), G(k,iων ) =
1 , iων − εk − (k,iων )
(2.26)
or after analytical continuation of the discrete imaginary Matsubara frequency onto the whole complex plane (iων → E), G(k,E) =
1 , E − εk − (k,E)
E = Re E + i Im E.
(2.27)
The above function is the Fourier transform of the retarded or advanced Green function (correspondingly to sign of the pole) [10] and its pole defines the
28
Physics of Metals – Preliminaries
quasiparticles in the system with interactions. The real part of the pole defines the energy of the quasiparticle whereas the imaginary part defines the quasiparticle lifetime (the lifetime of the quasiparticle arises owing to the scattering of interacting bare particles). The imaginary part of the pole equals the imaginary part of the mass operator. Hence, when the mass operator is real according to some approximation, the quasiparticles are stable under this approximation. This is the case for a normal Fermi liquid, where the mass operator is real in the vicinity of the Fermi surface in an approximation that is linear with respect to the distance from the Fermi surface (the Fermi surface is defined here for a system without interactions at T = 0 K) [9]. Upon assuming the continuity of the derivative of the mass operator near the Fermi surface, we have (k,iων ) = (pF ,0) +
∂ ∂ (p ,0 )iων , (pF ,0) (p − pF ) + ∂p ∂iων F
pF2 2m (from the Luttinger theorem, the relation between the Fermi momentum pF and the particle density is not perturbed by interactions [9]). Then a G(p,iων ) = , (2.28) iων − vF (p − pF ) μ − (pF ,0) =
where the residuum,
∂ (p ,0) a = 1− ∂iων F and
−1
pF pF ∂ + (p ,0) . vF = ∗ = a m m ∂p F
The analytical properties of retarded and advanced Green functions (related to their analytical continuation (2.28)) justify the definition of the quasiparticle energy in the form εp = vF p − pF  both for p > pF and for p < pF . Derivatives of the mass operator can be expressed, utilizing the Ward identities [9], via the vertex function corresponding to the sum of the ladder graphs in the particle–hole channel (with oppositely directed Green functions). The integral kernel related to this ladder sum has the form (k · q/(ω − k · q)), where ω and k are the energy and momentum transfer at scattering. One notices that the longwave limit at ω = 0 is equal to −1, whereas it is 0 at ω = 0, which gives rise to the introduction of limits of the vertex function: k when k → 0, ω = 0, and ω when k → 0,ω = 0, respectively. The interaction of the Landau quasiparticles is expressed via a 2 ω [9]. Hence, one can find the effective mass, using the quasiparticle interaction function.
2.2 Scheme of the Fermi Liquid Theory
=
29
+
+
Figure 2.3 The twoparticle Green function can be expressed on an effective vertex.
=
+
Figure 2.4 For the twoparticle interaction (the open square, i.e., the bare interaction vertex) the mass operator satisfies the equation in the figure, which follows from the fact that the two ends of the mass operator belong either to one bare vertex or to two distinct bare vertices. In the latter case one bare vertex must be substituted by a full vertex (all lines in the figure are full Green functions).
Simultaneously the constant a (the numerator in Eq. (2.28)), which gives the jump in the singleparticle distribution function for particles, rather than quasiparticles [10], on the Fermi surface at T = 0 K, disappears from the formalism (it has entered the definition of the Landau interaction). This jump a is caused by the presence of interactions (without interactions a = 1; in the presence of interactions a < 1). The vertex function is linked with the twoparticle Green function, as shown in Fig. 2.3, where the lines represent Matsubara Green functions that are diagonal in the indices ki = (iωi ,pi ), i.e., they are diagonal in the Matsubara frequency and momentum as in a space–time translationally invariant system. The mass operator satisfies the equation in Fig. 2.4, where the solid lines represent the Matsubara Green functions and the open square is the bare interaction whereas the shaded square is the full vertex (the vertex function). The equation for the vertex function cannot be written in terms of the bare interaction (the bare vertex) in the form of a ladder sum because the repeating element of a pair of Green functions may be of two types in general. The two Green functions in a repeating pair may be oriented in parallel (the particle–particle scattering channel) or in opposite directions (the particle–hole channel). In the latter case the Green functions may differ slightly in fourmomentum (energy and momentum) and either Green function may depend on the fourmomentum of the vertex function. Hence, as a result we are dealing with three different types of repeating ladders; see Fig. 2.5. Each of these three channels leads to a different Bethe–Salpeter equation for the appropriate part of the vertex function with the irreducible vertex function accommodated to each scattering channel. For antiparallel Green functions with a small fourmomentum transfer, the Bethe–Salpeter equation has the form shown in
30
Physics of Metals – Preliminaries
Figure 2.5 Various channels for scattering in the ladder structure of the full vertex; if the Green functions linking vertices are oriented in the same way, the channel is of the particle–particle type, but when these Green functions are in opposite directions, the channel is of the particle–hole type.
P1
...
+
+
P2  K
P1
+
= P1 + K
P2
P1 + K
P1
P2  K
P2
Q
P2  K
Q+K
P1 + K
P2
Figure 2.6 (Upper) The scheme of the ladder structure which leads to an equation of the Bethe–Salpeter type. Each scatttering type (as shown in Fig. 2.5) leads to a distinct Bethe–Salpeter equation for the full vertex (filled square) with different irreducible vertices (hatched square) associated with the distinct scattering channel. (Lower) The Bethe–Salpeter equation for the particle–hole channel with the small fourmomentum transfer allows for a description of the Landau Fermi liquid in the normal phase.
Fig. 2.6. This channel and the corresponding equation is of particular significance because the kernel of the integral equation for this channel is nonanalytical, which manifests itself in collective excitations in the normal Fermi liquid: the zero sound, spin waves, and Landau damping – the same effects as are described by the phenomenological Landau kinetic equation, as presented above. The particle–particle channel, however, leads to a different phenomenon – an instability of the normal Fermi liquid to the coherent scattering of particle pairs. This instability is assigned by a pole whose imaginary part agrees in sign with the bare interaction. For bareparticle attraction the normal Fermi liquid is thus unstable against the formation of Cooper pairs, resulting in another ground state – the superfluid or superconducting
2.2 Scheme of the Fermi Liquid Theory
31
Fermi liquid (for uncharged or charged carriers, respectively, e.g., He3 atoms or electrons in metal). The third channel (again of the electron–hole type) is not assigned by any singularity. The particle–hole channel with a small transfer of fourmomentum can be taken in two different limits (as the kernel is nonanalytical), k → 0 at ω = 0 or ω → 0 at k = 0. The former is denoted the k limit and the latter as the ω limit. Correspondingly, appropriate limits can be defined for the vertex function. Taking into account the form of the integral kernel in this channel for small transfers of the fourmomentum k = (k,ω), we obtain 2πia 2 vF qˆ · k δ(ε)δ(q − qF ) + ϕreg, vF ω − vF qˆ · k
(2.29)
where q = (ε,q) and ϕreg is the regular part of the product of two antiparallel Green functions in this channel,6 one can write the k and ω limits of the Bethe–Salpeter equation (Fig. 2.6): ω = k=0 − i dqk=0 ϕreg ω, (2.30) and
k = k=0 − i
2πia 2 dqk=0 − δ(ε)δ(q − pF ) + ϕreg k . vF
(2.31)
Equation (2.30) together with the initial Bethe–Salpeter equation can be rewritten in the following form (eliminating the irreducible vertex k=0 ): vF qˆ · k a 2 pF2 d q ω (2.32) = ω + 3 (2π) vF ω − vF qˆ · k or, in a more developed way, as ω αβ,γ δ (p1,p2,k) = αβ,γ δ (p1,p2 ) a 2 pF2 vF qˆ · k ω + d q αν,γ νβ,μδ (q,p2 ); μ (p1,q) 3 (2π) vF ω − vF qˆ · k (2.33)
here p2 and β,δ play the role of parameters only and the essential dependence is ˆ in the integral over direction, i.e., (pˆ 1,k), or (q,k) αβ,γ δ (p1,p2,k) = χαγ (p1,k)χβδ (p2,k)
6 For nonzero temperatures, Matsubara Green function integration over the fourvector is substituted by
summation over the Matsubara frequency and integration over the momentum [9, 10].
32
Physics of Metals – Preliminaries
and the second factor appears on both sides of (2.32). Next, one can rewrite Eq. (2.32) in the following form, suitable for determination of the poles of the vertex function: a 2 pF2 ω ˆ ˆ 1, q)ν ˆ ηξ (q,k). ˆ pˆ · k1 d q αξ (2.34) (ω − vF p · k1 )ναγ (pˆ 1,k) = ;γ η (p (2π)3 The following notation has been introduced above: ναγ (pˆ 1,k) =
pˆ 1 · k χαγ (p1,k). ω − vF pˆ 1 · k
Moreover, ω has been omitted – this function does not depend on k and is small in comparison with , which is large close to the singularity at a pole. The poles of the vertex function are simultaneously poles of the twoparticle Green function [9, 11], which, owing to the linear response theory of Kubo, defines a collective excitation via its singularities. Equation (2.34), as derived in the manner presented above, is identical (on setting h¯ = 1) with the Landau kinetic equation, the Landau quasiparticle interaction being given by a 2 ω . This is a central result of the microscopic Fermi liquid theory – the proof that the phenomenological Landau interaction of quasiparticles is the vertex function ω a 2 and the Landau kinetic equation is in fact the Bethe–Salpeter equation in the particle–hole channel for laddertype coherent scattering. Factoring out the residuum a through identities for the derivatives of the mass operator, which in fact result from conservation rules in the system (and called Ward identities), we arrive at a complete derivation, in a microscopic manner, of the previously formulated phenomenological theory of a Fermi liquid, with the heuristic concept of quasiparticles near the Fermi surface instead of the original electrons. The microscopic Green function theory is accurate and confirms the validity of the quasiparticle concept independently of the interaction strength, though it is limited to the socalled normal Fermi liquid7 and has the proviso that the interaction is of finite range (which is true for the Coulomb interaction of electrons screened by a positive ion background, as is the case for metals). Electrons in a normal Fermi liquid are identified with quasiparticles that are well defined near the Fermi surface and stable on it. The strong interaction of electrons screened by the ion background in metals is included in the definition of the quasiparticles; they are dressed with this interaction although some residual interaction between quasiparticles still exists. Via this residual interaction the effective mass of the quasiparticles and the characteristics of collective excitations are expressed (the zero sound and spin wave velocities). The effective mass is renormalized by the first 7 The theory of a normal Fermi liquid can be generalized to the cases of a superfluid or magnetic Fermi liquid
[9, 11, 10].
2.2 Scheme of the Fermi Liquid Theory
33
Landau amplitude of this interaction (in the isotropic case): m∗ = m(1 + F1 ). It can be found experimentally from the heat capacity of the metal (its electron part can be distinguished from the ionic part by their specific temperature dependences [12]). In a normal Fermi liquid the notion of the Fermi surface is utilized, although it is accurately defined for a fermion gas only. In an interacting system the Fermi surface for the original fermions is fuzzy. Nevertheless, a Fermi surface that is still well defined holds for quasiparticles. This Fermi surface is a map of the Fermi surface in a gas and the quasiparticles near this ground state are numbered by the lowenergy excitations in the gas [10]. Such a picture is general and can be applied to electrons in metals or to other fermionic systems. Quasiparticles are thus the original particles, dressed with the interaction. Their residual interaction is weak, which explains the common approximate picture of electrons in metals as free particles, despite their strong interaction as charged particles. The Fermi surface in gas is correctly defined at T = 0 K. With increasing temperature the Fermi surface blurs. For T εF this blurring is relatively small and the Fermi surface picture may be maintained (in metals εF is large, ∼ 104 −105 K, hence the Fermi surface picture is quite accurate even up to the melting temperature). Quasiparticles are stable states only on the Fermi surface, but when their distance from the Fermi surface increases, they become damped in proportion to (p − pF )2 [65, 66]. In the case of transport phenomena in metals, the related energies of excitations beyond the Fermi surface are small in comparison with the Fermi energy, and in practice the whole of the galvanomagnetic physics in metals takes place on the Fermi surface [12]. Thus, in related effects, only a relatively small fraction of electrons participate – those on the Fermi surface (the rest are hidden below the Fermi surface and are inactive). That there is a relatively small amount of active electrons in metals explains the experimentally observed values of the conductivity and other observed kinetic characteristics of metals, which could not be properly understood if all the electrons participated [12]. For other than a normal Fermi liquid, different collective states of fermions are also observed. They are superfluid or superconducting states and magnetic states. For these cases also, accurate microscopic descriptions are available. With regard to a superfluid or superconducting Fermi liquid (the latter for charged fermions such as electrons and the former for neutral fermions such as He3 atoms), we are dealing with a specific reorganization of the Fermi surface due to the instability of coherent scattering in the particle–particle channel. This instability occurs as an imaginary pole of the vertex function in the particle–particle channel at temperatures lower than the critical temperature and for attracting fermions, indicating another ground state. This new ground state of interacting fermions corresponds to the pairing of particles (as for the particle–particle channel) and must be defined beyond the normal Fermi liquid paradigm. The new state is of an emergent character, as is always the case for spontaneously broken symmetries. Here the gauge symmetry
34
Physics of Metals – Preliminaries
of the Hamiltonian of interacting (attracting) fermions breaks down. Despite the gauge symmetry of the Hamiltonian and the related particle number conservation, a ground state of the superfluid or superconducting type is not gauge invariant – the nonzero density of Cooper pairs (pairs of fermions on the Fermi surface with opposite momenta) cannot be present for a gauge invariant Hamiltonian and occurs via a spontaneous symmetry breaking and simultaneous locking of the wave function’s phase. For a wave function with fixed phase the particle number is not determined, owing to the appropriate uncertainty principle. The fixed phase corresponds, however, to a fixed inertial reference system in which the Cooper pairs flow without any resistance and thus are superfluid or superconducting. The pairs of fermions constitute bosons, which can all condense into the same singleparticle ground state at T = 0 K. If this state is of zero energy and zero momentum then it is impossible to determine the number of particles in the condensate. Hence, it is by virtue of the particlenumber–phase uncertainty principle that the phase is fixed, and this means that the reference frame is selected by quantum rules. In this system we are dealing with a superflow or supercurrent, respectively, without viscosity or resistance, unless we consider that the particles are excited to higher levels at higher temperatures (beyond the critical temperature). The pairs of fermions have an associated spin structure. Two 1/2 spins can be added to achieve a total spin of 0 (the singlet state) or 1 (the triplet state). Both situations are observed in experiments – in superconductors in metals the Cooper pairs are usually in a singlet spin state, whereas for superfluid He3 triplet pairs are present. A precise microscopic description of a Fermi liquid in the superfluid or superconducting phase has been developed [9, 10], though a simultaneous laddertype sum in the particle–hole and particle–particle scattering channels is technically nontrivial. The stability of the superfluid or superconducting state depends, however, on the quasiparticle interaction [65]. Gauge invariance breaking in the superfluid phase requires the inclusion, in terms of Green functions, of an anomalous type of Green function representing the Cooper pair condensate. Such a formalism has been developed both for a singlet Bardeen–Cooper–Schrieffer (BCS) superfluid [67] and for a triplet superfluid [68, 69]. The phenomena sketched above occur close to the Fermi surface in metals and do not exhaust the physics of these systems. In the energy scale exceeding the Fermi energy the picture of quasiparticles near the Fermi surface is irrelevant, but electrons may take part in the response to such energetic perturbations. This is the case for plasmons, which can be excited in metals by highenergy photons (typically of UV radiation type for bulk metals). The description of plasmons needs an approach different from the standard Fermi liquid model; this will be presented in what follows.
3 Quasiclassical Description of Plasmons in the Bulk Metal
The random phase approximation (RPA) theory of plasmons in bulk metals of Pines and Bohm is described. Details of the derivation are included. The role of the electron–electron interaction for coherent plasmon excitations of electrons in metal is emphasized; this interaction is essential for plasmon formation, indicating that plasmons do not exist in gaseous systems (in which there is no interaction). The screening of unbalanced charges by the electrons in a normal metal is briefly presented alongside the Thomas–Fermi scheme.
3.1 Random Phase Approximation Theory of Plasmons of Pines and Bohm Plasmons are fluctuations in the local electron density on the background of an inertial positive ion distribution. In order to describe the electron liquid oscillations corresponding to charge density fluctuations one considers a Hamiltonian for N electrons interacting with each other and with the positive ions, the oscillations of which can be neglected owing to their much greater mass in comparison with that of electrons. Thus the system of ions can be accounted for as a static positive ‘jellium’, i.e., a uniform positively charged background balancing the total charge of the electrons. The electronic part of this Hamiltonian can be written as H =
p2 e2 1 i + , 2m 2 i=j ri − rj  i
(3.1)
where m and e are the electron mass and charge, respectively. The fluctuations in the electron density can be represented as follows: δ(r − ri ) = ρk eik·r, (3.2) ρ(r) = i
k
where ρ(r) is the electron density at the point r, whereas the Fourier components ρk , given in (3.3) below, represent particular fluctuations of the electron density
35
36
Quasiclassical Description of Plasmons in the Bulk Metal
with respect to the uniform distribution ρ0 = N . It should be emphasized that the definition (3.2) carries a quasiclassical image of the electron system with defined positions ri of particles which in a fully quantum sense can only be referred to as variables (coordinates) of the multiparticle wave function (r1, . . . ,rN ). It is easy to see that e−ik·ri , (3.3) ρk =
i
which follows from the equality k eik·(r−ri ) = δ(r − ri ) (we assume here that the system volume V = 1). From the above it can be seen that, indeed ρ0 = i 1 = N . The Hamiltonian (3.1) may be rewritten in the following form:1 H =
p2 V k
i ρk+ ρk − N , + 2m 2 i k
(3.4)
where Vk = 4πe2 /k 2 is the Fourier transform of the Coulomb potential and the superscript ‘plus’ means the hermitian conjugate. The prime on the sum indicates that the component with k = 0 is omitted here, which corresponds to the cancellation of the uniform jellium and the uniform electron distribution with k = 0, i.e., ρ0 . It means that the uniform jellium has no impact on the electron fluctuations for k = 0. For the electron density fluctuations one can write out dynamic equation in the Heisenberg representation: ρ˙k =
1 [ρk,H ], i h¯
(3.5)
where the brackets indicate the commutator of ρk and H .
1 Here we employ the following calculation:
1 e2 e2 1 = d 3 r1 d 3 r2 δ(r1 − ri )δ(r2 − rj ) 2 ri − rj  2 r1 − r2  i=j
i=j
=
ik ·(r −r ) e2 1 eik1 ·(r1 −ri ) e 2 2 j d 3 r1 d 3 r2 2 r1 − r2  i=j
k1
k2
(for Dirac function representation, V = 1 is assumed). One can change variables to r1 = R + r/2, r2 = R − r/2 (the Jacobian for this variables change is equal to 1). The integral with respect to d 3 R gives δk1,−k2 . The sum over k2 can be thus performed and one can change indices so that k1 → k. Taking into account that k 2 φk = 4π q (the Fourier version of the Poisson equation, i.e., the first Maxwell equation for a pointlike charge q, div(−grad φ) = 4π qδ(r), in Gauss units), we arrive finally at an expression with only one sum over k. The sums over i = j of e±ik·ri(j ) give ρk+ ρk − N (N must be subtracted because the sum is over i = j ) multiplied by the Fourier transform of the Coulomb potential, e2 4π/k 2 , after performing the integration with respect to d 3 r.
3.1 Random Phase Approximation Theory of Plasmons of Pines and Bohm
For the Hamiltonian (3.4) we obtain2 hk k · pi ¯ 2 −ik·ri . − ρ˙k = i e + m 2m i
37
(3.6)
When looking for the secondorder derivative of the local electron density in the Heisenberg representation, a subsequent commutator, [ρ˙k,H ], has to be found. The result is3 2 4πe2 hk k · pi ¯ 2 ρ¨k = − e−ik·ri − − k · q ρk−q ρq . (3.7) + 2 m 2m mq q i 2 In the calculation of the commutator in (3.5) we take into account that
⎡ [ρk,H ] = ⎣ρk,
−h¯ 2 ∇j2 2m ⎛
j
= h¯ 2
j
− h¯ 2
⎤ ⎦
∇j · ⎝(−ik)e
−ik·rj
/2m +
⎞ e−ik·ri ∇j /2m⎠
i
e−ik·ri ∇j2 /2m,
i,j
which gives [ρk,H ] = −
−ik·r j e j
h¯ k · (−i h∇ h¯ 2 k 2 ¯ j) − 2m m
.
3 In the calculation of this subsequent commutator one must take into account that the operator ∇ acts on the j
position of the j th particle, rj ; in the case of the commutator [ρ˙k,H ] this operator is present both in ρ˙k (see Eq. (3.6)) and in H (in the former commutator (3.5) the operator ∇j is not present in ρk ). Hence, the first term on the righthand side of Eq. (3.7) is obtained as the result of the action of ∇j on the kinetic energy term in the
Hamiltonian and gives the square of the expression, i − k · (−i h∇ ¯ i )/m + hk ¯ 2 /2m , the same as in Eq. (3.6), but here divided by i h. ¯ The second term on the righthand side of Eq. (3.7) results from the commutator of ρ˙k with the interaction term in the Hamiltonian, i.e., ⎡ ⎤ e2 2π k · (−i h∇ ) ¯ i −ik·r + i ⎣−i e ρ q ρq ⎦ , q q2 m i ⎤ ⎡ e2 2π iq·r k · (−i h∇ ) ¯ i −ik·r −iq·r i l⎦. e e j e , = ⎣−i q q2 m i
j
l
This can be rewritten in the form
⎛ ⎞ e2 2π iq·r −ik·r iq·r −iq·r −iq·r j i i l i ⎝ ⎠. k · (iq)e e −h¯ e + e k · (−iq)e q q2m i
l
Changing the sign of q in the sum in the second term we get e2 4π k · qρk−q ρq . q mq 2
−i h¯
j
38
Quasiclassical Description of Plasmons in the Bulk Metal
The first term on the righthand side of the equation represents the contribution of the kinetic energy of the particles, whereas the second term is linked with the particle interaction. Let us rewrite the equation and shift the last term, taken for k = q, to the lefthand side of the equation (for k = q, the large factor ρ0 = N occurs in this term), which gives the formula [14–16], ρ¨k +
ωp2 ρk
=−
i
e
−ik·ri
hk k · pi ¯ 2 − + m 2m
2 −
4πe2 q=k
mq 2
q · k ρk−q ρq,
(3.8)
1/2 is the plasmon frequency of the electron gas (in Gauss where ωp = 4πne2 /m units). If one sets the righthand side of Eq. (3.8) to zero, it can be seen that the equation then describes, for each Fourier component ρk , harmonic oscillations at the frequency ωp . One can assess when it is possible to neglect the righthand side of Eq. (3.8) as follows. The first term on the righthand side is of order k 2 v02 ρk , where v0 is the Fermi velocity (v0 = pF /m∗ ). The second term contains the product of two fluctuations in the local electron density that have nonzero momenta (i.e., wave vectors). Because the positions ri of the electrons are random (and arbitrary), it follows that ρq=0 = i e−iq·ri is small (for a translationally invariant system, the expected value ρq=0 should be zero). Therefore this term, with the product of two such small quantities, may be omitted in the linear approximation – this is the random phase approximation (RPA) [16]. The random contributions of the phase factors e−iq·ri cancel out in the sum for q = 0, in contrast with the coherent sum for q = 0 (this property in fact reflects the behaviour of the Dirac delta function when represented as the integral of an exponential factor). Neglecting the first term on the righthand side of Eq. (3.8) is formally equivalent to taking the longwave oscillation limit k → 0. In this limit one can imagine a uniform oscillating shift of the whole electron liquid with respect to the static jellium – in this case the oscillations have the plasmon frequency ωp . For nonzero k, the kinetic energy contribution should be taken into account; this leads to a dispersion of the plasmon oscillations that is quadratic in k. One can assess that the kineticterm contribution will be small when k 2 v02 /ωp2 1, i.e., for k ωp /v0 . For small k the kinetic term does not play an important role, and in the system in question the coherent plasmon oscillating excitation dominates. In the opposite case, for large k, the kinetic energy dominates and this leads to individual excitations of the electrons. For free electron concentrations n ∼ 1023 /cm3 that are typical for metals, one obtains ωp ∼ 1016 /s, and so the energy of plasmon oscillations attains very high values, h¯ ωp ∼ 12 eV (even higher than the Fermi energy, which indicates that in plasmon oscillations all electrons take part, not just those close to the Fermi
3.2 Screening of the Coulomb Interaction in Metals
39
surface). If it were possible to excite a plasmon h¯ ωp by a single electron (i.e., a quasiparticle) with momentum h¯ k then, by virtue of energy and momentum conservation, p2 (p − h¯ k)2 − = h¯ ωp . 2m 2m
(3.9)
Because p ≤ p0 (where p0 is the Fermi momentum), for small k this process is impossible as h¯ ωp > εF (it is impossible to excite a plasmon by a single electron close to the Fermi surface; the excitations close to the Fermi surface, i.e., the Landau quasiparticles, do not interact directly with plasmons owing to the large energy incommensurability). Thermal fluctuations in the metal, which are close to the Fermi surface in energy, also do not interact with plasmons. One might suppose that plasmon excitations have a similar character to sound waves. Nevertheless, while for sound waves it is crucial that there are many scatterings on the scale of the sound period, ωτ 1 where τ is the scattering time rate, for plasmons, which are coherent fluctuations of all the electrons, collisions are harmful (they lead to the damping of plasmons); hence for plasmons the inverse inequality, ωτ ≥ 1, is required. 3.2 Screening of the Coulomb Interaction in Metals The electric interaction of charges of the electron and ion charges in metals reflects two important aspects of these systems; the high density of electrons, of the order of the Avogadro number per cm3 , with the same density of ion charges; and the high mobility of the light electron liquid in comparison to the massive and thus inertial positive ions. To consider the problem of screening by the electron fluid of some uncompensated positive charge q located at point r0 , one must solve the Poisson equation (i.e., the first Maxwell equation), div(−∇ψ(r)) = −ψ(r) = 4πqδ(r − r0 ) − 4πeδρ(r),
(3.10)
taking into account the presence of the charge q and of a screening electron cloud δρ(r) (for the sake of simplicity we can choose r0 = 0). Upon the assumption that local changes in the electron density are small on the scale of the interatomic distance one can reasonably expect that such small changes do not cause local changes in the Fermi energy. The local Fermi energy (or Fermi momentum) will equal the constant Fermi energy shifted by the potential ψ(r), i.e., h¯ 2 kF2 = εF + eψ(r), 2m
(3.11)
40
Quasiclassical Description of Plasmons in the Bulk Metal
where εF is the Fermi energy in the absence of the charge q. Taking into account the relation between the local density of electrons ρ(r) and the local Fermi momentum, one can write 3/2 2m 1 (kF (r))3 = (εF + eψ(r)) , (3.12) ρ(r) = n + δρ(r) = 3π 2 3π 2 h¯ 2 where n is the mean electron density. Provided that eψ(r)/εF 1, one can linearize Eq. (3.12) with respect to this small parameter, which gives the formula 3 eψ(r) . δρ(r) = n 2 εF
(3.13)
If one now substitutes Eq. (3.13) into Eq. (3.10), one obtains the Poisson equation in the form 6πne2 ψ(r) = −4πqδ(r). (3.14) − εF The Fourier transform of the above equation is 6πne2 2 −k − ψk = −4πq. εF
(3.15)
Hence, ψk =
4πq , k 2 + kT2 F
(3.16)
where kT F = 6πne2 /εF is the Thomas–Fermi wave vector [70, 16]. The reverse Fourier transform of the expression (3.16) determines the potential originating from the charge q and screened by the electron fluid. This potential has the form q (3.17) ψ(r) = e−kT F r . r Thus, the screening of the charge q takes place on a spatial scale 1/kT F , which for metals (where n is of the order of 1023 /cm3 and εF ∼ 10 eV) is comparable with the interatomic separation. Therefore the screening in metals is very effective, which, on the other hand, supports the accuracy of the jellium model.
4 Plasmon Excitations in NanometreSized Metallic Particles
This chapter presents the random phase approximation for plasmons in the case of finite nanometresized metallic particle. The calculation details are presented for a spherically symmetric particle. The stiff jellium defining the shape of a nanoparticle is accounted for in an explicit manner. The dynamic RPA equations for surface and volume plasmons in a metallic nanoparticle are derived and solved, resulting in the determination of the frequencies of the corresponding plasmon modes.
In the case of a metallic particle the problem of plasmon excitations is more complicated than in the bulk metal because of the presence of a particle surface. The lower the size of the particle, the more important is the role of its surface (the surface scales as a 2 , where a is the radius of the particle, whereas the volume scales as a 3 , and so for small values of a surface effects start to dominate).1 In the case of a finitesized metallic particle, the positive jellium can be assumed to be a uniform distribution of positive charge whose shape and volume coincide with those of the particle. For a spherical particle with radius a this jellium can be defined by the distribution function n(r) = n(a − r),
(4.1)
where n is the equilibrium positive charge density, n = ρZ (ρ is the number of ions per unit volume and Z is the ionization level of the ions in the metal). Hence n(r)e is the positive charge density of the uniform jellium in a ball with radius a.
1 For example, owing to the domination of surface effects for small particles their melting temperature decreases
with decreasing particle radius because melting is a surface phenomenon involving the destruction of the internal crystalline structure; for fewnanometresized nanoparticles of, e.g., Au their melting temperature is reduced to room temperature or lower, and so small pieces of metal can be melted even by the focusing of light.
41
42
Plasmon Excitations in NanometreSized Metallic Particles
It should be emphasized that in the case of a finitesized metallic particle, the electron liquid always spills out beyond the jellium rim to some extent. This creates an equilibrium state, in which mobile electrons try to escape beyond the jellium but then are attracted back by the locally uncompensated positive charge of the jellium. The equilibrium state thus corresponds to a electron cloud larger than jellium and with a diluted density due to its larger volume than that of the jellium. This spillout effect is important in ultrasmall metallic nanospheres (i.e., ‘clusters’) and has been studied for nanospheres with radii 1−2 nm, containing around 200–300 electrons [19, 21]. When the radius of a nanoparticle reaches larger values, e.g., 10 nm or greater, spillout loses its significance and can be neglected. The spillout effect may be assessed by the ratio of the volume of the spilled electrons and the volume of the particle defined by its jellium. The thickness of a spilled layer is of the order of the interatomic distance (the Thomas–Fermi radius), hence the spillout scales as 1/a and this surfacetype effect is negligible for a larger than about 5 nm. The Hamiltonian for a metallic nanoparticle can be written as follows: Hˆ =
Ne N Pˆj2 pˆ i2 u(Rj − Rj ) + + 2m j =1 2M i=1 j,j ,j =j
e2 1 w(ri − Rj ), + + 2 ri − ri  i,j
(4.2)
i,i ,i=i
where pˆ i , Pˆj are the momentum operators for the electrons and ions, respectively; m and M denote the masses of the electrons and ions, N is the number of ions, Ne = ZN is the number of electrons, Z is the dissociation level of ions, u denotes the effective potential (pseudopotential) of mutual interaction of the ions (the ions are usually of an irregular shape and thus can be treated only approximately as spherically symmetrical pointlike charges with interac tion potential 12 j,j ,j =j (Ze)2 /Rj − Rj ), and w is the interaction potential of the electrons and the ions (using the sphericalion approximation it equals 2 i,j −Ze /ri − Rj ). Now we can explicitly include the jellium model by adding and subtracting the terms n(R)d 3 R 2 ±e Z (4.3) Rj − R j and ±
i
e
2
n(r)d 3 r , ri − r
(4.4)
Plasmon Excitations in NanometreSized Metallic Particles
43
which describe the interaction of the jellium with the ions and electrons, respectively. In this way one can rewrite the Hamiltonian as the following sum, Hˆ = Hˆ e + Hˆ i + Hˆ ie , where the terms are respectively the Hamiltonians of the electrons, the ions and the electron–ion interaction: Ne 2 3 p ˆ 1 r e2 n(r)d i 2 + Hˆ e = −e , (4.5) 2m ri − r 2 ri − ri  i i,i ,i=i N 3 ˆJ2 P R n(R)d u(Rj − Rj ), (4.6) − e2 Z + Hˆ i = 2M Rj − R j =1 j,j ,j =j
and Hˆ ie =
N e ,N
w(Rj − ri ) +
i,j
2
e Z
j
n(R)d 3 R + e2 Rj − R i
n(r)d 3 r . ri − r
(4.7)
For socalled normal metals [16] (including the noble metals, alkali and transition metals) the pseudopotential in Eq. (4.6) of the ion interaction, u, shifted by interaction with the jellium, is negligibly small. The dynamic effect of the ions in Hˆ i is also small because of the large mass M of the ions and additionally because they are immobilized in a crystal lattice; thus Hˆ i can be neglected. When the interaction of electrons with ions is expressed by the jellium as in Eq. (4.7), Hˆ ie may also be omitted (this has been verified in numerous models, including numerical ab initio calculations for metallic clusters, by the application of the Kohn–Sham approach [19]). The remaining Hamiltonian for the electrons Hˆ e may be represented by the use of the quasiclassical local electron density in an analogous manner to the Pines–Bohm approach for the bulk metal (Eq. (3.4)). By a direct calculation one can show that 2 pˆ 2
1 i 3 e 2π d k n(k) ρ + (k) + ρ(k) Hˆ e = − 3 2 2m (2π) k i (4.8) 2
2π e 1 d 3 k 2 ρ + (k)ρ(k) − Ne , + (2π)3 k 3 −ik·r n(r) = n d 3 re−ik·r (a − r) is the transform where n(k) = d re Fourier 2 3 −ik·r 1/r is the of the jellium distribution in the nanosphere, and 4π/k = d re Fourier transform of the Coulomb potential.2 2 If we change to a discrete spectrum then
1 (2π )3
d3k · · · →
(note that previously V = 1 was assumed in formula (3.4)).
1 ... V k
44
Plasmon Excitations in NanometreSized Metallic Particles
In distinction to the bulk case (3.4), for a nanosphere the jellium is introduced explicitly (it can be generalized for other, nonspherical, nanoparticle shapes; then the isotropic function would be substituted by an anisotropic version adjusted to the particular nanoparticle shape). Moreover, the summation over k is substituted here by integration. In the expression (4.8) the local electron density (its Fourier component) is expressed by ρ(k) = j e−ik·rj , where rj is the position of the j th electron (in the quasiclassical sense), i.e., ρ(r) = j δ(r − rj ). Remembering that (1/(2π)3 ) d 3 keik·r = δ(r) we have 1 3 ik·r −ik·rj d ke e = δ(r − rj ). (4.9) (2π)3 j j Moreover, ρ + (k) = ρ(−k).3 An electron Hamiltonian in the form (4.8) allows us to find the first and secondorder derivatives of the operator for local fluctuations of the electron density (in the Heisenberg picture), according to the formulae dρ(k) d 2 ρ(k) 1 1 = [ρ(k), = [ρ(k), Hˆ e ], ˙ Hˆ e ]. 2 dt i h¯ dt i h¯ The first commutator leads to an expression analogous to Eq. (3.6), dρ(k) hk k · pˆ j ¯ 2 −ik·rj . − e =i + dt m 2m j 3 In the derivation of the second term in the expression (4.8) we have initially −e2 i which can be rewritten as − d 3 r1 e2 i δ(r1 − ri ) d 3 rn(r)/r1 − r and then
−
d 3 r1 d 3 re2
i
1 (2π )3
d 3 keik·(r1 −ri )
1 (2π )3
(4.10)
(4.11)
3 d rn(r)/ri − r,
d 3 k1 eik1 ·r n(k1 )
1 ; r1 − r
after the variable, exchange r1 − r = q, r1 + r = 2p, we obtain 1 1 3 pd 3 q −e2 d 3 kd 3 k1 eip·(k+k1 ) n(k1 ) eik·(q/2−ri ) eik1 ·(−q/2) ; d 6 q (2π ) i
the integral with respect to d 3 p/(2π )3 gives δ(k + k1 ) and the integral with respect to d 3 k1 can be performed. Next, with respect to d 3 q, we arrive at −
1 (2π )3
d3k
e2 4π 1 n(−k)ρ(k) = − k2 (2π )3
d3k
e2 2π n(k)(ρ + (k) + ρ(k)) k2
(in the last step the exchange of variables k → −k can be done in the first term in parentheses, provided that n(−k) = n(k) which is satisfied for a nanosphere). The last term in Eq. (4.8) can be obtained via an analogous calculation (the term −Ne in the last parentheses arises from the condition i = i in the last term in Eq. (4.5)).
Plasmon Excitations in NanometreSized Metallic Particles
45
The second commutator, in a similar way to the bulk case, leads to the expression 2 hk k · pˆ j d 2 ρ(k) ¯ 2 −ik·rj − = − e + dt 2 m 2m j e2 4π k · q (4.12) d 3 qρ(k − q) + n(q) m(2π)3 q2 4π k · q e2 d 3q ρ(k − q)ρ(q). − 3 m(2π) q2 The first term on the righthand side of Eq. (4.12) is related to the kinetic energy of the electrons, whereas the two last terms arise due to the commutation of the gradient operator in ρ˙ with the interaction terms in the Hamiltonian (4.8) (in analogy to Eq. (3.7)). We now represent the operator for local electron density fluctuations by the amount of this fluctuation above the uniform density distribution (charged oppositely to the jellium), i.e., ρ(r) = n(r) + δρ(r) (4.13) and, similarly, for the corresponding Fourier components (owing to the linearity of the Fourier picture), ρ(k) = n(k) + δρ(k). (4.14) Then we can easily rewrite Eq. (4.12) in the following form (note that n(k) does not depend on time; in the Heisenberg representation [n(k), Hˆ e ] = 0): h¯ 2 h¯ 2 k 2 h¯ 2 k 4 d 2 δρ(k) −ik·rj 2 − 2 (k · ∇j ) + 2 ik · ∇j + =− e dt 2 m m 4m2 j k·q 4πe2 (4.15) d 3 qn(k − q) 2 δρ(q) − 3 m(2π) q k·q 4πe2 d 3 qδρ(k − q) 2 δρ(q). − m(2π)3 q Note that for k = 0 the density fluctuation beyond the uniform distribution, δρ(k), in contrast to ρ(k) is not proportional to the number of electrons but is equal to zero. This means that the last term in Eq. (4.15) does not contain a coherent component with limiting longwave plasmon oscillations, as was the case for the bulk system. This coherent component can be identified as the penultimate term, however, where, for q = k, the term n(k − q) attains a macroscopically large value equal to the number of electrons in the system.4 4 Indeed, this follows because n(k) =
3 −ik·r d re n(a − r) and so n(0) = nV = N.
46
Plasmon Excitations in NanometreSized Metallic Particles
Another aspect concerns the singular point in the Fourier transform of the Coulomb interaction 4πe2 /q 2 . In the bulk case this singular point in the sum over q is removed via implicit inclusion of the screening jellium, which for a uniform distribution of electrons at q = 0 completely compensates the jellium. Thus implicit inclusion of the jellium in the bulk case is equivalent to the avoidance of the sum component with q = 0 (this fact is indicated by the prime on the sum over q in the bulk case). If the above integral representation is applied to describe a nanoparticle, this problem does not occur, however. The singularity at zero of the Fourier transform of the Coulomb interaction disappears upon integration, and the jellium is introduced explicitly and independently of this singularity. The variable δρ(k) is an operator (in particular, its derivatives with respect to time include the momentum operator) whose time dependence is expressed in the Heisenberg representation as derived above. In fact we are interested in a measurable quantity, the average of the density fluctuation operator with respect to the eigenfunction of the Hamiltonian. Taking such an average of both sides of Eq. (4.15), we obtain 2 2 2 2 4 h¯ h¯ k h¯ k ∂ δρ(k,t) = − e−ik·rj − 2 (k · ∇j )2 + 2 ik · ∇j + 2 ∂t m m 4m2 j k·q 4πe2 d 3 qn(k − q) 2 δρ(q,t) − 3 m(2π) q 2 k·q 4πe 3 d qδρ(k − q) 2 δρ(q) , −  m(2π)3 q (4.16) 2
where δρ(k,t) = δρ(k). The last term in Eq. (4.16) does not contain a coherent component (according to the above discussion) and wholly of second order with respect to the small departure δρ(k) of the density from the uniform distribution, which is a small quantity (note that the coherent contribution is not present in this term). Thus in the RPA method we can omit this term with the same justification concerning the summation of random phase factors as in the bulk case. The next approximation to be used in Eq. (4.16) has a quasiclassical character: we assume that the electron density changes only weakly on an interatomic distance scale. With such an assumption for the first term of Eq. (4.16), only the first component remains (for small k this term dominates). Hence, the contribution of the kinetic energy attains the form
Plasmon Excitations in NanometreSized Metallic Particles
47
2 2 2 2 4 h¯ h¯ k h¯ k − e−ik·rj − 2 (k · ∇j )2 + 2 ik · ∇j + m m 4m2 j 2 2 2 −ik·r h¯ 2 h ∇ 2k j 2 −ik·rj ¯ j e (k · ∇ ) e , (4.17) j m2 3 2m j j
where the last approximation is justified for a nanoparticle with spherical symmetry.5 In order to assess the contributions of the particular terms in Eq. (4.16) it is convenient to invert the Fourier i.e., to apply to both sides of this equation 3 transform, 3 ik·r the operation (1/(2π) ) d ke · · · . The expression (4.17) then attains the form of the mean value of the kinetic energy,6 ⎞ ⎛ 2 2 2 h ∇ ¯ 2k 1 j d 3 keik·r ⎝ e−ik·rj ⎠ 3 (2π) 3m 2m j ⎞ ⎛ 2 2 2 h¯ ∇j 1 2∇r ⎠ d 3 keik·r ⎝ e−ik·rj =− 3 (2π) 3m 2m j h¯ 2 ∇j2 2∇r2 , δ(r − rj ) (4.18) =− 3m 2m j which can be estimated using the conventional Thomas–Fermi formula, the socalled ρ 5/3 formula [16], 2 h¯ 2 ∇j2 3 (3π 2 )2/3 h¯ (ρ(r,t))5/3 . δ(r − rj ) (4.19) − 2m 5 2m j Because ρ(r,t) = n(r)+δρ(r,t), one can develop the above expression in a Taylor series and confine it to the term linear with respect to δρ(r,t). This development has the form 2 2 3 3 5 δρ(r,t) ¯ ¯ 5/3 2 2/3 h 5/3 2 2/3 h (3π ) [ρ(r,t)] (3π ) n (a − r) 1 + + ··· 5 2m 5 2m 3 n 3 εF n + εF δρ(r,t) (a − r), = 5 (4.20) 5 It is linked with averaging over the spherical angles in the product of two versors,
(d /(4π ))kˆi kˆj = (1/3)δij , where d = sin ddϕ. 6 Because (1/(2π )3 ) d 3 keik·(r−rj ) = δ(r − r ). j
48
Plasmon Excitations in NanometreSized Metallic Particles
where n(r) = n(a − r) and ((a − r))5/3 = (a − r), the Fermi energy εF = pF2 /(2m) = 32/3 π 4/3 h¯ 2 n2/3 /(2m), and the Fermi momentum pF = (3π 2 h¯ 3 n)1/3 . The above approximation has a quasiclassical character and was formerly discussed widely in comparison with ab initio numerical studies of metallic ultrasmall nanoparticles (clusters) of sizes of 1−2 nm with a limitingly small number of electrons [19, 71]. The reason for this limitation was the efficiency constraints of the numerical local density approximation (LDA) and timedependent LDA (TDLDA), both based on the Kohn–Sham approach.7 Nevertheless, it was proved [19] that going beyond the quasiclassical approximation does not bring any important corrections, especially in the case of nanoparticles. For nanoparticles the dominating term of highest order with respect to the gradient (which is actually included in the quasiclassical approximation) is even more significant in finite systems than in the bulk material because of the greater variation in the density induced by a particle border. Within the RPA scheme we neglect the secondorder term in interaction of electron fluctuations but the secondorder term in the interaction of the electrons with the jellium is maintained: k·q 4πe2 d 3 qn(k − q) 2 δρ(q,t). (4.21) − 3 m(2π) q The inverse Fourier transform of this term can be written in the form 2 k·q 1 3 ik·r 4πe d ke d 3 qn(k − q) 2 δρ(q,t) − 3 3 (2π) m(2π) q 2 1 3 ik·r 4πe d d 3 q d 3 r1 ke =− (2π)3 m(2π)3 k·q (4.22) d 3 r2 e−iq·r2 δρ(r2,t) × e−i(k−q)·r1 n(r1 ) 2 q 2 1 1 3 ik·r 4πe =− · d ke ∇ r (2π)3 i m(2π)3 q 3 3 −i(k−q)·r1 × d q d r1 e n(a − r1 ) 2 d 3 r2 e−iq·r2 δρ(r2,t). q However, (1(2π)3 ) d 3 keik·(r−r1 ) = δ(r − r1 ), and it is possible to perform the integration with respect to d 3 r1 , which leads to the following expression (the dot after the gradient operator denotes the scalar product ∇ · q),
7 Recently there have appeared TDLDA simulations for larger number of electrons – even up to 105 , but with
some additional simplifications.
Plasmon Excitations in NanometreSized Metallic Particles
49
1 4πe2 q d 3 qeiq·r n(a − r) 2 d 3 r2 e−iq·r2 δρ(r2,t) − ∇r · i m(2π)3 q 2 1 1 1 1 3 3 iq·(r−r2 ) 4πe = − ∇r · n(a − r) ∇r d r2 d qe δρ(r2,t) i m i (2π)3 q2
ωp2 1 3 = (4.23) ∇r · (a − r)∇r d r1 δρ(r1,t) . 4π r − r1  In the penultimate equality the variable of integration r2 has been renamed as interaction has been taken; r1 , and the inverse Fourier transform of the Coulomb 2 moreover, in the last line the quantity ωp = 4πne /m has been introduced, the frequency of volume bulk plasmons. Summarizing, after the steps described above, • as in the RPA, we neglect terms of second order in the fluctuations, • we take the inverse Fourier transform of the electron–jellium interaction (4.23), • we use a quasiclassical approximation for the kinetic energy contribution (4.18), (4.19), and (4.20). We then arrive at the following equation: 2 2 2 h¯ ∇j ∂ δρ(r,t) 2 = − ∇r2 δ(r − rj ) 2 ∂t 3m 2m j
ωp2 1 3 ∇r · (a − r)∇r d r1 δρ(r1,t) + 4π r − r1 
2 2 3 ∇ εF n + εF δρ(r,t) (a − r) = 3m r 5
ωp2 1 + ∇r · (a − r)∇r d 3 r1 δρ(r1,t) . 4π r − r1 
(4.24)
This equation can be transformed by utilizing the formula ∇r (a − r) = −ˆr δ(a − r),
(4.25)
where rˆ = r/r is the versor of the vector r. Thus the first term on the righthand side of Eq. (4.24) becomes
2 2 3 ∇ εF n + εF δρ(r,t) (a − r) 3m r 5
2 3 r =− ∇r εF n + εF δρ(r,t) δ(a − r) 3m 5 r r 2 2 (4.26) εF δ(a − r) ∇r δρ(r,t) + εF (a − r)∇r2 δρ(r,t). − 3m r 3m
50
Plasmon Excitations in NanometreSized Metallic Particles
The second term on the righthand side of Eq. (4.24) becomes
ωp2 1 3 ∇r · (a − r)∇r d r1 δρ(r1,t) 4π r − r1  (4.27) ωp2 r 1 =− δ(a − r)∇r d 3 r1 δρ(r1,t) − ωp2 (a − r)δρ(r,t). 4π r r − r1  The last term in the above equality follows from the relation 1 ∇r2 2 d 3 r1 δρ(r1,t) = −ωp2 (a − r)δρ(r,t), ωp (a − r) 4π r − r1 
(4.28)
because from Poisson’s equation we have −∇r2 (1/r − r1 ) = 4πδ(r − r1 ). Taking into account Eqs. (4.26) and (4.27), one can rewrite the dynamic equation for the electron liquid in the nanoparticle metal in the following form:
2 ∂ 2 δρ(r,t) 2 2 = εF ∇r δρ(r,t) − ωp δρ(r,t) (a − r) ∂t 2 3m
2 3 r − ∇r εF n + εF δρ(r,t) δ(a − r) 3m 5 r ! 2 ωp 2 r 1 εF ∇r δρ(r,t) + ∇ r d 3 r1 δρ(r1,t) δ(a − r). − 3m r 4π r − r1  (4.29) The structure of this equation forces the shape of the solution, including a part distinguished by the Dirac delta function, ∼ δ(r − a), at the nanoparticle surface and a finite part inside the nanoparticle. The general form of the solution can be thus written as follows: for r < a, δρ1 (r,t) (4.30) δρ(r,t) = for r = a (r ≥ a, r → a+); δρ2 (r,t) the indices 1,2 indicate disjoint parts of the domain of Eq. (4.29). After substitution of Eq. (4.30) into Eq. (4.29) one obtains the equations for both parts of the domain: 2 ∂ 2 δρ1 (r,t) = εF ∇r2 δρ1 (r,t) − ωp2 δρ1 (r,t) 2 ∂t 3m for r < a and
(4.31)
3 r εF n + εF δρ2 (r,t) δ(a + − r) 5 r 2 ωp 2 r 1 εF ∇r δρ2 (r,t) + ∇r d 3 r1 − 3m r 4π r − r1 
∂ 2 δρ2 (r,t) 2 =− ∇r 2 ∂t 3m
× {δρ1 (r1,t)(a − r1 ) + δρ2 (r1,t)(r1 − a)}] δ(a + − r) (4.32)
Plasmon Excitations in NanometreSized Metallic Particles
51
for r = a,(r ≥ ar → a+). Here = 0+ is an infinitely small shift of the argument applied to satisfy the formal definition of the Dirac delta (as the generalized distribution function is a linear functional in Hilbert space), which requires the singular point to be located inside an open set, not on its border. This formal definition via the limit = 0+ does not introduce any asymmetry with respect to the nanosphere surface, and is only a rigorous mathematical clarification ensuring the uniqueness of the Dirac delta definition.8 Thus, on the basis of the quasiclassical approximation we get two types of plasmon excitation in a metallic nanosphere: • surface plasmons with deltashape localization on the nanosphere surface, • volume plasmons defined inside the nanosphere. In the case of ultrasmall clusters, when spillout is relatively important, the surface is not sharply defined and is blurred by the spillout. For such small nanoparticles, with fuzzy surfaces, the surface and volume plasmon modes are coupled to some extent and their separation may be impossible. The emergence of a distinctly separate surface plasmon mode has been demonstrated numerically by the TDLDA method for around 60 electrons in the cluster, though this mode is still coupled to the volume modes. For a larger number of electrons, ∼ 105−7 , as in nanoparticles with radii around 5 − 10, nm the spillout effects are negligible and the quasiclassical RPA approach with a sharply defined nanoparticle surface is fully justified. However, it should be noted that some special situations must be considered with caution. For example, when a metallic nanosphere is embedded in a dielectric medium, these surroundings diminish the Coulomb interaction of electrons on the surface but certainly also in some nonzerothickness layer;9 this could be hard to include in the developed quasiclassical RPA model for a sharp surface (this situation will be addressed below). The solution of Eqs. (4.31) and (4.32) is performed taking into account the boundary conditions and the continuity conditions as well as the charge conservation constraint. It is convenient to represent the volume type of plasmon excitation in the form δρ1 (r,t) = n(f1 (r) + F (r,t))
for r < a,
(4.33)
which inserted into Eq. (4.31) results in the conditions ∇ 2 f1 (r) − kT f1 (r) = 0
(4.34)
∂ 2 F (r,t) vF2 2 = ∇ F (r,t) − ωp2 F (r,t), ∂t 2 3 r
(4.35)
and
8 It is well known that, in a nonrigorous sense, ∞ δ(x)dx = α where α = (0) can be chosen arbitrarily. 0 9 The interaction on the surface is influenced by the adjacent regions on both sides owing to the threedimensional electrodynamics.
52
Plasmon Excitations in NanometreSized Metallic Particles j1(x)
0.4
j2(x)
0.3
j3(x)
0.2 0.1 2
4
6
8
10
0.1 0.2
Figure 4.1 The positions of the Bessel function nodes depend on the function order, as shown for jl (x), l = 1,2,3.
6πne2 /vF = 3ωp2 /vF2 is the reciprocel of the Thomas–Fermi radius and ωp = 4πne2 /m is the volumeplasmon frequency in the bulk material. The solution for f1 (regular at zero) is as follows: where kT =
f1 (r) = α
e−kT a −kT r e − ekT r , kT r
α = const.
(4.36)
For the function F (r,t) we assume the initial condition F (r,0) = 0, which leads to F (r,t) = Fω (r) sin(ωt). Thus the function Fω satisfies a Helmholtztype equation, ∇ 2 Fω (r) + k 2 Fω (r) = 0,
(4.37)
where k 2 = 3(ω2 − ωp2 )/vF2 and the solution regular at the origin has the form √
Fω (r) ∼ jl (kr)Ylm ( ),
(4.38)
where jl (x) = (π/2x)Il+1/2 (x) is a spherical Bessel function (In (x) is a type1 Bessel function), Ylm ( ) is a spherical harmonic, and is a spherical angle in spherical coordinates. The boundary condition limr→a F (r,t) = 0 (in agreement with the quasiclassical approximation) leads to the constraint jl (ka) = 0, and thus to discrete values of the parameter k = knl = xnl /a, where xnl are consecutive nodes (n = 1,2,3, . . .) of the Bessel function jl (Fig. 4.1). In this way we obtain the frequency spectrum of the volumeplasmon selfoscillations in a metallic nanosphere, x2 2 (4.39) = ωp2 1 + 2 nl 2 . ωnl kT a Thus the general solution for F (r,t) has the shape F (r,t) =
∞ ∞ l l=0 m=−l n=1
Almn jl (knl r)Ylm ( ) sin(ωnl t).
(4.40)
Plasmon Excitations in NanometreSized Metallic Particles
53
It is noticeable that all the mode frequencies ωnl are larger than ωp , as follows from Eq. (4.39), i.e., in a metallic nanoparticle these volume plasmons are more energetic than in the bulk material, and this difference increases for lower radii a. This resembles the behaviour of energy levels in a narrow quantum well. For the surface plasmon modes we assume that (4.41) δρ2 (r,t) = nf2 (r) + σ ( ,t)δ(a + − r), 3 for r ≥ a, = 0+. The neutrality condition d rρ(r,t) = nV = Ne leads to the relations ∞ a 2 drr f1 (r) = drr 2 f2 (r), − 0 a 3 (4.42) d r(a − r)F (r,t) = 0, d σ ( ,t) = 0, from which one can determine that f2 (r) = βe−kT (r−a) /(kT r) and, taking into account the continuity condition 1 + f1 (r)r→a = f2 (r)r→a , one can determine the constant β = kT a − (kT a + 1/2)(1 − e−2kT a ) and the constant α = −(kT a + 1)/2 (the latter is needed for Eq. (8.9)). The functions describing the static spillout, with the assumed approximation, have the form kT a + 1 −kT (a−r) 1 − e−2kT r f1 (r) = − e , for r < a, 2 kT r
−kt (r−a) kT a + 1 e −2kT a ) f2 (r) = kT a − (1 − e for r ≥ a. 2 kT r
(4.43)
The scale of this static spillout of charge is thus governed by the Thomas–Fermi radius, i.e., it is of the order of the interparticle distance, and for large nanoparticles (a ∼ 5 nm) the spillout plays a marginal role. For nanoparticles of this size or greater, the spillout may be safely neglected without affecting the analysis of the plasmon excitations. In the framework of the semiclassical RPA model, the electrical balance is therefore kept separately for the volume modes and for the surface modes. In ultrasmall nanoparticles, especially for Ne < 60, this condition is not fulfilled because of the fuzzy surface, and the surface and volumeplasmon modes are not separable; for Ne > 60 this volume–surface coupling effect gradually disappears and for Ne ∼ 200 does not play a significant role despite the still pronounced spillout; for Ne > 105 (for nanoparticles with a > 5 nm) both the spillout and the surface–volume coupling are completely 3 negligible. One can see that from the neutrality condition, d r(a − r)F (r,t) = 0, it follows that A00n = 0, because d Ylm = 4πδl0 δm0 .
54
Plasmon Excitations in NanometreSized Metallic Particles
Let us now consider an explicit solution for the surface plasmons. In order to determine the selffrequencies for the surface plasmons, we need to consider Eq. (4.32) and the solution to it given by Eq. (4.41). The first term on the righthand side of Eq. (4.32) can be rewritten as 2εF 3 2εF 3 ∇ n + δρ2 ∇(a − r) + n + δρ2 3m 5 3m 5 2εF 3 1 ∂ 2εF ∂ 3 =− δ(a − r) n + δρ2 − n + δρ2 2 (r 2 δ(a − r)) 3m ∂r 5 3m 5 r ∂r
3 2εF 1 ∂ (4.44) =− n + δρ2 r 2 δ(a − r) , 2 3m r ∂r 5 where we have used the formulae r ∇(a − r) = − δ(a − r), r
r ∂ ∇= r ∂r
and, in spherical coordinates, =
1 ∂ 2∂ 1 ∂ ∂ 1 ∂2 r + sin θ + r 2 ∂r ∂r sin θ ∂θ ∂θ sin2 θ ∂φ 2
(note that for the function (r) only the first term contributes to ). The next term on the righthand side of Eq. (4.32) can be transformed into −
3 ωp2 2εF r r d r1 δρ(r1 ) δ(a − r) ∇δρ2 − δ(a − r) ∇ 3m r 4π r r − r1  3 2 ωp d r1 δρ(r1 ) ∂ ∂ 3εF δ(a − r) δρ2 − δ(a − r) . =− 3m ∂r 4π ∂r r − r1 
Equation (4.32) thus attains the form
3 ∂ 2 ρ2 2εF 1 ∂ 2 =− n + δρ2 r δ(a − r) ∂t 2 3m r 2 ∂r 5 3 ωp2 d r1 δρ(r1 ) 2εF ∂ ∂ − δ(a − r) δρ2 − δ(a − r) . 3m ∂r 4π ∂r r − r1 
(4.45)
(4.46)
Now we suppose that the solution of the above equation has the form δρ2 = 2 σ ( ,t)δ(a + 0+ − r) and multiply both sides of the equation Lby2 r . Then we find the integral with respect to r beween arbitrary limits, i.e., l r dr · · · , such that a ∈ (l,L) (this integration removes the Dirac deltas), which leads to the equation
Plasmon Excitations in NanometreSized Metallic Particles
a
2∂
2
σ ( ,t) 2εF =− 2 ∂t 3m
L
∂ dr ∂r
55
3 2 n + δρ2 r δ(a − r) 5
l
2εF − σ ( ,t) 3m
L r 2 drδ(a − r)
∂ δ(a − r) ∂r
l
−
−
ωp2
L
4π ωp2
∂ r 2 drδ(a − r) ∂r
∞
l
a
L
a
∂ r drδ(a − r) ∂r 2
4π l
r12 dr1
d
δρ2 (r2 ) r − r1 
d
δρ1 (r1 ) . r − r1 
r12 dr1
0
(4.47)
The first two terms on the righthand side of the above equation vanish, because 2εF − 3m
L
∂ dr ∂r
l
2εF =− 3m
3 2 n + δρ2 r δ(a − r) 5
L 3 2 n + δρ2 r δ(r − a) = 0 5 l
(4.48)
and L
L 1 ∂ 2 a2 2 dr δ (a − r) = δ (a − r) 2 ∂r 2 l l L μ 1 kT a 2 = 0. =− δ(a − r) lim m 2 μ→0 π μ2 + (a − r)2 l (4.49)
∂ r drδ(a − r) δ(a − r) = a 2 ∂r 2
l
L
The two last terms on the righthand side of Eq. (4.47) can be transformed using the formula [72],
1 1+
z2
− 2z cos γ
=
∞
Pl (cos γ )zl
for z < 1,
l=0
where l 4π ∗ Ylm ( )Ylm ( ) Pl (cos γ ) = 2l + 1 m=−l
56
Plasmon Excitations in NanometreSized Metallic Particles
are Legendre polynomials. This formula leads to the following: ⎧ ∞ la l−1 ⎪ ⎪ ⎪ Pl (cos γ ) for a < r1, ⎪ ⎪ ⎨ r l+1 1 ∂ l=0 1 = ∞ ⎪ ∂a a − r1  ⎪ (l + 1)r1l ⎪ ⎪ Pl (cos γ ) for a > r1, − ⎪ ⎩ a l+2
(4.50)
l=0
where a = ar/r, cos γ = a · r1 /(ar1 ). Employing Eq. (4.50), the last two terms in Eq. (4.47) can be transformed as follows: −
ωp2
L
∂ r drδ(a − r) ∂r
∞
2
4π
r12 dr1
d 1
a
l
=−
ωp2 4π
a
2
∞ r12 dr1 δρ2 (r1 )
d 1 a
=−
ωp2 4π
a
2
δρ2 (r1 ) r − r1 
1 ∂ ∂a a 2 + r 2 − 2ar cos γ 1 1
∞ r12 dr1 σ ( 1 )δ(a
d 1
+ 0 + −r1 )
l=0
a
=− =
ωp2 4π
a2
−ωp2 a 2
d 1 σ ( 1 )
∞ l l=0 m=−l
∞ la l−1
r1l+1
Pl (cos γ )
∞ l 1 4πl ∗ Ylm ( )Ylm ( 1 ) a 2 l=0 2l + 1 m=−l
l Ylm ( ) 2l + 1
∗ d 1 σ ( 1 )Ylm ( 1 )
and −
L
ωp2
∂ r drδ(a − r) ∂r
a
2
4π l
=−
ωp2 4π
a r12 dr1 nF (r1,t)
d 1 0
=
ωp2 4π
a
2
d 1
0
a2
r12 dr1
d 1 nF (r1,t)
1 ∂ ∂a a 2 + r 2 − 2ar cos γ 1 1
∞ (l + 1)r l
1
l=0
δρ1 (r1 ) r − r1 
a l+2
Pl (cos γ )
∞ l+1 rl Ylm ( ) r12 dr1 1l 2l + 1 a l=0 a
=
ωp2 n
0
×
l1 ∞ l1 =1 m1 =−l1
i
Almi jl1 (kl1 i r1 ) sin(ωl1 i t)
∗ d 1 Ylm ( 1 )Yl1 m1 ( 1 )
(4.51)
Plasmon Excitations in NanometreSized Metallic Particles
=
ωp2 n
∞ l l+1 Ylm ( )Almi 2l + 1 l=0 m=−l i
a
r1l+2 dr1 jl (kli r1 ) sin(ωli t). al
57
(4.52)
0
Equation (4.47) thus attains the form ∞ l l ∂ 2 σ ( ,t) 2 2 ∗ = −ω a ( ) d 1 σ ( 1 )Ylm ( 1 ) Y lm p ∂t 2 2l + 1 l=0 m=−l l+2 ∞ l l+1 r1 dr1 jl (kli r1 ) sin(ωli t). Ylm ( )Almi × 2l + 1 al l=0 m=−l i a
+
ωp2 n
0
(4.53) Assuming now that σ ( ,t) = the above equation, we obtain l ∞
Ylm ( )
l=0 m=−l
∞ l l=0
m=−l
qlm (t)Ylm ( ) and substituting it into
l ∞ ωp2 l ∂ 2 qlm (t) = − Ylm ( )qlm (t) ∂t 2 2l + 1 l=0 m=−l
+ ωp2 a ×
∞ l l+1 Ylm ( )Alm 2l + 1 l=1 m=−l i
r1l+2 dr1 jl (kli r1 ) sin(ωli t). a l+2
(4.54)
0
From this equation we notice that for l = 0 we get ∂ 2 q00 /∂t 2 = 0 and thus q00 (t) = 0 (since q(0) = 0 and limt→∞ q(t) < ∞). For l ≥ 1 we obtain ωp2 l ∂ 2 qlm (t) l+1 = − ωp2 qlm (t) + Alm n 2 ∂t 2l + 1 2l + 1 i
a
r1l+2 dr1 jl (kli r1 ) sin(ωli t), a l+2
0
(4.55) which induces the solution & l Blm qlm (t) = 2 sin ωp t a 2l + 1 +
i
Alm
(l + 1)ωp2 ωp2 − (2l + 1)ωli2
a n 0
r1l+2 dr1 jl (kli r1 ) sin(ωli t) a l+2
(4.56)
58
Plasmon Excitations in NanometreSized Metallic Particles
∞ l and δρ2 (r,t) = l=1 m=−l qlm (t)Ylm ( )δ(a − r). The first term in Eq. (4.56) describes the selffrequencies of surface plasmons, whereas the second term gives the surface plasmon oscillations induced by the volume plasmons. This induced part of the surface oscillations is nonzero only when the volume modes are excited and their amplitudes, Almi , are nonzero. The frequencies of selfoscillation of the sur√ face plasmons are equal to ωl0 = ωp l/(2l + 1), corresponding to the various multipole modes (numbered byl). Note that these frequencies are lower than the bulk plasmon frequency (ωp = ne2 4π /m in Gauss units or ne2 /(ε0 m) in SI units), whereas the volume plasmon modes oscillate with frequencies higher than ωp .
5 Damping of Plasmons in Metallic Nanoparticles
In this book our main attention is focused on plasmon damping, which is essential for energy transfer via plasmons. In this chapter various damping channels are discussed and compared. The attenuation rate for plasmons in metallic nanoparticles is derived in a farreaching analytical form. The contributions to plasmon attenuation of electron scattering and radiation losses are presented. An accurate account of the Lorentz friction of plasmon oscillations in metallic nanoparticles is given. There is close consistency between theory and experiment, not achieved previously and revealing the nonharmonic character of plasmon oscillations. The related corrections to the popular conventional Mie approach to plasmons and to the commercial software COMSOL are defined and illustrated.
Plasmonic oscillations in metallic nanoparticles have recently received considerable attention owing to their prospective applications in photovoltaics. Solar cells modified by deposition on their surface of metallic nanoparticles are regarded as promising a new generation of solar cells with enhanced efficiencies due to plasmon mediation in the solar energy harvesting [33, 36, 2, 73, 74]. An increase in the efficiency of the photoeffect in semiconductors due to the mediation of plasmons in metallic compounds has been proved experimentally to exceed even 100%, which causes a few per cent growth in the overall efficiency of a solar cell (because the light absorption is only the initial step in a long chain of processes contributing to the overall solar cell functionality and its efficiency). The crucial role in the plasmonaided photoeffect is played by the surface plasmons in the metallic nanoparticles, which can be easily excited by incident photons and can quickly transmit energy to the substrate semiconductor. This energy transit via plasmons is conditioned by various channels of plasmon damping, when the energy outflow reduces the plasmon oscillations. The higher the damping of plasmons, the more efficient is the energy transfer via plasmons, because the energy income from sunlight constantly supplements the losses through plasmon oscillations. Both the absorption and the emission of plasmons are linked by general quantum transition rules similar to those for ordinary optical transitions [75]. The latter are defined by the interaction 59
60
Damping of Plasmons in Metallic Nanoparticles
of an electromagnetic wave with a quantum system (the electron in an atom or a band electron in a semiconductor) via the kinematic momentum shift caused by the vector potential of the electromagnetic field. In the case of plasmons, however, quite different and much more efficient coupling channels between plasmons and electrons occur. To recognize all these channels for energy transfer via plasmons, an understanding of plasmon damping is essential. The energy of plasmon oscillations can be dissipated irreversibly into Joule heat by the scattering of electrons in a metallic nanoparticle. This unavoidable component of plasmon damping does not take part in the harvesting of solar energy in solar cells and causes parasite losses eventually to become phonon heatlike excitations in metallic nanoparticles (there are contributions from the scattering of electrons at metal imperfections and admixtures, from direct interaction with phonons and other electrons, and from scattering at the boundaries of a nanoparticle). Plasmon oscillations correspond to a variation in time of the acceleration of electrons; thus the related Lorentz friction [55, 76] caused by radiation of an electromagnetic wave also contributes to the plasmon damping. The term Lorentz friction is conventionally applied to electromagnetic emission in the farfield radiation zone in the dielectric surroundings of a metallic nanoparticle (or in the vacuum). However, when another electric charge system is present in the vicinity of the metallic nanoparticle, the different type of coupling in the nearfield zone may contribute to the plasmon energy losses. Such a situation occurs when the metallic nanoparticle is deposited on or embedded in a substrate semiconductor and the surface plasmons in the metallic nanoparticle couple with the semiconductor band electrons in the nearfield zone of plasmon radiation. This photonless energy transfer occurring at distances smaller than the plasmon resonance wavelength is especially large for dipole surface plasmons and causes a giant plasmonmediated photoeffect. Noteworthy is an interesting situation when the energy receiver (the substrate semiconductor) influences the energy emitter (the plasmons in the metallic nanoparticles). This effect goes beyond classical electrodynamics, which does not describe such a feedback. In the case of metallic nanoparticles this feedback is, however, strong and causes a large damping of plasmons which is different from that occurring when plasmons freely emit radiation in the dielectric (or vacuum) surroundings. The feedback effect for plasmons is very sensitive to the nanoparticle size [77]. This significant effect is neglected in the conventional Mie approach or in numerical solutions of the Maxwell–Fresnel problem (e.g., by COMSOL). To address this phenomenon is the basic goal of the present text. Radiation losses hamper the plasmon oscillations, but the higher the radiation losses, the better is the energy transmittance via plasmons. The radiation properties of plasmons also determine the subdiffraction plasmon–polariton weakly damped propagation in plasmonic wave guides consisting of metallic nanochains
Damping of Plasmons in Metallic Nanoparticles
61
or nanoarrays [3, 4, 39, 38, 78]. This phenomenon has prospective applications in nanophotonics and optoelectronics. One should note that ultrasmall metal nanoparticles (clusters) of radius a ∈ (1,5) nm exhibit very weak radiation [19, 71, 20, 17] and that plasmon damping at this size scale is primarily due to the electron scattering resulting in ohmic losses and to electron collisions with the cluster boundary. The scattering of electrons results in Joule heat energy dissipation. Nevertheless, with increasing nanoparticle size, the plasmon radiation intensity grows rapidly, mostly because of the strengthening of the plasmon oscillation amplitude, which is proportional to the number of electrons in a nanoparticle. This grows as a 3 with the nanoparticle radius a. In the case of the dielectric surroundings of a metallic nanoparticle the electronplasmaoscillation radiative losses can be accounted for by the Lorentz friction [55, 76]. As mentioned above, the Lorentz friction force acts on nonuniformly accelerating charges (as in the case of oscillating charges), which radiate electromagnetic waves. The radiated energy can be treated as an effective kinetic energy loss, caused by a fictitious force – the Lorentz friction force – hampering the electron motion. In the case of an oscillating dipole, as is the situation for the dipoletype surface plasmons on a metallic nanosphere, the Lorentz friction is proportional to the thirdorder time derivative of this dipole [55, 76]. The Lorentz friction can be included in a description of the surface plasmons in metallic nanospheres via the typical damping term in the oscillatory equation. However, this term is proportional to the firstorder time derivative of the oscillating dipole whereas, as stated above, the Lorentz friction is proportional to the thirdorder time derivative. The substitution of this thirdorder derivative by an appropriately lifted firstorder derivative is the essence of the perturbative approximation [23, 77]. Such an approximation results in an approximately a 3 increase in the radiation damping rate for plasmons with nanosphere radius a. Such a fast growth of the radiation losses with nanoparticle radius suggests that the Lorentz friction dominates the other attenuation channels in the case of sufficiently large nanospheres. However, the rapid growth of a 3 quickly violates the necessary perturbation convergence limits, which precludes the use of this approximation for nanospheres with larger radii (in the case of Au nanoparticles in vacuum the perturbation approximation is correct only for a ∈ (5,25) nm). In order to describe the effect of the Lorentz friction beyond the scope of the perturbation approach regime, linearization of the thirdorder derivative must be avoided and the whole contribution of the thirdorder derivative has to be accounted for accurately. As will be shown below, these nonlinear corrections are essential for nanospheres of radii a > 25−30 nm (for Au in vacuum). Accurate accounting for the Lorentz friction (by using the thirdorder time derivative) can explain the anomalous size dependence in
62
Damping of Plasmons in Metallic Nanoparticles
the light absorption that is observed in large metallic nanospheres (it is measured by the light extinction in watercolloidal solutions of metallic nanoparticles of varying size [77]). Exact inclusion of the Lorentz friction is critical for improving our understanding of the experimental data; this is unsatisfactory using the approximate perturbative approach, with a growing discrepancy occurring for the larger nanospheres (a > 30 nm for Au), when the perturbation approach fails. As mentioned above, small metallic nanoparticles (clusters) of size 1−5 nm do not exhibit a radiation efficiency as high as nanospheres with larger radii (especially for a > 10 nm, for Au in vacuum).1 Small metallic nanoparticles with radii of the order of a single nanometre were widely investigated in the 1980s, theoretically within the socalled local density approximation (LDA) or timedependent local density approximation (TDLDA) [19, 71, 20, 79], and experimentally for clusters of alkali metals such as Na or K, which confirmed their poor radiation efficiency. The electromagnetic radiation of plasmons in these small systems turned out to be weak owing to the relatively small amount of electrons oscillating in such clusters, but other unique properties were important at this scale. Special attention was paid to the socalled spillout of the electron liquid beyond the rim of the ion lattice and the influence of this effect on the plasmon oscillations, which is greater for smaller particles. Spillout results in the dilution of the electron density inside the system and this is a reason for the redshift of the resonance frequency of surface plasmons (which is proportional to the electron density) observed experimentally for ultrasmall nanoparticles of K and Na [19]. The spillout effect diminishes, however, with the increase of the nanoparticle size because of the lessening role of surfacerelated phenomena when the radius of the system grows. The spillout takes place on the scale of the Thomas–Fermi length [16], which is of subnanometre value and is lower by at least one or two orders of magnitude in comparison to the nanosphere radius when a > 5 nm. In larger nanoparticles the role of the radiation phenomena rapidly grows, and for a > 10 nm (for Au in vacuum) Lorentz friction dominates the plasmon damping. In metallic nanoparticles with sizes of several tens of nanometres the radiative plasmon effects are of primary significance, and many quantum effects such as spillout or Landau damping (corresponding to the decay of plasmons into electron–hole pairs that are of high energy with respect to the Fermi surface) [80] are completely negligible at this size scale. To gain insight into plasmon behaviour in relatively large electron systems with 105−8 electrons, i.e., with a nanosphere radius of several tens of nanometres, a > 5 nm, accurate numerical methods based on the Kohn–Sham approach (LDA 1 The range is similar also for Ag or Cu, but generally it depends on the metal type and on the dielectric
permittivity of the surroundings.
5.1 Damped Plasmonic Oscillations in Metallic Nanospheres
63
and TDLDA) are not useful as they are limited to a much smaller number of electrons, i.e., up to 200–300, as is the case for a ∼ 2−3 nm nanoparticles. As the electron number increases above 300, these numerical methods are less effective because numericaltype constraints rapidly slow down calculations even at highperformance facilities. For large nanoparticles, various versions of the random phase approximation (RPA) turn out to be useful instead [19, 71, 21, 23]. Of particular interest are large nanoparticles of the noble metals (gold, silver, and also copper) because the surface plasmon resonances in nanoparticles of these metals lie within the visible light spectrum, which is important for photovoltaic applications. The following sections contain a brief repetition of the analysis of the surface dipoletype plasmons in a single nanosphere within the RPA model [23, 77], as presented in the previous chapter, but with the inclusion of the damping effects caused both by scattering and radiation, the latter expressed by the fictitious Lorentz friction force acting on moving charges. A discussion of the difference between the perturbative approximation and the accurate treatment of the Lorentz friction will be presented in detail, together with a comparison with experiment. The last section focuses on some applications of the exact analysis of Lorentz friction to the widely developed Mie theory of the light properties of metallic nanoparticles, which are very useful and efficient for the interpretation of many experiments in the field of nanophotonics and plasmonics. 5.1 Damped Plasmonic Oscillations in Metallic Nanospheres in Dielectric Surroundings Let us consider a metallic (Au) nanosphere of radius a immersed in a dielectric environment with relative permittivity ε. We assume the presence of a varying external electric field which can excite plasmon collective oscillations modes in the nanosphere. Such a situation could correspond to the socalled dipole limit for interaction with light, i.e., the case when the wavelength of the incident light well exceeds the nanosphere dimension. The surface plasmon resonance for metallic nanospheres in the noble metal case, for Au, Ag, and even Cu, with radius a ∈ (5,100) nm occurs for light of approximately 500 nm wavelength; thus, the conditions for the dipole approximation are fulfilled and the resonant incident electromagnetic signal can be treated as homogeneous over the entire nanoparticle in the range of radii considered. We will analyse the collective reaction of the electron liquid to this spacehomogeneous but timedependent field in the spherical metallic nanoparticle assuming the jellium model. This means that we neglect the dynamics of the ions, according to the scheme presented in the previous chapter.
64
Damping of Plasmons in Metallic Nanoparticles
As was pointed out, the ion dynamics is inertial owing to the much higher mass of the ions in comparison to the electron mass and can be neglected.2 In the jellium model, the charge of the ion background is static and uniformly smeared over the whole nanosphere with density ne (r) = ne (a − r), ne = Ne /V , where Ne is the number of free electrons in the nanosphere, V is the volume of the nanosphere, is the Heaviside step function, and ene is the averaged density of the positive charge compensating the charge of the free electrons. The plasmonic oscillations in a metallic nanosphere can be described by the local electron density fluctuation, defined as in the RPA approach for the bulk metal developed by Pines and Bohm [15]: δ(r − rj ) e (t) , (5.1) ρ(r,t) = e (t) j where the rj define the quasiclassically positions of the electrons and e (t) is the multiparticle wave function of the electron system (for the Hamiltonian (5.4) below; see also (4.8)). The Fourier picture of (5.1) has the simple form ˆ (5.2) ρ(k,t) ˜ = ρ(r,t)e−ik·r d 3 r = e (t)ρ(k) e (t), where the operator ρ(k) ˆ = j e−ik·rj . The dynamic equation for this local electron density operator can be found by using the Heisenberg equation twice: ( ( d 2 ρ(k) ˆ 1 '' ˆ e , Hˆ e , = ρ(k), ˆ H (5.3) dt 2 (i h) ¯ 2 where He is the Hamiltonian for electrons in the metallic nanosphere in the jellium model, but with the electron interactions expressed by localelectrondensity operators that also include the interaction of the electrons with the jellium [23]: Ne * h¯ 2 ∇j2 2π ) ˆ+ e2 3 d k n ˜ (k) (k) + ρ(k) ˆ Hˆ e = − ρ − e 2m (2π)3 k2 j =1 ) * e2 3 2π ˆ+ (k)ρ(k) + d k ˆ − N ρ , (5.4) e (2π)3 k2 where n˜ e (k) = d 3 rne (r)e−ik·r . Equation (5.3), after averaging over the multiparticle wave function and, according to the RPA scheme, neglecting sums of exponents with random phases, finally attains the form [23], 2 The adiabatic approximation corresponds to neglecting the ion dynamics in comparison to the electron
dynamics, since the ions are much heavier, though for some specific purposes one can consider dualion plasmons in metals. These, however, have a marginal significance for the electron plasmon response [19].
5.1 Damped Plasmonic Oscillations in Metallic Nanospheres
65
∂ 2 δ ρ(r,t) ˜ 2 F 2 2 = δ ρ(r,t) ˜ − ω δ ρ(r,t) ˜ (a − r) ∇ p ∂t 2 3m
2 r 3 − ˜ ∇ F ne + F δ ρ(r,t) δ(a − r) 3m 5 r ! ωp2 r 1 2 F r 3 ∇δ ρ(r,t) ˜ + ∇ d r1 δ ρ(r ˜ 1,t) δ(a − r). − 3mr 4π r r − r1 
(5.5) In the above formula the Thomas–Fermi approximation for the kinetic energy has been used [16, 23] and ωp is the bulk plasmon frequency, so that ωp2 = 4πne e2 /m in Gauss units (in SI ωp2 = e2 ne /ε0 m). We have used ∇(a−r) = −(r/r)δ(a−r)), which gives rise to the Dirac delta distinguishing surface plasmon fluctuations in Eq. (5.5). Owing to the structure of Eq. (5.5), the general solution is thus decomposed into two parts related to the two distinct domains: for r < a, δ ρ˜1 (r,t) (5.6) δ ρ(r,t) ˜ = for r ≥ a (r → a+), δ ρ˜2 (r,t) corresponding respectively to the volume and surface charge fluctuations. These two parts of the local electron density fluctuations satisfy the following equations (for particularities of the relevant derivation see [23] and the previous chapter): 2 F 2 ∂ 2 δ ρ˜1 (r,t) = (5.7) ∇ δ ρ˜1 (r,t) − ωp2 δ ρ˜1 (r,t), 2 ∂t 3m and (in the next equation = 0+ is introduced formally to ensure the correct definition of the Dirac delta),
∂ 2 δ ρ˜2 (r,t) 2 r 3 =− ∇ F ne + F δ ρ˜2 (r,t) δ(a + − r) ∂t 2 3m 5 r 2 ωp r 2 F r 1 ∇δ ρ˜2 (r,t) + ∇ d 3 r1 − (δ ρ˜1 (r1,t)(a − r1 ) 3mr 4π r r − r1  (5.8) + δ ρ˜2 (r1,t)(r1 − a)) δ(a + − r). For the solution of Eqs. (5.7) and (5.8) we represent the two parts of the electron fluctuation, as described in the previous chapter, in the following manner: for r < a, δ ρ˜1 (r,t) = ne F (r,t) δ ρ˜2 (r,t) = σ ( ,t)δ(r + − a), = 0 +
for r ≥ a (r → a+),
(5.9)
supplemented with the initial conditions F (r,t)t=0 = 0, σ ( ,t)t=0 = 0 ( is the spherical angle, representing the spherical coordinate, θ and ϕ), with the neutrality condition F (r,t)r→a = 0, and with ρ(r,t)d 3 r = Ne .
66
Damping of Plasmons in Metallic Nanoparticles
After some algebra (as presented in detail in [23] and in the previous chapter) one finds for a nanoparticle with spherical symmetry (i.e., a nanosphere) that the volume plasmons are described by F (r,t) =
∞ ∞ l
Almn jl (knl r)Ylm ( ) sin(ωnl t)
(5.10)
l=1 m=−l n=1
and the surface plasmons are described by l ∞ Blm σ ( ,t) = Ylm ( ) sin(ω0l t) a2 l=1 m=−l
+
∞ ∞ l l=1 m=−l n=1
a ×
Almn
(l + 1)ωp2 2 lωp2 − (2l + 1)ωnl
r1l+2 dr1 l+2 jl (knl r1 ) sin(ωnl t), a
Ylm ( )ne
(5.11)
0
√ where jl (ξ ) = π/2ξ Il+1/2 (ξ ) is a spherical Bessel function, Ylm ( ) is a spher
2 /(kT2 a 2 ) are the frequencies of the volume plasical harmonic, ωnl = ωp 1 + xnl mon selfoscillations, kT = 6ne e2 /F is the Thomas–Fermi length (F is the Fermi energy), and xnl are the nodes of the Bessel function jl (ξ ); knl = xnl /a and √ ω0l = ωp l/(2l + 1) are the frequencies of the electron surface selfoscillations (the surface plasmon frequencies). In the formula for σ ( ,t), the first term corresponds to the surface selfoscillations while the second term describes the surface oscillations induced by the volume plasmons. The frequencies of the surface selfoscillations corresponding to multipole modes enumerated by l have the form & l , (5.12) ω0l = ωp 2l + 1 √ which, for l = 1, gives the dipoletype surface oscillation frequency ω01 = ωp / 3 originally found by Mie [18] (for simplicity, hereafter we will set ω1 = ω01 ). The advantage of this RPA approach consists in the oscillatory form of both Eqs. (5.7) and (5.8). Plasmon damping can thus be included in a phenomenological manner, by the addition of an attenuation term to the plasmon dynamic equations, i.e.,
−
2 ∂δρ1(2) (r,t) , τ0 ∂t
is added to the righthand sides of Eqs. (5.7) and (5.8). The damping ratio 1/τ0 accounts for electron scattering losses and can be approximated by the formula [24]
5.1 Damped Plasmonic Oscillations in Metallic Nanospheres
1 vF CvF + , τ0 2λB 2a
67
(5.13)
where C is a constant of order unity, a is the nanosphere radius, vF is the Fermi velocity in the metal, and λB is the electron mean free path in the bulk metal (including the scattering of electrons from other electrons, from impurities, and from phonons [24]); for example, for Au, vF = 1.396×106 m/s and λB 53 nm (at room temperature); the latter term in formula (5.13) accounts for the scattering of electrons at the boundary of the nanoparticle, whereas the former term corresponds to scattering processes similar to those in the bulk metal (leading to irreversible ohmic energy losses). Other quantum effects, as for example Landau damping (especially important in small nanoparticles [80, 79]), corresponding to the decay of a plasmon to a highenergy particle–hole pair, are of less significance for nanosphere radii larger than 2−3 nm [80] and are completely negligible for radii larger than 5 nm. The electron response to the driving field E(t) (which is homogeneous over the nanosphere, corresponding to the dipole approximation) resolves to a single dipoletype mode, effectively described by a threecomponent function denoted here as Q1m (t) (l = 1 and m = −1,0,1). The dynamical equation (5.8) reduces in this case to the following: 2 ∂Q1m (t) ∂ 2 Q1m (t) + + ω12 Q1m (t) 2 ∂t τ0 ∂t & √
( 4π ene ' Ez (t)δm,0 + 2 Ex (t)δm,1 + Ey (t)δm,−1 , = 3 m
(5.14)
√ where ω1 = ωp / 3ε is the dipole surface plasmon frequency found with the semiclassical RPA approach [23] (ωp = 4πne2 /m is the plasmon resonance frequency in the bulk metal and ε is the relative permittivity of the material surrounding the nanosphere).√For ε = 1 this frequency coincides with the classical Mie frequency, ωMie = ωp / 2ε + 1 [17]. The semiclassical RPA dipole frequency ω1 is somewhat smaller than ωMie for ε > 1, as illustrated in Fig. 5.1; this result is supported by a more exact numerical TDLDA calculus indicating some overestimation of the plasmon resonance frequency by the Mie formula [81]. Note that the classical Mie frequency is based on a greatly simplified dielectric function for the metal [18, 17]. The electron density fluctuations described by Eq. (5.14) are as follows: ⎧ for r < a, ⎨ 0, 1 δρ(r,t) = Q1m (t)Y1m ( ) ⎩ m=−1
for r ≥ a, r → a + .
(5.15)
68
Damping of Plasmons in Metallic Nanoparticles
0.6 p.
0.5 0.4
Mie
0.3 RPA
0.2 2
4
6
8
10
Relative dielectric permittivity of surroundings ε
Figure 5.1 For comparison, the RPA semiclassical formula for the dipole √ resonance frequency of surface plasmons in a metallic nanosphere,√ ω1 = ωp / 3ε, and the classical formula of Mie for this frequency, ωMie = ωp / 2ε + 1.
For the dipoletype plasmonic oscillations presented by Eq. (5.15), the dipole d(t) of the electron system can be written as follows: √ ( ' √ 2π 3 2Q1,0 (t) (5.16) d(t) = e d rrδρ(r,t) = √ ea 3 Q1,1 (t) Q1,−1 (t) 3 and the d(t) satisfies the following equation (obtained via rewriting Eq. (5.14)), 2 a 3 4πe2 ne ∂ 2 ∂ 2 d(t) = + (5.17) + ω E(t) = εa 3 ω12 E(t). 1 ∂t 2 τ0 ∂t 3m According to Eq. (5.16) the plasmon oscillation dipole scales with the nanosphere radius a as ∼ a 3 , which indicates that all the electrons in the sphere contribute to the surface plasmon excitations. This can be referred to the fact that the surface plasmon modes correspond to uniform translationtype oscillations of the whole electron liquid. Inside the sphere the uniformly shifted charge of the electrons is still exactly compensated by the static and uniform positive jellium, while an unbalanced charge density fluctuation occurs only on the surface. One can note that in the case of the volume plasmons the noncompensated charge density fluctuations are present inside the sphere, because the volume plasmon modes are related to compressional modes resulting in volume charge fluctuations not balanced by the jellium along the radial direction inside the nanosphere. The damping term 1/τ0 accounts for dissipation of the plasmon energy by electron scattering, similarly to that for the ohmic losses. This channel of energy dissipation includes all types of scattering phenomena: electron–electron, electron– phonon, and electron–admixture collisions, as is usually the case for ohmic losses, but additionally a contribution related to electron scattering on the nanoparticle boundary [24]. All these scattering processes cause the attenuation of plasmons, and their energy is dissipated irreversibly and finally converted into heat.
5.1 Damped Plasmonic Oscillations in Metallic Nanospheres
69
By reducing structural imperfections in the metal one can diminish these losses to some limiting value. The electron scattering channel of plasmon attenuation turns out to be especially important for small metallic nanoparticles, for which it is the predominant mechanism of plasmon damping, together with Landau damping [80, 79]. In small metallic nanoparticles radiation effects have a negligible role because of the low total number of electrons (∼ 100−300 for radius a ∼ 2−3 nm). Instead, for ultrasmall nanoparticles, nanosphereedge scattering plays a significant role as its contribution to the dampingtime ratio is proportional to 1/a and thus is large for small a but quickly diminishes when the radius increases. The scattering of electrons by the boundary of the nanosphere may undergo different regimes depending on the microscopic details of the surface. One can correct these regimes to two limiting model scattering types, reflection and diffusive, which differ in their attenuation rate. In order to model various types of boundary scattering of electrons one can introduce in Eq. (5.13) an effective constant C of the order of unity which can be helpful in accommodating the theory to the experimental data, utilizing the 1/a scaling of this attenuation channel. Below we will show that radiation losses, which also contribute to the overall attenuation of plasmons, start to be important in the case of larger metallic nanoparticles with a sufficiently large number of electrons. Radiation losses scale as a 3 (for nanospheres that are not too large, e.g., for Au up to about 30 nm) and therefore radiative losses quickly dominate the plasmon damping at the range of 10 nm (for Au, Ag, and Cu). Therefore, at some particular nanosphere size we encounter a crossover in the size dependence of the plasmon damping: for lower radii the size dependence scales as 1/a whereas for larger radii it scales as a 3 [77]. This pronounced crossover in the size dependence of surface plasmon damping is illustrated in Fig. 5.3. The radiation energy losses of oscillating electrons related to the surface plasmon timedependent dipole can be expressed by the Lorentz friction [55], i.e., by an
red
purple
violet
blue
Figure 5.2 In an experiment [77] with light passing through a colloidal solution of Au nanoparticles one can measure the extinction of light for various wavelengths; that depends strongly on the nanosphere size, resulting in a variation in the colour for colloidal solutions with different sized particles.
70
Damping of Plasmons in Metallic Nanoparticles
effective electric field hampering the movement of charges and thus lowering the amplitude of dipole oscillations: 2 ∂ 3 d(t) . 3c3 ∂t 3 Hence, one can rewrite Eq. (5.17) including the Lorentz friction term as 2 2 ∂ ∂ 2 + + ω1 d(t) = εa 3 ω12 E(t) + εa 3 ω12 EL, ∂t 2 τ0 ∂t EL =
or, in a more explicit form, for the case E = 0 we have 3 2 2 ω a ∂ ∂ ∂ 2 2 p + ω12 d(t) = d(t) . − d(t) + √ √ ∂t 2 ∂t τ0 3ω1 ε c 3 ∂t 2
(5.18)
(5.19)
(5.20)
One can solve Eq. (5.20) by application of the perturbation calculus, i.e., one can treat the righthand side of this equation as a small Therefore, in * ) 2perturbation. ∂ 2 the zeroth step of the perturbation calculus we get ∂t 2 + ω1 d(t) = 0 and thus (∂ 2 /∂t 2 )d(t) = −ω12 d(t). Next, in the firstorder step of the perturbation method, we substitute the latter formula into the righthand side of Eq. (5.20), obtaining, 2 2 ∂ ∂ 2 (5.21) + + ω1 d(t) = 0, ∂t 2 τ ∂t where the effective attenuation rate is given by 1 ωp a 3 ω1 1 + √ . = √ τ τ0 3 ε c 3
(5.22)
In these steps the Lorentz friction is accounted for in the total attenuation rate 1/τ utilizing the approximate perturbative linearization of the thirdorder derivative in Eq. (5.18). Such an approximation leads to an effective model of radiation losses within the scheme of the damped harmonic oscillator. Nevertheless, as mentioned previously, this approximation is justified only for small perturbations, i.e., when the radiation term, the second term in Eq. (5.22), which is proportional to a 3 , is sufficiently small, as required by the perturbation calculus limits. For nanospheres of radii a < 30 nm (e.g., for Au in vacuum) the perturbation constraints are not violated; this has been independently confirmed experimentally for Au and Ag nanospheres [77]. For nanosphere radii 5−30 nm the perturbation approximation explains the experimentally observed redshift of the resonance surface plasmon frequency with increasing radius a, recordable from the measurement of light extinction spectra [77]. In this case the solution of Eq.(5.21) has the following form: d(t) = d0 e−t/τ cos(ω1 t + φ), where ω1 = ω1 1 − 1/(ω1 τ )2 gives the experimentally observed redshift of the plasmon resonance owing to the ∼ a 3
5.2 Attenuation with Exact Inclusion of Lorentz Friction
71
Crossover of plasmon damping (Au vacuum, water)
Lorentz friction a3
C=1
0.04 0.03
0.35
0.02
0.30 0.00
0.25 0.04
1/(tw)
C=4
0.08
exact
0.06 0.01
0.20
scattering 1/a
perturbative
0.10
total
0.04
ε=2
C=1
0.02
5
10
15
20
0.00
ε=2
10
15
20
25
C=1
Lorentz friction a3
perturbative
total
0.03 scattering 1/a
5
0.02
0.15 0.10
0.01 0.00
ε=1 5
10
15
ε=1 0.05 0.00
5
10
15
exact
20
20
ε=2 25
30
35
40
a (nm)
Figure 5.3 For comparison, the different contributions to plasmon oscillation damping (Au nanoparticles in vacuum and in water) in the size region a ∼ 10−20 nm (in insets), where the crossover in the size dependence of the damping rate takes place. In the upper right inset the effect of changing the constant C in Eq. (5.13) is illustrated; this models two scattering regimes for electrons on a nanosphere boundary.
increase in damping caused by radiation losses in this size window. The Lorentz friction term in Eq. (5.22) starts to dominate plasmon damping for approximately a ≥ 12 nm (for Au and Ag it is almost independent of the relative permittivity of the surrounding medium ε, as is illustrated in the insets to Fig. 5.3) owing to its strong a 3 dependence; see Fig. 5.3. The plasmonic oscillation damping grows sharply with a, causing a redshift of the surface dipole plasmon resonance that is in very good agreement with the experimental data for 10 < a < 30 nm (Au and Ag) [77]. 5.2 Attenuation of Dipole Surface Plasmons with Exact Inclusion of the Lorentz Friction Let us consider the dynamic equation (5.20) for surface plasmons in a metallic nanosphere, now without substituting the Lorentz friction term
72
Damping of Plasmons in Metallic Nanoparticles
ωp a 3 ∂ 3 d(t) √ ∂t 3 c 3 by the approximate perturbative formula 2ω1 ωp a 3 ∂d(t) − √ . √ ∂t 3 ε c 3 2 √ 3ω1 ε
This approximate linearization of the thirdorder derivative of d(t) is justified only when the total attenuation term ! 2 ωp a 3 ∂ 2 ∂ 2 − + d(t) √ √ ∂t τ0 3ω1 ε c 3 ∂t 2 is sufficiently small. To compare the different contributions to Eq. (5.20) one must change to a dimensionless time variable t = ω1 t. Then Eq. (5.20) attains the form ωp a 3 ∂ 3 d(t ) ∂ 2 d(t ) 2 ∂d(t ) 2 + + d(t ) = √ . (5.23) √ τ0 ω1 ∂t 3 ε c 3 ∂t 2 ∂t 3 In Eq. (5.23) the dimensionless damping ratio caused by scattering is given by vF 2 vF 2 0.027 = + τ 0 ω1 ω1 2λb 2a for a = 10 nm (values for the other parameters are those for Au and Ag, as collected in Table 5.1) and diminishes with increasing radius a; see the Fig. 5.3 insets. One can also estimate the dimensionless coefficient of the Lorentz friction term in Eq. (5.23). It equals to ωp a 3 2 √ √ 3 ε c 3
Table 5.1 Nanosphere parameters assumed for calculation of the damping rates for surface plasmons Material
Au
Ag
bulk plasmon energy, hω ¯ p bulk plasmon frequency, ωp Mie dipole plasmon energy, √ h¯ ω1 Mie frequency, ω1 = ωp / 3 constant in Eq. (5.13), C Fermi velocity, vF bulk mean free path (room temp.), λB
8.57 eV 1.302 × 1016 /s 4.94 eV 0.752 × 1016 /s 1, 4 1.396 × 106 m/s 53 nm
8.56 eV 1.3 × 1016 /s 4.93 eV 0.75 × 1016 /s 1, 4 1.4 × 106 m/s 57 nm
5.2 Attenuation with Exact Inclusion of Lorentz Friction
73
and rapidly increases with the radius a because it is proportional to a 3 (for a = 10 nm it is rather small, 0.0104 but for a = 25 nm it increases more than ten times to 0.1638; the example is taken for Au nanospheres in vacuum). Utilizing the perturbation method to solve Eq. (5.23) one obtains the renormalized attenuation rate for the effective damping term in the form ωp a 3 1 1 + √ . √ ω1 τ 0 3 ε c 3 Owing to the rapid increase of the factor a 3 with the radius a, the effective damping term obtained by the perturbation approach quickly reaches the value 1, for which the oscillator enters the overdamped regime. The value 1 of this renormalized attenuation rate is attained at a 57 nm (for Au in vacuum). Nevertheless this is an artefact of the perturbation calculus, and one can check that the exact solution of Eq. (5.23) agrees sufficiently well with the solution obtained using the perturbation approach only up to a ∼ 20−30 nm. For higher values of a the rapid increase in the effective attenuation rate causes an unacceptable discrepancy between the perturbation approximation and the accurate solution, as we illustrate in Figs. 5.4 and 5.5. In Fig. 5.5 the selffrequency and the damping rate for dipoletype surface plasmons are plotted as functions of the nanosphere radius a, for the perturbation approximation, for which + , !2 , ωp a 3 1 1 + √ , ω = ω1 1 − √ ω1 τ 0 3 ε c 3 and for the exact solution of Eq. (5.23). The lines corresponding to the approximate solution end at a 57,64,69,72,75 nm (for Au with the relative dielectric permittivity of the surroundings ε = 1,2,3,4,5, respectively). At these values of a the effective attenuation rate found from the perturbation calculus reaches the limiting value 1 (when the corresponding resonance frequency vanishes and the resonance wavelength λ = c2π/ω → ∞). This limiting behaviour corresponds to the termination of oscillating solutions of the perturbative oscillatory equation. In this case we are in the overdamped regime, with an aperiodic solution. This is, however, an artefact caused by the perturbation solution method, which cannot be applied for too high a value of the perturbation term. For an exact solution of Eq. (5.23) this singular behaviour disappears and an oscillating solution exists for larger a as well. Thus, one can see that the plasmon resonance redshift is strongly overestimated within the framework of the perturbative approach to the
74
Damping of Plasmons in Metallic Nanoparticles Resonance frequency Au 1.0
1
0.8 0.6
exact
0.4
perturbative
0.2 0.0
0
20
40
60 80 100 120 140 a (nm)
Damping rate Au perturbative
0.25 0.20 1
exact
0.15
0.15 0.10
0.10
C=4
0.05
0.05 0.00
0.00
0
20
40
C=1 5
10
15
20
25
30
60 80 100 120 140 a (nm)
Resonance wavelength Au
1. × 10– 6
perturbative
(m)
8. × 10– 7 6. × 10– 7 exact
4. × 10– 7 2. × 10– 7
0
20
40
60 80 100 120 140 a (nm)
Figure 5.4 (Left and centre) The real and imaginary parts of the exact oscillating solution of Eq. (5.23): the resonance frequency and the damping rate given by Eqs. (5.24) are plotted as functions of the nanosphere radius a for two distinct dielectric surrounding media (vacuum and water); the lines corresponding to the perturbative solutions are presented for comparison. In the righthand panel the resonance wavelength is depicted versus the radius a for vacuum (ε = 1) and water surroundings (ε = 2); in the inset in the central panel the impact of the constant C in Eq. (5.13) is illustrated.
Lorentz friction unless the nanosphere radius is lower than ∼ 20 nm (for Au in vacuum). The dynamical equation for dipole surface plasmon excitations including the exact form for the Lorentz friction, i.e., Eq. (5.23), is a thirdorder linear differential
5.2 Attenuation with Exact Inclusion of Lorentz Friction Resonance frequency (Au)
75
Damping rate (Au)
1.0
1.0
0.8
0.8 exact
0.6
1
1
perturbative
0.6
0.4
0.4
0.2
0.2
exact
perturbative
0.0
0
20
40 60 a (nm)
80
100
0.0
0
20
40 60 a (nm)
80
100
Figure 5.5 The resonance frequency and the damping rate for the oscillating solutions of Eq. (5.23), for five different values of ε. The exact and the approximate perturbative approach dependences are presented. The termination of the perturbative solutions displays an artefact of the perturbation method.
equation. This equation can be solved exactly and the exponent coefficients of its solutions ∼ ei t can be listed in the following analytical form: i21/3 (1+6lq) iA − 21/3 = iα ∈ Im, 3l A 3l √ √ i(1−i 3)A − 3li + i(1+i22/33)(1+6lq) + =ω 1/3 3l A 2 6l −ω + i τ1 = − ∗2,
1 = − 3li −
2 =
3 =
+ i τ1 ,
(5.24)
) *1/3 ,q = 2 + 27l 2 + 18lq + 4(−1 − 6lq)3 + (2 + 27l 2 + 18lq)2 ) * 3 √ √ 1/τ0 ω1 and l = (2/3 ε) aωp /c 3 . Here Im stands for the set of imaginary numbers. The functions ω and 1/τ (in dimensionless units, i.e., divided by ω1 ) are plotted in Fig. 5.4 versus the nanosphere radius a. We note that Eq. (5.23) has two types of particular solutions ei t , with complex selffrequencies as given in Eq. (5.24). The solutions given by 2 and 3 describe oscillating behaviour with frequency ω and positive damping (note that i 2 and i 3 are mutually conjugate; thus 2 and 3 have real parts of opposite sign, but the same imaginary parts, these latter, being positive, correspond to the ordinary damping rate for positive time). The selffrequency given by 1 turns out to correspond to an unstable exponentially rising function, as 1 is a purely negative imaginary solution. Such an unstable solution is a wellknown artefact in Maxwell electrodynamics (see e.g. [55] for the particularities) and corresponds to infinite selfacceleration of a free charge exposed to the action of the Lorentz friction force. This solution in turn corresponds to a singular solution of the equation m˙v = const. × v¨ , which is associated with the formal renormalization of the socalled field mass of the charge. The field mass in Maxwell electrodynamics is infinite for a pointlike charge and is assumed to be cancelled by an arbitrarily where A =
76
Damping of Plasmons in Metallic Nanoparticles
assumed negative infinite nonfield mass, resulting in the ordinary mass of the charge (this is, however, not defined mathematically in a proper way, which links with some inconsistency in the classical electrodynamics of pointlike charges). Therefore, this unphysical singular particular solution should be discarded. The other, oscillatorytype, solutions describe damped oscillations which resemble the solution of the ordinary damped harmonic oscillator. It must be emphasized, however, that Eq. (5.23) does not describe a damped harmonic oscillator and therefore the attenuation rate and frequency (1/τ and ω as given by Eq. (5.24)) do not agree with corresponding quantities for an ordinary damped harmonic oscillator. They are expressed by the analytical formulae for 2 or 3 in Eq. (5.24). They can be easily evaluated for various values of a and compared with corresponding quantities found within the perturbationcalculusbased approach. Such a comparison is illustrated in Figs. 5.4 and 5.5. From the comparison presented in Fig. 5.4 one can note that application of the perturbation approach leads to a highly overestimated damping rate for a > 30 nm (for Au in vacuum). For 30 < a < 50 nm, for gold nanoparticles, a small underestimation of the resonance wavelength occurs whereas for a > 50 nm there is a rapid and very strong overestimation of the resonance wavelength, as illustrated in the lefthand panel in Fig. 5.4. Moreover, as has already been mentioned above, the approximate solution terminates at a = 57,64,69,72,75 nm (for Au; ε = 1,2,3,4,5 respectively), above which an approximate oscillatorytype solution does not exist within the perturbative calculus approach. One can finally conclude that utilization of the approximate formula to account for Lorentz friction damping in the form given by (5.22) is justified up to a 20 nm (for Au in vacuum); it causes only a small discrepancy (a practically negligible error in the damping rate and only a small underestimation of the resonance wavelength) at 20 < a < 30 nm. However, for a > 30 nm, for Au, these approximate perturbative parameters of the oscillatory plasmon excitations deviate strongly from the exact values. Also illustrated in Figs. 5.4 and 5.5 are the dependences of the limiting values for the radii listed above, which relate the accuracy of the perturbation approach for the radiative losses of plasmons to the relative permittivity of the surroundings of the metallic nanoparticles, ε. The accurate value of the damping rate as plotted in Fig. 5.4 reaches its minimum at a certain value of the nanosphere radius, ∗
a =
9 vF c3 ε 2 ωp4
1/4 ,
(5.25)
and reaches its maximum at a ∗∗ . We note that the latter value might be defined as the zero point of the appropriate derivative expressed analytically using Eq. (5.24), though the related formula for this derivative is cumbersome owing to the
5.3 Comparison with Data and Simplified Mie Approach
Table 5.2 Radius of the nanosphere corresponding to the minimal maximal (a ∗∗ ) values of surface plasmon damping
77
(a ∗ )
and
a ∗ , a ∗∗ (nm)
√ n= ε
Au
Ag
n = 1, vacuum n = 1.4 n=2
8.77, 57.4 10.4, 64.3 12.4, 72
8.78, 57.42 10.4, 64.4 12.4, 72.1
complicated analytical expression for the function 1/τ given by Eq. (5.24)). Both a ∗ and a ∗∗ are listed in Table 5.2 for ε = 1,2,4 (a ∗∗ depends weakly on the material, Au or Ag, whereas it depends strongly on the relative permittivity of the dielectric surroundings and is located approximately at 57 nm (for Au in vacuum)). 5.3 Comparison of Surface Plasmon Oscillation Features Including Lorentz Friction with the Experimental Data and Simplified Mie Approach For comparizon of the model results for surface plasmon damping in a metallic nanosphere with the experimentally observed behaviour, one can use published experimental data [77] for the extinction of light after passing through watercolloidal solutions of Au nanospheres with varying radii. Extinction peaks that correspond to plasmon excitations in metal nanospheres are plotted in Fig. 5.8, in the lefthand panel. In the righthand panel of this figure analogous data for Ag nanoparticles are presented for comparison, though the fit is not so good as for Au, most probably owing to surface imperfections of Ag nanospheres and their possible reshaping. For the Au nanoparticles, the coincidence of the peak positions, their widths, and the evolution with increase of the nanosphere radius is visible on comparison of Fig. 5.6 with Fig. 5.8. From the experimentally collected extinction peaks presented in Fig. 5.8 (left) one can extract their centre positions with respect to the nanosphere radius a. These points perfectly fit the resonance selffrequencies defined by the exact solution of Eq. (5.23) obtained by including the Lorentz friction. This coincidence of the exact solution with the experimental data points is visualized in Fig. 5.7 (left). In this figure the approximate perturbative curve is also plotted for comparison. The increasing discrepancy between the approximate perturbative solution and the experimental data for larger nanosphere radii is clearly visible, in contrast with the satisfactory agreement with the exact solution. Better fitting is obtained after inclusion of the skin effect renormalization for the Lorentz friction term by slightly reducing the number of electrons accessed by the
78
Damping of Plasmons in Metallic Nanoparticles Extinction spectra – model, Au nanoparticles 16
20
25
Intensity (a.u.)
14
40
15
12 10
50
8
75
6 4
10
2 0
400 450 500 550 600 650 700 750 800 850 900 Wavelength (nm)
Figure 5.6 Extinction spectra for nanoparticles of Au calculated as Lorentzian functions with centre positions and widths given by the resonance frequencies and damping rates of Eq. (5.24), for nanosphere radii as indicated. The similarity to the attenuation curves obtained by measurements [77] of extinction spectra for light passing through a small glass container filled with a watercolloidal solution of metallic nanospheres with various radii and with the same volume density of metallic components is noticeable; see the lefthand panel in Fig. 5.8. Wavelengths for plasmon resonance (Au, water) 9 × 10−7
9 × 10−7 experiment
experiment theory (Lorentz fr. exact)
l (m)
l (m)
8 × 10−7
theory (Lorentz fr. perturbative)
7 × 10−7 6 × 10−7 5 × 10−7
8 × 10−7
theory (Lorentz fr. exact) theory (Lorentz fr. perturbative)
7 × 10−7 6 × 10−7
0
20
40 60 a (nm)
80
100
5 × 10−7
0
20
40
60
80
100
a (nm)
Figure 5.7 (Left) For comparison, resonance selfenergies (expressed in terms of wavelength) for radiatively damped surface plasmons and experimental data from extinction measurements (data after [77]) for Au nanospheres in colloidalwater solution with radii 10, 15, 20, 25, 30, 40, 50, 75 nm: points, experiment; grey line, perturbative approximation; black line, exact inclusion of the Lorentz friction (ε = 2.6 and ωp renormalized by a factor 0.78, the same as in Fig. 5.6). (Right) A similar comparison for the surface plasmon resonances in colloidal Au particles of different radii (experimental data for radii 2.6, 10, 20, 25, 30, 40, 50, 60 nm, after Fig. 12.17 in [17]).
incident light wave to those in an activation layer of thickness h, i.e., by the factor (a 3 − (a − h)3 )/a 3 , where h < a, and by the accompanying reduction in plasmon frequency due to the lowering of the effective density. For the fittings presented in Fig. 5.7 we assumed a realistic skineffect layer thickness with corresponding reduction in the plasmon frequency.
79
Intensity (a.u.)
Intensity (a.u.)
5.3 Comparison with Data and Simplified Mie Approach
Wavelength (nm)
Wavelength (nm)
Figure 5.8 Attenuation curves for nanoparticles of Au (left) and Ag (right) obtained by measurement of extinction spectra for light passing through a watercolloidal solution of metallic nanospheres with various radii (after [77]); the deformation of the regular Lorentzian extinction feature shape is noticeable at a = 75 nm (Au) and at a = 30,40 nm (Ag).
The size dependence of the redshift of the surface plasmon resonances observed experimentally [82, 22, 77] can also be interpreted using the Mie approach [17, 83, 84]. To explain the crossover in the size dependence of the experimentally observed redshift of the plasmon resonance with increasing nanosphere radius, within the Mie theory two regimes are considered [83]: an intrinsic size effect (for a < 20 nm, for Au) and an extrinsic size effect (for a > 20 nm). The intrinsic size effect is associated with the dipole approximation of the Mie response, which is justified for nanosphere radii considerably smaller than the surface plasmon resonance wavelength. To account for absorption in the Mie approach, the dielectric function of the metallic nanosphere is accounted for phenomenologically. For relatively small particles, as in the case of the intrinsic size effect, this dielectric function includes electron scattering (as given by Eq. (5.13)), which results in a ∼ 1/a redshift of the dipole Mie resonance. Nevertheless, for larger nanospheres (with a greater than about 20 nm, for Au), for which it is observed experimentally that the resonance redshift rises with increasing a, the second mechanism is suggested in the Mie theory and referred to as the extrinsic size effect [83, 22]. The extrinsic regime in the Mie theory amounts to the inclusion of multipole mixing in the electromagnetic response, which leads to a related shift of the resonance energy with growth in radius. To obtain agreement with the experimentally observed size effect in the redshift of the plasmon resonance for larger nanospheres, the radiation correction to the dielectric function is introduced in the form of a model damping term proportional to the number of electrons and thus ∼ a 3 [84]. This overestimates, however, the radiative damping and in the extrinsic limit for the size effect in the Mie theory this toohigh redshift is reduced by inclusion of
80
Damping of Plasmons in Metallic Nanoparticles
the multipole components in the Mie response; this lowers the redshift for larger nanosphere radii. This lowering of the redshift is due to the increasing contribution of multipole plasmon excitations to the overall Mie response when the radius grows beyond the dipole approximation limit and to the related increase in the resonance energy [17], mitigating the redshift. A similar growth in the multipole surface plasmon resonance frequency is also observed in the framework of the RPA approach [23]; cf. Eqs. (5.11) and (5.12), where the multipolemode frequencies √ are ω0l = ωp l/(2l + 1) and they increase with l. To explain the Lorentzfrictioninduced corrections, let us first address the mutual links between the Mie theory and the microscopic RPA method. Note from [22] that the major drawback of the Mie theory and its modifications is that the underlying electron relaxation mechanisms responsible for the absorption of incident light are all included in the macroscopic material dielectric function, which does not distinguish between several possible energy dissipation processes. A microscopic picture for the plasmon absorption is therefore lacking within the Mie theory. It means that the Mie theory, which is a classical solution of the Maxwell equations for an incident planar electromagnetic wave with imposed spherical boundary conditions, does not include the internal electron dynamics in the metal except in the phenomenologically modelled dielectric function. The electron scattering processes, i.e., the dissipation due to electron–electron scattering, electron–phonon collisions, electron scattering from admixtures or crystal imperfections, and the nanoparticle boundary scattering, can be in principle calculated using the manybody framework typical for solids (such as the collision term in the Boltzmann equation or more generally by the Green function approach). All these contributions lead to the scattering time rate given by Eq. (5.13). This dissipationchannel time rate is used also in the Mie theory for small nanoparticle radii, for which in experiments a redshift proportional to 1/a is observed (note that Landau damping and the redshift scale similarly owing to spillout, which is important in ultrasmall nanoparticles (1−3 nm) [19] but negligible for radii of order 10 nm). For this range of radii (∼ 10 nm for Au) the dipole approximation holds, and this simplifies the Mietype response. Thus, the inclusion of the scattering using Eq. (5.13) gives reasonable agreement with experimental observations both in the Mie theory and in other approaches, including RPA. Within the Mie approach this is conveyed by the intrinsic size effect. Nevertheless, for larger radii (greater than about 20 nm for Au) the experimentally observed resonance redshift is not proportional to 1/a but, rather, is proportional to a or to some power of a, e.g., a 3 (for a not too large). As an intrinsic mechanism including only electron scattering does not offer such a behaviour, in the Mie response radiation losses are also taken into account [84] and simultaneously the mixing of multipole components is proposed. One can thus explain the experimentally observed inverted redshift because it rises with a, though irregularly for larger nanospheres as it is due
5.3 Comparison with Data and Simplified Mie Approach
81
to an increase in the radiationinduced damping. This is reduced, however, by multipole resonances which are shifted with lmultipole mode number towards higher energies. Nevertheless, the frontier between the dipole and multipole limits is not sharply defined and, rather, can be accommodated to the experimental data. The reason is that the resonance surface plasmon wavelength is around 500 nm (for Au), and even shifts with growth in radius to around 650 nm. Thus radii of 20 or 30 nm do not differ significantly on the wavelength scale and indeed the important multipole contribution occurs rather for larger nanospheres, at approximately a > 60 nm, as 2a/650 = 0.18 for a = 60 nm is much lower than onequarter of a wavelength and thus the electric field of an incident electromagnetic wave is still sufficiently homogeneous over the whole nanosphere; this justifies the dipole approximation. The Lorentzfrictioninduced radiation losses, which, for radii a < 10 nm (for Au), are much lower than the scattering term given by Eq. (5.13), for a > 12 nm strongly contribute to the plasmon energy dissipation (for Au in vacuum and for radii that are a little larger in the case of water surroundings), as visualized in Fig. 5.3. At these radiis the inverse time for dissipation caused by the radiation of energy (Lorentz friction) is similar to the inverse time for dissipation caused by scattering; indeed, if one estimates it from Eq. (5.13) for a = 12 nm, one obtains 7×1013 /s, and the second term in Eq. (5.22), the Lorentz friction term, is of the same magnitude. For larger a the Lorentz friction losses quickly dominate the plasmon damping, as depicted in Fig. 5.3. Thus for nanospheres with radii of the order of 5−10 nm (and even up to 15 nm, see Fig. 5.3) the Mie approach, neglecting the Lorentz friction losses, gives a reasonable intrinsic size effect. This is, however, not so when we are well past the crossover point and arrive at a ∼ 15−25 nm or more. For such radii, radiation losses dominate plasmon damping by a factor greater than 1 (it is about 5 at a = 20 nm). This was not included in the conventional Mie theory for the intrinsic size effect. Thus, the radiative damping of plasmons (i.e., the Lorentz friction) must be included (for a > 12 nm, at least) in the modelled (even by a simplified Lorentzian) dielectric function of the metallic nanosphere. This will give the required redshift in the corrected intrinsicsizeeffect regime even using the dipole approximation only. The irregular size effect of plasmon damping caused by the Lorenz friction, if accounted for accurately, explains well the experimentally observed irregular (i.e., not proportional to a 3 ) size effect for the redshift. This Lorentzfrictioninduced correction mixes, however, with the extrinsic size effect due to the multipole contributions, but it does this for radii a > 60 nm (for Au), significantly exceeding the previously suggested limit of 20 nm [83, 22, 84]. The quadrupole contribution, and the higher multipoles at larger radii, result in the deformation and further broadening of the extinction features, no longer allowing a Lorentzian form (the higherenergy quadrupole secondary broad peak occurs first at a smaller wavelength in association with the dipole peak, which is broadened
82
Damping of Plasmons in Metallic Nanoparticles
and red shifted by the Lorentz friction). In experiments it is visible for Au at 75 nm and Ag at 30−40 nm [77, 82]. Remarkably, for Ag this deformation of the extinction features occurs at smaller radii than for Au [77, 82], see Fig. 5.8; this is probably due to the lower resonance wavelength for Ag nanospheres (about 400 nm) and moreover to scattering by the nanosphere facets, charges, or molecular contamination [82]. Reference [83] raises the question of the role of stabilizing molecules attached to the surface of nanoparticles to prevent them from aggregation or precipitation in solution and also other contaminations of the nanoparticle surface which could affect the scattering and absorption of light in an extinction experiment with colloidal solutions of the more chemically reactive metals (such as Ag, in comparison to Au). By using an accurate treatment for the Lorentz friction term it was shown that the ∼ a 3 growth of the radiationinduced damping of plasmons accounted for phenomenologically in the Mie theory quickly saturates, which is quite reasonable and, what is more important, it agrees well with the experimental observations; it is clear that cubic growth cannot continue and must saturate and, actually, the curve even starts to drop for larger a, as shown in Figs. 5.4 and 5.5. Thus, inclusion of the exact form of the Lorentz friction damping rate, as given by Eqs. (5.24), in the modelled dielectric function for a nanosystem (needed in the Mie theory and especially important in the intrinsicsizeeffect regime) is a significant correction to the Mie approach and contributes to the interpretation of light extinction measurements for Au nanospheres with radii in the region of 10–80 nm. Thus the intrinsic regime with the inclusion of Lorentz friction can be extended to larger radii (up to about 60 nm for Au), where the extrinsic multipole effect starts to contribute with gradually growing intensity for higher radii; however, up to 60 nm the extrinsic effect mixes rather weakly with the effects of saturation and lowering of the damping rate due to Lorentz friction. Multipole corrections cannot be avoided for radii a > 60 nm, as is evident from the deformation of the Lorentzian shape of the extinction features, accompanied by their significant broadening, for Au observed at a = 75 nm [77, 82]. The accurate microscopic analysis of the Lorentz friction carried out within the RPA approach supports the modelling of the dielectric function needed in the Mie theory and thus can be utilized to prolong the intrinsic size effect in the Mie approach beyond the 20 nm size limit, to larger radii for which the dipole approximation still holds (up to approximately 60 nm for Au). One should note however, that since the dielectric function simultaneously represents all energy dissipation channels in a combined manner, details of the size effect caused by the exact form of the Lorentz friction (beyond the scope of the Mie theory at present [84]) must be included in the modelled dielectric function. Thus, the specific size dependence of the damping time rate for plasmons due to Lorentz friction, derived from an exact solution of the relevant RPA equation for the electron density dynamics
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
83
in nanospheres (as depicted in Figs. 5.4 and 5.5), may be employed to explain the observed irregular size effect of plasmon resonance in the radius window 10−60 nm for Au. We can conclude that the damping of surface plasmons in large metallic nanospheres is overwhelmed by the radiation energy losses, which strongly exceed the electron scattering attenuation of plasmons for nanosphere radii larger than a critical value (approximately 12 nm for Au in vacuum). The radiation losses can be expressed by the socalled Lorentz friction, which hampers plasmon oscillations in a metallic nanoparticle. The related damping rate is proportional initially to the volume of the nanosphere; this results from the perturbative approach to the Lorentz friction contribution to plasmon damping. This rapid increase of the radiation losses saturates, however, for larger nanospheres and then slowly drops down. The deviation of the perturbative approximation with respect to the exact Lorentz friction term grows quickly for a > 30 nm (for Au in vacuum) and means that one has to dismiss the harmonic damped oscillator approximation as a model of plasmon damping. The solution of the dynamical equation for the local electron density including the exact form of the Lorentz friction determines both the resonance frequency of plasmons and their damping beyond the damped harmonic oscillator model. The related irregular sizedependent redshift of the plasmon dipole resonance agrees very well with the experimental data for metallic nanospheres with large radii (10−75 nm for Au). 5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles The ability to manipulate light at a sub wavelength scale is attributed to highenergy collective excitations in metals called plasmons. The properties of these excitations in metallic nanoparticles depend on their size and shape, on the surrounding medium, and on the light frequency [85–87]. The unique properties of plasmons in metallic nanostructures have found applications in photonics, optoelectronics, and photovoltaics [2, 88, 89, 3]. The classical solution of the metal–insulator Fresnel problem with spherical boundaries was found by Mie [18], and was soon generalized to the spheroidal case [90]. Mie theory utilizes the decomposition of a planar electromagnetic wave in a basis of spherical functions, as is appropriate for the spherical boundary conditions imposed by the geometry of small metallic particles that are scattering and absorbing incident light. This problem can be solved analytically within classical electrodynamics, but the metal characterization must be made phanomenologically in the form of a model dielectric function defining the metallic material. The assumed dielectric function is modelled from experimental data for bulk samples, and the strong size dependence at the nanoscale is typically neglected. The aim was to improve the predefined dielectric function by utilizing the knowledge of plasmons
84
Damping of Plasmons in Metallic Nanoparticles
in metallic nanoparticles gained from the quantum RPA method, as presented in previous sections. This approach allows for precise modelling of the dielectric function for a nanoparticle, but only of spherical shape. For an analysis of plasmons in nanoparticles of an arbitrary shape, numerical methods must be employed. For the solution of such problems many methods have been developed based on the finite element approximation for the solution of the Maxwell–Fresnel differential equations, including, e.g., the finite difference time domain method [91, 92] and the boundary element method [93]. The main idea of such numerical calculations of the electromagnetic field distribution is a simulation of the space–time field dynamics on a discrete predefined grid and the achievement of convergence when the scale of the grid is shortened. There have been reported extensive numerical studies of the optical properties of metallic nanoparticles in a variety of particle shapes [29, 84, 95, 95]. Also, shelltype particles [94] including those covered with a dielectric [96] have been studied. Easy access in numerical simulations to the variation of both the shape and size of the metallic elements allows for the recognition of plasmon resonances in the case when multipole modes contribute to the electromagnetic response [29, 84]. Nevertheless, all numerical simulations of the electromagnetic response of metallic nanostructures are limited by a serious drawback relating to the predefined dielectric function of a metal component, which is a prerequisite for a numerical procedure. This dielectric function is usually taken from experiment, but in bulk or thinfilm geometries, and is much different from that for a nanostructure, which has, however, not been measured. The most significant error is related to the neglect of the strong plasmon damping in nanostructures, which is not present in the bulk substance. Simplified phenomenological trials to model the plasmon damping in nanoparticles are also insufficient. As shown above, the perturbation approach, resulting in an a 3 growth in the plasmon damping is, however, not justified for radii a > 30 nm (for Au in vacuum) [26]. To enhance the accuracy an exact formula for the plasmon damping must to be utilized, which gives the proper behaviour of the Lorentz friction in metallic nanoparticles. Instead of the ∼ a 3 rapid increase, saturation of damping growth occurs, as depicted in Fig. 5.9. The perturbation approach may be used only for particles with radii lower than about 30 nm (Au); for larger nanoparticles the exact solution of the dynamical equation for plasmons differs significantly. This has a pronounced consequence that plasmon oscillations in larger nanoparticles are not of the harmonic type. In particular, the relation between the damping rate and the frequency shift, being of damped oscillatortype form, & ω1
=
ω12 −
1 , τ2
(5.26)
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles Resonance frequency Au
0.6
exact
0.4
perturbative
0.20 0.15
6. × 10−7 exact
4. × 10−7
0.15 0.10
0.10
2. × 10−7 0
20
40
60
80
a (nm)
100 120 140
C=4
0.05
0.05
0.2 0.0
exact
1
(m)
1
perturbative
8. × 10−7
0.8
Damping rate Au 0.25 perturbative
Resonance wavelength (Au)
1. × 10−6
1.0
85
0
20
40
60 80 100 120 140 a (nm)
0.00
0.00
0
20
40
C=1 5
10
60
15
80
20
25
30
100 120 140
a (nm)
Figure 5.9 The real (lefthand panel) and imaginary parts (righthand panel) of the exact oscillating solution given by Eq. (5.27) versus nanosphere radius a, for two distinct dielectric surrounding media (vacuum and water). The resonance frequency expressed as the resonance wavelength (central panel). The lines corresponding to the perturbative solutions are presented for comparison; in the inset in the righthand panel the effect of changes in the constant C in Eq. (5.13) is illustrated.
where ω1 is the shifted resonance frequency, does not hold for larger nanoparticles. The exact solutions for the damping rate and the selffrequency including Lorentz friction are as follows [26] (the exponents of the solutions depend on ei t for the selfmodes of Eq. (5.23) (cf. Eq. (5.24)), in apparent disagreement with Eq. (5.26): i i21/3 (1 + 6lq) iA − − 1/3 = iα ∈ Im, 3l 3lA 2 3l √ √ i i(1 + i 3)(1 + 6lq) i(1 − i 3)A 1 (5.27) + =ω+i ,
2 = − + 2/3 1/3 3l 2 3lA 2 6l τ 1
3 = − ω + i = − ∗2, τ ) *1/3 , q = 1/τ0 ω1 , B = 2 + 27l 2 + 18lq, where A = B + 4(−1 − 6lq)3 + B 2 ) *3 aω and l = 3√2 ε c√p3 . To better visualize the difference between the exact and perturbation solutions one can illustrate the functions for ω and 1/τ (in dimensionless units, i.e., divided by ω1 ) in Fig. 5.9 versus the nanosphere radius a, The Lorentz friction terms representing the radiative losses of surface dipole plasmons and the selffrequency of these plasmons are complicated functions with respect to the particle radius, as given by Eq. (5.27) (expressed by imaginary and real parts of
, correspondingly). A perturbativetype approximation of the plasmon damping by a simple ∼ a 3 dependence is erroneous outside a relatively narrow size window, e.g., 12−30 nm for Au in vacuum [27, 26]. The numerical study of plasmon resonances in metallic nanoparticles normally utilizes the finite element method to solve the Maxwell–Fresnel equations with the dielectric function for the metal assumed as a prerequisite. Such an approach is realized by the commercial system COMSOL. Alternatively, the Mietype approach is very popular, being numerically quick as it is based on a semianalytical formulation [18, 29, 84, 17]. The Mie approach utilizes an analytical solution of
1 = −
86
Damping of Plasmons in Metallic Nanoparticles
the Maxwell equations for an incident planar wave scattered and absorbed by a metallic sphere including all multipole terms, which is an advantage of the method. The disadvantage of this approach consists in the phenomenological assumption of the dielectric function for a metallic nanoparticle, usually modelled upon the Drude form, typically using experimental data for the bulk material. None of the microscopic electron dynamics details are directly described in this way in which it is assumed that all the electron dynamics is included in the dielectric function taken from experiment. The problem is, however, that this dielectric function is not only dependent on the material but is also strongly sensitive to the nanoparticle size and shape, which cannot be experimentally expressed in a single factor, as is needed for the Mietype calculus. Therefore, the modelling of the electron liquid response, as presented previously, with the quantum RPA method, may serve as an important supplementation to the numerical Mie algorithm. The same holds for other methods of solution of the Maxwell–Fresnel equations utilizing the finite element method in both the space and time domains, such as are implemented in the numerical system COMSOL. In the case of spherical geometry COMSOL rederives the analytical Mie solution for the scattering and absorption cross sections. The COMSOL system is especially convenient for the study of nanoparticle geometries other than spherical. Practically any shape of nanoparticle may be assumed without any difference in efficiency of the finite element numerical procedure. The drawback is, however, the same here as in the Mietype approach – the complete classical electrodynamical model has no access to specific plasmon behaviour at the nanoscale. The predefined dielectric function used in COMSOL is also of Drude form, with parameters taken from experiment for the bulk material, thus neglecting the strong size dependence of the plasmon resonance and damping at the nanoscale. To apply the finite element method practically for a solution of the Maxwell– Fresnel equation for a metallic nanoparticle, one can use the commercial software package COMSOL Multiphysics 5.0, including the Wave Optics module [97]. The usefulness of COMSOL in plasmonic structure modelling has been verified by comparison with other calculation methods such as the Mie theory or the multiple expansion method [98]. The COMSOL system consumes considerable information resources; however, it is quick and efficient if applied to relatively simple threedimensional models only [94] or more complicated two or onedimensional models (including, e.g., plasmon–polariton propagation along nanoparticle chains [99]). The most important advantage of the COMSOL simulation is its flexibility with regard to the shape and material composition of the analysed system. The drawback of such plasmon simulation is, as in the Mie approach, the predefined phenomenological dielectric function in the Drude–Lorentz form [17], which is not specific to the nanoscale corrections. Often a linear interpolation of the experimental results
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
87
from bulk or thinfilm measurements is used [100] with some phenomenological size corrections for small particles (a < 20 nm) [25], in the following form:
1 1 2 − 2 (ω,a) = (ω,a = ∞) + ωp 2 ω2 + γ∞ ω + γ (a)2
ωp2 γ (a) γ∞ +i , (5.28) − 2 2 2 2 ω ω + γ (a) ω + γ∞ where γ (a) = γ∞ +AvF /a and γ∞ = vF /λB . We propose to improve this approach via inclusion of the exact attenuation term as given by Eqs. (5.27), obtained by the RPA method presented in previous chapters. For an illustrative model we will consider a system of domains: a metallic nanosphere with radius a with its centre at the origin, and with dielectric medium surrounding the particle, conventionally assumed as perfectly matched layers (PMLs) which quench backreflections from boundaries. The restriction to a spherical symmetry allows us to reduce the model to onequarter of the sphere, but the generalization to an arbitrary shape is obvious. The nanoparticle is assumed to be illuminated by a plane electromagnetic wave polarized in the z direction and propagating along the x direction. The thickness of the PMLs of the surrounding medium is accommodated to the incident radiation wavelength. The discretization essential for COMSOL simulation is achieved by a builtin free meshing algorithm, which selects a suitable space division into tetrahedral finite elements in the domain of the nanoparticle and the surrounding medium. The PMLs are divided into five spherical layers by using a mesh with spherical symmetry. The maximum element size inside the metal is chosen to suit the nanosphere radius, as a/5 for a < 60 nm and 13.5 nm for a > 60 nm. For the surrounding medium, the maximum element size is chosen as λ/6. The extinction cross section is estimated via the sum of the scattering and the absorption, given by the formulae 4 ˆ S · nd , (5.29) Qsc = √ 0 /μ0 E02 4 Uv dV , (5.30) Qabs = √ 0 /μ0 E02 V where is the boundary between the PMLs and surrounding medium, nˆ is a vector normal to the surface, E0 is the amplitude of the electric component of the incident electromagnetic wave, S is the Poynting vector, Uv indicates ohmic heat losses in the nanoparticle and V is the nanoparticle volume. The surface plasmon resonance simulated by the commercial numerical COMSOL system3 includes simultaneously all multipole components of the 3 The COMSOL system utilizes a numerical solution of the Maxwell–Fresnel differential equations by the
method of finite elements; it uses as prerequisites the material parameters, including the predefined dielectric
88
Damping of Plasmons in Metallic Nanoparticles
wavelength (nm)
a = 70 (nm)
Normalized em field (V/m)
Normalized em field (V/m)
Norm. ext. cross section (a.u.)
wavelength (nm)
Farfield em distribution
a = 20 (nm)
a = 70 (nm)
a = 140 (nm)
wavelength (nm)
a = 140 (nm)
Normalized em field (V/m)
a = 20 (nm)
Norm. ext. cross section (a.u.)
Norm. ext. cross section (a.u.)
Extinction cross section
Nearfield em distribution
a = 140 (nm) Normalized em field (V/m)
a = 70 (nm) Normalized em field (V/m)
Normalized em field (V/m)
a = 20 (nm)
Figure 5.10 The extinction spectra, farfield scattering radiation, and nearfield electric field distribution for three Au nanospheres with radii equal to 20 nm, 70 nm, and 140 nm. The field distributions correspond to illumination by an electromagnetic wave with wavelength 400 nm. The emergence of higher harmonics (multipole) modes with increasing particle radius (density maps in colours are given in [28]) can be seen.
electromagnetic response. It is noticeable that, for particles larger than ∼ 0.2 of the wavelength of the incident light, the quadrupole mode contributes. Figure 5.10 shows for comparison the optical response of three Au nanospheres with radii 20 nm, 70 nm, and 140 nm. The particles are embedded in water and illuminated with an electromagnetic wave with wavelength 400−1200 nm. The influence of the nanosphere radius on the optical response of the system is visible in the extinction spectra (top), the farfield scattering radiation distribution (middle), and the nearfield electric field distribution (bottom). In the case of a relatively small function of a metal (in the form of a Drude model [17]); the advantage of the COMSOL system consists in its ability to solve arbitrary asymmetric nanoparticleshape problems including various types of deposition of a metallic nanoparticle on arbitrary substrates; the disadvantage is the neglect of quantum plasmon effects, important in the nanoscale.
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
Wavelength (nm)
Wavelength (nm)
89
Wavelength (nm)
Figure 5.11 Normalized extinction spectra calculated for Au, Ag, and Cu nanospheres surrounded by water (ε = 1.77) with COMSOL (points) and spectra obtained with the Mie model (solid lines) for various size of nanospheres of these metals: Au (30−140 nm), Ag (20−60 nm), Cu (20−100 nm). The Mie– COMSOL agreement corresponds to the same dielectric function being assumed as the prerequisite for both fully equivalent solutions of the Maxwell–Fresnel equations.
particle with radius 20 nm and illuminated with a 400 nm wavelength planar wave (a/λ = 0.05), the dipole approximation is justified and only a dipoletype response is visible. However, for 70 nm (a/λ = 0.175) the quadrupole mode occurs, whereas for particles with radius 140 nm (a/λ = 0.35) the octupole mode also contributes. Some extinction spectra for Au, Ag, and Cu nanospheres obtained by a COMSOL simulation are presented in Fig. 5.11. From the extinction spectra we can determined the surface plasmon resonance wavelength as a function of the nanosphere radius. The resonance wavelength redshift with increase in the nanosphere radius is visible. The COMSOL resonances were compared with experimental data taken from the extinction spectra measured in colloidal solutions of metallic nanoparticles with various sizes. The resonances were compared also with the theoretical microscopic quantum predictions within the RPA approach including the exact Lorentz friction. This comparison for Au (presented in Fig. 5.12) shows good agreement of the exact RPA calculations with the experimental data and the numerical estimations lifted by the exact Lorentz friction. By virtue of the agreement of the simulation with the experimental data one can conclude that the observed redshift in plasmon resonance is caused mostly by the radiative damping of plasmon oscillations, i.e., by the Lorentz friction. For plasmons in metallic nanoparticles as described in the RPA approach one should take into account also the skin effect, due to which effectively only electrons from an outer layer of thickness h of the nanoparticle are excited by external radiation. These electrons contribute also to the Lorentz friction term, which describes the plasmon damping; hence this term must then be reduced by the factor (a 3 − (a − h)3 )/a 3 when h < a. Note that in the case of Ag nanoparticles the experimental data are shifted to longer wavelengths in comparison to both the numerical and theoretical predictions,
Damping of Plasmons in Metallic Nanoparticles
Resonance wavelength (nm)
90
Au
Radius (nm)
Figure 5.12 The COMSOL (grey dotted line with points), Mie (grey dotted line with stars), and RPA predictions (black line shows exact RPA calculations of Lorentz friction, grey solid line shows approximate Lorentz friction calculation) and the experimental data: A, [77]; B, [101]; C, [102]. The plots are for the plasmon resonance redshift as a function of nanosphere radius for Au nanospheres. For small radii (10−20 nm) the change in the resonance wavelength is relatively small; then we observe an increase in the redshift ‘speed’ (for 20−60 nm), and finally stabilization (> 60 nm).
as is visualized in Fig. 5.13. This discrepancy is probably caused by the silver nanoparticle synthesis method, which could leave on the silver surface a residual amount of organic surfactant (citrate) or other optically active molecules utilized in the synthesis. This effect can be illustrated by COMSOL simulation via the addition of a dielectric coating to the model of the Ag nanoparticle. In Fig. 5.14 one can observe a relatively large shift in the plasmon resonance due to the additional dielectric shell (with refractive index n = 1.5 in the figure). Also, the dependence on the refractive index of the dielectric shell with thickness 10 nm is visualized. Both an increase in the shell thickness and an increase in the refractive index of the shell material cause a redshift of the resonance wavelength. This shift in the first case is relatively small, from 407 nm at d = 4 nm to 419 nm at d = 20 nm in comparison to 423 nm for an infinite layer thickness. The optimal fit between the theory and experimental data for Ag is obtained using a refractive index value 1.5 for the dielectric outer layer. The behaviour described above at the infinite limit for the thickness of the outer dielectric layer shows that the plasmon resonance wavelength can be strongly affected by the surroundings of the nanoparticle (which can be utilized in, e.g., refractive index detectors). In the case of Ag (see Fig. 5.15) the resonance wavelength could be shifted from 400 nm in air to 1000 nm in a medium with
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
91
Resonance wavelength (nm)
Ag
Radius (nm)
Figure 5.13 For comparison, COMSOL predictions (grey line with small points) and RPA predictions (black line, exact inclusion of the Lorentz friction; solid grey line for approximate Lorentz friction) and experimental data (A, [77]; B, [103]; C, [85] for the plasmon resonance redshift as a function of nanosphere radius for Ag nanospheres.
d (nm)
Wavelength (nm)
Wavelength (nm)
Figure 5.14 Normalized extinction cross sections for Ag nanospheres covered with dielectric shells of various thicknesses d with fixed refractive index n = 1.5 (left) and with fixed thickness d = 20 nm and different refractive indices n (right).
refractive index equal to 4. One can also notice that the higher multipole resonances accompanying the dipole resonance are proportionally shifted (see Fig. 5.15). In COMSOL simulation one can easy consider the case of elongated nanoparticles such as spheroids or rods. In such a geometry with cylindrical symmetry, two different surface plasmon modes, longitudinal (oscillations along the long axis) and transverse (oscillations along the short axis), exist. These modes can be
92
Damping of Plasmons in Metallic Nanoparticles
Wavelength (nm)
Wavelength (nm)
Figure 5.15 Normalized extinction spectra for Au (left) and Ag (right) nanospheres for dielectric surroundings with various refractive indices. The resonance peak shifts towards longer wavelengths with increasing refractive index of the surrounding medium.
observed, when illuminating the nanoparticle with light of different polarizations. In the case of a spheroidshaped particle, the Ganss development of the Mie theory in the dipole limit is analytically available [25], allowing the following condition for the frequencies of both modes: Re (ωres ) =
m (Li − 1) , Li
(5.31)
where (ωres ) is the value of the dielectric function of the metal at the resonance frequency, m is the dielectric permittivity of the surrounding medium, Li are the socalled geometrical depolarization factors determined by the particle geometry, 1 1 − e2 1 − Lx 1+e , Ly,z = −1 + Lx = ln , (5.32) e2 2e 1 − e 2 where e2 = 1 − χ 2 (χ is the aspect ratio). In Fig. 5.18 we illustrate the extinction cross sections for a nanorod with aspect ratio (length/width) equal to 3 for different polarizations of the incident light; these were calculated using COMSOL. The angle α in Fig. 5.16 varies from 0o to 90o , i.e., from an electric field perpendicular to the long rod axis to one parallel to the long rod axis. The related electric field distributions (on the sections along the long and short rod axes) are illustrated in Fig. 5.17. By varying the light polarization, two modes can be excited in a selective manner. The longitudinal one dominates. For a polarization angle larger than 30o (see Fig. 5.18) only one mode is visible. Additionally, in Figs. 5.18 and 5.19 the dependence of resonance wavelength on particle ratio is presented. The Mie approach in its original version [18] gives an analytical formulation for the scattering and absorption cross sections in the case of spherical geometry and
Normalized extinction cross section (a.u.)
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
93
a (deg) 90°
a
60°
Wavelength (nm)
Figure 5.16 Extinction spectra for nanorods for various incident light polarizations relative to the rod axis.
3.0
a = 90°
3.0
a = 90°
3.0
2.5
2.5
2.5
2.0
2.0
2.0
a = 90°
7 6 5
a = 90°
6×1016 5 4
4 1.5
1.5
3
1.5 3
1.0
1.0
0.5
0.5
0.0
0.0
2
1.0
2
0.5
1
1
0.0
0
0
Electric field amplitude (V/m)
a = 90°
Figure 5.17 The electric field distribution near metallic nanorods for different incident light polarizations (wavelength 600 nm) relative to the rod axis. One can observe two plasmon excitations: longitudinal, excited when the light is polarized parallel to the rod axis, and transverse, when the light is polarized perpendicularly to the rod axis (density maps are given in colour in [28]).
the easiest form for the dielectric function of the metallic nanoparticle [17]. It can be developed for ellipsoid symmetry also [17]. Because of this analytical formulation, it is much quicker to use in calculations than a numerical solution of the Maxwell–Fresnel equations. To meet the experimental data the Mie approach has been improved, mostly via phenomenological modelling of the dielectric function of the metallic particle. The original formulation [17] gives the Mie frequency as
94
Damping of Plasmons in Metallic Nanoparticles
Figure 5.18 Extinction spectra for Au nanorods with various aspect ratios y/x. The incident light is polarized parallel to the rod axis.
Wavelength (nm)
Wavelength (nm)
Figure 5.19 Extinction spectra for Au prolate spheroids with different aspect ratios. (Left) The incident light is polarized parallel to the larger particle axis; (right) the incident light is polarized perpendicularly to that axis.
√ independent of the sphere size, ωMie = ωp / 3 in the simplest case, which does not agree with experimental observations. For ultrasmall nanoparticles some radius dependence can be introduced by the dependence of the volume plasmon frequency √ ωp on the electron density n (ωp ∼ n) and by accounting for the dilution of electrons caused by spillout. The resulting redshift of the Mie resonance agrees with observations for extremely small nanoparticles, where spillout is important [19]. For larger nanospheres this correction disappears together with the spillout
5.4 Numerical Modelling of Plasmon Resonances in Metallic Nanoparticles
95
contribution ∼ 1/a. Nevertheless, for the range a ∈ (5,75) nm (for Au in vacuum) a strong size dependence of the surface plasmon resonance is observed that is clearly beyond the simplest version of the Mie approach. Moreover, at a ∼ 12 nm (Au in vacuum) a crossover in the size dependence of the resonance frequency is observed. To cope with this problem, some artificial corrections to the Mie approach have been applied. To explain this crossover in the size dependence of the experimentally observed redshift of the plasmon resonance in metallic nanoparticles with growing nanosphere radius, two regimes of the Mie theory were introduced in [83]: an intrinsic size effect (for a < 20 nm for Au) and an extrinsic size effect (for a > 20 nm). The intrinsic size effect refers to the dipole approximation of the Mie response, when other multipole contributions are neglected. Simultaneously, the electron scattering energy dissipation is included in the dielectric function (with the damping rate defined by Eq. (5.13)), which gives a ∼ 1/a redshift of the dipole Mie resonance due to the ∼ 1/a contribution of scattering from the nanoparticle boundary. For larger nanospheres (approximately for a > 20 nm for Au), when experimentally the resonance redshift rises with increase in a, an extrinsic mechanism is introduced into the Mie theory [83, 22]. The latter mechanism corresponds to the inclusion of the multipole response and corrections for the pole of the dipole response component. To obtain agreement with the experimentally observed size effect in the redshift of the plasmon resonance in larger nanospheres, radiation corrections to the dielectric function have been introduced that are proportional to the number of electrons and thus ∼ a 3 [84]. This overestimates, however, the radiative damping for radii > 30 nm (for Au). This phenomenological modelling in the Mie approach gives the crossover in the surface plasmon resonance from 1/a to a 3 using the dipole approximation only (by modifying the metal’s dielectric function). The frontier between the dipole and multipole limits is not sharply defined and multipole corrections occur gradually with stronger intensity for larger nanoparticles. As we have demonstrated, the Lorentzfrictioninduced radiation losses strongly contribute to plasmon energy dissipation for a > 12 nm (for Au in vacuum). Thus, for nanospheres with radii of order of 5−10 nm (and even up to 15 nm, see Fig. 5.3) the Mie approach gives a reasonabe intrinsic size effect neglecting the Lorentz friction losses. This does not hold, however, at a ∼ 15−25 nm or at larger scales for the radius. For such radii radiation losses dominate the plasmon damping. This is not included in the conventional Mie theory for the intrinsic size effect. The accurate irregular size effect of plasmon damping caused by Lorentz friction (as presented previously, see formula (5.27)) explains well the experimentally observed irregular (i.e., not proportional to a 3 ) size effect for the redshift. Therefore the Mie approach must be modified by Eq. (5.27) instead of the incorrect a 3 contribution to the dielectric function. This strongly modifies the dipole contribution in the Mie response in
96
Damping of Plasmons in Metallic Nanoparticles
consistency with observations up to a < 60 (for Au in vacuum) without any multipole contributions. The latter start to be important for radii a > 60 nm (Au) significantly exceeding the previously suggested limit of 20 nm as the onset of the extrinsic regime [83, 22, 84]. This agrees better with observations – the multipole contribution for a > 60 nm (Au) results in deformation and greater broadening of the extinction features, no longer allowing a Lorentzian form (the higherenergy quadrupole secondary broad peak occurs first at smaller wavelength in association with the dipole peak broadened and redshifted by the Lorentz friction). In the experimental results it is visible for Au at 75 nm [77, 82]. As previously discussed [27, 26], the ∼ a 3 growth of the radiationinduced damping of plasmons, phenomenologically accounted for in the Mie theory, must quickly saturate. Thus, the inclusion of the exact form of the Lorentz friction damping rate (as given by Eq. (5.27)) in the modelled dielectric function for nanosystems (needed in the Mie theory and especially important in its intrinsic size effect regime) gives a significant correction of the Mie approach. The intrinsic Mie regime with inclusion of the Lorentz friction can be extended to larger radii (up to abuot 60 nm for Au), where the extrinsic multipole effect starts to contribute with gradually growing intensity for higher radii; however, up to 60 nm the extrinsic effect mixes rather weakly with the saturation and lowering of the damping rate due to Lorentz friction [27]. The multipole corrections cannot be avoided for radii a > 60 nm. The deformation of the Lorentzian shape describing the extinction features is accompanied by their significant broadening, for Au observed at a = 75 nm [77, 82]. However, in the radius window 10–60 nm (for Au) the dipole approximation is sufficient to explain the observed irregular size effect of plasmon resonance, provided the accurate Lorentz friction contribution (5.27) to dipole plasmon damping is included. The analysis presented above agrees well with the experimental data for Au. As mentioned above, some underestimation for Ag of the resonance wavelength is probably connected with the modification of the surface of Ag nanoparticles caused by the chemical manufacturing method. Similar properties are confirmed and verified by a microscopic RPA approach to plasmons, using a COMSOL finite element numerical solution of Maxwell equations and application of the conventional Mie approach. The Mie and COMSOL methods must be, however, suitably lifted to incorporate the size effect at the nanoscale by appropriate modelling of the dielectric function. Agreement is clear, owing to the common geometry of the considered nanoparticles for any approach. It is important, however, that the form of the true dielectric function is greatly different from that of the bulk metal supported by experimental data for the bulk metal or thin films at best. Thus, it has been demonstrated that the corrections required at the nanoscale can be taken from the microscopic RPA model of plasmons, including plasmon damping due to the Lorentz friction, which is found to be strongly sizesensitive.
6 Plasmon Photovoltaic Effect
One of the most important applications of nanoplasmonics is the mediation of light capture in a semiconductor by surface plasmons in metallic nanoparticles deposited on the semiconductor substrate. The increase in efficiency of solar cells thus metallically modified on the nanoscale has been experimentally demonstrated. In this chapter we provide a microscopic quantum explanation of the plasmoninduced photovoltaic phenomenon. Using Fermi’s golden rule the efficiency of the plasmonmediated channel for solar energy transfer is derived in analytical form. A comparison with experiments is given. Moreover, an experiment demonstrating the depth range of the plasmonic photoeffect in the substrate semiconductor of a metallized solar cell is described.
Considerable interest in the socalled plasmonic photovoltaic effect has emerged within the past decade. This is a result of the experimental demonstration of a significant increase in efficiency of the photoeffect when the incidentphoton energy transfer to electrons is mediated by surface plasmons in metallic nanoparticles deposited on the photoactive surface of the photodiode or semiconductor solar cell [32–36, 104–106]. The planar density of the metallic nanoparticle coverage that causes a strong effect is rather small – in the range 108−10 per cm2 for Au or Ag nanoparticles randomly distributed on the surface. It has been demonstrated that more dense coverings do not lead to strengthening of the effect but, in contrast, may even diminish the photovoltaic efficiency. The covering densities mentioned above and the typical sizes of nanoparticles, with radius a ∈ (10,50) nm, make these coverings inexpensive even though noble metals may be used (the best is Au, superior over Ag or Cu in lifting the efficiency of the photoeffect). The problem is, however, the technique of nanoparticle deposition in large scales and the durability of the metallic nanocoverings of solar cells in commercial use. The discovery of the plasmonmediated photoeffect is of great prospective importance for the development of a new generation of solar cells with enhanced efficiency, especially for improvement via the metallic nanomodifications of thinfilm cells, and even organic cells and perovskite cells (the latter are especially 97
98
Plasmon Photovoltaic Effect
interesting owing to their simple and cheap chemical methods of manufacture) [36, 2, 105, 107–112, 73, 74]. The feasibility of plasmonic improvements has been supported by the successful application of metallic nanocomponents to about a factor of ten increase in Raman spectrometer resolution via the concentration of local laser illumination near the curvature of metallic nanoconcentrators [113, 114]. A similar improvement of scanning tunnelling microscopy by the utilization of surface plasmons has been proposed [115]. Moreover, another phenomenon that is worthy of consideration is plasmonassisted transport in metallic nanostructures, using hybridized collective modes of surface plasmons and photons, i.e., plasmon– polaritons [3, 116], with properties that are highly attractive for applications in optoelectronics [3, 4] with subdiffraction arrangements of light–plasmon circuits. In such circuits, light signals are converted into plasmon–polaritons with the same energy but with a wavelength one or two orders of magnitude lower [116, 39, 38, 78]. This direction of research meets also the rapidly developing, field of metamaterials. As was demonstrated in Chapter 4, in finite nanometrescale metallic systems new types of plasmon oscillation arise that do not occur in the bulk case. These new types of oscillation are called surface plasmons and correspond to a translational movement of the electron liquid with respect to the ion jellium, resulting in unbalancedcharge fluctuations at the surfaces of the finite nanoparticles. Oscillations that have an inhomogeneous compressional character along the system radius are referred to as volume plasmons in the finite system, in close analogy to plasmons in the bulk case. Remarkably, the energies of the surface plasmon modes are lower than the bulk plasmon energy hω ¯ p whereas the energies of the volume plasmon modes in nanoparticles are larger than hω ¯ p , as was shown in Chapter 4. Finite metallic systems have been widely investigated by a thorough quantum analysis, including the application of the shell model for a small number of electrons in analogy to multielectron atoms, and by the development of numerical quasiexact studies employing the Kohn–Scham approximation (which is efficient up to about 300 electrons only) [19–21, 71, 79]. For larger nanoparticles the random phase approximation (RPA) approach proves to be effective [21, 19, 71]. As a rule, in this treatment, the jellium model is utilized. In this model the ion dynamics are considered negligible because in metals the ions have a much greater inertia than the electron fluid owing to the much greater mass of the ions compared with the electron mass [19–21]. In bulk metals, the plasmon energy is hω ¯ p = e2 n/(ε0 m) 10 eV, which is larger than the Fermi energy. This fact indicates that plasmons are not excitations near the Fermi surface and that they interact only weakly with the Landau quasiparticles (the electrons near the Fermi surface) because of the large energy incommensurability. The origin of such highenergy plasmon excitations is the
Plasmon Photovoltaic Effect
99
Coulomb interaction between the electrons and between the electrons and the jellium, described in the Pines–Bohm RPA theory of plasmons [16, 14, 15], as presented in Chapter 3. Progress in the RPA formulation of plasmons in metallic nanospheres [23] has enabled the description of both volume and surface plasmons in spheres with radii ranging between approximately 5 nm and 100 nm especially interesting for Au, Ag or Cu particles, because at this particlesize range the surface plasmon resonances of these metals are in the visible part of the electromagnetic spectrum, conveniently overlapping with the sun’s spectrum at the Earth’s surface. In this size range of metallic nanoparticles, the quasiclassical RPA approach proves to be sufficiently accurate. For smaller clusters more precise quantum models are needed, especially for radii of 1–2 nm, for which the pronounced surface effects are of primary importance. One such effect is the socalled spillout of the electron liquid beyond the jellium rim. The spillout occurs on the scale of the Thomas–Fermi length [16] and gradually loses its significance as the sphere radius increases. Similarly, another quantum phenomenon, the Landau damping of plasmons as a result of their decay into highenergy particle–hole excitations far from the Fermi surface [80], is of decreasing significance as the radius increases. These quantum phenomena, although of importance for small metallic nanoparticles clusters, are negligible for radius a > 5 nm. In smaller nanoparticles, the spillout effect is considered to be the reason for the redshift of the dipole surfaceoscillation frequency (the Mie frequency) as a result of the decrease in the electron density caused by spillout. For ultrasmall nanoparticles, this redshift property has been confirmed experimentally in K, Au, and Ag [71]. In larger metallic nanospheres a strong redshift of the plasmon resonance is also observed but is apparently caused by another mechanism because, for a > 5 nm, all surfaceinduced effects are negligible. The most important factor in larger metallic nanospheres, in the radius range a ∈ (5,100) nm, is the rapid enhancement of radiation losses of plasmon oscillations whereas radiation is rather insignificant in small metallic nanoparticles. The radiationlossinduced damping of plasmons causes a redshift of the resonance, and this satisfactorily explains the plasmonic frequency shift in large metallic nanospheres [77], as was shown in Chapter 5. Plasmon damping via the radiation phenomenon in large nanospheres explains why such metallic particles are so efficient in lightenergy transfer. The large radiation effect for plasmons in metallic nanoparticles means that they also have large absorption. So they quickly gather energy from incident light photons. When metallic nanoparticles are deposited on the photoactive surfaces of a semiconductor (as in solar cells) the coupling of plasmons to the substrate semiconductor band electrons opens an especially efficient channel for energy transfer [32–34, 117–120].
100
Plasmon Photovoltaic Effect
Thus metallic nanospheres (or nanoparticles of other shapes [121]) can act as light converters because of their capability for high absorption and radiation of energy, which originates from the mutual mirror relationship between the two directions of quantum transitions [75]. The incident photon energy that is absorbed in surface plasmon oscillations in metallic nanoparticles can thus be transferred to a semiconductor substrate in a very efficient manner, highly exceeding the efficiency of the ordinary photoeffect. We can identify the origin of this efficiency enhancement as being due to two competing factors. The first is the local concentration of the electric field of the surface plasmon oscillations near the curvature of a metallic nanoparticle and, as a result, collecting the energy of many photons, increasing step by step the plasmon oscillation amplitude. The latter effect is proportional to a 3 (a is the nanosphere radius) and reflects the fact that all electrons in the nanosphere participate in the oscillations even though charge fluctuations occur only on the surface because of the screening by the jellium of translational oscillations in the internal volume. The second factor is the possibility of indirect interband electron transitions in the semiconductor substrate, which are allowed for a system with broken translational symmetry. This occurs for the dipole interactions of the surface plasmon oscillations in the local nanoscale system. The momentum conservation rule is not restrictive here, in contrast with the ordinary photoeffect. In the ordinary photoeffect the momentum (or quasimomentum) of an electron undergoing a photoninduced transition between the valence and conduction bands does not change because of the extremely low momentum of photons that is required for consistency in energy with the forbidden gap in the semiconductor (because of the high velocity of light). This results in socalled vertical optical transitions, significantly reducing the efficiency of the conventional photoeffect. However, when there are mediating interactions with plasmons, all indirect interband excitations are allowed, which enhances the efficiency of this channel. It is clear that this effect favours nanospheres of smaller radius, for which the breaking of translation invariance is more important, whereas the effect weakens with increasing radius. This concept was originally formulated in [23] and was recently utilized in another publication [122]. It was also discussed in an earlier paper [109]. In the next section we summarize briefly the model constructed previously to describe plasmon oscillations in large metallic nanospheres in the framework of the RPA approach [23], in analogy to the Pines–Bohm RPA theory of plasmons in a bulk metal [16, 14]. We recall that an advantage of this approach [23, 77] is its fully analytical formulation, which enables its straightforward and controllable application to a description of plasmon damping; numerically, the problem is beyond the capability of even large simulations.
6.1 Semiclassical RPA Approach to Plasmons in Large Metallic Nanospheres 101
6.1 Semiclassical RPA Approach to Plasmons in Large Metallic Nanospheres The RPA theory of plasmon excitations in metallic nanospheres [23] is effective and sufficiently accurate for large nanoparticles of radius a ∈ (5,100) nm. For such large nanoparticles, the spillout of electrons beyond the jellium rim is negligible, which allows for the separation of the volume and surface types of charge oscillation. Otherwise, when the Thomas–Fermi length, i.e., the scale of the spillout, is significant in comparison to the radius, the surface becomes fuzzy, which leads to the mixing of the surface and volume charge fluctuations. It has been proven via TDLDA numerical calculations employing the Kohn–Sham approach to multielectron clusters [19, 71] that the separation of the volume and surface modes becomes clear for more than approximately 60 electrons, whereas for smaller nanoparticles the mixing of modes occurs in accordance with the shell model. The Thomas–Fermi length in a metal is of the order of the interparticle separation; therefore, for a > 5 nm, we can safely assume that the mixing of modes disappears, similarly to other surfacetype effects [80]. Although spillout was included in the original formulation of the RPA approach [23], in the following description we will completely neglect it because the Thomas–Fermi length is on the subnanometre scale, more than one order of magnitude smaller than the nanosphere radii considered. For completeness we briefly summarize again the most important steps in the description of plasmons in nanoparticles. Similarly to the treatment in the RPA approach for a bulk metal as formulated by Pines and Bohm [14–16], the local electron density can be represented by the quasiclassical formula [16, 15], δ(r − rj ) e (t) , (6.1) ρ(r,t) = e (t) j where the Dirac deltas quasiclassically define the positions of the electrons. The Fourier picture of Eq. (6.1) takes the convenient form ˆ (6.2) ρ(k,t) ˜ = ρ(r,t)e−ik·r d 3 r = e (t)ρ(k) e (t), where the operator ρ(k) ˆ is given by j e−ik·rj . The dynamic equation for this local electron density operator can be determined using the Heisenberg equation in the form ( ( ˆ d 2 ρ(k) 1 '' ˆ e , Hˆ e , = ρ(k), ˆ H dt 2 (i h) ¯ 2
(6.3)
102
Plasmon Photovoltaic Effect
where the Hamiltonian He for the electrons in a metallic nanosphere based on the jellium model (cf. Eq. (4.8)) is given by 2 Ne * 2 h¯ ∇j2 e 2π ) ˆ+ 3 − − d Hˆ e = k n ˜ (k) (k) + ρ(k) ˆ ρ e 2m (2π)3 k2 j =1 ) * e2 3 2π ˆ+ (k)ρ(k) + d k ˆ − N ρ (6.4) e , (2π)3 k2 3 3 −1 −ik·r d rne (r)e−ik·r and 4π/k 2 = d rr 1e : The jellium where n˜ e (k) = [19, 17, 123] consists of the background ion charge uniformly distributed over the sphere; ne (r) = ne (a − r), where ne = Ne /V and ne e is the average positive charge density, V = 4πa 3 /3 is the sphere volume, and is the Heaviside step function. Equation (6.3), after averaging over the multiparticle wave function and, according to the RPA scheme, neglecting the multiplications of density fluctuations with different phases, ultimately attains the following form [23]:
˜ 2 F 2 ∂ 2 δ ρ(r,t) 2 = ˜ − ωp δ ρ(r,t) ˜ (a − r) ∇ δ ρ(r,t) ∂t 2 3m
2 r 3 − ˜ ∇ F ne + F δ ρ(r,t) δ(a − r) 3m 5 r ! ωp2 r 2 F r 1 3 ∇δ ρ(r,t) ˜ + ∇ d r1 δ ρ(r ˜ 1,t) δ(a − r). − 3mr 4π r r − r1  (6.5) In the above formula the Thomas–Fermi approximation for the kinetic energy has been used [16, 23] and ωp is the bulk plasmon frequency, ωp2 = 4πne e2 /m (in SI units, ωp2 = e2 ne /(ε0 m)). Here we have used ∇(a − r) = (−r/r)δ(a − r)), which gives rise to the surface plasmon fluctuations indicated by the Dirac delta in Eq. (6.5). Because of the structure of Eq. (6.5), its general solution can be decomposed into two parts related to two distinct domains, as was discussed in Chapter 4, and we rewrite them here: for r < a, δ ρ˜1 (r,t) (6.6) δ ρ(r,t) ˜ = for r ≥ a (r → a+), δ ρ˜2 (r,t) corresponding to the volume and surface charge fluctuations, respectively. These two components of the local electron density fluctuations satisfy the following equations (see Eq. (5.7)): 2 F 2 ∂ 2 δ ρ˜1 (r,t) = ∇ δ ρ˜1 (r,t) − ωp2 δ ρ˜1 (r,t) ∂t 2 3m
(6.7)
6.1 Semiclassical RPA Approach to Plasmons in Large Metallic Nanospheres 103
and (see Eq. (5.8), here, = 0+,
∂ 2 δ ρ˜2 (r,t) 2 r 3 =− ∇ F ne + F δ ρ˜2 (r,t) δ(a + − r) ∂t 2 3m 5 r 2 ωp r 1 2 F r ∇δ ρ˜2 (r,t) + ∇ d 3 r1 − (δ ρ˜1 (r1,t)(a − r1 ) 3mr 4π r r − r1  (6.8) + δ ρ˜2 (r1,t)(r1 − a)) δ(a + − r). To solve Eqs. (6.7) and (6.8), let us represent the two components of the electron fluctuation in the following manner: for r < a, δ ρ˜1 (r,t) = ne F (r,t) δ ρ˜2 (r,t) = σ ( ,t)δ(r + − a), = 0 + ,
for r ≥ a (r → a+),
(6.9)
with initial conditions F (r,t)t=0 = 0 and σ ( ,t) t=0 = 0 ( is the spherical (solid) angle); moreover, F (r,t)r→a = 0 and ρ(r,t)d 3 r = Ne is the neutrality condition. After some algebra [23] one can find, given the spherical symmetry of the system, F (r,t) =
∞ ∞ l
Almn jl (knl r)Ylm ( ) sin(ωnl t)
(6.10)
l=1 m=−l n=1
and l ∞ Blm σ ( ,t) = Ylm ( ) sin(ω0l t) a2 l=1 m=−l
+
∞ ∞ l
Almn
(l + 1)ωp2 2 lωp2 − (2l + 1)ωnl
l=1 m=−l n=1 a r l+2 × dr1 1l+2 jl (knl r1 ) sin(ωnl t), a
where the jl (ξ ) =
√
Ylm ( )ne
(6.11)
0
π/(2ξ )Il+1/2 (ξ ) are the spherical Bessel functions, the Ylm ( )
2 are spherical harmonics, the ωnl = ωp 1 + xnl /(kT2 a 2 ) are the frequencies of the volume plasmon selfoscillations, kT = 6ne e2 /F is the Thomas–Fermi length (F is the Fermi energy), the xnl are the nodes of the Bessel function jl (ξ ), knl = √ xnl /a, and the ω0l = ωp l/(2l + 1) are the frequencies of the electron surface selfoscillations (the surface plasmon frequencies). The function F (r,t) describes the volume plasmon oscillations whereas the function σ ( ,t) describes the surface plasmon oscillations. In the formula for σ ( ,t), Eq. (6.11), the first term
104
Plasmon Photovoltaic Effect
corresponds to surface selfoscillations, whereas the second term describes surface oscillations induced by the volume plasmons. The frequencies of the surface selfoscillations are & l , (6.12) ω0l = ωp 2l + 1 which, for l = 1, gives the dipoletype surface oscillation frequency originally √ found by Mie [18, 17], ω01 = ωp / 3 (for simplicity, we denote it as ω1 = ω01 ). 6.2 Damping of Plasmons in Large Nanospheres Now we again summarize the most important aspects of plasmon damping. The advantage of the RPA Eqs. (6.7) and (6.8) for the volume and surface plasmons in a metallic nanoparticle is their oscillatory form. This property allows phenomenological inclusion of the damping of the plasmons, in analogy to oscillator damping, via the addition to the righthand sides of Eqs. (6.7) and (6.8) the term −
2 ∂δρ1(2) (r,t) , τ0 ∂t
with indices 1 or 2, respectively. The damping of the plasmons that is included in τ0 accounts for the scattering of electrons from other electrons, from defects, from phonons, or from nanoparticle boundaries; all these scattering channels lead to a damping rate expressed by the simplified formula [24] vF CvF 1 + , τ0 2λB 2a
(6.13)
where C is a constant of order unity, a is the nanosphere radius, vF is the Fermi velocity in the metal, and λB is the electron mean free path in the bulk (including effects due to the scattering of electrons on other electrons, on impurities and on phonons [24]). As was discussed previously (see Eq. (5.13)), the latter term in Eq. (6.13) accounts for the scattering of electrons from the boundary of the nanoparticle, whereas the former term corresponds to scattering processes similar to those in the bulk. The other effects, such as Landau damping (especially important in small clusters [80, 79]), which corresponds to the decay of a plasmon into a highenergy particle–hole pair, are of less significance for nanosphere radii larger than 2−3 nm [80] and are completely negligible for radii larger than 5 nm. Irreversible dissipation of the plasmon energy due to scattering, as expressed by (6.13), affects each mode of both the volume and surface plasmons. In the case of interest here, i.e., that of plasmons induced by incident sunlight, one can observe that only dipole surface plasmons will contribute to the electromagnetic response of a nanosphere of radius a ∈ (5,100) nm. This follows from the restriction imposed
6.2 Damping of Plasmons in Large Nanospheres
105
by the dipole approximation, which holds in the case of such metallic nanospheres; in this case the resonance wavelength (corresponding to photons of energy hω ¯ 1, which, for Au and Ag, is of the order of 500 nm) is far larger than the nanosphere radius and the electric field of the incident light is essentially homogeneous over the entire nanoparticle. Such a forcing electric field can excite only the dipole mode of the surface plasmons, which can be represented by the function Q1m (t), m = −1,0,1. This function satisfies the following equation (which is Eq. (6.8) for just the l = 1 spherical component, with damping and a homogeneous forcing field): 2 ∂Q1m (t) ∂ 2 Q1m (t) + + ω12 Q1m (t) 2 ∂t τ0 ∂t & √
( 4π ene ' Ez (t)δm0 + 2 Ex (t)δm1 + Ey (t)δm−1 . = 3 m The corresponding electron density fluctuations are given by ⎧ for r < a, ⎨ 0 1 δρ(r,t) = Q1m (t)Y1m ( ) for r ≥ a, r → a + . ⎩
(6.14)
(6.15)
m=−1
Because the l = 1 case describes dipoletype fluctuations, one can calculate the dipole of the plasmon oscillations given by Eq. (6.15): 4π (6.16) eq(t)a 3 . D(t) = e d 3 rrδρ(r,t) = 3 This dipole can be represented by the vector q(t), which is related to the functions √ √ Q1m (t) as follows: Q11 (t) = 8π/3qx (t), Q1−1 (t) = 8π/3qy (t), and Q10 (t) = √ 4π/3qx (t). The vector q(t) satisfies the following equation (cf. Eq. (6.14)): 2 ∂ ene 2 ∂ 2 + + ω1 q(t) = E(t). (6.17) 2 ∂t τ0 ∂t m 6.2.1 Radiation from Dipole Surface Plasmons – Lorentz Friction for Plasmons Plasmon oscillations are themselves a source of electromagnetic radiation. This radiation depletes the energy of the plasmons, resulting in hampering of their oscillations, which can be regarded in terms of the Lorentz friction in the case of an oscillating and radiating dipole [55]: EL =
2 ∂ 3 D(t) , 3c3 ∂t 3
(6.18)
106
Plasmon Photovoltaic Effect
where EL represents an additional electric field hampering the charge oscillations (the Lorentz friction), c is the speed of light, and D(t) is surface plasmon oscillation dipole. According to Eq. (6.16), we arrive at the following form for EL : 2e 4π 3 ∂ 3 q(t) . a 3c3 3 ∂t 3 Substituting this expression into Eq. (6.17), we obtain 2 ene ∂ 2 ∂ 2 ) ω1 a *3 ∂ 3 q(t) 2 q(t) = + . + ω E(t) + 1 ∂t 2 τ0 ∂t m 3ω1 c ∂t 3 EL =
(6.19)
(6.20)
In the zerothorder approximation (neglecting attenuation and for E = 0), 2 ∂ 2 + ω1 q(t) = 0. ∂t 2
(6.21)
In the next step of the perturbation approach, which is iteratively applied to solve Eq. (6.20), one substitutes −ω12 q(t) for ∂ 2 q(t)/∂t 2 (according to Eq. (6.21)) in the second term on the righthand side of that equation. Thus the Lorentz friction term is included in a renormalized damping rate τ : 2 ene 2 ∂ ∂ 2 + + ω1 q(t) = E(t), (6.22) 2 ∂t τ ∂t m where
1 ω1 ) ω1 a *3 vF CvF 1 ω1 ) ω1 a *3 + + . = + τ τ0 3 c 2λB 2a 3 c
(6.23)
The contributions of scattering and radiation to the overall damping of the plasmons, in the framework of the perturbation approach presented above, are given for comparison in Fig. 6.1 (left). The renormalized damping increases rapidly with increasing radius a and causes a significant redshift of the selffrequency of the freedipoletype surface plasmon oscillations, ω1 = 1 0.25
1.0
0.20
0.8
0.15 0.10
0.6
ω12 − 1/τ 2 . The radiusdependent
0.4 0.2
0.05 20 40 60 80 100 120
a (nm)
20 40 60 80 100 120
a (nm)
Figure 6.1 Real and imaginary parts of the solution of Eq. (6.20), i.e., the selffrequency and the damping rate, given by Eq. (6.24), versus a (1/τ and ω in units of ω1 ).
6.2 Damping of Plasmons in Large Nanospheres
107
shift in the resonance caused by strong radiationinduced plasmon damping has been confirmed experimentally [77] via measurements of light extinction in colloidal solutions of nanoparticles of different sizes (in [77], such measurements are reported for Au nanospheres of 10−80 nm radius and Ag nanospheres of 10−60 nm radius). These measurements support the a 3 increase in plasmon damping described above. However, for a > 30 nm, some deviation from this a 3 increase is evident in experimental results [77]. This deviation is related to the constraints of the applied perturbative solution procedure. With increasing a, the attenuation rapidly increases as a 3 and can no longer be treated as a small perturbation. Thus, an exact solution of Eq. (6.20) is necessary. This equation is a thirdorder linear differential equation and can be solved exactly. The related selffrequency and its damping rate are given by the following expression: 1 τ i =− + 3l
ω+i
√ i(1 + i 3)(1 + 6lq) ) *1/3 3 × 22/3 l 2 + 27l 2 +18lq + 4(−1 − 6lq)3 + (2 + 27l 2 + 18lq)2 *1/3 √ ) i(1 − i 3) 2 + 27l 2 + 18lq + 4(−1 − 6lq)3 + (2 + 27l 2 + 18lq)2 + , 6 × 21/3 l (6.24)
where q = 1/τ0 ω1 and l = (2/3) (aω1 /c)3 . The functions ω and 1/τ (in dimensionless units, i.e., divided by ω1 ) are plotted in Fig. 6.2 versus nanosphere radius a. Strong deviation from the perturbatively obtained behaviour, 1/τ ∼ a 3 , is apparent for a > 30nm. For a < 25 nm, the approximate perturbative expressions for 1/τ and ω = ω1 1 − (1/ω1 τ )2 agree with the exact solution in Eq. (6.24). The Lorentz friction term is given in Eq. (6.23) (and also in Eq. (6.24) for a lower than approximately 11 nm, for Au and Ag). In this size regime for metallic particles, we encounter a conspicuous crossover of the attenuation rate with respect to a. The minimum damping is achieved at 1/4 9 vF c3 ∗ (6.25) ε a = 2 ωp4 and for a < a ∗ the damping ratio increases with decreasing a approximately as 1/a, whereas for a > a ∗ this ratio increases with increasing a in proportion to a 3 (if a < 25 nm, for Au in vacuum). The value of a ∗ can be estimated for Au and Ag; see Table 6.1. As is apparent in Fig. 6.1, the attenuation rate 1/τ reaches a maximum at a certain value of a. This value, denoted by a ∗∗ , is also listed in
108
Plasmon Photovoltaic Effect
Table 6.1 Radii of a nanosphere corresponding to the minimal value of surface plasmon damping (a ∗ ) and to the maximal value (a ∗∗ ) a ∗ , a ∗∗ (nm)
√ ε
Au
Ag
1, vacuum 1.41 1.73
8.77, 57.4 10.4, 64.3 11.5, 68.7
8.78, 57.42 10.4, 64.4 11.6, 68.8
Crossover of plasmon damping (Au) Lorentz friction ~
0.04
0.35
total
0.30
scattering ~ 1 a
0.25
appr.
1
1
0.03
Damping rate (Au)
a3
0.20
0.02
0.15 exact
0.10
0.01
0.05
0.00 4
6
8
10
12
Radius a (nm)
14
0.00
5
10
15
20
25
30
35
40
a (nm)
Figure 6.2 (Left) Crossover in the size dependence of the damping rate: the contributions to the damping rate of surface plasmon oscillations in a nanosphere as a function of the nanosphere radius, including the scattering attenuation (∼ vF /(2λB ) + CvF /(2a)) (midgrey line) and the Lorentz friction damping (∼ a 3 ) (light grey line). For radii greater than approximately 11 nm (for Au), the second channel dominates the overall damping (black line). (Right) The damping rate calculated with the perturbative treatment of the Lorentz friction, as in Eq. (6.23), with, for comparison, the damping rate calculated using the exact formula (6.24) for the Lorentz friction.
Table 6.1 (one can observe that a ∗ and a ∗∗ depend weakly on the material but more strongly on the dielectric forming the surroundings). In the region of the crossover in the size dependence of the plasmon damping, the perturbative approximation agrees with the exact solution, as illustrated in Fig. 6.2 (right). However, the perturbatively calculated damping is heavily overestimated for a > 30 nm (for Au in vacuum). At a 57 nm (for Au in vacuum), the perturbative value of 1/τ ω1 equals 1, which corresponds to the overdamped regime for the oscillatory equation. This is an artefact of the perturbation approach and has been removed in the exact solution of Eq. (6.20) presented
6.3
Transfer of Sunlight Energy Mediated by Surface Plasmons
109
in Eq. (6.24). Theexact oscillating solution also exists for a > 57 nm, although the relation ω = ω1 1 − 1/(τ ω1 )2 no longer holds (for a > 25 nm). The resonance selffrequency and the attenuation rate are given by the exact formula (6.24) and are illustrated in Figs. 6.1 and 6.2 (right). The exact solution in Eq. (6.24) improves the fit with experiment of the resonance frequency of dipole surface plasmons. The radiative damping of plasmons in metallic nanospheres, as described above, corresponds to the free oscillations of a dipole in vacuum or in dielectric sur√ roundings (in the latter case, ω1 must be renormalized by the factor 1/ ε, where ε is the relative permittivity of the surrounding dielectric medium). If, however, another electrical system is present in the vicinity of the nanosphere, the situation changes significantly. The coupling of plasmons to other charged systems causes resonant energy transfer, which results in an increase in the plasmon damping. For the case in which a nanosphere is deposited on the surface of a semiconductor, the nearfield coupling of the plasmons with the band electrons of the semiconductor must be taken into account. In such a case, a quantum mechanical estimation of the related attenuation rate can be found by applying the Fermi golden rule to the semiconductor interband transitions induced by dipole nearfield coupling with the plasmons [23, 124]; we will analyse this in the following section for nanospheres of various radii deposited on a semiconductor substrate. 6.3 Transfer of Sunlight Energy to a Semiconductor Mediated by Surface Plasmons through the Channel of Dipole Coupling in the NearField Regime 6.3.1 Fermi Golden Rule for Band Electron Transitions due to Coupling with Plasmons The presence of an energy receiver in the vicinity of metallic nanospheres with plasmons, as in the case of a semiconductor layer on which nanoparticles are deposited, provides a channel for energy transfer from the plasmons to the band electrons. The plasmon damping in this case is highly modified in comparison with free oscillations in a metallic nanoparticle placed in dielectric surroundings and radiating energy in the farfield zone. In the latter case the locally planewave photons take away energy via the conventional Lorentz friction mechanism. These photons have no contact with the source after being emitted. In the nearfield zone when plasmons couple with the band electrons in the substrate semiconductors the situation is different. In the nearfield zone photons have not yet been formed and the coupling of the emitter and the receiver causes a strong mutual influence. Beyond this zone the classical Maxwell electrodynamics properties of the emitter depend on the receiver, which must be taken into account quantum mechanically using
110
Plasmon Photovoltaic Effect
the quantum transition scheme [75]. To assess the efficiency of energy transfer from the plasmons to the semiconductor substrate via the nearfield coupling of plasmons and electrons, we will apply the Fermi golden rule. This allows for the calculation of the transition probability per time unit for an electron to hop between the valence and conduction bands as a result of the coupling of the electrons to the dipole surface plasmons in a metallic nanosphere. The Fourier components of the magnetic field (Bω ) and electric field (Eω ) produced at a distant point R by a monochromatic plasmonic dipole oscillation at the origin, D = D0 e−iωt , can be represented by the equations [55] ik ik 1 ˆ Bω = √ [D0 × n] (6.26) − 2 eikR R R ε and
2 2 k 1 1 k 3 ik 3ik ˆ nˆ · D0 ) − − 2 + 3 D0 eikR, (6.27) Eω = + 2 − 3 + n( ε R R R R R R
where we use the following notation for the retarded argument: iω (t − R/c) = iωt − ikR and nˆ = R/R. The contributions with denominators R 3 , R 2 , and R are referred to as the near, medium and farfield zones of the dipole radiation, respectively. For interactions with the adjacent layer of the semiconductor, the nearfield zone is of the most significance. One can therefore neglect the terms containing that e ikR = /1 for the near field, 1/R and 1/R 2 . Under the further assumption . one obtains Bω = 0 and Eω = (1/εR 3 ) 3nˆ nˆ · D0 − D0 , which corresponds to the dipole electric field. The magnetic field disappears in the nearfield zone. Photons are not created yet at these small distances much less than the resonance wavelength. Thus, the related potential for the nearfield interaction of the Mietype surface plasmons with the band electrons can be written as follows [55]: e nˆ · D0 sin(ωt + α) = w+ eiωt + w − e−iωt , w = eψ(R,t) = εR 2 (6.28) − ∗ e eiα + nˆ · D0 . w = w = εR 2 2i The terms in w+ and w− correspond to emission and absorption, respectively (nˆ = R/R and D0 is the plasmon dipole amplitude). We will consider the emission of energy from the plasmon oscillations and the transfer of this energy to the electron system in the semiconductor substrate. The semiconductor band system is modelled here in the simplest form, the singleband parabolic effectivemass approximation. According to the Fermi golden rule, the interband transition probability is given by the expression w(k1,k2 ) =
2 2π k1 w + k2 δ(Ep (k1 ) − En (k2 ) + h¯ ω), h¯
(6.29)
6.3
Transfer of Sunlight Energy Mediated by Surface Plasmons
111
where the Bloch states in the conduction and valence bands are assumed to be plane waves (for the sake of simplicity): k 1 =
1 eik1 ·R−iEp (k1 )t/h¯ , (2π)3/2 h¯ 2 k2 Ep (k1 ) = − ∗1 − Eg , 2mp
k2 =
1 eik2 ·R−iEn (k2 )t/h¯ , (2π)3/2
h¯ 2 k22 En (k2 ) = , 2m∗n
(6.30)
where the indices n and p refer to electrons from the conduction and valence bands, respectively, and Eg is the forbidden gap. Here, let us make a technical comment. The electron wave functions as given above are assumed to be normalized to the Dirac delta, which corresponds to infinite particle movement and a continuous energy spectrum. The modulus squared of the wave function does not, in this case, carry a probabilistic interpretation, for which it must be normalized to unity. To restore proper normalization, the expression 2 2π k1 w + k2 δ(Ep (k1 ) − En (k2 ) + hω) w(k1,k2 ) = ¯ h¯ must be the squared Dirac delta function, which can be expressed by the divided by 2 factor V /(2π)3 , taking into account that 1 V d 3 reik·r = δ(k) (for k = 0) (V → ∞). (6.31) 3 (2π) (2π)3 The same factor occurs, however, from the density of states, when
2 one integrates over all initial and final states k1,k2 , which results in the factor 2V /(2π)3 (the factor 2 arises because of spin degeneracy). Thus, the renormalization factors mutually cancel. Taking into account the renormalization described above, we find the matrix element 1 1 e iα d 3R (6.32) e nˆ · D0 2 e−i(k1 −k2 )·R . k1 w + k2 = (2π)3 ε2i R Here, the integrals can all be computed analytically. After some algebra, one arrives at the expression (see also the derivation of Eq. (6.75) below) ∞ −1 eeiα 1 d sin(qR) k1 w + k2 = cos (2π) dR D 0 (2π)3 ε q dR qR a (6.33) iα iα 1 ee D0 · q sin(qa) a→0 1 ee D0 · q = −−→ . (2π)2 ε q2 qa (2π)2 ε q2 To estimate the absorption probability per time unit, a summation over all initial and final states in both bands must be performed. Thus, we arrive at the following formula for the transition probability: . / (6.34) δw = d 3 k1 d 3 k2 f1 (1 − f2 )w(k1,k2 ) − f2 (1 − f1 )w(k2,k1 ) ,
112
Plasmon Photovoltaic Effect
where f1 and f2 represent temperaturedependent Fermi–Dirac distribution functions for the initial and final states, respectively. Emission and absorption are included but, for room temperature, one can assume that f2 0 and f1 1, which leads to 3 (6.35) δw = d k1 d 3 k2 · w(k1,k2 ). In the above formula, we have eliminated the state density factors through probability normalization, as mentioned above. After integrating we arrive at the expression (see Eq. (6.85) below) ¯ − Eg )e2 D02 1 sin2 (xaξ ) 4 μ2 (m∗n + m∗p )2(hω dx 1 − x2 δw = ∗ ∗ 3 (xaξ )2 mn mp 2π h¯ 5 ε2 0 (6.36) e2 D02 2 1 sin2 (xaξ ) 4 μ2 2 = ∗ ∗ ξ dx 1−x . 3 mn mp 2π h¯ 3 ε2 (xaξ )2 0 In the limiting cases, we obtain (see the derivation of Eq. (6.87) below) ⎧ ¯ − Eg )e2 D02 ⎪ 4 μ m∗n m∗p (hω ⎪ ⎪ for aξ 1, ⎨ 3 h¯ 5 ε2 δw = (6.37) √ ⎪ 4 μ3/2 2 hω ⎪ ¯ − Eg e2 D02 ⎪ ⎩ for aξ 1, 3 a h¯ 4 ε2 where 2(hω ¯ − Eg )(m∗n + m∗p ) . ξ= h¯ In the latter case represented in Eq. (6.37) we have applied the approximation ∞ 1 sin2 (xaξ ) 1 sin2 (xaξ ) π 2 dx 1 − x ≈ (for aξ
1) d(xaξ ) = , 2 2 (xaξ ) aξ 0 (xaξ ) 2aξ 0 1 √ whereas in the former case 0 dx 1 − x 2 = π/4. Note that the above formulae are fundamentally distinct from those for the ordinary photoeffect, for which (see Section 6.5, the derivation of Eq. (6.84)) √ 2 εE0 V 4 2 μ5/2 e2 3/2 (hω δw0 = (6.38) ¯ − Eg ) . 3 ∗2 3 mp ωεh¯ 8π hω ¯ Taking that the number of photons in the volume V is equal to 2 into account
εE0 V /(8π hω) , the probability of singlephoton absorption by the semiconductor ¯ per unit time takes the following form for the ordinary photoeffect: √ 2 −1 εE0 V 4(4) 2 μ5/2 e2 = (hω − Eg )3/2, (6.39) q0 = δw0 3 ¯ 8π hω 3 m∗2 ωε h ¯ ¯ p where the factor 4 corresponds to the spin degeneracy of the band electrons.
6.3
Transfer of Sunlight Energy Mediated by Surface Plasmons
113
6.3.2 Plasmon Damping Rate due to NearField Coupling with SemiconductorBand Electrons The probability per time unit of a transition between states of the band electrons in the semiconductor substrate is given by Eq. (6.37), as derived in Section 6.5 below in accordance with the Fermi golden rule. Let us emphasize that because of the absence of momentum conservation for the nearfield dipole coupling in the vicinity of a nanosphere, all interband transitions contribute, not only the direct ones (as in the case of interaction with a plane wave). This results in the enhancement of the transition probability for nearfield coupling in comparison with the photon (planewave) absorption rate in a semiconductor in the ordinary photoeffect. However, this enhancement is gradually quenched as the radius a increases, as is expressed in Eq. (6.37). Assuming now that dipole plasmon oscillations are excited by the rapid switching off of the uniform electric field, so that E(t) = E0 (1 − (t)), we consider the dipoletype solution for surface plasmons [23],
D(t) = [0,0,D0 e−t/τ cos(ω1 t)]
(6.40)
with D0 =
e2 ne 4π 3 E0 a . 3 mω12
(6.41)
In such a case, one can estimate the total energy transfer A to the semiconductor (assuming that the dominant channel of dissipation is the nearfield interaction with the semiconductor substrate, neglecting the shift of ω1 with respect to ω1 caused by dissipation, and using Eq. (6.37) for δw): ∞ A=β 0
δwhω ¯ 1 dt = β hω ¯ 1 δwτ /2
⎧ (6.42) ¯ 1 − Eg )e2 D02 2 βω1 τ μ m∗n m∗p (hω ⎪ ⎪ for aξ 1, ⎨ 4 2 √ h¯ε = 3 3/2 ⎪ τ μ 2 hω βω 2 ¯ 1 − Eg e2 D02 1 ⎪ ⎩ for aξ 1, 3 a h¯ 3 ε2 where β accounts for the proximity constraints, not included microscopically in the model, that reduce the nearfield contact of the sphere with the semiconductor medium. For the case of nanospheres deposited on the surface of a semiconductor layer, β ∼ h2 /a 2 ∼ 10−3 for a ∼ 50 nm (h is the effective range of the nearfield coupling), whereas for nanospheres that are entirely embedded in their semiconductor surroundings, β would be significantly enhanced. Comparing the value given by the formula (6.42) with the energy loss estimated in [23] (the total energy of the plasmon oscillations), one finds that
114
Plasmon Photovoltaic Effect
⎧ 4βμ m∗n m∗p (hω ¯ 1 − Eg )e2 a 3 ⎪ ⎪ ⎨ 1 3h¯ 4 ε √ = 3/2 4βμ 2 hω τ ω1 ⎪ ¯ 1 − Eg e 2 a 2 ⎪ ⎩ 3h¯ 3 ε
for aξ 1, (6.43) for aξ 1.
For nanospheres of Au deposited on an Si layer, we obtain for a in nm ⎧ √ ∗ ∗ mn mp ⎪ 3μ ⎪ for a
0.15 m/(m∗n + m∗p ), 44.092βa ⎨ 1 m m (6.44) = ) μ *3/2 τ ω1 ⎪ ⎪ 2 ⎩ 13.648βa for a 0.15 m/(m∗n + m∗p ), m where for light (heavy) carriers in Si, m∗n = 0.19m(0.98m) and m∗p = 0.16m(0.52m), with m the bare electron mass, μ = m∗n m∗p /(m∗n + m∗p ), Eg = 1.14 eV, ε = 12, and hω ¯ 1 = 2.72 eV. For these parameters and for nanospheres with radius a in the range 5−50 nm, the second case of Eq. (6.44) applies. The value of the parameter β obtained from a fit to the experimental data is equal to approximately 0.002 (see Table 6.2 for the details of this fitting). One can also notice that for a very high value of β (β > β ∗ in Fig. 6.3), the plasmon oscillator enters the overdamped regime. The energy transfer to the semiconductor substrate via the nearfield coupling channel is so efficient that it quenches free plasmon oscillations. In this case the estimation of the damping rate presented above is not applicable because free oscillations are thus not possible in the case of such strong attenuation. Nevertheless, it is possible for oscillations to continue but in the forcedoscillator regime. In this case, the energy transfer to the substrate system (calculated on the basis of on the Fermi golden rule and given by Eq. (6.42)) is equal to the output power of the forcing field. According to the standard formula for a harmonically forced and damped oscillator, this output power (averaged over the oscillation period) is equal to P =
E02 a 3 ωp2 3
ω2 τ . (ω12 − ω2 )2 τ 2 + 4ω2
(6.45)
Table 6.2 Fitting the parameter β to the experimental data presented in [33] for Au nanospheres on an Si layer a ns (nm) (108 /cm2 )
−2 hω ¯ = hω ¯ 1 1 − 2 (τ ω1 ) (eV) (theoretical)
h¯ ω (eV) (exp.) I /I
50 40 25
2.37 (β = 0.0016), 2.14 (β = 0.002), 2.25 (β = 0.0018) 2.58 (β = 0.0016), 2.48 (β = 0.002), 2.53 (β = 0.0018) 2.70 (β = 0.0016), 2.68 (β = 0.002), 2.69 (β = 0.0018)
2.25 2.48 2.70
0.8 1.6 6.6
1.55 1.9 1.75
6.3
Transfer of Sunlight Energy Mediated by Surface Plasmons
115
a (nm) Figure 6.3 Critical value β ∗ of the β parameter for a plasmon oscillator in the overdamped regime β > β ∗ as a function of the nanosphere radius a.
We also have, for the power of the plasmonic energy output, P = β hωδw. ¯ A comparison of the two expressions yields ωp2 a 3 1 δw β hω . = ¯ 2 τ 3ω D02
(6.46)
Note that, in such an approach, one obtains the damping rate as a function of the photon frequency. Moreover, it should be noted here that a phenomenological approach analogous to that for a driven and damped oscillator will not correspond exactly to a real quantum system of plasmons, which are quantum quasiparticles that are given by the poles of an appropriate response function (i.e., a retarded Green function), where the real and imaginary parts of the pole are well defined. However, in the case of strong coupling with a nearby receiver of energy when the damping is strong, the similarity to the quasiparticle model lessens (quasiparticles do not exhibit frequency and damping rates identical to those of a forced and damped oscillator). Thus, for the strong damping case, and especially when the corresponding oscillator model lies in the overdamped regime, the quasiparticle approach to these forced plasmon oscillations does not hold. For the damped and driven oscillator approach, one can consider the driven oscillations of a plasmon with a frequency far lower than the free plasmon resonance frequency and with a damping rate that is dependent on the frequency of the forcing field. A comparison of the results for the damping rates obtained using the two approaches is presented in Fig. 6.4, where it is evident that, for wavelengths close to the dipole surface plasmonic resonance, the damping rate for the damped and driven oscillator model is slightly greater than the corresponding damping rate obtained using the quasiparticle approach to the plasmons.
116
Plasmon Photovoltaic Effect
t –1 (1015s–1)
1.2
a = 100 nm
1.0 0.8
80 nm
0.6 0.4
60 nm
0.2
40 nm 20 nm
0.0 200
400
600
800
1000
l (nm)
t –1 (1015s–1)
1.2
l = 600 nm
1.0 0.8 0.6 0.4 0.2 0.0 0
20
40
60
a (nm)
80
100
Figure 6.4 (Upper panel) The damping rate τ −1 versus the wavelength λ and the nanoparticle radius a, estimated in the phenomenological approach to plasmon oscillations using the damped and driven oscillator model, in which the damping is dependent on ω = 2π c/λ (solid line), and also in the quasiparticle plasmon model, in which the damping rate is independent of ω (broken lines). In the lower panel the damping rate for λ = 600 nm versus a is presented.
6.3.3 Transfer of Light Energy via the Plasmon Channel To assess the efficiency of the plasmon nearfield coupling channel, one can estimate the ratio of the probability of energy absorption in the semiconductor via the mediation of the surface plasmons (per single photon incident on a metallic nanosphere, qm ) to the probability of energy absorption in the semiconductor directly from planewave illumination (also per single photon, q0 , as given by Eq. (6.39)). The probability qm is equal to the product of δw, given by Eq. (6.37), and the number of metallic nanospheres Nm divided by the photon density, with an additional phenomenological factor β that is responsible for all effects that are not directly taken into account (such as deposition separation and surface properties reducing the coupling strength): 2 −1 εE0 V . (6.47) qm = βNm δw 8π hω ¯ In the balanced state, when incoming light energy is transferred to the semiconductor via plasmon nearfield coupling, we can consider the stationary solution
6.3
Transfer of Sunlight Energy Mediated by Surface Plasmons
117
for a driven and damped plasmon oscillator. The driving force is the electric field of the incident plane wave, and the damping force is the nearfield energy transfer described by 1/τ , calculated using formula (6.37) in the manner described in the previous subsection. The resulting redshifted resonance, with a simultaneously reduced amplitude, allows the energy transfer to the semiconductor to accommodate to balance the incident photon energy. Within this model, the amplitude of the resonant plasmon oscillations D0 (ω) is thus determined by f (ω) =
1
.
(ω12 − ω2 )2 + 4ω2 /τ 2
The extremum of the redshifted resonanceis attained at ωm = ω1 1 − 2(ω1 τ )−2 ,
with the corresponding amplitude ∼ τ/ 2 ω12 − τ −2 . The shift is proportional to 1/(ω1 τ 2 ) and scales with the nanosphere radius a, in a similar manner, i.e., diminishing with decreasing a, to that observed in experiments [33] (note again that for scatteringinduced 1/τ0 , the dependence on a is the opposite, i.e., it increases with decreasing a). In the case of this energy transfer balance, according to Eq. (6.37) one obtains ⎧ ⎪ 128 2 3 μ m∗n m∗p e6 n2e ω 2 ⎪ ⎪ ( hω − E ) f (ω) for aξ 1, π a ¯ ⎨ βC0 g 9 m2 h¯ 4 ε3 qm = ⎪ 128 √ 2 2 μ3/2 e6 n2e ω 2 ⎪ ⎪ hω − E 2π a f (ω) for aξ 1, ⎩ βC0 ¯ g 9 m2 h¯ 3 ε3 (6.48) where f (ω) is given above and corresponds to the amplitude factor for the forced oscillator and D0 = (e2 ne E0 4πa 3 /(3m))f (ω); furthermore, C0 = Nm 4/3πa 3 /V , V is the volume of the semiconductor, and ξ = 2(hω ¯ − Eg )(m∗n + m∗p )/h. ¯ Given that q0 is the direct photoeffect transition probability (see (6.39)), the ratio qm /q0 can be expressed as follows: ⎧ 2 3 √ 8π a βC0 m∗n (m∗p )5/2 e4 n2e ω2 f 2 (ω) ⎪ ⎪ √ ⎪ ⎪ 3 ⎨ 3 2μ3/2 m2 hω ¯ − Eg h¯ ε2
qm = ⎪ q0 ⎪ 8π 2 a 2 βC0 (m∗p )2 e4 n2e ω2 f 2 (ω) ⎪ ⎪ ⎩ 2 3μm2 (hω ¯ − Eg )h¯ ε2
for aξ 1, (6.49) for aξ 1.
This ratio proves to be of order 104 × 40β/H (nm) (note that, at a typical surface density of nanoparticles, e.g., ns ∼ 108 /cm2 , C0 = ns 4πa 3 /(3H ) where H is the depth of the semiconductor layer). This, including the phenomenological factor β and the depth H , is sufficient to explain the scale of the experimentally observed strong enhancement of the absorption and emission rates. The strong enhancement of the transition probability is related to the fact that momentumnonconserved
118
Plasmon Photovoltaic Effect
transitions are allowed; however, it rapidly decreases with increasing radius a in accordance with formula (6.37). For example, for a ∼ 10−60 nm this results in a reduction in the transition probability, which can be included [23] by means of the effective phenomenological factor β (with a fitted experimental value of β 28 × 10−3 (50/a(nm))2 ) in the case of the atomic limit, a = 0. The enhancement of the nearfieldinduced interband transition in the case of large nanospheres, however, is still significant because the diminished role of the sizerelated quenching of the transitions is partially compensated by the ∼ a 3 growth of the dipole amplitude of the plasmon oscillations. The high (although decreasing with increasing a) efficiency of the nearfield energy transfer from the surface plasmons to the semiconductor substrate is primarily attributable to the contribution of all interband transitions, not just the direct (vertical) transitions as in the case of the ordinary photoeffect, because of the absence of the momentum conservation constraints on the nanosystem. The strengthening of the probability transition as a result of the contribution of all indirect interband paths of excitation in the semiconductor is probably responsible for the experimentally observed strong enhancement of the light absorption and emission in diode systems mediated by the surface plasmons in nanoparticle surface coverings [32–34, 117–119]. For comparison with experiment, we can estimate the photocurrent in the case of an Si photodiode with a metallically modified photoactive surface. This photocurrent is given by I = eN(q0 + qm )A, where N is the number of incident photons, q0 and qm are the probabilities of singlephoton absorption in the ordinary photoeffect [59] and of singlephoton absorption mediated by the presence p of metallic nanospheres, respectively, and A = τfn /tn + τf /tp is the amplification n(p) factor; here τf are the recombination times of carriers of both signs and tn(p) are the drive times, i.e., the times required for the carriers to traverse the distance between electrodes. From the above formulae, it follows that if I = I (qm = 0), is the photocurrent without metallic modifications then I qm =1+ , I q0
(6.50)
where the ratio qm /q0 is given by Eq. (6.49). The results are given in Fig. 6.5 and reproduce the experimental behaviour well [33]. Both channels of photon absorption that result in a photocurrent in the semiconductor sample are included, namely, direct ordinary photoeffect absorption, with the transition probability q0 , and plasmonmediated absorption, with transition probability qm . Note also that certain additional effects, such as the reflection of incident photons or destructive interference on the metallic net, may contribute; these effects are accounted for phenomenologically in the plasmonmediated channel by the fitted experimental factor β. However, these corrections are rather
6.3
Transfer of Sunlight Energy Mediated by Surface Plasmons model fitting experimental data
model fitting experimental data
119
model fitting experimental data
Figure 6.5 Dependence of the normalized photocurrent I (λ)/I : for comparison, the experimental data [33] for (left) a = 25 nm and ns = 6.6 × 108 /cm2 , (centre) a = 40 nm and ns = 1.6×108 /cm2 , and (right) a = 50 nm and ns = 0.8×108 /cm2 (H = 3 μm).
weak for the low densities of metallic coverings considered here, of the order of 108 /cm2 , and for nanosphere sizes much lower than the resonance wavelength, although they would play a stronger reducing role for larger concentrations and larger nanosphere sizes [105, 111]. The resonance threshold is accounted for by the damped resonance envelope function in Eq. (6.50), which also includes the semiconductor bandgap limit. As indicated in Fig. 6.5, the relatively high value of qm /q0 ∼ 104 40β/H (nm) enables, by an increase in β or a reduction in H (at constant ns ), a significant enhancement in the efficiency of photoenergy transfer to the semiconductor that is mediated by the surface plasmons in the nanoparticles deposited on the active layer. However, because an enhancement of β could easily push the system into the overdamped regime, the more favourable prospect is to lower H , as in a thinfilm solar cell with a smaller activelayer depth. Using an Si photodiode, a photocurrent enhancement close to the factor 2 was achieved (see the solid lines in Fig. 6.5). The structure of the diode in the experiment was optimized to reveal the plasmonic effect and was not the structure used in highefficiency siliconbased solar cells. The estimated junction depth was approximately 80 nm from the device surface, i.e., sufficiently close to justify the nearfield approximation for dipole coupling with plasmons. It is worth noting that a strong photocurrent enhancement was observed at relatively low surface concentrations of the metallic nanocomponents. However, in many efficiencyoptimized devices used in real solar cells, experimentally observed enhancements due to metallic nanocomponents are not so pronounced [36]. The details of the experimental setup utilized for the fitting presented in Fig. 6.5 are described in [33]. The plasmon effect is related only to the shallowest layer of the photodiode, at a depth of a few hundred nanometres at most, and plays an important role in the particular diode setup with
120
Plasmon Photovoltaic Effect
suitably located active layer only. If the active layer is located at a larger distance from the metal nanoparticle plasmonic light converters then the strengthening of the efficiency would disappear. The overall behaviour of I /I (ω) = 1 + qm /q0 , as calculated in accordance with Eq. (6.49) and depicted in Fig. 6.5, is quite consistent with the experimental observations [33] in terms of the positions, heights, and shapes of the photocurrent curves for the different samples (the strongest enhancement is achieved for a = 40 nm). Plasmon mediation in solar energy harvesting also opens the possibility of nonlinear photovoltaic (PV) effects related to high concentration of the electric field in the local surroundings of the metallic nanoparticles [125]. In the case of such PV effects, twophoton absorption is considered as an important nonlinear channel [126] but the inclusion of metallic nanocomponents would cause another effect, that of local modification of the band structure in the substrate semiconductor, which would interfere with the absorption of energy via the dipole channel from surface plasmons. Remarkable is the presence of nonlinear effects even at relatively small intensities of the incident photon beam [125, 127]. These nonlinear phenomena lie outside our present consideration but ought to be taken into account in a more realistic analysis together with other competing factors; the result would finally be an increase in the efficiency of solar cells due to the plasmon effect being less than the strengthening factors obtained within the idealized and simplified models. 6.4 Experimental Demonstration of the Proximity Constraints of the Plasmon Effect The problem arises of how large is the range of the plasmon photovoltaic effect. An experimental verification of the micrometre scale of this range has been performed [30]. The idea of this experiment consists in the preparation of a doublelayered semiconductor substrate structure with a spacer layer separating the metallic nanoparticles from the bottom layer. The bottom layer and the spacer layer are photoactive, but their contributions to the photocurrent can be distinguished because of the different spectral characteristics of both materials. Measurement of the photocurrent with and without metallic nanoparticles deposited on the top of the spacer layer enables a determination of the range of the plasmonic effect in comparison with the spacer thickness. The spacer material in the experimental setup was ZnO, with a direct band gap of 3.34 eV [128]. The spacer layer consisted of vertically aligned nanorods of ZnO [129] with length of about 1 μm and diameter of order 300 nm. Such a structure is manufactured by a deposition method [130]. In the experiment with the layered
6.4 Proximity Constraints of the Plasmon Effect
121
Figure 6.6 Micrographs of the ZnO nanorod structure deposited on the Si substrate.
Figure 6.7 (Left) Magnified SEM image showing the Ag nanoparticles covering the ZnO nanorods. (Right) AZO layer is deposited on the ZnO nanorods with their Ag covering, to provide a transparent conductive oxide layer, with thickness 350 nm.
structure described above, ntype ZnO nanorods were used that had been grown via a lowtemperature hydrothermal method on the Si substrate, see Fig. 6.6. The tops of the ZnO nanorods were then covered with silver nanoparticles with radius approximately 5 nm. Images obtained using SEM of the structure before deposition of a transparent AZO1 film are shown in Fig. 6.6, and at a higher magnification in Fig. 6.7. The sample with Ag nanoparticles and the related reference sample without 1 ZnO doped with aluminum to produce a lowresistivity but highly transparent layer.
122
Plasmon Photovoltaic Effect
nanoparticles are shown in Figs. 6.6 and 6.7. The ZnO nanorods in Fig. 6.6 have a hexagonal shape, indicating the wurtzite crystalline structure. The surface density of the Ag nanoparticles was about 5 × 1010 /cm2 . As the bottom substrate, ptype Si(100) wafer was used. The substrate with ZnO seeds on its surface was next placed in a reaction mixture. Here the growth of the ZnO nanorods proceeded at atmospheric pressure and a temperature of approximately 60 ◦ C. The hexagonal final nanorods were of ∼ 1 μm in length and 300 nm in diameter. On the top of ZnO nanorods, Ag nanoparticles with radius ca. 5 nm were distributed via shortduration sputtering (Fig. 6.7 (left)). The total system was finally covered by an AZO film of thickness 350 nm by means of lowtemperature atomic layer deposition. The AZO layer serves as a transparent conductive layer (Fig. 6.7 (right)). The photoresponsivity was measured using a PV quantum efficiency measurement system with a temperature control. No bias was applied during the measurement, so that the zerobias photocurrent was measured. The result of the photoresponsivity measurement is illustrated in Fig. 6.8. Notice that the pronounced increase (by a factor 2) in PV efficiency due to the plasmonic effect is observed only as a result of the ZnO layer of nanorods covered with Ag nanoparticles, whereas the efficiency of the Si substrate at distances from the Ag nanoparticles of more than 1 μm was much more weakly affected. This observation provides direct evidence that the plasmonic PV efficiency enhancement is a shortrange effect not exceeding 1 μm distance between the metallic nanoparticles and the substrate. In Fig. 6.8 the photoresponsivity of the pSi/nZnO/Ag NPs/AZO system under study and that of a reference diode without nanoparticles, pSi/nZnO/AZO, as well as that for a sole Si photodiode are shown for comparison. The spectral responsivity for the tested system with and without Ag nanoparticles was lower than that of the commercial Si photodiode within the whole wavelength range because the diodes under study were not optimized to reach the best performance (unlike the reference Si diode). Within the 400–600 nm wavelength range, the responsivity does not follow the linear dependence expected for Si. Instead, the measured responsivity grows and reaches a local maximum plateau. Silver nanoparticles deposited on top of the whole structure increase the effect, with an additionally hump around 500 nm. Other studies of the pSi/nZnO [131, 132] and nSi/pZnO [133] systems suggest that the enhancement of the responsivity within the 400−600 nm wavelength range is due to the subbandgap trap states in ZnO and at the ZnOSi interface [131, 132]. All these arguments support the interpretation that the signal within 400−600 nm is related to the ZnO layer [134]. Some authors [135] have also highlighted the role of surface defects in ZnO nanostructures, which could enhance the
6.4 Proximity Constraints of the Plasmon Effect
123
Wavelength (nm) Figure 6.8 Spectral responsivity of the calibrated Si photodiode (open circles) and the studied pSi/nZnO(nanorods)/AZO photodiode, without silver nanoparticles (triangles) and with silver nanoparticles (squares). NR, nanorods as in Fig. 6.6; NP, nanoparticles as in Fig. 6.7; Au, ohmic bottom contact. There is a strengthening, by a factor ∼ 2, of the PV response of the twolayer system consisting of ZnO nanorods (with length approximately 1 μm) deposited on the Si substrate and covered with Ag nanoparticles of approximately 5 nm in radius; the band structure of ZnO allows one to distinguish the related PV response from that of the Si component of the system and to observe that the plasmon effect applies only to the nearby nanorods with respect to the Ag nanoparticles.
range of the photoresponsivity especially effectively for a nanorod geometry with a strongly developed surface. This is the most probable scenario for the increased photoresponsivity within the energy range of the spectrum shown in Fig. 6.8 below the band gap of ZnO. The ordinary photoeffect in both components of the twolayer structure under study allows us to distinguish the plasmonic strengthening in the two layers, mostly because of the different band gaps in ZnO and Si. When metallic nanoparticles were deposited on the top of the spacer, a significant increase (by a factor 2) of the photocurrent was observed in the frequency region relating to ZnO. The region relating to Si exhibited significantly reduced changes, demonstrating that the separation of the metallic nanocomponents by a distance of 1 micrometre strongly reduced the plasmonic effect in the bottom Si layer. This finding indicates that the plasmonic photovoltaic effect may be particularly beneficial in ultrathinfilm solar cell technology.
124
Plasmon Photovoltaic Effect
6.5 Calculation of the Matrix Element for the Fermi Golden Rule Expression (6.37) Let us calculate in detail the probability per time unit for interband transitions of electrons in a substrate semiconductor on which metallic nanospheres with radius a are deposited. These transitions are induced by photonexcited surface plasmons in the metallic component. The surface plasmons excited in the nanosphere couple to the semiconductor band electrons in the nearfield regime. The situation is similar to the ordinary photoeffect, though the perturbation of the electron system in the semiconductor is not of planewave form as in the case of the direct illumination of a semiconductor by incident photons, but attains the form of dipoletype nearfield electric interaction [55, 23]. This causes a change in the matrix element in the relevant Fermi golden rule formula. The potential for the nearfield interaction of the surface Mietype plasmons with the band electrons can be written as [55] e nˆ · D0 sin(ωt + α) = w+ eiωt + w − e−iωt , w = eψ(R,t) = ε0 R 2 (6.51) − ∗ e eiα + nˆ · D0 . = w = w ε0 R 2 2i The terms w+,w− correspond to emission and absorption, respectively (nˆ = R/R, D0 is the dipole surface plasmon amplitude). We choose the first term in order to consider the emission of energy from the plasmon oscillations and its transfer to the electron system in the semiconductor substrate. We model the semiconductor band system using the simplest singleband parabolic effectivemass approximation. The interband transition probability is given by the Fermi golden rule: 2 2π k1 w + k2 δ(E(k1 ) − E(k2 ) + hω), (6.52) w(k1,k2 ) = ¯ h¯ where the Bloch states in the conduction and valence bands are assumed to be plane waves for the sake of simplicity, k1 =
1 eik1 ·R−iE(k1 )t/h¯ , (2π)3/2 h¯ 2 k2 E(k1 ) = − ∗1 − Eg, 2mp
k2 =
1 eik2 ·R−iE(k2 )t/h¯ , (2π)3/2
h¯ 2 k22 E(k2 ) = , 2m∗n
(6.53)
the indices n,p refer to electrons from the conduction and valence bands, respectively, and Eg is the forbidden gap. The electron wave functions are normalized to the Dirac delta function, which corresponds to an infinite movement and a continuous energy spectrum. The modulus squared of the wave functions do not have, in this case, a probabilistic interpretation (for which normalization to unity is required); therefore the expression, 2 2π < k1 w + k2 > δ(E(k1 ) − E(k2 ) + hω) w(k1,k2 ) = ¯ h¯
6.5 Calculation of Fermi Golden Rule Expression
125
Figure 6.9 The reference frame is chosen such that the vector q is oriented along the z axis, while the vector D0 lies in the xz plane.
2 has to be divided by the delta Dirac function squared, i.e., by the factor V /(2π)3 . This factor corresponds to proper normalization of the probability, because V 1 d 3 reik·r = δ(k) (for k = 0) (V → ∞). (6.54) (2π)3 (2π)3 Note that the same factor occurs also in the density of states when one integrates over all the initial and final states k1,k2 . The two integrals both give the factor 2 2V /(2π)3 (the factor 2 is caused by spin degeneracy). Thus, the renormalization factors cancel (independently of V → ∞). Taking into account the renormalization described above, one finds that 1 1 e iα d 3R (6.55) k1 w + k2 = e nˆ · D0 2 e−i(k1 −k2 )·R . 3 (2π) ε0 2i R Let us introduce the vector q = k2 − k1 . One can choose the coordinate system in such a way that the vector q is oriented along the z axis, and the vector D0 lies in the zx plane (as depicted in Fig. 6.9). Then, q = (0,0,q), nˆ = R/R = (sin 1 cos ψ1, sin 1 sin ψ1, cos 1 ), R = R(sin 1 cos ψ1, sin 1 sin ψ1, cos 1 ), D0 = D0 (sin ,0, cos ) and q · R = qR cos 1, nˆ · D0 = D0 (sin sin 1 cos ψ1 + cos cos 1 ). Hence,
1 1 e iα d 3R k1 w k2 = e nˆ · D0 2 e−i(k1 −k2 )·R 3 (2π) ε0 2i R ∞ 2 π iα R 1 ee = dR × sin 1 d1 D 0 (2π)3 ε0 2i R2 a 0 2π × dψ1 {cos cos 1 + sin sin 1 cos ψ1 }eiqR cos 1 +
0
(6.56) (6.57)
126
Plasmon Photovoltaic Effect
=
1 eeiα D0 cos 2π (2π)3 ε0 2i
∞
π
cos 1 sin 1 d1 eiqR cos 1 .
dR a
0
(6.58) In the integral over dψ1 the second term in the braces vanishes and only the first term contributes, with a factor 2π. Note that π π d d 2 sin x ix cos 1 . cos 1 sin 1 d1 e = −i sin 1 d1 eix cos 1 = −i dx 0 dx x 0 (6.59) Thus ∞ −1 eeiα 1 d sin qR D0 cos (2π) dR k1 w k2 = 3 (2π) ε0 q dR qR a 1 eeiα 1 sin qa 1 1 eeiα = → . D cos D cos 0 a→0 0 (2π)2 ε0 q qa (2π)2 ε0 q (6.60) +
The lower limit of the integral with respect to R is taken as a (the nanosphere radius). In this manner one can constrain the accessible space for planar waves in the semiconductor (if one assumes, for a model, a nanosphere completely embedded in the surrounding material). This is, however, a crude approximation as the tunnelling effect would certainly allow access to the inner nanoparticle space, to some extent at least. Moreover, if the nanosphere is deposited on the semiconductor surface one can confine the integration with respect to d1 to the segment [0,π/2], instead of [0,π]. In this case we obtain the following matrix element: ∞ 1 eeiα 1 d 1 − eiqR D cos (2π) dR 0 (2π)3 2iε0 q dR qR a iα iqa 1 ee 11−e 1 1 eeiα = D cos D0 cos , → 0 a→0 2 2 (2π) 2iε0 q qa (2π) 2iε0 q (6.61)
k1 w+ k2 =
because π/2 π/2 d d 1 − eix ix cos 1 . cos 1 sin 1 d1 e = −i sin 1 d1 eix cos 1 = dx 0 dx x 0 (6.62) In the limit a = 0, the modulus of the matrix element will be twice as small as in the case when the integration over d1 is taken over the whole space.
6.5 Calculation of Fermi Golden Rule Expression
127
Now we will integrate over all initial and final states of both bands. One can substitute the related integration over k1,k2 with integration over q,k2 . Scalar products are invariant under coordinate system rotation; therefore the result of integration will be the same whether q is along the z axis or D0 is the along the z axis. In the latter case gives the deviation of q with respect to z direction – this choice of reference frame is convenient for integration with respect to dq. Thus we arrive at a formula for the transition probability in the following form: 3 (6.63) δw = d k1 d 3 k2 (f1 (1 − f2 )w(k1,k2 ) − f2 (1 − f1 )w(k2,k1 )) , where f1,f2 are the temperaturedependent Fermi–Dirac distribution functions for the initial and final states, respectively. Emission and absorption are included in the overall transition probability, but for room temperatures one can assume f2 0 and f1 1, which leads to 3 (6.64) δw = d k1 d 3 k2 w(k1,k2 ). The above formula does not include the density state factors since they are cancelled by the probability renormalization, as mentioned above. We thus have to calculate the following integral: D02 cos2 sin2 (qa) h¯ 2 k12 h¯ 2 k2 e2 3 3 δ + − (h¯ ω − Eg ) , δw = d k2 d q (2π)3 h¯ ε0 q2 (qa)2 2m∗n 2m∗p (6.65) with 1 1 k22 + β q 2 − γ h¯ 2 k12 h¯ 2 k2 , + − ( h ω − E ) = δ cos − δ ¯ g 2 2m∗n 2m∗p α + β 2β qk2 2β qk2 where α = h¯ 2 /2m∗n , β = h¯ 2 /2m∗p , γ = h¯ ω−Eg , α = α/(α + β), β = β/(α + β), γ = γ /(α + β). For each integral with respect to k2 and q the coordinate system can be rotated independently, and for the integration over dk2 we choose again the orientation of q along the z axis, which leads to the spherical angle 2 in the product k2 · q = k2 q cos 2 . The expression for δw thus attains the form ∞ π 2 e2 D02 3 sin (qa) cos 2 δw = × dk2 k2 d2 sin 2 d q q 2a2 q2 (2π)3 hε ¯ 02 0 0 2π 1 1 k22 + β q 2 − γ . (6.66) × dψ2 δ cos 2 − α + β 2β qk2 2β qk2 0
128
Plasmon Photovoltaic Effect
Integration over d2 employs the Dirac delta. The relevant nonzero contribution (due to integration over d cos 2 ) is conditioned by the inequality −1
2 × 10 ⎪ Eg 1 ⎨ a ⎪ ξ h¯ ω − Eg ⎪ ⎪ for > 0.02, ⎩ < 2 × 10−9 (m) Eg and the value of this range weakly depends on the effective masses and Eg . Thus for nanoparticles with radii a > 2 nm the first regime holds only close to Eg (less
7.1 Probability of Electron Interband Excitation Due to Plasmons
137
than 2% of the distance of h¯ ω to the limiting Eg ), whereas the second regime holds in the rest of the ω domain. For comparison, ⎧ hω ¯ − Eg ⎪ −9 ⎪ > 0.5 × 10 (m) for < 0.5, ⎪ Eg 1 ⎨ a ⎪ ξ hω ¯ − Eg ⎪ ⎪ for > 0.5; ⎩ < 0.5 × 10−9 (m) Eg the first region widens considerably, to about 50% of the relative distance to Eg , but this holds only for ultrasmall nanoparticles (a < 0.5 nm). For larger nanoparticles, e.g., with a > 10 nm, the second regime thus dominates. Note that the above formula, Eq. (7.9), and its explicit form in limiting situations given by Eq. (7.10), is a generalization of the ordinary photoeffect, for which the transition probability is different [59]: √ 2 εE0 V 4 2 μ5/2 e2 3/2 (hω δw0 = (7.11) ¯ − Eg ) . 3 3 m∗2 8π hω ¯ ¯ p ωε h The number of photons of a frequencyω electromagnetic wave with electric field component amplitude E0 contained in the volume V equals εE02 V /(8π h¯ ω); hence, the probability of singlephoton absorption by the semiconductor per time unit attains the following form for the ordinary photoeffect [59]: √ 2 −1 εE0 V 4(4) 2 μ5/2 e2 = (hω − Eg )3/2 ; (7.12) q0 = δw0 3 ¯ 8π hω 3 m∗2 ωε h ¯ ¯ p as before, the factor 4 corresponds to the spin degeneracy of the band electrons. In the case of plasmon mediation, all oblique interband transitions contribute, not only vertical transitions (as in the ordinary photoeffect). This results in an enhancement of the transition probability for nearfield coupling in comparison with the planewave absorption rate in a semiconductor in the ordinary photoeffect. This enhancement is, however, gradually quenched with the growth in the radius a, as expressed by Eq. (7.10). The probability qm of energy absorption in a semiconductor, via the mediation of surface plasmons, per single photon incident on the metallic nanospheres equals the product of δw, given by Eq. (7.10), and the number Nm of metallic nanoparticles divided by the photon density and multiplied by the additional phenomenological factor β responsible for all effects not directly accounted for (such as deposition separation and surface properties reducing the coupling strength, as well as energy losses due to electron scattering and radiation from the farfield zone, i.e., Lorentz friction [55], into the upper hemisphere if the metallic nanoparticle is not completely embedded in the substrate semiconductor medium): 2 −1 εE0 V . (7.13) qm = βNm δw 8π hω ¯
138
Efficiency Enhancement by Nanoparticles: Material Dependence
7.2 Damping Rate for Plasmons in a Metallic Nanoparticle Deposited on a Semiconductor Assuming that the energy acquired by the semiconductor band system, A, is equal to the output of the plasmon oscillation energy, which results in plasmon damping, one can estimate the corresponding damping rate of the plasmon oscillations. Namely, at the damped plasmon amplitude D0 (t) = D0 e−t/τ , one finds for the total transmitted energy ⎧ 2 2 ⎪ ¯ g )e D0 2 βωτ μ m∗n m∗p (hω−E ⎪ ⎪ for aξ 1, ⎪ ∞ ⎨3 h¯ 4 ε2 A=β δwhωdt=β hωδwτ /2= ¯ ¯ √ ⎪ ⎪ 2 βωτ μ3/2 2 hω ¯ − Eg e2 D02 ⎪ 0 ⎪ for aξ 1, ⎩ 3 a h¯ 3 ε2 (7.14) where τ is the damping time rate and β accounts for losses not included in the model. Comparing the value of A given by the formula (7.14) with the energy loss by plasmon damping estimated in [23] (i.e., the initial energy of the plasmon oscillations, which is transferred step by step to the semiconductor, A = D02 /(2εa 3 )), one finds ⎧ ⎪ 4βωμ m∗n m∗p (hω ¯ − Eg )e2 a 3 ⎪ ⎪ for aξ 1, ⎪ ⎨ 3h¯ 4 ε 1 = (7.15) √ τ ⎪ ⎪ − Eg e 2 a 2 4βωμ3/2 2 hω ¯ ⎪ ⎪ for aξ 1. ⎩ 3h¯ 3 ε By τ we denote here the large damping rate of plasmons due to energy transfer to the semiconductor substrate, greatly exceeding the internal damping, characterized by τ , the latter being due to the scattering of electrons inside the metallic nanoparticle [23] (1/τ 1/τ ). We have neglected the radiation of plasmon energy to the farfield upperhemisphere zone, i.e., the Lorentz friction effect, which is also smaller than the nearfieldzone energy transfer to the substrate [23]. For example, for nanospheres of Au deposited on an Si layer we obtain, for ω = ω1 (the Mie selffrequency), with a in nm, ∗ ∗ ⎧ mn mp ⎪ 3μ ⎪ ⎨44.092βa for aξ 1, 1 m m = (7.16) ) *3/2 τ ω1 ⎪ ⎪ ⎩13.648βa 2 μ for aξ 1, m for light (heavy) carriers in Si, m∗n = 0.19m(0.98m), m∗p = 0.16m(0.52m); m is the bare electron mass, μ = m∗n m∗p /(m∗n + m∗p ), Eg = 1.14 eV, and h¯ ω1 = 2.72 eV. For these parameters and for nanospheres with radius a in the range 5−50 nm, the lower case of Eq. (7.16) applies (at ω = ω1 ). The parameter β fitted from the experimental data [33, 23] equals to about 0.001.
7.2 Plasmons in a Metallic Nanoparticle Deposited on a Semiconductor
139
In another scenario, when the output of the plasmon energy is recovered by continuous income from sunlight, one can consider an energybalanced regime. In an idealized case, the whole incoming energy of the monochromatic electromagnetic wave of frequency ω is transferred to the semiconductor via plasmons, and we are dealing with the stationary state of a driven and damped plasmon oscillator. Even though a free undamped plasmon has the Mie selfresonance frequency √ ω1 = ωp / 3, where ωp is the bulk frequency, the frequency of plasma oscillations equals the driven electric field frequency, ω, of the incident electromagnetic wave. Because of instantaneous leakage of the plasmon energy in the near field to the semiconductor substrate, this large damping of plasmons causes a redshift and a widening of the resonance, as is the case for every damped and driven oscillator. The widened resonance enables the energy transfer from plasmons to electrons to embrace also frequencies lower or larger than the Mie frequency but it is limited from below by the semiconductor forbidden gap Eg /h. ¯ The incident sunlight frequency dispersion covers the visible spectrum and also some UV and infrared tails. The total efficiency of the plasmon channel corresponds to a sum (integration) over all Fourier components ω > Eg /h¯ of the light including its interference with the intensity distribution in the spectrum of sunlight. To model this behaviour it is necessary to consider separately each single monochromatic electromagnetic mode, i.e., the Fourier component ω. The electric field of such a mode excites plasmons with the same frequency, and this plasmon is damped at a rate 1/τ (Eq. (7.15)). This damping causes a redshift of the resonance and reduces the resonance amplitude, which in turn accommodates itself to balance the energy transfer to the semiconductor from the incident sunlight at frequency ω. Within this damped and driven oscillator model, the amplitude of plasmon oscillations D0 (ω) is constant in time and shaped by 1 . f (ω) = (ω12 − ω2 )2 + 4ω2 /τ 2 = ω 1 − 2(ω1 τ )−2 , The extreme of the redshifted resonance is attained at ω m 1 with corresponding amplitude ∼ τ / 2 ω12 − τ −2 . The redshift is proportional
to 1/(ω1 τ 2 ). In the case of the energy transfer balance described above, one obtains, according to Eq. (7.10), ⎧ 128 2 3 μ m∗n m∗p e6 n2e ω 2 ⎪ ⎪ ⎪ βC a ( hω − E ) f (ω) for aξ 1, π ¯ g ⎨ 0 9 m2 h¯ 4 ε3 (7.17) qm = 3/2 6 2 ⎪ √ ⎪ 128 μ e n ω e ⎪βC 2 ⎩ 2π 2 a 2 2 hω for aξ 1, ¯ − Eg 3 3 f (ω) 0 9 m h¯ ε where f (ω) is the amplitude factor given above for the driven damped oscillator and D0 = (e2 ne E0 4πa 3 /(3m))f (ω) in Eq. (7.10); the amplitude of the electric
140
Efficiency Enhancement by Nanoparticles: Material Dependence
field, E0 , in the incident electromagnetic wave cancels from Eq. (7.17) due to normalization to a single photon as in Eq. (7.13); C0 = Nm 4/3πa 3 /V where V is the volume of the semiconductor and Nm is the number of metallic nanospheres. The ratio qm /q0 revealing the improvement of the plasmonmediated photoeffect over the ordinary photoeffect can be expressed as follows: ⎧ √ 2 3 4 2π a βC0 m∗n m∗p (m∗p )2 e4 n2e ω2 f 2 (ω) ⎪ ⎪ ⎪ for aξ 1, ⎪ 3μ3/2 m2 hω qm ⎨ ¯ − Eg hε ¯ 2 = (7.18) ⎪ 2 2 ∗ 2 4 2 2 2 q0 ⎪ a βC (m ) e n ω f (ω) 8π 0 ⎪ p e ⎪ ⎩ for aξ 1. 2 3μm2 (hω − E ¯ g )ε This ratio turns out to be of the order of 104 β40/H (nm) for a surface density ns ∼ 108 /cm2 of nanoparticles (as in an experiment in [33]); note that C0 = ns 4πa 3 /(3H ), where H is the thickness of the semiconductor layer. On inclusion of the phenomenological factor β and the thickness H (it was confirmed experimentally that the range of the nearfield zone exceeds the Mie wavelength, i.e., it is not shorter than 1 μm), the above ratio is sufficient to explain the scale of the experimentally observed strong enhancement of the absorption rate in semiconductors due to plasmons. This strong enhancement of the transition probability is linked with the admission of momentumnonconserving transitions, which are, however, reduced with the growth of the radius a. The strengthening of the nearfieldinduced interband transitions, in the case of large nanospheres, is, however, still significant as the quenching of oblique interband transitions is partly compensated by the ∼ a 3 growth of the amplitude of dipole plasmon oscillations. The tradeoff between these two competing sizedependent factors is responsible for the experimentally observed enhancement of light absorption and emission in diode systems mediated by surface plasmons in nanoparticle surface coverings [32–34, 117–119]. 7.3 Efficiency of the Light Absorption Channel via Plasmons for Various Materials The metals most often used in plasmon photovoltaics are nanoparticles of Au and Ag (sometimes also of Cu) because their surface plasmon resonances are located within the visible light spectrum. These nanoparticles can be deposited on various semiconductor substrates with different material parameters. We will list here the appropriate parameters for comparison with experiment, for various configurations of plasmon solarcell systems. In order to compare with experiment one can estimate the photocurrent in the case of a semiconductor photodiode with a metallically modified photoactive surface. This photocurrent is given by I = eN(q0 + qm )A, where N is the number of incident photons and q0 and qm are respectively the probabilities of singlephoton absorption in the ordinary photoeffect [59] and of singlephoton absorption mediated by the presence of metallic nanospheres, as
7.3
Efficiency of the Light Absorption Channel for Various Materials
141
Table 7.1 Plasmon energies measured in metals Metal
Bulk plasmon energy (eV)
Surface plasmon energy (eV)
Li Na K Mg Al Fe Cu Ag Au
6.6 5.4 3.8 10.7 15.1 10.3 6 3.8 4.67
3.4 3.3 2.4 6.7 8.8 5.0 3.5 3.5 2.7
Table 7.2 Mie frequency ω1 in Eq. (7.18) Metal
Au
Ag
Cu
Mie frequency
4.11 × 1015 /s
5.2 × 1015 /s
5.7 × 1015 /s
Table 7.3 Substrate material parameters for Eq. (7.18) (m = 9.1 × 10−31 kg, the mass of a bare electron; lh, light holes; hh, heavy holes; L, longitudinal; T, transverse) Semiconductor
m∗n
m∗p
Eg
Si GaAs CIGS
0.9m L[101], 0.19m T[110] 0.067m 0.09m−0.13m
0.16m lh, 0.49m hh 0.08m lh, 0.45m hh 0.72m
1.12 eV 1.35 eV 1−1.7 eV
p
derived in the previous section: A = τfn /tn + τf /tp is the amplification factor, n(p) where τf is the annihilation time for both sign carriers and tn(p) is the drive time for carriers, i.e., the time from traversing the distance between the electrodes. From the above formulae, it follows that (here I = I (qm = 0), i.e., I is the photocurrent without metallic modifications), I qm (7.19) =1+ , I q0 where the ratio qm /q0 is given by Eq. (7.18). In Tables 7.1 and 7.3 we list parameters for metallic nanoparticles and for semiconductor substrates, which allows comparison of the ratio qm /q0 (ω) for various material configurations using Eq. (7.18). Besides the explicit entering of the effective masses m∗n and m∗p and of Eg into Eq. (7.18), these parameters contribute also to the damping rate 1/τ via the function f (ω) (defined below Eq. (7.17)), utilizing Eq. (7.15), and finally again Eq. (7.18).
142
Efficiency Enhancement by Nanoparticles: Material Dependence
(a)
Wavelength (nm)
(c)
Wavelength (nm)
(d)
Wavelength (nm)
Ra
diu
s2
5–
50
(nm
)
(b)
Wavelength (nm)
Figure 7.1 (a) Dependence of the normalized photocurrent (I /I )(λ) on wavelength for radius a increasing from 25 nm (bottom) to 50 nm (top); the step is 2 nm (H = 4 μm, ns = 1.6 × 108 /cm2 ). (b) The same as in (a) with threedimensional visualization of the redshift of the maximum with radius growth. (c) Dependence of the normalized photocurrent (I /I )(λ) on wavelength for increasing layer depth H , from 4 μm (top) to 10 μm (bottom); the step is 0.5 μm (a = 20 nm, ns = 1.6 × 108 1/cm2 ). (d) Comparison with the experimental data, which are given in the inset [33]: A, a = 25 nm (fitting is better for 19 nm), ns = 6.6 × 108 1/cm2 ; B, a = 40 nm, ns = 1.6 × 108 1/cm2 ; C, a = 50 nm, ns = 0.8 × 108 1/cm2 (H = 3 μm).
All the material parameters as well as the geometry and size parameters modify both Eqs. (7.18) and (7.17), which give the eventual relatively complicated dependence of the plasmonmediated photoeffect efficiency (qm /q0 )(ω) with respect to material, size, and deposition type. We illustrate this dependence in the series of Figs. 6.5 and 7.1–7.6.
7.3
Efficiency of the Light Absorption Channel for Various Materials
143
The formula (7.18) is exemplified in Fig. 6.5 for Au nanoparticles deposited on an Si semiconductor (continuous line) which reproduces well the experimental behaviour (dashed line) [33]. Both channels of photon absorption resulting in photocurrent in the semiconductor sample are included, the direct ordinary photoeffect absorption with transition probability given by q0 and the plasmonmediated absorption with probability qm , respectively. Note also that some additional effects such as the reflection of incident photons or destructive interference on the metallic net will contribute and are accounted for phenomenologically in the plasmonmediated channel by an experimentally fitted factor β. The collectiveinterferencetype corrections are rather weak for the considered low densities of metallic coverings, of the order of 108 /cm2 , and nanosphere sizes much lower than the resonance wavelength, though for larger concentrations and larger nanosphere sizes the reflection of photons would play a stronger reducing role [111]. The resonance threshold is accounted for by the damped resonance envelope function in Eq. (7.19), which includes also the semiconductor bandgap limit. As indicated in Fig. 6.5, the relatively high value of qm /q0 ∼ 104 40β/H (nm) enables a significant growth in efficiency of photoenergy transfer mediated by surface plasmons in nanoparticles deposited on an active layer by an increase in β or a reduction in H (at constant ns ). However, since an enhancement of β easily induces the overdamped regime of plasmon oscillations, the more suitable would be the lowering of H , especially convenient in thinfilm solar cells. The overall behaviour of (I /I )(ω) = 1 + qm /q0 calculated according to the relation (7.19), and depicted in Fig. 6.5, agrees quite well with the experimental observations [33] in the position, height, and shape of the photocurrent curves for distinct samples (the strongest enhancement is achieved for a = 40 nm, for Au nanoparticles and an Si substrate). This corresponds to the rather surprising dependence, nonmonotonic and with a local maximum, of the efficiency measure, (qm /q0 )(ω), with respect to metallic nanoparticle size a as expressed by Eq. (7.18). Such a size dependence has been confirmed experimentally [33]. In Fig. 7.2 we present the spectral dependence of the plasmonic efficiency enhancement qm /q0 for different substrates (Si, CIGS, GaAs) for Au nanoparticles with radius a = 50 nm and nanoparticle concentration ns = 108 /cm2 . Note that for the CIGS substrate (copper indium gallium diselenide) the spectral characteristic is narrower and blueshifted in comparison to those for Si and GaAs. Figure 7.3 reveals the increase in efficiency of the plasmon effect with growth of the forbidden gap Eg with other parameters unchanged. An especially significant material parameter is the hole mass, see Fig. 7.4; this can be seen from Eq. (7.18). The hole mass m∗p enters the denominator in Eq. (7.12) for the ordinary photoeffect and also the numerator in Eq. (7.18). The higher is the mass m∗p the lower is the efficiency q0 of the ordinary photoeffect, and, in turn, the higher is the ratio qm /q0 .
144
Efficiency Enhancement by Nanoparticles: Material Dependence qm/q0
Au, a = 50 nm, ns = 108/cm2
20
GaAs Si CIGS
15
10
5 0.7
0.8
0.9
1.0
1.1
1.2
ω/ω1 (ω1 = 4.11×1015
Figure 7.2 For comparison, the effectiveness of the plasmon channel expressed by qm /q0 (see Eq. (7.18)) for Si, GaAs, and CIGS substrates, for Au nanoparticles with radius 50 nm and surface density 108 /cm2 .
qm/q0
Au, a = 50 nm, ns = 108/cm2 40 35 30
Eg = 1.5 [eV] Eg = 1.35 [eV] Eg = 1.14 [eV]
mp* = 0.16 m mn* = 0.25 m
25 20 15 10 0.7
0.8
0.9
1.0
1.1
1.2
ω/ω1 (ω1 = 4.11x1015 [1/s])
Figure 7.3 For comparison, the effectiveness of the plasmon channel expressed by qm /q0 (see Eq. (7.18)) for varying Eg but with the same effective masses of electrons and holes of the substrate semiconductors, covered with the same Au nanoparticles with radius 50 nm and surface density 108 /cm2 .
In Fig. 7.5 a comparison for Au, Ag, and Cu nanoparticles is presented for two sizes (a = 50,25 nm). The blueshift of the spectral characteristics for Ag and Cu in comparison to Au is noticeable (see also Fig. 7.6) and is even clearer for lowerradius nanoparticles, owing to the narrowing of the spectral curves (see Fig. 7.6, lower panels). From a comparison in Fig. 7.6 of the upper and lower panels, for the Si and CIGS substrates with Au, Ag, Cu nanoparticles of size a = 50,25 nm (at nanoparticle concentration ns = 108 /cm2 ) it can be seen that the Au nanoparticles utilize the visible spectrum in a better manner than the Ag or Cu nanoparticles. The advantage presented by Au nanoparticles is greater in the case of an Si substrate but is reduced for a CIGS substrate because of blueshift of Eg
7.3
Efficiency of the Light Absorption Channel for Various Materials 8
145
2
qm/q0
Au, a = 50 nm, ns = 10 /cm 100
Eg = 1.14 eV mn* = 0.25 m
80
60
mp = 0.7m mp = 0.35m mp = 0.16m
40
20
0.7
0.8
0.9
1.0
1.1
1.2
ω/ω1 (ω1 = 4.11×1015/s)
Figure 7.4 For comparison, the effectiveness of the plasmon channel expressed by qm /q0 (see Eq. (7.18)) for varying hole mass m∗p but the same electron mass m∗n and the same value of Eg , for a substrate semiconductor covered with the same Au nanoparticles with radius 50 nm and surface density 108 /cm2 .
25
20
Si photodiode, a = 25 nm, n = 108/cm2 qm/q0
qm/q0
Si photodiode, a = 50 nm, n = 108/cm2
Cu Ag Au
20
Cu Ag Au
15
15
10
5
10 0.8
0.9
1.0
1.1
1.2
ω/ω1 (ω1 = 4.11×1015/s)
0.8
0.9
1.0
1.1
1.2
ω/ω1 (ω1 = 4.11×1015/s)
Figure 7.5 For comparison, the effectiveness of the plasmon channel expressed by qm /q0 (see Eq. (7.18)) for the same substrate semiconductor, Si, with Au, Ag, and Cu nanoparticles of the same radius, 50 nm (left) and 25 nm (right), and the same surface density, 108 /cm2 .
in CIGS with respect to Si. In the case of CIGS (especially for large nanoparticles, a = 50 nm), the advantage of Au over Ag in the overall utilization of the sunlight spectrum disappears, whereas it is pronounced in the case of an Si substrate. This is so because of the cutoff of the nearinfrared part of sunlight in spectral absorption of CIGS, in contrast with Si, and which favours Ag more than Au nanoparticles; see Fig. 7.6. Below we describe an experimental confirmation of this behaviour of Si and CIGS substrates, under laboratory sunlighttype illumination, by Yamashita DensoYSS50 Aunder AM1.5 [31]. For nanoparticles of Au and Ag of size a = 50 nm, optimized using Eq. (7.18), deposited on multicrystalline Si (mcSi) and on copper indium gallium diselenide (CIGS) solar cells, the measured [31] overall increase in cell efficiency is as much
Efficiency Enhancement by Nanoparticles: Material Dependence visible infrared qm/q0
Si photodiode a = 50 nm, n = 108/cm2
UV
Au Ag Cu
Eg solar light sprectrum
15
ω/ω1 (ω1 = 4.11×10 /s) visible infrared
Si photodiode a = 25 nm, n = 108/cm2
UV
qm/q0
Au Ag Cu
Eg solar light sprectrum
15
ω/ω1 (ω1 = 4.11×10 /s) visible infrared
UV
qm/q0
CIGS photodiode a = 50 nm, n = 108/cm2
Au Ag Cu
Eg solar light sprectrum
15
ω/ω1 (ω1 = 4.11×10 /s) visible infrared
CIGS photodiode a = 25 nm, n = 108/cm2
qm/q0
146
UV Au Ag Cu
Eg solar light sprectrum
15
ω/ω1 (ω1 = 4.11×10 /s)
Figure 7.6 For comparison, the effectiveness of the plasmon channel expressed by (qm /q0 )(ω) (see Eq. (7.18)) for the same substrate semiconductor Si (upper) and CIGS (lower) with Au, Ag, and Cu nanoparticles of the same radius, 50 nm (left) and 25 nm (right), and the same surface density, 108 /cm2 . Plots are made versus the sunlight spectrum as background. The figures illustrate the accommodation of the spectral characteristics of the plasmonmediated photoeffect, (qm /q0 )(ω), to the sunlight spectrum for different materials and covering parameters. The white arrows indicate the positions of the forbidden gap for Si and CIGS, respectively, on the background of the solar light spectrum. These positions accommodate themselves to the frequency ratio ω/ω1 on the horizontal axis. The vertical axis shows the efficiency growth on the same scale for Au, Ag, and Cu and is not related to the vertical height of the solar spectrum. By comparison of the top panel with Fig. 7.5 (left) the influence of the depositiontype parameter β, taken here five times larger than in Fig. 7.5, can be seen.
Efficiency of the Light Absorption Channel for Various Materials
147
Current density (mA/cm2)
Current density (mA/cm2)
7.3
Current density J (mA/cm2)
Current density J (mA/cm2)
Figure 7.7 For comparison, the solarcell efficiency due to plasmon modification for a multicrystal Si solar cell, expressed as an increase in the area beneath the grey curve with respect to the area below the black curve. The photoactive surface is modified by (left) Au nanoparticles and (right) Ag nanoparticles [31].
Figure 7.8 For comparison, the solarcell efficiency due to plasmon modification for the CIGS cell expressed as an increase in the area beneath the grey curve with respect to the area below the black curve. The photoactive surface is modified by (left) Au nanoparticles and (right) Ag nanoparticles [31].
as 5%. The application of suitable concentrations of Au and Ag nanoparticles onto mcSi solar cells increases their efficiency by 5.6% and 4.8%, respectively [31]. The application of Au and Ag nanoparticles onto the surface of CIGS solar cells improves their efficiency by 1.2% and 1.4%, respectively [31]. This can be seen in Figs. 7.7 and 7.8 giving the increase in solarcell overall efficiency (the ratio of the area beneath the I–V curve for a metallically improved solar cell and for a clean solar cell; the same size (radius 50 nm) and the same concentration from the 5% colloidal solution sputtering over the surface has been applied to different samples). For more details see [31]. Worth noting is the agreement of the experimentally observed difference in the efficiency increase due to the plasmon effect in both cases, that of mcSi cells and that of CIGS cells, if one compares the results of applying Au and Ag
148
Efficiency Enhancement by Nanoparticles: Material Dependence
Figure 7.9 Visualization by electron microscopy (EM) photography of the distribution of metallic nanoparticles of Au on the surface of the multicrystalline Si solar cell under study for the plasmonic effect, as shown in Fig. 7.7; the very low surface concentration of metallic components is visible.
particles (at the same nanoparticle size and the same surface concentration). This behaviour agrees with theoretical studies of the dependence on material of the plasmon effect, as shown above. From Figs. 7.2–7.5 we see that, for an Si substrate, Au nanoparticles with radii 50 nm utilize the solar light spectrum better than Ag or Cu particles (see Fig. 7.5), and indeed in the experiment for Au nanoparticles (see Fig. 7.7) the efficiency growth is about 10% larger than for Ag nanoparticles of the same size and concentration on the substrate mcSi solar cell. Interestingly, for the substrate CIGS cell the effect is weaker and inverted; see Fig. 7.8. This is also noticeable from the theoretical modelling, owing to the different Eg and effective masses of carriers for CIGS with respect to those for mcSi. The maxima of the efficiency enhancement curves for Au and Ag mutually shift in such a way that, for CIGS, Ag nanoparticles are somewhat better suited to the solar light spectrum than Au nanoparticles. However, to analyse these effects in more detail, measurements of the spectral characteristics of all the structures considered, with varying but monochromatic illumination should be performed. Summarizing this section, it has been demonstrated using the Fermi golden rule that the efficiency of energy transfer between surface plasmon oscillations in a metallic nanoparticle and the substrate semiconductor depends on the parameters describing the nanoparticles (their radius and material) and on the semiconductor parameters (the energy gap and the effective masses of electrons and holes). The formula which generalizes the ordinary photoeffect to the plasmonmediated photoeffect agrees well with experimental measurements on a laboratory photodiode configuration. The measured ratio of the photocurrents in setups with and
7.3
Efficiency of the Light Absorption Channel for Various Materials
149
without metallic nanocomponents was compared with the theoretically predicted scenario. Quantitative consistency is achieved both for the shape of the spectral characteristics and for the particlesize dependence (as illustrated for an Si diode with deposited Au nanoparticles having radii 25, 40, and 50 nm). Qualitative agreement has been demonstrated also for complete solar cells, where the plasmon effect is obscured by other elements of the extensive series of effects, in addition to the efficiency of the absorption of photons only, resulting in the overall solarcell efficiency. Experimental data have been compared for a multicrystalline Si solar cell and a CIGS (copper indium gallium diselenide) solar cell covered, or not covered, with Au or Ag nanoparticles with radii of the order of 50 nm. The increase in the overall photovoltaic efficiency for metallically modified cells varies between 1.5% (CIGS) and 6%(Si), depending on the nanoparticle concentration (for concentrations that are too dense the efficiency drops, owing to destructive interference and reflection). There is a better increase in efficiency (by about 10%) for Au nanoparticles in comparison to Ag nanoparticles, for an Si cell, whereas for a CIGS cell the difference between the effects of Ag nanoparticles and Au nanoparticles is inverted and strongly reduced. This also agrees qualitatively with the theoretical predictions, taking into account the differences in Mie frequency in Au and Ag and also the different semiconductor parameters for Si and CIGS. As has been shown, the mediation of plasmons in metallic nanoparticles on top of the photodiode can enhance the efficiency of the photoeffect, even by a factor 2 (i.e., 100% increase), which has been confirmed experimentally for an Si photodiode covered with Au nanoparticles with radius 40 nm and surface concentration ∼ 108 /cm2 . Such a large increase is, however, reduced in commercial Si solar cells to about a 5% overall efficiency increase (and to about 2% in CIGS cells). Such an increase is not large but still of interest as in the competitive energy market the green renewable energy of solar cells is at present too costly, and any cost reduction, including via an increase in efficiency, is strongly desirable. The application of metallic lowdensity and lowcost nanocoverings with Au particles might allow an increase of 5% of the typical efficiency of a commercial Si cell [31], which captures about 14%–17% of the energy of illumination [136]. For thinfilm cells and flexible plastic cells the efficiency is much lower. Thus, increasing it by even a few per cent by easily applied metallic coverings would seem to be significant. There are, however, problems, e.g., with the durability of such coverings deposited by sputtering onto the surface of a cell. In this regard a very interesting idea is to embed metallic nanoparticles in a thin film of a solar cell of perovskite type, which might be threedimensionally printed together with nanoparticles inside, taking advantage of the lowtemperature and chemicaltype manufacturing of such cells (perovskite cells are especially in prospect now, because their efficiency is still growing and exceeds even 23%).
8 Numerical Simulation of Plasmon Photoeffect
We demonstrate in this chapter that the direct application of numerical packages such as COMSOL to the plasmonic effect in solar cells metallically modified at the nanoscale may be significantly inaccurate if quantum corrections are neglected. The nearfield coupling of surface plasmons in metallic nanoparticles deposited on the top of a solar cell with the band electrons in the semiconductor substrate strongly enhances the damping of the plasmons in the metallic components. This effect is not accounted for in standard numerical packages using a Drudetype dielectric function for the metal (taken from measurements in bulk or for thin layers) as the prerequisite for the numerical electromagnetic field calculus. Inclusion of the proper corrections for plasmon damping causes enhancement of the plasmoninduced photoeffect efficiency of a metallized photodiode by several dozen per cent, at least, in comparison to the effect induced by the electric field concentration near the metallic nanoparticles. This is consistent with the experimental observations, which cannot be explained only by local the increases in the electrical field near the curvature of metallic nanoparticles, as determined by the finite element solution of the Maxwell–Fresnel boundary problem given by a numerical system like COMSOL. The proper damping rate for plasmons can be identified by application of the Fermi golden rule to the plasmon coupling with the band electrons. We demonstrate this effect by comparison of the COMSOL simulation of the plasmonic photoeffect with and without quantum corrections verified by the related experimental data.
The strengthening of sunlight energy harvesting in solar cells mediated by surface plasmons in metal nanoparticles deposited on a photoactive solarcell surface is caused by three effects: (1) the strong concentration of the electric field of the incident electromagnetic wave close to regions of the metallic components with a large local curvature, as is the case for small nanoparticles, (2) the large amplitude of plasmon oscillations in metallic nanoparticles (particularly in larger nanoparticles, with a larger number of electrons), and (3) the enhancement of the probability of interband transitions in a semiconductor substrate caused by the breaking of translational symmetry for a nanoparticle coupled, in the nearfield regime of the surface plasmons, with the substrate semiconductorband electrons
150
Numerical Simulation of Plasmon Photoeffect
151
[32, 2, 110–112, 23]. The transition probability for electrons excited from the valence band to the conduction band in a semiconductor, essential for the efficiency of the photovoltaic effect, grows owing to the electric field amplitude enhancement and to the admission of oblique transitions not prohibited here by momentum conservation [23]. For the ordinary photoeffect [59], when photons directly induce interband transitions in a semiconductor, these interband transitions are confined to only vertical jumps between states with almost the same momentum, owing to the momentum conservation rule and the very small momentum of sunlight photons (due to the large velocity of light, c = 3 × 108 m/s), which hardly changes the electron momentum during scattering. For an excitation energy hω ¯ beyond the forbidden gap Eg of the substrate semiconductor, the photon dispersion hω ¯ = cq gives q p, where p ∼ π h¯ / l is the semiconductorband quasimomentum scale in the Brillouin zone (l denotes the semiconductor’s elementary cell linear size). Thus, the change in the band electron momentum q = p2 − p1 is negligible on the scale of the Brillouin zone and so p1 p2 (because of the large value of c); thus only the vertical, momentumconserving, interband transitions contribute to the ordinary photoeffect when the transition is caused by free photons with momentum h¯ ¯ ). q and energy hω ¯ = cq (described by a plane wave ∼ ei(q·r−hωt)/ The interaction of band electrons with surface plasmons from the metallic nanoparticles deposited on the semiconductor surface opens another channel for energy transfer of the solar light to the semiconductor substrate. Plasmons in metallical nanoparticles of several dozen nanometres size are strongly damped by Lorentz friction; thus, they also heavily absorb electromagnetic radiation near the plasmonic resonance. Hence, even sparse metallic coverings with such particles (Au, Ag, or Cu nanoparticles of 10−50 nm radius are to be preferred, because of the location of their surface plasmon resonances in the visible spectrum of light) can capture a large fraction of the incident solar light and quickly transfer this energy to the substrate semiconductor owing to the strong nearfieldzone coupling of plasmons with band electrons in the semiconductor. In the nearfield regime [55, 76] the potential of a plasmon dipole in a nanosphere is proportional to 1/R 2 (where R is the distance from the sphere’s centre), which in the Fourier picture overlaps with all quasimomenta in the substrate semiconductor’s Brillouin zone. This is unlike the direct interaction of incident photons with the semiconductor, which contributes only via a single planewave Fourier component [59]. The plasmonmediated channel of energy transfer dominates the absorption of light and changes the efficiency of the photoeffect. This channel is, however, not accounted for in the conventional solution of the Maxwell–Fresnel problem by, e.g., the numerical COMSOL system, which utilizes predefined dielectric functions of the metal and semiconductor; they are modelled
152
Numerical Simulation of Plasmon Photoeffect incident light
Au dipole of surface plasmon
a 15 nm [27, 26]. The energy transfer is strongest via the nearfield coupling of plasmons to band electrons in the semiconductor substrate; this causes a strong damping of plasmons, which is what lies behind the experimentally observed giant plasmon enhancement of the photoeffect [137, 118, 2, 110–112, 23, 32–36] but is not accounted for in a conventional COMSOL simulation. Note that this strong damping of plasmons (due to radiation) gives rise to a related strong absorption rate of the metallic components, which act as effective collectors of the incident sunlight even if their surface density in the solarcell covering is low. The surface plasmon oscillations have undefined momentum, as localized oscillations. The band electrons are assigned, however, with quasimomenta in the crystal, an initial one, p1 , and a final one, p2 . These can be arbitrarily chosen because momentum conservation is ruled out by the matrix element of the local dipole
154
Numerical Simulation of Plasmon Photoeffect
interaction for the plasmoninduced transition of electrons, in contrast with the direct coupling with planewave photons in the ordinary photoeffect (the condition p1 = p2 strongly limits the photoeffect efficiency). In the present chapter we briefly summarize the theoretical scheme of the plasmonaided photoeffect and compare the analytical model with numerical simulations using COMSOL. In what follows we provide a description of the Lorentz friction and the plasmon damping caused by these radiation losses, in order to emphasize the large absorption ability of metallic nanoparticles of appropriately selected size. Then we describe the energy transfer from plasmons to band electrons in metallically improved solar cells, which is crucial for the efficiency enhancement due to the plasmon photoeffect. Next, we provide an analysis of the numerical modelling of the plasmon photoeffect and draw a conclusion about how to correct the COMSOL software, widely utilized in plasmon photovoltaic system simulation, via inclusion of an appropriately lifted dielectric function for the metallic nanoparticles. The latter corrections make the COMSOL simulation more realistic (they change the result for the plasmoninduced efficiency of the photoeffect by at least one order of magnitude), so improving the ability of COMSOL simulations to be compared with experiment [31–33, 111, 137–144]. Typical metals suitable for the plasmonic photoeffect are Au, Ag, and also Cu, whose surface plasmon resonances in nanoparticles overlap with the visible light spectrum. The typical size of the nanoparticles varies between 10 nm and 100 nm in diameter and the surface density of the metallic coverages is usually 108−10 /cm2 . It is remarkable that such sparse coverings with very small particles on the surface of a photocell can significantly enhance its photoefficiency (e.g., by a factor 2 in the photodiode setup reported in [33]). This phenomenon corresponds to the exceptionally high radiative abilities of metallic nanoparticles of such sizes. Neglect of it is the source of the failure of conventional COMSOL simulations. Note also that strengthening the nanoparticle surface concentration does not lead to further growth in the efficiency; conversely, too dense a coverage appears to be counterproductive because reflection and destructive interference reduces the plasmon photovoltaic effect. The possibility of improving the efficiency of solar cells via some inexpensive and technologically feasible methods is now of considerable significance because the efficiency of commercial solar cells is still not high enough. To increase the efficiency, various strategies have been considered, including, quantum dot admixtures in multilayer cells to better adjust the absorption spectrum to the dispersion of the solar light on the earth’s surface or a metallic nanoscale improvement of the light absorption efficiency. We will demonstrate that the latter effect has a
8.1 Lorentz Friction Channel for Energy Losses
155
quantum character and, in order for the theoretical modelling to agree with the experimental observations, one must abandon the conventional classical methods of plasmonics using the finite element method (as, e.g., in COMSOL); the discrepancy of the classical simulation with the exact quantum approach, and also with the experimental data, reaches several dozen per cent. So, a large error is caused by the neglect, in the classical methods, of the very effective quantum channel for energy transfer between the plasmons in metallic nanoparticles and the band electrons in the semiconductor substrate. This channel can be accounted for in terms of the Fermi golden rule as follows. The golden rule is applied to the interband transition of electrons in the semiconductor substrate. These transitions are induced by the coupling of these electrons to plasmons excited by incident solarlight photons in the metallic nanoparticles. This channel for energy transfer appears to overwhelm the solarlight absorption in solar cells thus metallically modified. 8.1 Lorentz Friction Channel for Energy Losses of Surface Plasmons in a Metallic Nanoparticle Plasmon oscillations in metallic nanoparticles have been widely analysed using various methods: the numerical Kohn–Shamtype approach [19, 20] but restricted to ultrasmall nanoparticles only (because of numerical constraints); the random phase approximation approach (RPA) [14, 16, 21, 23]; and classical solution of the Fresnel–Maxwell equations [17]. The latter approach is usable for arbitrarysized particles but is limited by its neglect of quantum effects important at the nanoscale for metallic particles. The Mie approach [17], like the numerical solution of the Fresnel–Maxwell boundary problem by the finite element method utilized by, e.g, the COMSOL system, suffers from the need to use a phenomenologically predefined dielectric function for the metallic components as a prerequisite for the calculation algorithm. This dielectric function (in Drude form [17]) should comprise all quantum effects related to plasmons, but this is not so because the assumed frequency and damping of plasmons are taken from bulk metal values (at best from measurements on thin films), not from metallic nanoparticle measurement. It has been demonstrated that the size effect for metallic nanoparticles is predominant for the range of nanoparticle radius a ∈ (15,100) nm (for Au in vacuum) [27, 26], resulting in a different Mie response and COMSOL estimations, in comparison with models with the bulk dielectric function taken as the prerequisite for the calculus. The reason for this discrepancy is the strongly growing radiation losses of plasmons (i.e., the Lorentz friction losses) in the case of nanoparticles with
156
Numerical Simulation of Plasmon Photoeffect
1.00
0.20
Loretz friction and electron scattering
0.15
0.95
0.10
a
0.90
0.05 0.85 20
30
40
50
60
70
electron scattering
0.00 20
30
a (nm)
50
60
70
a (nm)
1.0
harmonic perturbative appr.
0.30
0.8 exact
0.6
0.20
exact Lorentz friction and electron scattering
0.4 0.10
0.2 0.0
40
harmonic perturbative appr.
0
50
100 150 200 250 300 a (nm)
electron scattering
0.00
0
50
100 150 200 250 300 a (nm)
Figure 8.2 Size dependence of the resonance surface plasmon oscillations (dipole mode) including the Lorentz friction in a metallic (Au) nanoparticle in vacuum, for radius a ∈ (20,70) nm (upper) and a ∈ (5,300) nm (lower). The anharmonic oscillation regime caused by the thirdorder time derivative for the Lorentz friction force [55, 76] (black line) is apparently (see Eq. (8.1)) quite different from the harmonic approximation for the Lorentz friction (grey line) [27, 26]. The overdamped regime does not occur for the exact inharmonic oscillations (black curve), whereas the approximate harmonic oscillations (grey curve) stop when the damping rate 1/τ reaches 1 (the resonance frequency ω and the damping rate 1/τ are expressed in dimensionless units, i.e., they are divided by ω1 ). The additional curve at lower right shows the electron scattering damping, which is much less than the Lorentz friction losses for a > 20 nm and diminishes with growth in a.
a ∈ (15,100) nm (for Au in vacuum but similarly also for Ag and Cu and other dielectric surroundings); these losses are not present either in smaller nanoparticles or in the bulk metal (as is noticeable in Fig. 8.2). This figure presents the resonance frequency and related damping obtained by solution of the RPA dynamic equation for surface plasmons in metallic nanoparticles [23, 27, 26] with inclusion of the Lorentz friction force, which is proportional to the thirdorder time derivative of the plasmon dipole [55, 76]. The related anharmonic behaviour of the plasmon oscillations caused by this thirdorder time derivative is a remarkable effect. The plasmon frequency and
8.1 Lorentz Friction Channel for Energy Losses
157
damping are no longer linked by the ordinary relation, ω = ω1 1 − (1/τ0 ω1 )2 , which conventionally results in an overdamped regime of quenched oscillations when 1/τ0 ω1 > 1. The exact solution including the Lorentz friction is always of an oscillatory type, with complex frequency (without any quenching of the oscillations) as follows: ω+i
1 τ
i =− + 3l
+
√ i(1 + i 3)(1 + 6lq) ) *1/3 3 × 22/3 l 2 + 27l 2 + 18lq + 4(−1 − 6lq)3 + (2 + 27l 2 + 18lq)2
*1/3 √ ) i(1 − i 3) 2 + 27l 2 + 18lq + 4(−1 − 6lq)3 + (2 + 27l 2 + 18lq)2 6 × 21/3 l
, (8.1)
where q = 1/(τ0 ω1 ) and l = (2/3) (aω1 /c)3 . The functions ω and 1/τ (in dimensionless units, i.e., divided by ω1 , the bare frequency, not shifted by damping) are plotted in Fig. 8.2 versus the nanosphere radius a. A strong deviation from harmonic behaviour is apparent for a > 40 nm. The absence of an overdamped regime is very clear. The electron scattering losses vF CvF 1 = + τ0 2lB 2a (where vF is the Fermi velocity in the metal, lB is the mean free path in the metal, and C 1 is a factor depending on the reflection type of the electron scattering at the nanoparticle boundary) [24, 23] are displayed in Fig. 8.2, and it is noticeable that this loss channel is negligible for a > 25 nm (for Au in vacuum) in comparison with the Lorentz friction losses. It must be emphasized that in the conventional Mie and COMSOL approaches [17] only 1/τ0 is accounted for, and this is a source of the abovementioned discrepancies with the experimental observations. It is clear that such strong plasmon damping as that via the Lorentz friction channel must be included for a realistic description of plasmon phenomena at the scale of metallic nanoparticles a ∈ (15,100) nm. If such nanoparticles are deposited on a semiconductor surface to mediate the photoeffect, the situation changes again in a significant manner. The coupling of plasmons with the substrate band electrons opens an especially efficient channel for energy transfer, and this channel dominates the plasmon damping – it is stronger than the Lorentz friction damping. To describe this channel the quantum approach must be applied in the framework of the Fermi golden rule.
158
Numerical Simulation of Plasmon Photoeffect
8.2 Fermi Golden Rule for Probability of Electron Interband Excitation due to Plasmons in a Metallic Nanoparticle Let us consider now a metallic nanoparticle (of Au, Ag, or Cu) of spherical shape with radius a ∈ (5,70) nm deposited on a semiconductor substrate with an embedded p–n junction for the photodiode setup schematically presented in Fig. 8.1. We assume that in the metallic nanoparticle incident sunlight excites a surface plasmon of dipole type. Such a plasmon is excited by incident photons with frequency close to the dipole surface plasmon resonance, which in Au, Ag, or Cu nanoparticles with radii of several tens of nanometres falls at a wavelength ∼ 500 nm, i.e., it is much greater than the nanoparticle dimension. Thus, the electrical component of the electromagnetic wave is almost homogeneous along the whole nanoparticle and the dipole regime is fulfilled, i.e., only the surface plasmon dipole mode can be excited by this electromagnetic wave. Repeating the derivation presented in Section 7.1, 7.2, and 7.3 of the previous chapter one can estimate the probability of the plasmoninduced transitions of band electrons between the valence and conduction bands in the semiconductor substrate via application of the Fermi golden rule [75]. As we have already explained in previous chapters, in the case of metallic nanoparticles deposited on a photoactive semiconductor layer, plasmons induce in the substrate oblique interband transitions of the band electrons, not only vertical transitions as in the ordinary photoeffect. This results in the enhancement of the transition probability for the nearfield coupling of plasmons with band electrons in comparison with the photon (planewave) absorption rate in a semiconductor in the conventional photoeffect. This enhancement of the transition probability due to the admission of nonmomentumconserving interband hopping is, however, gradually quenched with growth in the radius a, which leads to a specific tradeoff for the efficiency increase because larger nanoparticles are preferred owing to their stronger dipole amplitude, proportional to a 3 . From the algebra detailed in Sections 7.1–7.3 we obtained an analytical formula for the efficiency ratio of the plasmonmediated photoeffect transition probability per single incident photon and the ordinary photoeffect transition probability per single incident photon including the abovementioned tradeoff: ⎧ √ 2 3 4 2π a βC0 m∗n m∗p (m∗p )2 e4 n2e ω2 f 2 (ω) ⎪ ⎪ ⎪ for aξ 1, ⎪ 3μ3/2 m2 hω qm ⎨ ¯ − Eg hε ¯ 2 (8.2) = ⎪ q0 ⎪ 8π 2 a 2 βC0 (m∗p )2 e4 n2e ω2 f 2 (ω) ⎪ ⎪ for aξ 1, ⎩ 3μm2 (hω ¯ − Eg )ε2 where qm is the probability of interband transitions in the substrate semiconductor induced by the dipole surface plasmon in the nanoparticle (per single incident photon exciting the plasmon),
8.2 Fermi Golden Rule for Probability of Electron Interband Excitation
∗ ∗ ⎧ μ mn mp 128 e6 n2e ω 2 ⎪ 2 3 ⎪ ⎪ ( hω − E ) f (ω) ¯ g ⎨βC0 9 π a m2 h¯ 4 ε3 qm = ⎪ ⎪ 128 √ 2 2 μ3/2 e6 n2e ω 2 ⎪ ⎩βC0 hω − E 2π a f (ω) ¯ g 9 m2 h¯ 3 ε3
159
for aξ 1, (8.3) for aξ 1,
where f (ω) =
1 (ω12 − ω2 )2 + 4ω2 /τ 2
is the amplitude factor for the driven and damped oscillator and D0 = (e2 ne E0 4πa 3 /(3m))f (ω) in Eq. (7.10); the amplitude of the electric field, E0 , in the incident electromagnetic wave is obtained from Eq. (7.17) by the normalization per single photon as in Eq. (7.13); C0 = Nm 4/3πa 3 /V where V is the volume of the semiconductor and Nm is the number of metallic nanospheres. The denominator q0 is the probability of an interband transition induced by a single incident photon in the ordinary photoeffect, √ 4(4) 2 μ5/2 e2 (hω − Eg )3/2 . (8.4) q0 = 3 ¯ 3 m∗2 ωε h ¯ p The plasmon damping rate is estimated as ⎧ √ 2 3 4βωμ m∗n m∗p (hω−E ¯ g )e a ⎪ ⎨ 4 1 3h¯ ε = √ √ 3/2 2 2 2 hω−E 4βωμ ¯ τ ⎪ ge a ⎩
for aξ 1,
(8.5)
for aξ 1.
3h¯ 3 ε
By τ we denoted here the short time scale for the large damping rate, 1/τ , of plasmons due to the energy transfer to the semiconductor substrate, which greatly exceeds the internal (within metal) damping characterized by 1/τ0 , the latter being due to the scattering of electrons inside the metallic nanoparticle [23] (1/τ0 1/τ ). The radiation from the farfield zone towards the upper hemisphere (i.e., the Lorentz friction for the plasmon) is also smaller than the nearfieldzone energy transfer to the substrate [23]. Let us repeat here our comment on the two limiting cases, aξ 1 and aξ 1, given in the above formulae, with ξ = 2(h¯ ω − Eg )(m∗n + m∗p )/h¯ . Notice that 1 a ξ
0
> 2 × 10−9 m
for
< 2 × 10−9 m
for
hω−E ¯ g Eg hω−E ¯ g Eg
< 0.02, > 0.02,
and this range depends weakly on the effective masses and Eg . Thus for nanoparticles with radii a > 2 nm the first regime holds only close to Eg (for less than 2%
160
Numerical Simulation of Plasmon Photoeffect
of the distance to the limiting Eg ), whereas the second regime holds for the rest of the ω domain. For comparison, ⎧ hω ¯ − Eg ⎪ ⎪ > 0.5 × 10−9 m for < 0.5, ⎨ 1 Eg a hω ¯ − Eg ⎪ ξ ⎪ for > 0.5. ⎩ < 0.5 × 10−9 m Eg The first region widens considerably, to about 50% of the relative distance to Eg , but holds only for ultrasmall size of nanoparticles (a < 0.5 nm. For larger nanospheres, e.g., for a > 10 nm, the second regime is dominates. The ratio qm /q0 turns out to be of order of 104 × 40β/H (nm) for a surface density of nanoparticles (as in the experiment reported in [33]) ns ∼ 108 /cm2 ; note that C0 = ns 4πa 3 /(3H ) in Eq. (8.2) and H is the thickness of the semiconductor layer. Including the phenomenological factor β and the thickness H (it has been confirmed experimentally that the range of the nearfield zone exceeds the Mie wavelength, i.e., it is not shorter than 1 μm), formulae (8.2) and (8.5) are sufficient to explain the scale of the experimentally observed strong enhancement of the absorption rate in semiconductors due to plasmons. This strong enhancement is linked with the admission of momentumnonconserving transitions but is, however, reduced with growth in the radius a. The strengthening of the nearfieldinduced interband transitions in the case of large nanospheres is, however, still significant as the quenching of the oblique interband transitions is partly compensated by the ∼ a 3 growth in the amplitude of the dipole plasmon oscillations. The optimized tradeoff between these two competing sizedependent factors is responsible for the experimentally observed enhancement of light absorption and emission in diode systems mediated by surface plasmons in nanoparticle surface coverings [32–34, 118, 119]. The photocurrent in the photodiode can be expressed as I = eN(q0 + qm )A, where N is the number of incident photons and q0 and qm are the probabilities of singlephoton absorption in the ordinary photoeffect [59] and of singlephoton absorption mediated by the presence of metallic nanospheres, respectively, as p n(p) are derived above; A = τfn /tn + τf /tp is the amplification factor, where τf the annihilation times for the carriers, and tn(p) are the drive times for the carriers (the times for traversing the distance between the electrodes). From the above definitions, it follows that the efficiency measure for the plasmon photovoltaic effect attains the form (here I = I (qm = 0), i.e., I is the photocurrent without metallic modifications) I qm =1+ , I q0 where the ratio qm /q0 is given by Eq. (8.2).
(8.6)
8.2 Fermi Golden Rule for Probability of Electron Interband Excitation a 25 nm a 40 nm a 50 nm
1.30 1.25
3.0 2.5
1.15
2.0
1+qm/q0
1+qm/q0
a 25 nm a 40 nm a 50 nm
3.5
1.20
161
1.10 1.05 0.6
0.7
0.8
0.9
1.0
1.1
1.5
1.2
0.6
0.7
0.8
0.9
1.0
1.1
1.2
1
1
50
50
2.50
45
45 1.20
1.20
50
1.15
2.25
1.10 1.05 40
40
0.6
1.15
0.8
2.00
40
30
1.75
1.0
1.10 1.05
30
35
a (nm)
a (nm)
1.2
35
0.7
0.8
50
2.0
1.25
1.5 40
1.0 0.6
30
1+qm/q0 25 0.6
1.50
2.5
0.8
1+qm/q0 0.9
1.0
1.1
1.2 1
25 0.6
0.7
0.8
30 1.0 1.2
0.9
1.0
1.1
1.2 1
Figure 8.3 Size dependence of the photoeffect efficiency enhancement due to plasmon mediation in light absorption, (left) for constant total mass of all metallic nanoparticles deposited on the Si substrate and (right) for constant surface concentration of particles (surface layer with thickness H = 3 μm, proximity factor β = 0.0005, density of Au nanoparticles (left) ns = 50 × 108 (25/a)3 /cm2 and (right) 50 × 108 /cm2 with radius a ∈ (25,50) nm). The redshift with growth in nanoparticle size is noticeable. The efficiency increase I /I0 = 1 + qm /q0 (see Eqs. (8.6) and (8.2)) depends on the nanoparticle size and material, on the semiconductor parameters, and on ns (ω is the frequency of the incident light in dimensionless units, i.e., divided by ω1 ).
The material parameters as well as the geometry and size parameters modify both Eqs. (8.2) and (8.3), which gives an eventual relatively complicated dependence of the plasmonmediated photoeffect efficiency (qm /q0 )(ω) with respect to the material, size, and deposition type. We illustrate this dependence in Fig. 8.3. The formula (8.2) is exemplified in this figure for Au nanoparticles deposited on an Si semiconductor, which reproduces well the experimental behaviour [33] (the required material data are listed in Tables 7.2 and 7.3). Both channels of photon absorption resulting in photocurrent in the semiconductor sample are included, direct photoeffect absorption for which the probability of transitions is given by q0 and plasmonmediated absorption with probability qm , respectively. Note also that some additional effects such as the reflection of incident photons or destructive interference on the metallic net would contribute, and these are accounted for
162
Numerical Simulation of Plasmon Photoeffect
phenomenologically in the plasmonmediated channel by an experimentally fitted factor β. The collectiveinterferencetype corrections are rather weak for the low densities of metallic coverings considered, of the order of 108−9 /cm2 , and for nanosphere sizes much lower than the resonance wavelength (∼ 500 nm); however, for larger concentrations and larger nanosphere sizes, they would play a stronger reducing role (by reflecting photons) [111, 31]. The resonance threshold is accounted for by the damped resonance envelope function in Eq. (8.6), including the semiconductor bandgap limit. As indicated in Fig. 8.3, the relatively high value of qm /q0 ∼ 104 × 40β/H (nm) enables significant growth in efficiency of photoenergy transfer to a semiconductor mediated by surface plasmons by an increase in β or a reduction in H (at constant ns ). Because an enhancement of β could easily induce the overdamped regime of plasmon oscillations the more effective prospect would be the lowering of H , especially convenient in thinfilm solar cells. This reflects the fact that the damping of plasmons due to their coupling with band electrons in the substrate semiconductor can greatly exceed the Lorentz friction. Electron scattering losses do not play a significant role in comparison with the dominant channel of energy flow. The overall behaviour of I /I = 1 + qm /q0 calculated according to the relation (8.6), and depicted in Fig. 8.3 agrees well with the experimental observations [33], in the position, height, and shape of the photocurrent curves for distinct samples. In the previous chapter we compared the spectral dependence of the plasmonic efficiency enhancement on substrate (Si, CIGS – copper indium gallium diselenide), for the same Au, Ag, and Cu nanoparticles with radius a = 50, 25 nm and the same nanoparticle concentration ns = 108 /cm2 . From this comparison, in Fig. 7.6, for Si and CIGS substrates with Au, Ag, or Cu nanoparticles of size a = 50,25 nm (at nanoparticle concentration ns = 108 /cm2 ) one notices that the Au nanoparticles utilize the visible sunlight spectrum better than Ag or Cu nanoparticles. The advantage of Au nanoparticles is greater in the case of an Si substrate and is reduced for a CIGS substrate, because of the blueshift of Eg in CIGS with respect to Si. In the case of CIGS (especially for larger nanoparticles, a = 50 nm), the advantage of Au over Ag in the overall utilization of the sunlight spectrum disappears, whereas it is pronounced in the case of an Si substrate. This is so because of the cutoff of the near infrared part of sunlight in the spectral absorption of CIGS, in contrast with that of Si, which favours Ag more than Au nanoparticles; see Fig. 7.6. This behaviour agrees with experimental observations [31]. For nanoparticles of Au and Ag of size a = 50 nm, optimized due to Eq. (8.2), that are deposited on multicrystalline silicon (mcSi) and on CIGS solar cells, the measured [31] overall increase in cell efficiency is as much as 5%. The application of Au and Ag nanoparticles to mcSi solar cells increases their efficiency by 5.6% and 4.8%, respectively [31]. The application of Au and Ag nanoparticles to the
8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL
163
surfaces of CIGS solar cells improves their efficiency by 1.2% and 1.4%, respectively [31]. 8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL The commercial numerical package COMSOL is a convenient tool for solving, by the finite element method, differential equations with imposed arbitrary boundary conditions. It can be utilized to solve the Maxwell–Fresnel problem for arbitrary geometry and material composition of the analysed systems (see COMSOL Multiphysics 5.0, Wave Optics module, http://www.comsol.com). In particular, solar cells can be modelled in this way, including the plasmonic effect induced by the metallic nanoparticles deposited on a cell surface. The great advantage of COMSOL is its flexibility with regard to nanoparticle size and shape, deposition type, and the material of the metallic components and of the semiconductor substrate. In order to simulate a solar cell using the COMSOL system, an appropriate geometric arrangement is required for the setup and also the predefinition of the material parameters, i.e., the dielectric functions for all components of the investigated device. The dielectric function defines the electric susceptibility of a material, linking the displacement electric field D with the external electric field E, D(ω,k) = ε(ω,k)E(ω,k), where ω and k are Fourier variables in the time and space domains, respectively. The real part of the dielectric function defines the refractive index of a material, whereas the imaginary part describes light absorption. All macroscopic processes of the light–matter interaction are included in an effective manner in this function, which also includes quantum effects. Such compressed material microscopic information allows for a completely classical consideration of the Maxwell–Fresnel problem of light scattering and absorption at interfaces in complex multimaterial systems with various configurations. The photon absorption probability (per single photon and time unit) is given for the case of the ordinary photoeffect by Eq. (7.11), i.e., √ 4 2 μ5/2 e2 4πε0 εE02 V 3/2 (hω (8.7) δω0 = ¯ − Eg ) , 3 m2p ωεh¯ 3 8π hω ¯ and for the case when the photoeffect is mediated by metallic nanoparticles it is given by Eq. (7.10), i.e., √ 4 μ3/2 2 hω ¯ − Eg e2 D02 . (8.8) δω = 3 a16π 2 ε02 ε2 h¯ 4 These functions can be used to assess the imaginary part of the dielectric function of materials in the photovoltaic problem including the plasmon effect. The absorption
164
Numerical Simulation of Plasmon Photoeffect
coefficient, α(ω) = h¯ ωδω, links with the imaginary part of the dielectric function as follows: ε (ω) = (nc/ω)α(ω), where n is the refractive index, ε = ε + iε . The plasmon dipole amplitude, D0 in Eq. (8.8), can be found from the irradiated total power: 4πε0 λ4 4πε0 λ4 2 D0 = S · dσ, (8.9) P = (2π)4 c (2π)4 c where P is the total power radiated by the dipole, S is the Poynting vector, and is the nanoparticle surface. For COMSOL simulation, the total energy of the light absorbed in the semiconductor substrate can be calculated by integrating the square of the electric field over the semiconductor volume: ω ns εwith(without) (ω)E 2 dV , (8.10) Qwith(without) (ω) = 4π V where ε is the imaginary part of the dielectric function of the semiconductor substrate either with or without metallic nanoparticles deposited, respectively (‘without’ will be noted as ‘0’). The enhancement of the light absorption due to plasmonic elements (called the efficiency enhancement of the plasmon photoeffect) can be defined as the ratio of the light energy absorbed by the semiconductor substrate covered with metallic nanoparticles and that without any metallic coverage: A(ω) =
Qwith (ω) . Q0 (ω)
(8.11)
One can next estimate the enhancement of the shortcircuit current, Isc , in the cell due to the presence of metallic nanoparticles, averaging over the solar spectrum, Qwith (ω)F(ω)dω Isc = , (8.12) Q0 (ω)F(ω)dω where F(ω) is the standard solar global spectrum, conventionally named as AM1.5G. For COMSOL calculations a unit cell must be defined, e.g., as shown in Fig. 8.4. Simulations with such a unit cell consist of three domains: (1) the air surroundings, (2) the semiconductor substrate, and (3) the metallic nanoparticle. One can consider two models: a model consisting of a single metallic nanoparticle on a substrate (which can then be multiplied by the nanoparticle concentration, neglecting, however, all interparticle electromagnetic interaction), and a model consisting of a periodic metallic nanoparticle array deposited on a semiconductor substrate. The latter model allows inclusion of the interparticle electromagnetic interference effect, which is sensitive to the particle separation. Despite which model is considered, the simulation goes via two steps. In the first step the background electric field distribution must be calculated, i.e., the
8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL
air Si
Λ
(1)
Port: absorption of outgoing electromagnetic wave
Au
Perfectly matched layers
(2a)
air Si
Au
Periodic boundary conditions E1 = E2 eikΛ
air Si
Periodic boundary conditions E1 = E2 eikΛ
PML
Periodic boundary conditions E1 = E2 eikΛ
Periodic boundary conditions E1 = E2 eikΛ
Port: definition of incident electromagnetic wave E0 eikz
165
PML
(2b)
Figure 8.4 The scheme of the unit cell of the numerical model for COMSOL. (1) The first calculation step – evaluation of the background electric field as the reference field distribution for the second step. (2a) The second step for the singleparticle model (no periodic conditions are imposed). (2b) The second step for the metallic nanoparticle (MNP) array model with the periodic Floquet conditions imposed. (Figs. 8.4–8.10 after [145]).
electric field distribution in the case of a plane electromagnetic wave incident on a semiconductor substrate without plasmonic nanoparticles. This referential field distribution is used for comparison in the second step of simulation, the evaluation of the scattered electric field caused by the the presence of metallic nanoparticles deposited on the semiconductor surface. In both the models of system arrangements mentioned above, the first step is identical. The incident light is assumed to be a plane wave propagating vertically along the z axis using two ports. At the top boundary the incoming plane wave parameters are defined and, at the bottom boundary, the parameters of the wave transmitted through the substrate are defined. On the lateral boundaries the Floquet periodic boundary conditions are conventionally assumed, which allows one to simulate a large system via the effective multiplication of the calculation unit cell. In the singleparticle model, for a simulation of one independent particle in the calculation cell, in the second step one defines an additional domain surrounding the calculation cell and absorbing all outgoing light (the socalled perfectly matched layers, PMLs), instead of the periodic conditions. The PML assumption allows us to reduce the simulation area, which is important for temporal optimization of the numerical algorithm. The nanoparticles in this model are completely independent and occur as a multiplication of the single nanoparticle. The neglect of interparticle effects corresponds to low concentrations of the metallic coverage. The width of the computation unit cell was assumed to be 350 nm, the height of the air surroundings 300 nm, the Si substrate thickness is set to 200 nm, and the PML thickness to 150 nm.
166
Numerical Simulation of Plasmon Photoeffect
In the model with a periodic array of metallic nanoparticles, in the second step of the simulation we use again the Floquet periodic boundary conditions on the lateral boundaries and set an additional PML at the top and at the bottom of the computational cell. The width of the computational cell was assumed to vary in the range ∈ (90,360) nm, the height of the air surroundings is set to 300 nm, the Si substrate thickness to 400 nm, and the PML thickness to 150 nm. Outside the PML domains, tetrahedral mesh elements were used with size equal to a/5 inside the metallic nanoparticle and of radius a inside the Si substrate. The simulations were performed assuming the dielectric function for Si with modified absorption is given by the formula (7.10) and the results were compared with a similar simulation using a dielectric function for Si without any metallic modification taken from [146]. The dielectric function of the Au was modelled within the Drude–Lorentz approximation with damping rate given by Eq. (6.43). The results of the COMSOL simulations are presented in Figs. 8.5–8.10 and in Tables 8.1 and 8.2. Notice that the neglect of plasmon damping causes a
Table 8.1 The photocurrent enhancement for the model of an MNP array on an Si substrate (see Eq. (8.12)), for MNP radii a = 20, 30, 40, 50, 60 nm and array periods = 3a, 4a. The results were obtained for the model using dielectric functions correctly modified in their imaginary part. We used solar spectrum AM1.5G to calculate the photocurrent enhancement from Eq. (8.12). Radius (nm)
= 3a
= 4a
20 30 40 50
1.66 1.87 1.97 1.98
1.44 1.71 1.91 1.97
Table 8.2 The photocurrent enhancement for the model of an MNP array on an Si substrate. The MNP radii were taken as a = 20, 30, 40, 50, 60 nm and the array periods as = 3a,4a. The results were obtained for the model using the bulk semiconductor dielectric function without metallic components [146] and the dielectric function of the metal without the proper plasmon damping. The solar spectrum AM1.5G was used. Radius [nm]
= 3a
= 4a
20 30 40 50
0.996 1.006 1.011 1.006
0.999 1.010 1.014 1.014
8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL
Ratio of light absorbed in Si to total incident light
Periodic model FGR modified ε'' (ω) 1
nonmodified ε'' (ω) 1
(a)
0.8
0.8
0.6
0.6
0.4
0.4
90 100 110 120
0.2
0
4
6 λ (m) ×
Absorption enhancement A
5
(c)
4
3
160 200 240 without MNPs Λ (nm)
0.2
(b)
(a) 8
0
4
10− 7 1.2
90 100 110 120 160 200 240
8 6 − 7 λ (m) × 10
(d)
1
0.8
Λ (nm)
2
0.6
1
4
6
8
λ (m) × 10− 7
a = 40 nm β = 0 .001
(d)
(c) 0
(b)
0.4 (m) × 10− 7
Figure 8.5 The periodic model. (a, b) The enhancement of light absorption in the Si substrate as a function of the incident wavelength for various sizes of the unit cell. (c, d) The efficiency enhancement of the system given in Eq. (8.11) as a function of the incident wavelength. (a, c) Results obtained for the model using the dielectric function of the semiconductor ε (ω) modified by the plasmondamping contribution (the energy leaving the plasmons is absorbed by the semiconductor substrate). (b, d) Results obtained for the model using the nonmodified dielectric function for the bulk semiconductor [146]. The calculations were made for MNPs of radii a = 40 nm and for array periods = 90, 100, 110, 120, 160, 200, 240 nm describing the lowering of the nanoparticle concentration.
167
168
Numerical Simulation of Plasmon Photoeffect
Ratio of light absorbed in Si to total incident light
Periodic model FGR modified ε'' (ω) 1
nonmodified ε'' (ω) 1
(a)
0.8
0.8
0.6
0.6
0.4
a (nm)
0.4
0.2
20 25 30 35 40
0.2
0
4
6
8
(b)
0
λ (m) × 10− 7 7 6
Absorption enhancement A
λ (m) × 10− 7 1.2
(c) 2
45 50 55 60 without MNPs
(d)
1.1 1.5
5 4
a (nm)
1
1 4
5
6
7
0.9
λ (m) × 10 − 7
3
0.8 2 0.7 1 4
6
8
λ (m) × 10− 7
β = 0 .001 Λ = 3a
20 25 30 35 40 45 50 55 60
0.6
λ (m) × 10− 7
Figure 8.6 The periodic model. (a, b) Absorption enhancement in the Si substrate as a function of the incident wavelength for varying radii of the MNPs. (c, d) The efficiency enhancement from Eq. (8.11) as a function of the incident wavelength for varying radii of the nanoparticles. (a, c) Results obtained in the model using a modified ε (ω). (b, d) Results obtained in the model using an inappropriate (nonmodified) dielectric function taken from bulk measurements [146]. The calculation was made for MNP arrays with the period = 3a and radius a = 20, 25, 30, 35, 40, 45, 50, 55, 60 nm.
8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL
Ratio of light absorbed in Si to total incident light
Singleparticle model FGR modified ε'' (ω)
1
(a)
1
0.8
0.8
0.6
0.6
nonmodified ε'' (ω)
(b)
20 30 40 50 60 without MNPs a (nm)
0.4
0.4
0.2
0.2
0
4
6
8
0
λ (m) × 10− 7 12
λ (m) × 10− 7
(c)
(d) 1.1
Absorption enhancement A
10 8 1.05 6 1
4
β = 0 .001 8 n s = 8 × 10 (cm2)
2 0.95 0
4
6 8 λ (m) × 10− 7
λ (m) × 10− 7
Figure 8.7 Singleparticle model. (a, b): The absorption enhancement in the Si substrate as a function of the incident wavelength for varying radii of the MNPs ( chosen to conserve surface density ns at 8 × 108 /cm2 ). (c, d) The efficiency enhancement factor from Eq. (8.11) as a function of the incident wavelength for varying sizes of nanoparticles and constant concentration. (a, c) Results obtained for the model using modified ε (ω). (b, d) Results obtained for the model using the irrelevant nonmodified bulk dielectric function [146]. The calculations were made for a single MNP deposited on an Si substrate with radius a = 20, 30, 40, 50, 60 nm, β = 0.001 and for an effective MNP concentration (accommodated by changes in ) ns = 8 × 108 /cm2 .
169
170
Numerical Simulation of Plasmon Photoeffect Periodic model 1
(a)
90 100 110 120 160 200 240 single
σabs
1.5
1
0.8
0.6
Λ (nm) a = 40 nm β = 0 .001
0.5
(b)
σroz
2
0.4
0.2
0
0
λ (m) ×
10− 7
λ (m) × 10− 7
single model (dashed line) 2
(c)
20 25 30 35 40 45 50 55 60 periodic a (nm)
3 2.5
σabs
2 1.5 1
1.5
σroz
3.5
1
(d)
20 25 30 35 40 single a (nm)
0.5
0.5 0
4
6
8
λ (m) × 10− 7
0
λ (m) × 10− 7
Figure 8.8 The periodic model. (a, c) The absorption cross section of an Au nanoparticle deposited on an Si substrate as a function of the incident wavelength for varying singlecell size (a) and varying nanoparticle radius (c). (b, d) The scattering cross section for an Au nanoparticle deposited on an Si substrate; the corresponding cross sections obtained in the case of the singleparticle model are indicated by dashed lines. (a, b) Results obtained from the periodic MNP array model with constant MNP radii a = 40 nm and array period taken from the set = 90, 100, 110, 120, 160, 200, 240 nm. (c, d) Results obtained from the periodic MNP array model with varying MNP radii a = 20, 25, 30, 35, 40, 45, 50, 55, 60 nm and array period = 3a. All cross sections are normalized to the particle surface area.
8.3 Numerical Modelling of the Plasmon Photoeffect by COMSOL
171
Periodic model FGR modified ε'' (ω)
Photocurrent enhancement
2
1
1.9 1.8
0.9
1.7 0.8
1.6 1.5 1.4
2
Photocurrent enhancement
nonmodified ε'' (ω) (b)
(a)
a = 40 nm β = 0 .001 0
1
2 Λ (m) × 10− 7
0.7 3
0 Λ (m) × 10− 7 1
(c)
(d)
0.98
1.95
0.96 1.9 0.94 1.85
0.92
1.8
0.9 0.88
1.75 1.7
Λ = 3a β = 0 .001 2
4 6 radius a (m) × 10− 8
0.86 2
4 6 radius a (m) × 10− 8
Figure 8.9 The periodic model. (a, b) The photocurrent enhancement from Eq. (8.12) as a function of MNP array period. The radii of the MNPs are assumed to be a = 40 nm. (c, d) The photocurrent enhancement as a function of MNP radius. (a, c) Results obtained in the model using modified ε (ω). (b, d) Results obtained in the model using the nonmodified bulk dielectric function [146]. We used the solar spectrum AM1.5G.
reduction in the efficiency of the photoeffect by at least one order of magnitude, both in the singleparticle model (i.e., neglecting the electromagnetic interaction between particles), see Figs. 8.7 and 8.10, and in the periodic array model (including the electromagnetic interaction of the metallic nanoparticles); see
172
Numerical Simulation of Plasmon Photoeffect Model of single particle FGR modified ε'' (ω)
nonmodified ε'' (ω) 1.06
5
Photocurrent enhancement
4 3.5
(a)
1 ·10 8 3 ·10 8 5 ·10 8 7 ·10 8 9 ·10 8
4.5
1.05
1.04
n s (cm2) β = 0 .001
(b)
1 ·10 8 3 ·10 8 5 ·10 8 7 ·10 8 9 ·10 8 n s (cm2)
3
1.03
2.5 1.02 2 1.01 1.5 1
2
4
6
radius a (m) × 10− 8
1
2
4
6
radius a (m) × 10− 8
Figure 8.10 The singleparticle model. (a, b) The photocurrent enhancement (Eq. (8.12)) as a function of MNP radius calculated for the model of the single MNP on Si substrate. The photocurrent enhancement is showed for various MNPs concentrations ns . We used solar spectrum AM1.5G. (a) Results obtained in the model using the modified ε (ω) by the plasmon damping. (b) Results obtained in the model using nonmodified inappropriate dielectric function taken from the measurement in bulk [146].
Figs. 8.5, 8.6, 8.8, 8.9. The effect caused by plasmon damping is similarly strong in the case of absorption in the Si substrate including the mediation of nanoparticles (Figs. 8.5–8.7) and in the case of the absorption cross section, Fig. 8.9. In both cases a significant size effect is visible, manifesting itself in a strong dependence on the nanoparticle radius and on the calculation of the cell dimension (changing the latter is equivalent to varying the nanoparticle concentration). For the photocurrent, the strengthening achieves as much as two orders of magnitude in comparison to including the field concentration close to the nanoparticles only according to the Maxwell–Fresnel solution without quantum corrections (see, e.g., Fig. 8.10). A quantitative comparison is exemplified in Table 8.1 for the COMSOL simulation with inclusion of quantum corrections versus a similar simulation without quantum corrections; see Table 8.2. This comparison agrees with the presentation in Figs. 8.5–8.9. An advantage of the COMSOL simulation is its ability to account for the electromagnetic interaction of the nanoparticles (simplified, however, to nearest neighbours only, via the periodic conditions imposed in the nanoparticle array model). The reducing role of a strong density of metallic coverage is noticeable; this is probably due to collective reflection, see Figs. 8.5, 8.6, 8.8, 8.9. This reducing effect of too large a concentration is, however, considerably weakened by the inclusion of quantum corrections related to the giant damping of plasmons described above.
8.4 Comparison with Experiment
173
The COMSOL simulation presented here is confined to sphericalshaped metallic nanoparticles. It makes little difference, however, to simulate arbitraryshaped nanoparticles with arbitrarytype deposition on the semiconductor substrate (in particular, it is easy to include the case of a nanoparticle partly or completely embedded in a semiconductor medium). This flexibility of COMSOL simulation is its great advantage. It is reasonable to expect that a variation in nanoparticle shape would not cause significant changes with respect to the behaviour described for spherical nanoparticles, as the shape change would influence only the selfmodes of the dipole surface plasmons; this would merely shift the resonance frequency slightly, practically without any modification of the plasmon damping due to coupling with the band electrons in the semiconductor substrate. The latter can be, however, more strongly affected by the type of deposition of the nanoparticles. The nearfield coupling of plasmon dipole oscillations in the metallic nanoparticle with the band electrons in the semiconductor substrate can be considerably enhanced if the nanoparticle is embedded in a semiconductor medium. The practical realization of this stronger coupling may be arranged by using a sandwich structure with the metallic nanoparticles located in between the semiconductor layers. Though such an experiment has not been performed, one might expect a growth in the plasmonmediated photoeffect owing to the strengthening of coupling of plasmons to electrons in all directions in the surrounding semiconductor. 8.4 Comparison with Experiment Observation of the strong enhancement of the photoeffect induced by the mediation of light energy transfer to the semiconductor substrate by surface plasmons in metallic nanoparticles deposited on the photoactive surface has been reported for various experimental setups. Some of these observations are collected in Table 8.3. In various experiments also different methods of nanoparticle covering manufacturing are used. For instance, in Refs. [147, 148] gold nanoparticles on the semiconductor surface are produced by pulsed laser deposition. The size of particles is controlled by the number of ablation shots and the surrounding gas pressure. In [149] the method of magnetron sputtering production of Au:TiO2 films was applied. Recently much attention has focused on perovskite solar cells due to the easy availability of lowtemperature and cheap technology and simultaneously very high efficiency. The incorporation of Ag:Zn nanoparticles in the perovskitebased solar cell [150, 151] has led to improved device performance by 4.52% to 5.70%. Application of Au barshaped particles or multishell spherical Agbased nanoparticles has led to a record increase of perovskite cell efficiency up to even 30%– 40% [153]. The incorporation of bimetallic nanoparticles or coreshell nanoparticles in perovskitebased solar cells is a promising strategy as it allows for better
174
Table 8.3 Measured values of the photocurrent enhancement in Si solar cells and Si photodiodes with deposited metallic nanoparticles. For the various setups and nanoparticle deposition parameters, different increases in the photoeffect efficiency have been observed experimentally, as reported in the references indicated. The majority of the observed behaviour cannot be explained only by the local concentration of the electromagnetic field near the curvature of nanoparticles as accounted for by the conventional COMSOL modelling, and agreement of the experimental data with the theoretical simulation needs the inclusion of the plasmon damping contribution, as described earlier. However, some exceptionally low efficiency increases (or even decreases) evidence the complicated competition of various factors beyond the model considered, being apparently sensitive to the position of the pn junction active layer in the substrate or to destructive interference effects or reflection from too dense coverings. (Table after [145].) Metal
Size (nm)
Shape
Concentration (cm−2 )
Enhancement
pn Junction depth (nm)
Type
Ref.
Au Au Au
50 80 100
spherical spherical spherical
6.6 × 108 1.6 × 108 0.77 × 108
18% (max1 80%) 31% (max1 100%) 38% (max1 60%)
80
cSi
[33]
Au
100
spherical
9.9 × 108
2.8%
500
cSi2
[138]
0.3 × 108
Au Au Au Au Au
100 100 100 100 100
spherical spherical spherical spherical spherical
1.5 × 108 3.2 × 108 6.67 × 108 10 × 108
5.6% 2.0% 3.3% −2.8% −7.5%
> 5003
mcSi4
[31]
Au
100
spherical
3.5 × 108
3.3%
500
cSi5
[139]
1 2 3 4 5
The maximal value of absorption enhancement per single wavelength. Commercialy available n/p Si solar cell produced by Silicon Solar Inc. Emitter thickness is 500 nm. Antireflection coating from SiN of thickness 70 nm. ntype Si wafer (001) of thickness 300 μm and donor concentration around 1015 cm−3 .
Au Au
diameter 20, height (2;3) diameter 65
island spherical
1.3 × 1011 10 × 108
20% (max1 40%) 18%
— 300
aSi:H/cSi6 cSi7
[111] [140]
Ag Ag Ag
40 66 108
island island island
124 × 108 67 × 108 25 × 108
127% 283% 592%
160 160 160
SOI8 SOI8 SOI8
[137]
Ag Ag
thickness 12, 14, 169 diameter (120;140), height (45;60)
island island
— 30 × 108
19%, 14%, 2%10 354%
— 95
Si SOI8
[141] [32]
Ag
thickness 12 and 16 9
island
—
33% and 16%10
1250
SOI11
[141]
Ag Al In
25:91 22:81 17:25
spheroidal spheroidal spheroidal
38%12 40% 30%
17% 21% 23%
— —
cSi13 cSi13 cSi13
[144]
Ag
∼ 60
island
31%
0%
> 15014
cSi
[142]
cylindrical
19%15
cSi16
[143]
Al 6 7 8 9
diameter 190, height 70
49%
Heterojunction aSi:H/cSi (ptype(100)); the thickness of the aSi:H layer is 18 nm. Si wafer with transparent graphene electrode. Silicononinsulator (SOI). Nanoparticle coverage was fabricated by the annealing of silver film of a particular thickness (12, 14, 16 nm) at temperature 200◦ C for 50 minutes. 10 Enhancement averaged over the solar spectrum AM1.5G. 11 Silicononinsulator (SOI); top Si layer thickness 1250 nm. 12 For dense coverings the percentage of metallized surface is shown. 13 Solar cell covered by 20 nm layer of TiO separating nanoparticles from silicon. 2 14 Emitter thickness is 150 nm.15 Periodic, period 380 nm.16 Solar cell covered by 40 nm layer of SiO separating nanoparticles from silicon. 2 175
176
Numerical Simulation of Plasmon Photoeffect
accommodation to the absorption spectrum in the material. Caesium doping is also considered to improve perovskite solar cells [152]. Nanomodifications of dye solar cells have also investigated [154]; by a careful tuning of the amount of organic fluorophore in the hybrid coating material, a maximum increase in power conversion efficiency exceeding 4% is achieved in plastic organic cells [155]. Other metals have been also tested for use as nanocomponents including, e.g., aluminium and titanium besides gold and silver [156, 157], the most popular, as well as multishape particles (Ag) [158]. 8.5 Conclusions By COMSOL simulations it has been demonstrated that the neglect of quantum corrections to the dielectric functions of photocell materials causes a large error reaching more than one order of magnitude in the assessment of the photoeffect efficiency increase due to plasmon mediation in the light energy absorption. The dielectric functions of all materials in the photocell setup must be predefined as prerequisites for the COMSOL calculation. These dielectric functions are strongly affected by the quantum effect of nearfield coupling between plasmons and band electrons, accounted for by the Fermi golden rule approach. At the nanoscale this coupling opens a highly effective channel of energy transfer, which modifies the dielectric functions of both the metallic nanoparticle and the coupled semiconductor substrate. They are different from the corresponding material characteristics taken from experiments in bulk and separately for the two coupled subsystems. This is a source of the abovementioned large error in the simulation of the photovoltaic efficiency if the material dielectric functions are taken from conventional data tables. Thus it must be emphasized that the plasmon photovoltaic effect is caused not by the local concentration of electric field near the curvature of the metallic components but by the quantum effect of coupling between plasmons and electrons. The latter is beyond the ability of COMSOL simulation, which can properly include the local electric field strengthening near the metallic nanoparticles but cannot account for the coupling effect. This effect must be included by appropriate modification of the dielectric functions of both the metallic components and the semiconductor. As verified by COMSOL, such a modification of the dielectric functions gives realistic values of the plasmoninduced efficiency enhancement consistent with the experimental observations. By application of the quantum Fermi golden rule scheme it has been demonstrated that the efficiency of the energy transfer channel between the surface plasmon oscillations in metallic nanoparticles and the substrate semiconductor is dependent on the material parameters of both components (the radius and material and surface concentrations of the metallic nanoparticles, the energy gap, the effective masses of the electrons and holes, and the dielectric permittivity of
8.5 Conclusions
177
the substrate). The analytical formulae for the plasmon–photoeffect efficiency and the time rate of the related plasmon damping allow optimization of the plasmonmediated photoeffect in solar cells. For example, an Si photodiode covered with Au nanoparticles achieves maximal efficiency if covered with Au nanoparticles with radii of few tens of nm and surface density 108−9 /cm2 . Other solar cells, such as CIGS (copper indium gallium diselenide) achieve a lower efficiency increase by metallization because of the worse accommodation of the semiconductor material parameters to the solar spectrum modified by plasmon mediation. The increase in the overall photovoltaic efficiency for the metallically modified cells considered by us varies between 1.5% (CIGS) and 6% (Si), depending on the nanoparticle concentration (note that concentrations that are too dense cause an efficiency decrease owing to destructive interference and reflection). Thus, it has been demonstrated that metallic nanoparticles deposited on the surface of a photodiode can enhance the efficiency of the photoeffect by as much as a factor 2 (i.e., a 100% increase), which has been confirmed experimentally (for Au nanoparticles with a radius 40 nm deposited on Si at a concentration of 108 /cm2 ). Such a large increase is, however, reduced in commercial Si solar cells to ∼ 5% of overall efficiency increase (and to ∼ 2% in CIGS cells), because the photon absorption is only one in a long series of factors resulting in the final efficiency of a solar cell. The strong plasmon photovoltaic effect is caused mainly by quantum effects; the efficiency enhancement found by COMSOL without quantum corrections (i.e., when only the concentration of the electrical field close to the curvature of the metallic nanoparticles is accounted for) does not exceed 0.1, i.e., is lower than the quantum effect by at least one order of magnitude. One can thus conclude that conventional numerical modelling (as in the COMSOL system with the material parameters supplied in packets attached to the system) is erroneous if carried out with the neglect of quantuminduced corrections to the dielectric functions of all components of metallized solar cells. The conventional COMSOL simulations without quantum corrections fail in comparison with experimental observations of the plasmonmediated photoeffect. A realistic explanation of this effect is possible exclusively in the developed quantum approach. Let us mention also the nonlocal plasmon effects in the metallic nanoparticles which also cause corrections to the conventional COMSOL (or Mie) approach. Nonlocal effects in metallic nanostructures are related to the spatial dispersion of the dielectric function, i.e., D(r) = ε(r,r )E(r )d 3 r (here, D and E denote the electric displacement field and the electric field, respectively, and ε(r, r ) denotes the nonlocal dielectric function). The nonlocal effects in the system can be accounted for via the hydrodynamic approach to electrodynamics, including the use of a quasiclassical kinetic Boltzmanntype equation (or Navier–Stokes equation) to describe the nonuniform electronic medium. As the latter involves the Fermi
178
Numerical Simulation of Plasmon Photoeffect
velocity of electrons and a microscopic scattering integral, the nonlocal approach is customarily called a quantum correction to the classical electromagnetic approaches to plasmons such as the Mie theory. This resembles the situation for the skin effect, in particular for its anomalous version [12] where a nonlocal electromagnetic response is essential. As in the case of discrimination between the normal and anomalous skin effect regimes, the roleplaytime scales according to the electron scattering and the incident electromagnetic wave frequency, or the plasmon oscillation frequency in the case of plasmons. This gives an estimate for the applicability of nonlocal corrections to surface plasmons in nanoparticles: namely, the scattering time a/vF , where a is the nanoparticle radius, should be lower than the plasmon time period 2π/ω1 (where ω1 is the Mie frequency), which gives approximately a < 5 nm for the nanoparticle radius for Au as the range of nonlocal plasmon effects. Indeed, the nonlocal corrections calculated using the hydrodynamic approach appear to be important for small metallic clusters with a ∼ 3 nm. At this size the nonlocal corrections cause as much as a ∼ 10% blueshift of the Mie plasmon frequency [159] but the effect quickly disappears at higher a: for a > 5 nm the nonlocal corrections are small and are completely negligible at the size a ∈ (10,100) nm regarded as of interest for applications due to the large Lorentz friction. Nonlocal plasmon effects in small clusters meet, however, with the spillout effect [19] and Landau damping [123, 79], which are pronounced at the scale a ∼ 2−3 nm. To precisely describe these phenomena, together timedependent density operator theory [160] and a numerical ab initio calculation timedependent local density approximation (TDLDA) are used, employing the Kohn–Sham equation approach [161]. This is the reason for addressing nonlocal effects in quantum regime, though they are treated as somewhat classical in the hydrodynamic approach [162–164]. Nonlocal effects manifest themselves also in the plasmonmediated photovoltaic effect [165, 159] but only for small and ultrasmall nanoparticles (not larger than a ∼ 5 nm) or for fewnanometre separations between particles. At larger size scales nonlocal corrections are small compared with the quantum effect of the strong coupling of plasmons with the substrate semiconductor presented above to simplify.
9 Plasmon–Polaritons in Metallic Nanoparticle Chains
In this chapter the collective plasmon modes in a metallic nanochain are described in an accurate and farreaching analytical formulation. The related problem of plasmon– polaritons in metallic chains is of considerable significance for applications in optoelectronics. Conventional optoelectroncs is limited by diffraction constraints to the micrometre size scale of optical fibres, greatly exceeding the nanoscale of the electronic elements. The exchange of photons by plasmon–polaritons with the same energy but with group velocity lower by orders of magnitude allows for the avoidance of diffraction constraints when an optical fibre is substituted by a metallic nanochain. The latter appears to be an almost perfect plasmon–polariton wave guide without any radiation losses. The theoretical formulation of plasmon–polariton theory presented here supplements previous numerical simulations. The theory allows the explanation of the variety formerly observed in numerical models for plasmon–polariton properties, including some misleading artefacts resulting from approximate numerical solutions of the related singular nonlinear problem. In particular, superluminal plasmon–polariton propagation, observed in numerical experiments, has been excluded by an accurate solution using the theory presented in the chapter.
As discussed previously, the investigation of plasmon oscillations in metallic nanoparticles, besides its fundamental character, also has great significance for applications. Metallic surface modifications of solar cells at the nanoscale exhibit a growth in photovoltaic efficiency owing to plasmon mediation in sunlight energy harvesting [104, 32, 33, 105, 34, 35]. On the other hand, periodic linear structures of metallic nanoparticles – metallic nanochains – serve as plasmon wave guides having low damping [3, 116, 4]. The wavelengths of plasmon– polaritons propagating in such structures are considerably shorter in comparison with light of the same frequency [166, 40, 38]. This allows for the avoidance of the diffraction limits for light circuits, when one transforms the light signal into a plasmon–polariton wave [1, 5, 6]. This is regarded as promising for the forthcoming construction of plasmon optoelectronic nanodevices that are not available in ordinary light wave guides because of diffraction constraints.
179
180
Plasmon–Polaritons in Metallic Nanoparticle Chains
a d x
Longitudinal polarization
z y
Figure 9.1 A chain of metallic nanospheres in which the plasmon–polariton can propagate with longitudinal polarization (plasmon dipole oscillations along the chain) or tranverse polarization (dipole oscillations perpendicular to the chain axis).
Metallic clusters with size 1–2 nm have been widely investigated both theoretically, within the socalled timedependent local density approximation (TDLDA) [19, 71, 20, 79], and experimentally, especially for small clusters of alkali metals such as Na or K. Extremely small metal clusters contain a low number of electrons and have poor radiation properties; thus for energy transfer, by including plasmon–polaritons, larger particles are more suitable. Larger metallic nanoparticles of size several dozen nm manifest radiative properties that overwhelm the plasmon behaviour at this scale. For such nanoparticles, with a size of tens of nanometres, variants of the random phase approximation (RPA) have turned out to be appropriate and useful [19, 71, 21], as has been demonstrated in previous chapters. In particular, much attention has been focused on large nanoparticles of noble metals (Au, Ag, and Cu) because of the location of the surface plasmon resonances in particles of these metals within the visible light spectrum. Owing to the intense radiation of surface plasmons in large nanoparticles, special interest has been paid to plasmon–polariton wave guides in the form of chains consisting of these nanoparticles [41, 167, 168]; see Fig. 9.1. Nearfield microscopy applied to such systems has directly demonstrated the longrange propagation of a plasmon–polariton signal along these structures. For instance, in [169], the observation of 5 μmrange propagation in gold nanoparticles with average radius a = 50 nm aligned in an equidistant chain with the separation between neighbouring spheres d = 200 nm has been reported. In a series of papers [24, 170, 39, 171, 166], the practically nondamped propagation of collective plasmonic modes in Au and Ag nanochains has been demonstrated over distances of ∼ 0.5 μm, and energy
9.1 Plasmon Oscillations in Metallic Nanospheres
181
transfer along the chain was directly confirmed. Such a long range of plasmon– polariton propagation, reaching visible light wavelengths and revealing a reduced group velocity, below 0.1c [170, 171, 166], fits well with the requirements of subdiffraction nanophotonics. In [172], the weakly damped propagation of plasmon– polaritons along Ag nanowires with diameters of about 100 nm over distances of about 20 μm was reported. In [40], similarly longrange values for the practically undamped propagation of plasmon–polaritons in various metallic nanostructures were summarized. The theoretical estimation of plasmon–polariton attenuation in metallic nanochains made within a dipole–dipole interaction model using finite element numerical methods leads to rather larger values for the attenuation take over (∼ 3 dB/15 μm) than those observed experimentally [40, 169]. In the present treatise, we solve the problem of this discrepancy by means of a rigorous treatment of collective surface plasmon propagation along a nanochain, including retardation effects for the near, medium, and farfield zones of plasmon dipoles and describing plasmon oscillations in individual nanospheres within the RPA approach via an analytical calculus. The radiative properties of collective surface plasmons in nanospheres aligned in the chain will be studied and described, taking into account the near, medium, and farfield contributions to the dipole coupling between elements of the chain and including retardation effects. The ideal vanishing of radiation losses in the chain for a wide spectrum of collective plasmonic wavetype modes will be demonstrated. The undamped plasmon–polariton modes induced by an external persistent oscillating electric forcing field can be identified. The frequency of these modes equals the frequency of the external field, and their amplitude is maximal for resonance with the plasmon–polariton selfmode frequency. The calculus of plasmon selfmode frequencies, their attenuation rates, and their group velocities will be detailed for longitudinal and transverse polarizations of collective excitations and for a variety of chain parameters. The problem of the logarithmic singular contribution caused by the farfield component of the dipole interaction will be solved for the selfenergy of plasmon–polaritons with transverse polarization and the similar problem caused by the mediumfield component for the group velocities of both polarizations, with a link to the numerical simulations of the longrange kinetics of plasmon–polaritons in metallic nanochains will also be solved [173–176]. 9.1 Plasmon Oscillations in Metallic Nanospheres We will consider a chain of metallic (Au or Ag) nanospheres of radius a located in a dielectric environment, with dielectric constant ε, in the presence of a dynamic external electric field applied to some part of the chain. We will analyse a collective wavetype reaction of the electron liquid in the metallic components of the chain
182
Plasmon–Polaritons in Metallic Nanoparticle Chains
to this field. To describe this composite system, let us first briefly summarize the properties of plasmon oscillations for the single metallic nanosphere analysed in previous chapters, paying special attention to the surface plasmon damping caused by radiation of electromagnetic waves by the charged plasma oscillations. Conventionally, a jellium model for each metallic nanosphere is assumed, in which the positive charge of the ion background is static and uniformly smeared over the whole nanosphere: ne (r) = ne (a − r),
ne = Ne /V ,
where Ne is the number of free electrons in the nanosphere, V is the volume of the nanosphere, is the Heaviside step function, and ene is the averaged density of the positive charge compensating the charge of the free electrons. The fluctuations in the local electron density in the nanosphere can be divided into surface and volume parts: 0 for r < a, δρ1 (r,t) (9.1) δρ(r,t) = δρ2 (r,t) for r ≥ a (r → a+). These two parts of the local electron density fluctuations satisfy equations derived in the framework of the random phase approximation (RPA), 2 F 2 ∂ 2 δρ1 (r,t) = ∇ δρ1 (r,t) − ωp2 δρ1 (r,t) ∂t 2 3m and
(9.2)
r 3 F ne + F δρ2 (r,t) δ(r − a) 5 r 2 ωp r 2 F r 1 − ∇δρ2 (r,t) + ∇ d 3 r1 3mr 4π r r − r1 
∂ 2 δρ2 (r,t) 2 =− ∇ 2 ∂t 3m
× (δρ1 (r1,t)(a − r1 ) + δρ2 (r1,t)(r1 − a))] δ(r − a),
(9.3)
where ωp2 = 4πne e2 /m is the bulk plasmon frequency; F is the Fermi energy, ne is the equilibrium density of electrons (equal to the jellium density), and m is the electron mass. The analysis and solution of the above equations has been given explicitly in previous chapters, resulting in the determination of the plasmon selfmode spectrum, for both the volume and surface modes. Nevertheless, this RPA treatment does not account for plasmon damping. In order to include the damping of plasmons in a phenomenological manner, one adds an attenuation term to the plasmon dynamic oscillatorytype equations, i.e., the terms (−2/τ0 )∂δρ(r,t)/∂t added to the righthand sides of both Eqs. (9.2)
9.1 Plasmon Oscillations in Metallic Nanospheres
183
and (9.3). The damping rate 1/τ0 (as already discussed in previous chapters) accounts for electron scattering losses [24], 1 vF CvF + , τ0 2λb 2a
(9.4)
where C is a constant of order unity, a is the nanosphere radius, vF is the Fermi velocity in the metal, λb is the electron mean free path in the bulk metal (including the scattering of electrons on other electrons, on impurities, and on phonons [24]). For example, for Au, vF = 1.396 × 106 m/s and λb 53 nm at room temperature; the latter term in Eq. (9.4) accounts for the scattering of electrons at the boundary of the nanoparticle, whereas the former term corresponds to scattering processes similar to those in the bulk. Other effects, such as Landau damping (especially important in small clusters [80, 79]), corresponding to the decay of a plasmon to a highenergy particle–hole pair, are of less significance for nanosphere radii larger than 2−3 nm [80] and are completely negligible for radii larger than 5 nm; here we consider large nanospheres with radii ≥ 10 nm. Note that for the growth in this radius range a lesser role is played also by the electron liquid spillout effect [19, 20], though this is of primary importance for small clusters [19, 21]. Besides the homogeneous Eqs. (9.2) and (9.3) determining the selffrequencies of plasmon modes, dual inhomogeneous equations should be written with an explicit expression for the forcing factor. This factor would be the timedependent electric field, e.g., the electric component of the incident electromagnetic wave. For the electromagnetic wave frequency that is in resonance with the plasmons in the metallic nanosphere, the wavelength (being of the order of 500 nm in this case) greatly exceeds the nanosphere size (with radius 10−50 nm); thus the dipoleregime conditions are fulfilled. For a forcing field E(t) that is almost uniform over the nanosphere, which corresponds to the dipole approximation, only the dipole surface mode can be excited. Then the electronliquid response resolves itself into a single dipoletype mode described by the function Q1m (t) (i.e., with l = 1 and m = −1, 0, 1, the angular momentum numbers relating to spherical symmetry and describing the dipole mode). The function Q1m (t) satisfies the equation ∂ 2 Q1m (t) 2 ∂Q1m (t) + + ω12 Q1m (t) 2 ∂t τ0 ∂t & √
( 4π ene ' = Ez (t)δm,0 + 2 Ex (t)δm,1 + Ey (t)δm,−1 , (9.5) 3 m √ where ω1 = ωp / 3ε; this is a dipole surface plasmon Mietype frequency [18] and ε is the dielectric constant of the nanosphere surroundings [23]. The function Q1m (t) is the only contribution to the plasmon response to a homogeneous uniform
184
Plasmon–Polaritons in Metallic Nanoparticle Chains
electric field. Thus, for such a uniform forcing field, the electron density fluctuations attain the form [23] ⎧ for r < a ⎨ 0 1 δρ(r,t) = (9.6) Q1m (t)Y1m ( ) for r ≥ a (r → a+), ⎩ m=−1
where Ylm ( ) is a spherical harmonic with l = 1. For plasmon oscillations given by Eq. (9.6), one can calculate the corresponding dipole D(t), as demonstrated in previous chapters: ⎧ 3 2π ⎪ (t) = e d rxδρ(r,t) = eQ1,1 (t)a 3, D ⎪ x 3 ⎪ ⎨ (9.7) eQ1,−1 (t)a 3, Dy (t) = e d 3 ryδρ(r,t) = 2π 3 ⎪ ⎪ ⎪ ⎩ D (t) = e d 3 rzδρ(r,t) = 4π eQ (t)a 3, z 1,0 3 and D(t) satisfies the equation (rewriting Eq. (9.5))
2 a 3 4πe2 ne ∂ 2 ∂ 2 D(t) = + + ω E(t) = εa 3 ω12 E(t). 1 ∂t 2 τ0 ∂t 3m
(9.8)
The phenomenological oscillatorytype damping term in the above equation includes all types of scattering phenomena, i.e., electron–electron, electron– phonon, electron–admixture interactions, as well as the contribution caused by the scattering of electrons at the nanoparticle boundary [24]. Electron scattering effects cause significant attenuation of plasmons, especially important in small metal clusters. These contributions to the damping time rate are proportional to 1/a and are of less significance with growth in radius. There is also, however, another important channel of plasmon damping caused by radiation losses, not included in the formula for τ0 . We will show that the contribution to the overall attenuation of plasmons caused by the radiation losses scales as a 3 , and therefore for large nanospheres the radiative losses dominate plasmon damping. The radiative losses of oscillating charges, related to the plasmon dipole variation in time, can be expressed by the Lorentz friction [55], i.e., by an equivalent fictitious electric field slowing down the motion of charges, EL =
2 ∂ 3 D(t) . 3c3 ∂t 3
Thus, one can rewrite Eq. (9.8) including the Lorentz friction term,
2 ∂ 2 ∂ 2 + + ω1 D(t) = εa 3 ω12 E(t) + εa 3 ω12 EL, ∂t 2 τ0 ∂t
(9.9)
(9.10)
9.1 Plasmon Oscillations in Metallic Nanospheres
√ or more explicitly, for the case when E = 0, since ω1 = ωp / 3ε, !
2 ωp a 3 ∂ 2 ∂ ∂ 2 2 2 + ω1 D(t) = D(t) . − D(t) + √ √ ∂t 2 ∂t τ0 3ω1 ε c 3 ∂t 2
185
(9.11)
Applying now a perturbation procedure for solving Eq. (9.11) and treating the righthand side of this equation .as the perturbation, one obtains in the zeroth step of / 2 2 2 the perturbation procedure ∂ /∂t + ω1 D(t) = 0, from which (∂ 2 /∂t 2 )D(t) = −ω12 D(t). Therefore, in the first step of the perturbation procedure, one substitutes the latter formula into the righthand side of Eq. (9.11), obtaining
2 ∂ 2 ∂ 2 (9.12) + + ω1 D(t) = 0, ∂t 2 τ ∂t where 1 ω1 1 + √ = τ τ0 3 ε
ωp a √ c 3
3 .
(9.13)
In this way, we have included the Lorentz friction in the total attenuation rate 1/τ , which is justified for nanospheres that are not too large, i.e., when the second term in Eq. (9.13), proportional to a 3 , is sufficiently small to fulfil the perturbation procedure constraints. For nanospheres with radius 10−30 nm, this approximation is justified and has been verified experimentally for Au and Ag nanospheres [77]. It is worth emphasizing the ability of this perturbative approach to explain the experimentally observed redshift of the surface plasmon resonance frequency with growing a (visible in the extinction spectrum of light passing through watercolloidal solutions of metallic nanospheres with various radii [77]). Indeed, −t/τ cos(ω1 t + φ), where the solution of Eq. (9.12) is of the form D(t) = Ae ω1 = ω1 1 − 1/(ω1 τ )2 ; the latter gives the experimentally observed redshift of the plasmon resonance due to ∼ a 3 growth of the attenuation caused by the radiation losses. The Lorentz friction term in Eq. (9.13) dominates the plasmon damping for a ≥ 12 nm (for Au and Ag) owing to this a 3 dependence. The plasmon damping grows rapidly with a and results in a pronounced redshift of the resonance frequency in good agreement with the experimental data for 10 < a < 30 nm (Au and Ag) [77]. In this size range of metallic particles, we find a conspicuous crossover of the attenuation rate in its dependence on a. The minimum of damping is achieved at 1/4 9 vF c3 ∗ (9.14) ε a = 2 ωp4 and, for a < a ∗ , the damping rate grows with decreasing a approximately as 1/a, while for a > a ∗ the rate grows as a 3 with increasing a. The value of a ∗ can be estimated for Au, Ag, and Cu; see Table 9.1.
186
Plasmon–Polaritons in Metallic Nanoparticle Chains
Table 9.1 Radius of the nanosphere corresponding to the minimal value of surface plasmon damping.
n=
√
a∗ ε
n = 1, vacuum n = 1.4, water n=2
Au
Ag
Cu
8.78 10.4 12.4
8.77 10.42 12.41
8.82 10.5 12.5
9.2 Radiative Properties of a Metallic Nanosphere in a Chain When a metallic nanosphere is an element of a chain created by similar nanospheres equidistantly distributed along a line, one has to take into account that its radiation losses may be modified by energy income from other nanospheres when, in the total system, a collective plasmon excitation propagates. The periodicity of the chain makes the system similar to a onedimensional crystal; see Fig. 9.2. The interaction between nanospheres can be considered as a dipoletype coupling. The minimal separation of nanospheres in the chain is d = 2a, where d is the distance between neighbouring sphere centres, but we will consider d > 3a, because the dipole approximation for plasmon interaction in the nanosphere chain is sufficiently accurate for d > 3a since then the contribution of multipole interactions can be neglected. Various numerical largescale calculations of the electromagnetic field distribution in such systems have been made, including dipole and also multipole interactions between the plasmonic oscillations in metallic components [41, 167, 168]. It is worth noting that a model of interacting dipoles [177, 178] was developed first for the investigation of stellar matter [179, 180] and only then was it adopted for metal particle systems [181, 182]. Numerical studies beyond the dipole model [41, 168] indicate that the dipole model is sufficiently accurate when the particle separation is not lower than the particle radius. Otherwise, multipole contributions to the interaction start to be important [183]. Assuming that in a sphere located at the point r we have an oscillating dipole D, then, at another point at a position r0 with respect to r, this dipole causes an electric field in the following form (it includes the relativistic retardation of electromagnetic signals) [55, 76], ∂2 1 1 ∂ 1 1 − 2 2 − D(r,t − r0 /v) − E(r,r0,t) = ε v ∂t r0 v∂t r02 r03 2 ∂ 1 1 ∂ 3 3 + n0 (n0 · D(r,t − r0 /v)), + + (9.15) ε v 2 ∂t 2 r0 v∂t r02 r03 √ where n0 = r0 /r0 and v = c/ ε. The above formula includes terms corresponding to the nearfield zone (the denominator with r03 ), the mediumfield zone (the
9.2 Radiative Properties of a Metallic Nanosphere in a Chain
187
Nanochain a
x z
d
y
Figure 9.2 Metallic nanospheres with radius a are aligned along the chain axis with separation d between chain elements. At top right are shown the transverse and longitudinal plasmon polarizations.
denominator with r02 ), and the farfield zone (the denominator with r0 ) in the dipole field. This allows us to write out a dynamical equation for the plasmon oscillations in each nanosphere of the chain; they can be numbered by an integer l (d denotes the separation between nanospheres in the chain, d > 3a). The vectors r and r0 are collinear if the origin is associated with a nanosphere in the chain. Therefore, the equation for surface plasmon oscillations on the lth sphere is as follows:
2 m=∞ l − md 2 ∂ ∂ 2 2 3 + Eα md,t − + ω1 Dα (ld,t) = εω1 a ∂t 2 τ0 ∂t v m=−∞, m=l + εω12 a 3 ELα (ld,t) + εω12 a 3 Eα (ld,t).
(9.16)
The first term on the righthand side of Eq. (9.16) describes the dipoletype coupling between nanospheres, and the other two terms correspond to the contribution to plasmon attenuation due to the Lorentz friction (as described in the previous section) and to the external forcing field. The index α enumerates the polarizations; for longitudinal polarization α = z and for transverse polarization α = x(y), with respect to the chain orientation (assumed to be in the z direction). According to Eq. (9.15), we have: ∂ 1 2 d × Dz (md,t − m − ld/v), + Ez (md,t) = 3 εd m − l3 vm − l2 ∂t ∂2 ∂ 1 1 d d2 Ex(y) (md,t) = − 3 + + 2 εd m − l3 vm − l2 ∂t v l − d ∂t 2 × Dx(y) (md,t − m − ld/v).
(9.17)
Taking advantage of the chain periodicity (in analogy to the Bloch states in crystals with the reciprocal quasimomentum lattice), one can assume that Dα (ld,t) = Dα (k,t) e−ikld
0≤k≤
2π . d
(9.18)
188
Plasmon–Polaritons in Metallic Nanoparticle Chains
One can assert this in a more formal manner, taking the Fourier picture of Eq. (9.16) as follows. As the dipoles are localized at nanosphere centres, the system is discrete, similarly to the case of phonons in a onedimensional crystal. One can thus apply a discrete Fourier transform (DFT) with respect to the positions, whereas an ordinary continuous Fourier transform (CFT) would be with respect to time. The DFT is defined for a finite set of numbers, so we can consider a chain with 2N + 1 nanospheres, i.e., of length L = 2Nd. Thus, for any discrete characteristics f (l), l = −N, . . . ,0, . . . ,N of the chain, such as a selected polarization of the dipole distribution, one is dealing with the DFT picture: f (k) =
N
f (l)eikld ,
(9.19)
l=−N
where k = 2π /(2Nd)n, n = 0, . . . ,2N. This means that kd ∈ [0,2π ] owing to the periodicity of the equidistant chain, with separation between nanosphere centres equal to d. The Born–Karman boundary condition is imposed on the whole system, resulting in the above form of k. In order to account for the infinite length of the chain, one can take the limit N → ∞, which causes the variable k to be quasicontinuous, but we still have kd ∈ [0,2π ]. As will be described in Section 9.3, one arrives at the Fourier picture of Eq. (9.16), with a DFT for positions and a CFT for time: a3 2 2 2 −ω − i ω + ω1 Dα (k,ω) = ω21 3 Fα (k,ω)Dα (k,ω) + εa 3 ω21 E0α (k,ω), τ0 d (9.20) with, setting x = kd and ξ = ωd/v, ∞ cos(mx) cos(mξ ) Fz (k,ω) = 4 cos(mx) + ξ sin(m) m3 m2 m=1 ! ∞ 1 3 cos(mx) cos(mx) + 2i sin(mξ ) − ξ cos(mξ ) , ξ +2 3 m3 m2 m=1 ∞ cos(mx) cos(mx) cos(mξ ) + ξ sin(mξ ) Fx(y) (k,ω) = −2 3 m m2 m=1 2 cos(mx) −ξ cos(mξ ) m ∞ cos(mx) cos(mx) 2 3 sin(mξ ) + ξ cos(mξ ) −i − ξ +2 3 3 m m2 m=1 2 cos(mx) −(ξ ) sin(mξ ) . (9.21) m
9.2 Radiative Properties of a Metallic Nanosphere in a Chain
189
Figure 9.3 The shaded regions (0 < kd ± ω1 d/v < 2π ) in which the radiation losses vanish for infinite chains of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d/a ∈ [3,6] (ω = ω1 , v = c).
10
15
15
10
10
5
z
d=3a d=4a d=5a
z
z
15
5
5
0
0
0 0
1
2
3 kd
4
5
6
0
1
2
3 kd
4
5
0
6
1
2
3 kd
4
5
6
Figure 9.4 The function Im Fz (k;ω = ω1 ) for infinite chains of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d = 3a, 4a, 5a ([46]). d=3a d=4a d=5a
10
5
5
0
0 0
1
2
3 kd
4
5
6
15 x y
10
15 x y
x y
15
10 5 0
0
1
2
3 kd
4
5
6
0
1
2
3 kd
4
5
6
Figure 9.5 The function Im Fx(y) (k;ω = ω1 ) for infinite chains of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d = 3a, 4a, 5a ([46]).
A direct calculation of the functions Im Fz (k,ω) and ImFx(y) (k,ω), which correspond to the radiative damping for the longitudinal and transverse plasmon– polariton polarizations, respectively, will be given in Section 9.3; see Eqs. (9.27) and (9.29). We show there that both these functions vanish when 0 < kd ±ωd/v < 2π (the corresponding region is indicated in Fig. 9.3). Outside this region, the radiative damping expressed by the functions Im Fα (k,ω) is not zero, which for the longitudinal and transverse modes is illustrated in Figs. 9.4 and 9.5, correspondingly.
190
Plasmon–Polaritons in Metallic Nanoparticle Chains
9.3 Calculation of the Radiative Damping of a Plasmon–Polariton in a Chain Both sides of Eq. (9.16) can be multiplied by ei(kld−ωt) /2π and then, one can perform a summation with respect to the nanosphere positions and an integration over t. Taking into account that 1 2π
∞ N
Dα
∞ l=−N
md ±md + ld;t − v
e−i(kld−ωt) dt = ei(∓kmd+ωmd/v) Dα (k,ω), (9.22)
one thus obtains the following equation in Fourier representation (a DFT for the nanosphere positions and a CFT for time):
a3 2 2 −ω − i ω + ω1 Dα (k,ω) = ω12 3 Fα (k,ω)Dα (k,ω) + εa 3 ω12 E0α (k,ω), τ0 d (9.23) 2
where k = 2πn/(2Nd), n = 0,1, . . . ,2N , i.e., kd ∈ [0,2π ], due to the periodicity of the chain with equidistant separations d of the nanospheres, and the form of k is due to the Born–Karman boundary condition with the period L = 2Nd. For N → ∞ (the infinitechain limit), k is a quasicontinuous variable. In Eq. (9.23) we have, again setting x = kd, ξ = ωd/v, Fz (k,ω) = 4
∞ cos(mx) m=1
m3
cos(mx) cos(mξ ) + ξ sin(mξ ) m2
! ∞ 1 3 cos(mx) cos(mx) sin(mξ ) − ξ cos(mξ ) , ξ +2 + 2i 3 m3 m2 m=1 ∞ cos(mx) cos(mx) cos(mξ ) + ξ sin(mξ ) Fx(y) (k,ω) = −2 3 m m2 m=1 2 cos(mx) −ξ cos(mξ ) m ∞ cos(mx) cos(mx) 2 3 sin(mξ ) + ξ cos(mξ ) −i − ξ +2 3 3 m m2 m=1 2 cos(mx) −ξ sin(mξ ) . (9.24) m
9.3 Calculation of the Radiative Damping of a Plasmon–Polariton in a Chain 191
Some summations in the above equations can be done analytically [184]: ⎧ ∞ sin(mz) ⎪ π −z ⎪ ⎪ = , for 0 < z < 2π, ⎪ ⎪ ⎪ 2 ⎪ m=1 m ⎪ ⎪ ⎪ ∞ ⎪ cos(mz) 1 1 ⎪ ⎪ ⎪ , = ln ⎪ ⎨ m 2 2 − 2 cos(z) m=1
∞ ⎪ cos(mz) π2 π 1 ⎪ ⎪ = − z + z2, for 0 < z < 2π, ⎪ ⎪ 2 ⎪ m 6 2 4 ⎪ m=1 ⎪ ⎪ ⎪ ∞ ⎪ ⎪ sin(mz) π2 1 π ⎪ ⎪ = z − z2 + z3, for 0 < z < 2π . ⎪ ⎩ 3 m 6 4 12 m=1
(9.25)
Using the above formulae, one can show that if 0 < kd ± ωd/v < 2π then ∞
sin(m(x + ξ )) − sin(m(x − ξ )) Im Fz (k,ω) = 2 m3 m=1 2 cos(m(x + ξ )) + cos(m(x − ξ )) + ξ3 −ξ 2 m 3
2 π 1 π 2 3 =2 (x + ξ ) − (x + ξ ) + (x + ξ ) 6 4 12
2 π 1 π 2 3 −2 (x − ξ ) − (x − ξ ) + (x − ξ ) 6 4 12
2 π π 1 2 − 2ξ − (x + ξ ) + (x + ξ ) 6 2 4
2 2 π π 1 2 (9.26) − 2ξ − (x − ξ ) + (x − ξ ) + ξ 3 ≡ 0. 6 2 4 3 However, if kd − ωd/v < 0 or kd + ωd/v > 2π for some values of the wave vector k then a more general formula is needed. By using the Heaviside step function, one can extend Eq. (9.25) to the second period of their lefthand sides; note that for d/a ∈ [2,10], a < 25 nm, the periods after the second are not reached for kd ∈ [0,2π). The extended form for Im Fz (k,ω) is as follows, x = kd, ξ = ωd/v,
2 π 1 π Im Fz (k,ω) = (2π − x − ξ )2 (x + ξ ) − (x + ξ )2 + (x + ξ )3 6 4 12
2 π π + (−2π + x + ξ )2 (x + ξ − 2π) − (x + ξ − 2π)2 6 4 1 + (x + ξ − 2π)3 12
192
Plasmon–Polaritons in Metallic Nanoparticle Chains
1 π2 π (x − ξ ) − (x − ξ )2 + (x − ξ )3 6 4 12
2 π π − (−x + ξ )2 (x − ξ + 2π) − (x − ξ + 2π)2 6 4 1 + (x − ξ + 2π)3 12
2 π π 1 2 − (2π − x − ξ )2ξ − (x + ξ ) + (x + ξ ) 6 2 4
2 π π 1 2 − (−2π + x + ξ )2ξ − (x + ξ − 2π) + (x + ξ − 2π) 6 2 4
2 π π 1 2 − (−x + ξ )2ξ − (x − ξ + 2π) + (x − ξ + 2π) 6 2 4
2 2 π π 1 2 (9.27) − (x − ξ )2ξ − (x − ξ ) + (x − ξ ) + ξ 3 . 6 2 4 3
− (x − ξ )2
The function given by Eq. (9.27) is depicted in Fig. 9.4. Equation (9.27) allows one to account for the inconsistency of the periodic functions given by the sums of the sines and cosines with the nonperiodic Lorentz friction term and the inconsistency of the arguments kd ± ωd/v of the trigonometric functions beyond the first period. Figure 9.3 gives the solution of the equation (kd − ωd/v)(kd + ωd/v − 2π) = 0, which determines the region for x = kd versus d/a inside which exact cancellation of the Lorentz friction by the radiative energy income from other nanospheres takes place. In Fig. 9.4, this cancellation is presented for various nanosphere diameters, for longitudinally polarized plasmon collective excitations. A similar analysis can be done for transversely polarized excitation, i.e., for Im Fx(y) (k,ω). This function is exactly zero only for the regions 0 < kd − ωd/v < 2π and 0 < kd + ωd/v < 2π , where one can write Im Fx(y) (k,ω) = −
∞
sin(m(x + ξ )) − sin(m(x − ξ ))
m3
m=1
cos(m(x + ξ )) + cos(m(x − ξ )) m2 2 2 sin(m(x + ξ )) − sin(m(x − ξ )) + (ξ )3 −ξ m 3
2 π 1 π =− (x + ξ ) − (x + ξ )2 + (x + ξ )3 6 4 12
2 1 π π 2 3 + (x − ξ ) − (x − ξ ) + (x − ξ ) 6 4 12 −ξ
9.3 Calculation of the Radiative Damping of a Plasmon–Polariton in a Chain 193
π2 π 1 − (x + ξ ) + (x + ξ )2 6 2 4
2 π π 1 2 +ξ − (x − ξ ) + (x − ξ ) 6 2 4 1 2 1 + ξ 2 [π − x − ξ ] − ξ 2 [π − x + ξ ] + ξ 3 2 2 3 ≡ 0.
+ξ
(9.28)
Nevertheless, outside the regions 0 < kd ± ωd/v < 2π the value of Im Fx(y) is nonzero, as is demonstrated in Fig. 9.5 and as can be accounted for by the following formula, again x = kd, ξ = ωd/v): π2 1 π 2 3 (x + ξ ) − (x + ξ ) + (x + ξ ) Im Fx(y) (k,ω) = −(2π − x − ξ ) 6 4 12
2 π π − (−2π + x + ξ ) (x + ξ − 2π) − (x + ξ − 2π)2 6 4 1 + (x + ξ − 2π)3 12
2 1 π π 2 3 + (x − ξ ) (x − ξ ) − (x − ξ ) + (x − ξ ) 6 4 12
2 π π + (−x + ξ ) (x − ξ + 2π) − (x − ξ + 2π)2 6 4 1 + (x − ξ + 2π)3 12
2 π π 1 + (2π − x − ξ )ξ − (x + ξ ) + (x + ξ )2 6 2 4
2 π π 1 2 + (x − ξ )ξ − (x − ξ ) + (x − ξ ) 6 2 4
2 π π 1 2 + (−2π + x + ξ )ξ − (x + ξ − 2π) + (x + ξ − 2π) 6 2 4
2 π π 1 2 + (−x + ξ )ξ − (x − ξ + 2π) + (x − ξ + 2π) 6 2 4 1 2 + (2π − x − ξ ) ξ [π − x − ξ ] + (−2π + x + ξ ) 2 1 2 1 × ξ [3π − x − ξ ] − (x − ξ ) (ξ )2 [π − x + ξ ] 2 2 1 2 2 − (−x + ξ ) (ξ ) [−π − x + ξ ] + ξ 3 . (9.29) 2 3
194
Plasmon–Polaritons in Metallic Nanoparticle Chains
Figure 9.6 The sums (a)
∞ n=1
sin(nx) n ,
∞
(b)
n=1
cos(nx) , n2
(c)
∞ n=1
sin(nx) , n3
for x ∈
(−1,15). ,
,
,
0.10
0.10
0.10
(2/3)( 1a/v)3
0.08
1/(
0.08
3
)+(a/d) /2 Im Fz
0.08
0
0.06
0.06
0.06
0.04
0.04
0.04
0.02
0.02
0.02
0.00
0
1
2
3 kd
4
5
6
0.00
0.00 0
1
2
3 kd
4
5
6
0
1
2
3 kd
4
5
6
Figure 9.7 For comparison, the various contributions to collective plasmon damping in the chain, for longitudinal polarization. The solid line corresponds to the total damping rate (in dimensionless units) 1/ω1 τz = 1/ω1 τ0 + (a 3 /2d 3 ) Im Fz (k), and the flat part of this line displays the remaining, ohmic, contribution at that part of the kperiod where all the electromagnetic losses vanish; the dashed line indicates the Lorentz friction value (in dimensionless units), 13 (ω1 a/v)3 .
This function is plotted in Fig. 9.5. The discontinuities on the borders between the regions with vanishing radiative damping and with nonzero radiative attenuation sin(nz) (see Fig. 9.6), which enters are caused by the discontinuous function ∞ n=1 n Im Fx(y) but not Im Fz (see Eq. (9.24)). In order to compare the magnitudes of the various contributions to the damping of the collective plasmons in the chain, let us plot the dimensionless values for the longitudinal polarization, 1 a3 1 + 3 Im Fz (k) = ω1 τ ω1 τ0 2d
3 (in Fig. 9.7) in comparison to the Lorentz friction contribution 13 ωv1 a (broken line line in Fig. 9.7). In this figure note that for small nanospheres (a = 10 nm) the Lorentz term is lower than the ohmic attenuation (the flat part of the solid line, see also Eq. (9.4)), while for larger nanospheres (a = 15,20 nm) the Lorentz friction dominates as it is proportional to a 3 . For these larger nanospheres, the Ohmic damping is also lower owing to the a −1 term in Eq. (9.4). The same can be demonstrated for transverse polarization, as is shown in Fig. 9.8.
9.4 Plasmon–Polariton SelfModes in a Chain Propagation ,
,
, 0.10
0.10
0.10
(1/3)( 1a/v)
0.08
3
3
1/(
0.08
0
)+(a/d) /2ImFx(y)
0.08
0.06
0.06
0.06
0.04
0.04
0.04
0.02
0.02
0.02
0.00
0.00
0
1
2
3 kd
195
4
5
6
0
1
2
3 kd
4
5
6
0.00
0
1
2
3 kd
4
5
6
Figure 9.8 For comparison, the various contributions to collective plasmon damping in the chain, for transverse polarization: the solid line corresponds to the total damping rate (in dimensionless units) 1/ω1 τx(y) = 1/ω1 τ0 +(a 3 /2d 3 )Im Fx(y) (k), and flat part of this line displays the remaining, ohmic, contribution at that part of the kperiod where all electromagnetic losses vanish; the dashed line indicates the Lorentz friction value (in dimensionless units) 13 (ω1 a/v)3 .
9.4 Plasmon–Polariton SelfModes in a Chain Propagation The real parts of the functions Fα renormalize the selffrequency of the plasmon– polaritons in the chain, while the imaginary parts renormalize the damping of these modes. Re Fα (k,ω) and Im Fα (k,ω) are functions of k and ω. For a firstorder approximation in the perturbation approach, one can put ω = ω1 in Re Fα and also in the residual nonzero Im Fα , the latter being outside the region 0 < kd ± ω1 d/v < 2π. Let us emphasize, however, that the vanishing of Im Fα (k,ω) inside the region 0 < kd ± ωd/v < 2π holds for any value of ω [44] and thus also for the exact solution for the frequency, not only for ω = ω1 . Therefore, one can rewrite the dynamic Eq. (9.20) for plasmon–polariton modes in the chain in the following form: * ) (9.30) −ω2 − i τα2(k) ω + ωα (k)2 Dα (k,ω) = εa 3 ω21 E0α (k,ω), where the renormalized attenuation rate (in the perturbation approach) is given by ⎧ ⎪ ⎨
1 = τα (k) ⎪ ⎩
1 τ0 1 τ0
for 0 < kd ± ω1 d/v < 2π, +
a 3 ω1 2d 3
Im Fα (k,ω1 )
for kd − ω1 d/v < 0
(9.31)
or kd + ω1 d/a > 2π,
and the renormalized selffrequency (in the perturbation approach) is given by a3 2 2 ωα (k) = ω1 1 − 3 Re Fα (k,ω1 ) . (9.32) d Equation (9.30) can easily be solved for both the inhomogeneous and the homogeneous (E0α = 0) cases. The general solution of Eq. (9.30) has the form of a sum
196
Plasmon–Polaritons in Metallic Nanoparticle Chains
of the general solution for the homogeneous equation and a single particular solution of the inhomogeneous equation. The first of these includes initial conditions and describes damped selfoscillations with frequency 1 1 (9.33) ωα = ωα2 (k) − 2 , τα (k) i.e., for each k and α,
Dα (k,t) = Aα,k ei(ωα t+φα,k ) e−t/τα (k),
(9.34)
where the constants Aα,k and φα,k are adjusted to the initial conditions. For the inhomogeneous case, the particular solution is as follows: 1 , Dα (k,t) = εa 3 ω21 E0α (k)ei(γ t+ηα,k ) 2 2 (ωα (k) − γ )2 + 4γ 2 /τα2 (k)
(9.35)
for the assumed single Fourier time component E0α (k,t) = E0α (k)eiγ t and tg(ηα,k ) = 2γ /τ (α,k)/(ω(α,k)2 − γ 2 ), the usual expression for a forced oscillator. Let us emphasize that E0α (k) is a real function since E0α (ld)∗ = E0α (ld) = E0α (−ld). An appropriate choice of the latter function, which in practice is a choice of the number of externally excited nanospheres in the chain, e.g., as made by a suitably focused laser beam, allows for the modelling of its Fourier picture E0α (k). This gives the envelope of the wave packet if one inverts the Fourier transform in the solution Eq. (9.35) back to the position variable. For the case of the external excitation of a single nanosphere, the wave packet envelope includes homogeneously all the wave vectors k ∈ [0,2π). The larger the number of nanospheres that are simultaneously excited, the narrower is the envelope for the k wave packet. For E0α (ld)∗ = E0α (ld) = E0α (−ld), the Fourier transform has the same properties, i.e., E0α (k)∗ = E0α (k) = E0α (−k), and the latter equality can be rewritten, owing to the periodicity 2π /d of k, as E0α (−k) = E0α (2π /d − k) = E0α (k). The inverse Fourier picture of Eq. (9.35) (its real part) has the form 2π/d dk cos(kld − γ t − ηα,k ) εa 3 ω12 E0α (k) Dα (ld,t) = 0
×
1 (ωα2 (k)
−
γ 2 )2
+ 4γ 2 /τα2 (k)
.
(9.36)
This integral can be evalued by virtue of the mean value theorem as follows: Dα (ld,t) =
2π cos(k ∗ ld − γ t − ηα,k∗ ) εa 3 ω12 E0α (k ∗ ) d 1 × . ∗ 2 2 (ωα (k ) − γ )2 + 4γ 2 /τα2 (k ∗ )
(9.37)
9.4 Plasmon–Polariton SelfModes in a Chain Propagation
197
The above expression describes undamped wave motion with frequency γ and velocity, amplitude, and phase shift determined by k ∗ . The amplitude attains its maximal value at the resonance, when 1 γ = ωα (k ∗ ) 1 −
2 (τα
(k ∗ )ω
α (k
∗ ))2
.
(9.38)
In a chain subject to a persistent timedependent electric field excitation applied to some number (even a small number) of nanospheres, one is dealing with an undamped wave packet propagating along the whole chain. Such modes depend on the particular shaping of the wave packet by the specific choice of chain excitation, which may be responsible for the experimentally observed long–range, practically undamped, plasmon–polariton propagation [169, 171, 39, 40]. The selfmodes described by Eq. (9.34) are damped, and their propagation depends on appropriately prepared initial conditions admitting nonzero values of Aα,k . These initial conditions might be prepared by switching off a timedependent external electric field initially exciting some fragment of the chain. The resulting wave packet may embrace the wave numbers k from some specified region of [0,2π). If only the wave numbers k for which 0 < kd ± ω1 d/v < 2π contribute to the wave packet, its damping is then only of ohmic type (as shown in Section 9.3). The corresponding value of 1/τ0 decreases with growing a (see Eq. (9.4)); thus, a longer range of these excitations in the chain can be obtained for larger spheres. The limiting value of 1/τ0 = vf /2λB ∼ 1013 /s gives the maximal range of propagation for these plasmon–polariton modes ∼ 0.1cτ0 ∼ 10−6 m; for the group velocity of the wave packet, we have assumed ∼ 0.1c as its maximum value (though depending on the radius and separation of the nanospheres). The group velocity, calculated for both polarizations, is presented in Section 9.5. Though the presented above analysis applies to chains consisting of ideal nanospheres, the conclusions hold also for other shaped particles and agree with the experimental observations, at least qualitatively. In [171], the propagation of plasmon–polaritons in a nanochain of Ag rodshaped particles (90 : 30 : 30 nm oriented with their longer axes perpendicular to the chain in order to enhance nearfield coupling [39], with facetoface separation of 70 nm) is evidenced by observing the luminescence of a dye particle, located in proximity to the transmitting electromagnetic signal but distant from the pointlike excitation source, over a range of 0.5 μm. The observed behaviour has been supported by finite difference time domain (FDTD) numerical simulations. Several samples of the chain were fabricated by electron beam lithography in the form of a twodimensional matrix with sufficiently wellseparated individual chains. The energy blueshift of the plasmon resonance for the nanorods in the chain in comparison with that for a single particle was observed as about 0.1 eV
198
Plasmon–Polaritons in Metallic Nanoparticle Chains
(see Fig. 4 in [171]). This agrees with our estimation of the reduced radiated losses in a chain in comparison with the strong Lorentz friction for a single metallic nanoparticle and the related smaller redshift of damped oscillations. The position of maximum resonance in the chain is located at a higher energy for the transverse polarization mode than for the longitudinal mode [170], which also agrees with the theoretical predictions. In [39] it was indicated that FDTD simulations give lower values of the group velocities for both polarizations, and higher attenuation rates, in comparison with these quantities previously estimated [170, 24] with the simplified pointdipole model with nearfield interactions only and neglecting retardation effects. Let us note, however, that the simplified approach, including only the nearfield contribution to the electric fields of the interacting dipoles, leads to an artefact, i.e., for some values of the chain parameters d and a, an instability of the collective dynamics occurs [185]. This instability is completely removed by the inclusion of the medium and farfield contributions to the electric field of the dipole and by rigorous inclusion of the relativistic retardation [44]. Nevertheless, the dipole interaction model, even if it includes, besides the nearfield contribution, the medium and farfield contributions and all retardation effects, still suffers from the absence of the magnetic field component needed for the complete description of farfield wave propagation, which might be of particular significance for ferromagnetic metallic nanochains. Moreover, as has been demonstrated in [186–188], for large separations in a metallic nanochain, the scattering of electromagnetic radiation dominates the signal behaviour in the chain, which then acts as a Bragg grating for plasmon–polaritons. For ellipsoidal Au nanoparticles (210 : 80 nm) deposited on the top of a silicon wave guide, the change of regime from collective plasmon–polariton guiding to the Bragg scattering scenario takes place for distances between nanoparticles exceeding about 1 μm [186, 188]. This proves that the dipole coupling model for a nanochain works quite well for a wide range of chain parameters, in practice up to the order of a micron for the distance between the metallic elements in the chain, which supports the qualitative argument that the Bragg grating regime is not efficient for subwavelength distances and justifies the applicability of the present model. The SNOM measurements of nearfield coupled plasmon modes in metallic nanochains [166], interpreted within the classical fieldsusceptibility formalism [187], also support the sufficiency of the dipole approximation for nanosphere radii a of order of 10−30 nm and chain separations d not exceeding ∼ 10a. 9.5 The SelfFrequencies and Group Velocities of Plasmon–Polaritons in a NanoChain According to Eqs. (9.32) and (9.33), for the selffrequencies of plasmon–polaritons in a chain one can write out their explicit form using the expressions for Fα (k,ω1 )
9.5 SelfFrequencies and Group Velocities of Plasmon–Polaritons
199
given by Eq. (9.21). The real parts of the functions Fα (k,ω1 ) renormalize the corresponding frequencies for both polarizations, and they attain the following form (still with the perturbative approach, according to Eq. (9.32)), setting x = kd and ξ1 = ω1 d/v, ! ∞ cos(mx) a 3 cos(mx) 2 2 cos(mξ1 ) + ξ1 sin(mξ1 ) ωz (k) = ω1 1 − 3 4 d m=1 m3 m2 ∞ a 3 cos(m(x + ξ1 )) + cos(m(x − ξ1 )) 2 = ω1 1 − 3 2 d m=1 m3 sin(m(x + ξ1 )) − sin(m(x − ξ1 )) , (9.39) +ξ1 m2
ω2x(y) (k)
=
ω21
= ω21
∞ cos(mx) a 3 cos(mx) cos(mξ1 ) + ξ1 sin(mξ1 ) 1 + 32 3 d m=1 m m2 cos(mx) −ξ1 2 cos(mξ1 ) m ∞ a 3 cos(m(x + ξ1 ) + cos(m(x − ξ1 )) 1+ 3 d m=1 m3
sin(m(x + ξ1 )) − sin(m(x − ξ1 )) m2 cos(m(x + ξ )) 1 + cos(m(x − ξ1 )) 2 . −ξ1 m +ξ1
(9.40) The shift in the selffrequencies of the plasmon–polaritons caused by their attenuation is accounted for by Eq. (9.33) where ωα (k) is given by Eqs. (9.39) and (9.40) and where τα (k) has the form as in Eq. (9.31). Taking into account the explicit forms for Im Fα (k,ω1 ), i.e., Eqs. (9.27) and (9.29), one can easily calculate the selffrequencies ωα (k); these functions are shown in Figs. 9.9 and 9.10 for longitudinal and transverse polarizations, respectively. Note that, for the transverse polarization, in Eq. (9.40) the sum ∞ cos(m(x + ξ1 )) + cos(m(x − ξ1 )) m=1
m
(9.41)
can be performed analytically according to Eqs. (9.25), resulting in the contribution 1 − ln[(2 − 2 cos(x + ξ1 ))(2 − 2 cos(x − ξ1 ))] 2
(9.42)
Plasmon–Polaritons in Metallic Nanoparticle Chains
z
(k) [ 1]
200
Figure 9.9 The selffrequency ωz (k) of a plasmon–polariton with longitudinal polarization in an infinite chain of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d = 3a, 4a, 5a calculated using the perturbation approach ([46]). a
a
10 nm Au
(k)
x(y)
15 nm Au
a
(1 s) 1016
(1 s) 1016 0.82
20 nm Au
(1 s) 1016
d=3a d=4a d=5a
0.82
0.81
0.80
0.80
0.80 0.79
0.78
0.78
0.76
0.77
0.75 0.70
0.74 1
2
3
4
5
6
kd
1
2
3
4
5
6
kd
1
2
3
4
5
6
kd
Figure 9.10 The selffrequency ωx(y) (k) of a plasmon–polariton with transverse polarization in an infinite chain of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d = 3a, 4a, 5a calculated using the perturbation approach. The logarithmic singularities are artefacts of the perturbation method of solution of Eq. (9.20); in the exact solution of this equation all singularities are quenched; see Section 9.6 ([46]).
(the other sums in Eqs. (9.39) and (9.40) have to be performed numerically). The logarithmic singularity in the selffrequencies for the transverse plasmon– polaritons on the rim of the region 0 < x − ξ1 < 2π (inside which radiative damping vanishes) is indicated in Fig. 9.10. This singularity causes a hyperbolic discontinuity in the transversepolarizationmode group velocity (see Fig. 9.12). Nevertheless, the logarithmic singularity in the selfenergy and the related hyperbolic discontinuity in the group velocity for transverse polarization turn out to be artefacts of the perturbation solution of Eq. (9.20). The exact numerical solution of this equation demonstrates the effective quenching of the logarithmic singularity to a small local minimum, resulting in a finite groupvelocity discontinuity, as will be shown in Section 9.6. This property of the transverse polarization mode of plasmon–polaritons in a chain, caused by interference of the farfield components of the dipole interactions between nanospheres, was analysed numerically in [43, 173] and commented on in [44]. Numerical studies of plasmon–polariton propagation in metallic nanochains [43, 173–175] indicate a mode that is very narrow and weak but long range, in addition to the wide spectrum of quickly damped modes. This ‘fainting’ longrange mode has been associated
9.5 SelfFrequencies and Group Velocities of Plasmon–Polaritons vz (m/s)
4
vz
d=3a d=4a d=5a
10 7
2 10 7 1
2
3
4
5
6
kd
– 2 10 7 – 4 10 7
vz (m/s)
201
a
20 nm Au
2
3
vz (m/s)
1 10 8
6 10 7 4 10 7 2 10 7
5 10 7 1
– 2 10 7 – 4 10 7 – 6 10 7
2
3
4
5
6
kd
1
4
5
6
kd
– 5 10 7 – 1 10 8
Figure 9.11 The group velocity vz (k) of a plasmon–polariton with longitudinal polarization in an infinite chain of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d = 3a, 4a,5a calculated with the perturbation approach; the logarithmic singularity in the perturbation formula for vz (though not in the formula for ωz ) leads to c being exceeded locally; this artefact of the perturbation approach is removed by the exact solution (see Section 9.6).
a (m s) 10 7
2 1
a
2
3
15 nm Au
(m s) 10 7
(m s) 10 7
d=3a d=4a d=5a
4
vx(y)
10 nm Au
4
4
2
2 4
5
6
kd
1
2
3
4
5
6
kd
1
–2
–2
–2
–4
–4
–4
2
3
4
5
6
kd
Figure 9.12 The group velocity vx(y) (k) of a plasmon–polariton with transverse polarization in an infinite chain of Au nanospheres with radius a = 10, 15, 20 nm and chain separation d = 3a, 4a, 5a calculated with the perturbation approach. The hyperbolic singularity is an artefact of the perturbation method of solution of Eq. (9.20); the exact solution of this equation reduces this singularity to a narrow local jump of the group velocity not exceeding c (see Section 9.6). The small asymmetry of the approximated singularities is caused by the imposition of the hyperbolic singularity and the additional logarithmic singularity of vx(y) (k) at the same point.
with constructive interference of the farfield part of the dipole–dipole interaction of the nanospheres in a chain, resulting in local enhancement of the transversepolarizationmode group velocity in the near vicinity of singularity points (on the light cone). In order to find the group velocities of particular selfmodes of plasmon– polaritons in a chain, the derivative of ωα (k) with respect to k must be obtained, which, according to Eqs. (9.31), (9.33), (9.39), and (9.40), is straightforward though involving extended calculus. The sums in the formulae for ωα (k) still cannot be performed analytically, except for the sum with denominator m in Eq. (9.40). The resulting group velocity values calculated numerically for both polarizations and for kd ∈ [0,2π) and d/a ∈ [3,10] are presented in Figs. 9.11 and 9.12 (for a = 10, 15, 20 nm for both polarizations).
202
Plasmon–Polaritons in Metallic Nanoparticle Chains
9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy The imaginary part of the complex variable ω, the solution of Eq. (9.20), defines the plasmon–polariton attenuation, while the real part of ω gives the selffrequency of these oscillations (in the case of the homogeneous equation, i.e., when E0α (k,ω) = 0). The derivative of this selffrequency with respect to the wave vector k defines the group velocity of the particular mode. Because of the logarithmic singular term in the farfield transverse contribution to the dipole interaction in the chain (x = kd and ξ = ωd/v), ∞ 1 [cos(m(x + ξ )) + cos(m(x − ξ ))] m m=1
(9.43)
1 = − ln [(2 − 2 cos (x + ξ )) (2 − 2 cos (x − ξ ))] , 2 one cannot apply the perturbation method to solve the dynamical equation, at least in the region close to the singularity (on the light cone). Note that, with the perturbation approach, one substitutes ω by ω1 (the Mie frequency) on the righthand side of Eq. (9.20). This produces, however, a hyperbolic singularity in transverse group velocity by virtue of Eq. (9.43). Moreover, with the perturbation approach, the logarithmic singularity occurs for both polarizations, which is noticeable if one takes the derivative with respect to k of Eqs. (9.39) and (9.40). All these singularities occur at isolated points for which kd ± ω1 d/v = lπ, where l is an integer. Both hyperbolic and logarithmic divergences in the perturbation formula for group velocities at this point would result in the local exceeding of c by the corresponding group velocities. To resolve the problem of these unphysical divergences, the exact solution of Eq. (9.20) must be found; because of the divergence of Eq. (9.43) the corresponding contribution cannot be treated as a perturbation any longer. An exact solution of the highly nonlinear Eq. (9.20), found numerically by use of a Newtontype procedure at 1000 points for kd ∈ [0,2π), is plotted in Figs. 9.13–9.20, for both polarizations of the plasmon–polaritons. From Figs. 9.13 and 9.15 (see also Figs. 9.16–9.19), we notice by comparison with the corresponding plots obtained with the perturbation method that, for longitudinal polarization, the exact solutions for the selffrequencies do not differ significantly from those obtained with the perturbation procedure, but the change suffices to remove the logarithmic divergence from the derivative of the selffrequency. For the transverse polarization, the difference is also not important for the attenuation plot. However, for the transverse polarization selffrequency in the case of the exact solution, we have the quenching of the logarithmic divergence (9.43), in contrast with the approximated version obtained with the perturbation approach. Instead of
9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy a = 10 nm (Au), d = 4a
a = 10 nm (Au), d = 4a
0.05
5 10 6
1.00 0.99
0.04 –Im ωx(y)
1.01
vx(y) (m/s)
Re ωx(y)
1.02
203
a = 10 nm (Au), d = 4a
0 – 5 10 6
0.03 0.02 0.01
0
200
400
600
800
0
1000
200 400 600
800 1000
0
kd (2π/1000)
200
400
600
800
1000
kd (2π/1000)
kd (2π/1000)
Figure 9.13 The exact solution for the selffrequency and the damping rate of the transverse polarization mode of plasmon–polaritons in a nanochain (ω is given in ω1 units); the solution of Eq. (9.20) was found for 1000 points on the segment [0, 2π ). In the middle, the plot for the group velocity of the transverse polarization mode is presented; it has hyperbolictype singularities corresponding to the logarithmictype singularities of the selfenergy (left) mixed with the additional logarithmictype singularity of the group velocity itself. All singularities are, however, truncated, which is visualized in the brokenline regions in Fig. 9.14 ([45]). a = 10 nm (Au), d = 4a
0.05
2 10 8
0.988 0.986 0.984
0.04 Im ωx(y)
vx(y) (m/s)
0.990 Re ωx(y)
a = 10 nm (Au), d = 4a
a = 10 nm (Au), d = 4a
0.992 1 10 8 0 –1 10 8 156
157
158
155
159
156
157
158
0.00 155
159
kd (2π/1000)
kd (2π/1000)
0.986 0.984 0.982 157.564
6 10 8 4 10 8 2 10 8 0 –2 10 8 –4 10 8 157.556
159
0.04 Im ωx(y)
vx(y) (m/s)
Re ωx(y)
158
a = 10 nm (Au), d = 4a
0.988
157.560
157
0.05
a = 10 nm (Au), d = 4a
kd (2π/1000)
156
kd (2π/1000)
a = 10 nm (Au), d = 4a
0.990
157.556
0.02 0.01
0.982 155
0.03
0.03 0.02 0.01
157.560 kd (2π/1000)
157.564
0.00 157.556
157.560 kd (2π/1000)
Figure 9.14 Twolevel magnified view of the truncated singularity region for the transverse plasmon–polariton mode in a nanochain in the exact solution of Eq. (9.20); the most enhanced scale is in the lower panels (ω is given in ω1 ).
an infinite singularity, we observe in the exact plot for the transverse polarization selffrequencies only a relatively small minimum, resulting then conveniently in a finite group velocity not greater than c. This quenching logarithmic singularity into a small local minimum is presented in Fig. 9.14 (right); on the left, the correction to the discontinuity step in the damping of the transverse mode caused by the logarithmic contribution to Eq. (9.20) is presented. The exact solution of the dynamic equation (9.20) thus resolves the problem of the risky logarithmic divergent contribution of the transverse farfield part of the dipole interaction and regularizes the final solution for the corresponding
157.564
204
Plasmon–Polaritons in Metallic Nanoparticle Chains a
10 nm Au , d
4a
a
1.04
10 nm Au , d
4a
0.035
1.02 z
z
0.030
1.00
0.025

0.98
0.020 0.015
0.96 0
200
400 kd
600 1000
800
0
1000
200
400 kd
600 1000
800
1000
Figure 9.15 The exact solution for the selffrequency and the damping of the longitudinal mode of plasmon–polaritons in a nanochain (ω is given in ω1 units) ([45]). a = 10 nm (Au), d = 4a
0.04
1.01
Im ωx(y)
Re ωx(y)
a = 10 nm (Au), d = 4a
0.05
1.02
1.00
0.03 0.02
0.99 0.01 0
200
400 600 kd (2π/1000)
800
1000
0
200
400 600 kd (2π/1000)
800
1000
Figure 9.16 The exact solution for the selffrequency and the damping of the transverse mode of plasmon–polaritons in a nanochain (ω is given in ω1 units) ([45]).
characteristics of the plasmon–polariton modes. In the vicinity of singularity points in the domain for kd, the group velocity, though still well below the velocity of light, is, however, greater than the group velocities in other regions of the k wave vector domain. This might elucidate former numerical observations [43] of the longrange propagating mode for the transversely polarized plasmon–polariton in a nanochain. In view of the above analysis, one can argue that the long range of the related mode [43] is connected to a locally higher value of its group velocity, but not to the lowering of its damping. Even though the real part of the function Fz and thus of ωz (k) (Eq. (9.39)) is given by a continuous function, the corresponding group velocity will have a logarithmic singularity, as the derivative of ωz (k) with respect to k will contain the sum [cos(m(x +ξ1 ))−cos(m(x −ξ1 ))]/m (recall that ξ1 = ω1 d/v), arising from the last term in Eq. (9.39) after taking the derivative. A similar term is also present in the perturbation formula for ωx(y) (k) in Eq. (9.40). The origin of these terms for both polarizations is the mediumfield contribution to the dipole interaction in the chain. At the points x ± ξ1 = 2πp, p integer, the logarithmic singularity again produces an
9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy
205
Transverse polarization
a = 10 nm (Au), d = 4a
0.04
1.01
–Im ωx(y)
Re ωx(y)
a = 10 nm (Au), d = 4a
0.05
1.02
1.00
0.03 0.02
0.99 0.01 0
200
400 600 kd (2π/1000)
800
0
1000
200
400 600 kd (2π/1000)
800
1000
longitudinal polarization a = 10 nm (Au), d = 4a
1.04
a = 10 nm (Au), d = 4a 0.035 0.030
–Im ωz
Re ωz
1.02 1.00 0.98
0.025 0.020 0.015
0.96 0
200
400 600 kd (2π/1000)
800
1000
0
200
400 600 kd (2π/1000)
800
1000
Figure 9.17 Exact solution for the selffrequency and damping rate of transversely (upper) and longitudinally (lower) polarized plasmon–polariton modes in a nanochain (ω is given in ω1 units). Presented is a solution of Eq. (9.20) at 1000 points in the sector kd ∈ [0,2π); in the plot for the selffrequency of the transverse mode a truncated logarithmictype singularity in the selfenergy is indicated; for longitudinal polarization the almost vertical local slope of selffrequency is indicated.
artefact whereby the group velocity vz exceeds c. This precludes the applicability of the perturbation approach, at least close to points of singularity. Therefore, instead of putting ω = ω1 in the function Fα on the righthand side of Eq. (9.16) as in the perturbation method of solution of this equation, one must solve the nonlinear equation directly, in the homogeneous case neglecting E0α . As mentioned above, this exact solution can be found numerically by a Newtontype procedure, and both the real and imaginary parts of ω can be determined, point by point, in the whole region kd ∈ [0,2π). For the longitudinal polarization of the group velocity, the exact solution is presented in Fig. 9.20. The exact solutions for vz do not exhibit any singularities: the logarithmic singularity of the perturbation term is quenched to only a small local extremum, similarly to what was demonstrated above for the transverse polarization. The logarithmictype singularity in the selfenergy of the transverse plasmon– polaritons in the chain is the feature that essentially differentiates these modes from the longitudinally polarized modes. This singularity is caused by the sum of the farfield parts of the electric fields of all the nanoparticle dipoles, which influences the charge oscillations in each component of the chain and produces a hyperbolictype discontinuity in the group velocity only for the transversely polarized modes. In addition to this discontinuity, the mediumfield component of the electric dipole
206
Plasmon–Polaritons in Metallic Nanoparticle Chains a = 10 nm (Au), d = 4a
a = 10 nm (Au), d = 4a
1.01
vx(y) (m/s)
Re ωx(y)
1.02
1.00
5 106 0 –5 106
0.99 0
200
400 600 kd (2π/1000)
800
0
1000
a = 10 nm (Au), d = 4a
vx(y) (m/s)
vx(y) (m/s)
1 108 0 –1 108 156
157 158 kd (2π/1000)
400 600 800 kd (2π/1000)
1000
a = 10 nm (Au), d = 4a
2 108
155
200
159
6 108 4 108 2 108 0 –2 108 –4 108 157.556
157.560 kd (2π/1000)
157.564
Figure 9.18 Exact solution for the group velocity of the transverse plasmon– polariton mode in a nanochain for a = 10 nm and d = 4a; the solution of the nonlinear equation (9.20) removes the logarithmic singularity – the remaining local very narrow extremes are truncated at exactly the value of c. In the near vicinity of the singular point the solution was found for more than 1000 values of kd (lower panels: magnification of the marked areas in the upper panels); the asymmetry at the singular points is caused by the imposition of hyperbolic and logarithmic truncated singularities of the group velocity for the transverse mode.
interaction produces a logarithmictype singularity in the group velocity for both polarizations (though any singularity in the selfenergy). We use here the terms logarithmictype or hyperbolictype singularity to distinguish the behaviour of the group velocities obtained by the exact solutions for the selfenergies for both polarizations, which are sharpened and truncated at c owing to relativistic constraints imposed on the dynamic equation and manifesting themselves in the form of its solution. The retardation of electric signals prohibits the collectiveexcitation group velocity from exceeding the velocity of light. This quenching concerns the infinite singularities which occur in the perturbation expressions for the selfenergy and then in the perturbation formulae for the group velocities. The relativistic invariance of the dynamic equation for collective dipole plasmon oscillations in a chain prevents, however, the group velocity of particular plasmon– polariton modes from exceeding the velocity of light. Thus, the exact solution of the dynamic equation inherently also possesses this property. Exact selfenergies have a suitably regularized dependence with respect to k, such that their derivatives do not exceed c. It is worth emphasizing, for the sake of completeness, that the inclusion of the magnetic field of the dipoles does not modify this scenario, because the magnetic field contribution to the selfenergies is at least two orders lower than the electric field contribution; the reason is that the Fermi velocity of electrons is two orders
9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy a = 10 nm (Au), d = 3a
a = 10 nm (Au), d = 3a
1.05
5 107
vz (m/s)
Re ωz
207
1.00 0.95
0
–5 107
0.90 0
200
400 600 kd (2π/1000)
800
0
1000
200
a = 10 nm (Au), d = 3a
vz (m/s)
Re ωz
0.9250 0.9245
110.2 110.4 kd (2π/1000)
1000
a = 10 nm (Au), d = 3a
0.9255
0.9240 110.0
400 600 800 kd (2π/1000)
3.0 2.5 2.0 1.5 1.0 5.0
110.6
108 108 108 108 108 107 0 110.0
110.2 110.4 kd (2π/1000)
110.6
Figure 9.19 Exact solution for the group velocity of the longitudinally polarized mode of a plasmon–polariton in a nanochain for a = 10 nm and d = 3a; the almost vertical slope of the selffrequency (righthand panels) is limited by the velocity of light (lower panels: magnification of the marked areas in the upper panels). a = 10 nm (Au) d = 3 a
0.95
0
vz (m/s)
1.00
1.02 Re ωz
5 10
7
1.00 0.98
–5 10 7
0.96
0.90 400
600
800
0
1000
200
a = 10 nm (Au) d = 3 a
vz (m/s)
0.9255 0.9250 0.9245 110.2
110.4
kd [2π/1000]
800 1000
0
kd [2π/1000]
kd [2π/1000]
0.9240 110.0
400 600
110.6
3.5 3.0 2.5 2.0 1.5 1.0 5.0
10 8 10 8 10 8 10 8 10 8 10 8 10 7 0 110.0
200
400
600
800
0
1000
200
0.9925 0.9920 0.9915 110.4
110.6
0.9910 236.4
236.8
237.2
3.0 2.5 2.0 1.5 1.0 5.0
10 8 10 8 10 8 10 8 10 8 10 7 0 236.4
236.8 kd [2π/1000]
kd [2π/1000]
Figure 9.20 The exact solution for the group velocity vz of the longitudinal mode of plasmon–polaritons in a nanochain for a = 10 nm and d = 3a,4a, respectively, and the corresponding exact solutions for Re ωz (left). The exact solution of the dynamic equation (9.20) removes the logarithmic singularity in the group velocity. The remaining local very narrow extremes are truncated exactly at c (in close vicinity to the singular points, the solution was found for more than 1000 points kd. In the bottom panels, the plots correspond to the marked regions in the upper panels at an enhanced scale).
lower than the velocity of light, which significantly reduces the Lorentz force. Therefore, the magnetic field of the dipoles [55, 76], ik 1 − 2 eikr0 , Bω = ik(Dω × n) r0 r0
600
800 1000
a = 10 nm (Au) d = 4 a
0.9930
kd [2π/1000]
400
kd [2π/1000]
a = 10 nm (Au) d = 4 a
a = 10 nm (Au) d = 3 a
110.2
6 10 7 4 10 7 2 10 7 0 –2 10 7 –4 10 7 –6 10 7
kd [2π/1000]
vz (m/s)
200
Re ωz
0
Re ωz
a = 10 nm (Au) d = 4 a
1.04 vz(m/s )
Re ωz
a = 10 nm (Au) d = 4 a
a = 10 nm (Au) d = 3 a
1.05
(9.44)
237.2
208
Plasmon–Polaritons in Metallic Nanoparticle Chains
though contributing to the farfield and mediumfield parts of the plasmon– polariton selfenergies does not significantly change the similar terms due to the electric field and leads to corrections that are two orders lower and thus practically negligible. It must be emphasized, however, that the role of the magnetic field may change considerably in the case of magnetictype metallic chains. If a ferromagnetic material is used to prepare the chain components, one can expect a strengthening of magnetic effects in the surface plasmon collective dynamics for the chain. Thus, the consideration presented, while appropriate for noble metals, need to be lifted to much more complicated magnetoplasmonics for magnetic metals. This is, however, beyond the scope of the present treatise. The distinction between the truncated singularities in the group velocities for transverse and longitudinal polarizations of plasmon–polaritons as demonstrated above sheds light on the discussion of longrange plasmon–polariton modes in metallic nanochains studied by numerical simulations with the Green function method for differential equations [173, 176, 174]. The truncated singularities in group velocities indicated above, i.e., the very narrow logarithmictype truncated singularity for the longitudinal polarization and the wider hyperbolictype singularity superimposed on a narrow logarithmictype truncated singularity for the transverse polarization, facilitate an understanding of the peculiarities of numerical studies. The longrange propagation of narrow modes observed in numerical simulations might be linked to the local enhancement of the group velocity of kmodes in singular regions. In simulations [43, 174, 173] it has been assumed that a single selected nanosphere in the chain is initially excited and then the range of propagation for various modes of plasmon–polaritons is observed. A pointlike initial excitation corresponds in the Fourier picture to a uniform excitation of all kmodes, including those in singular regions. The different character of the truncated singularities, being originally infinite divergences in the perturbation series, for the longitudinal and the transverse polarizations results in different features in the corresponding modes (the local narrowing of the group velocity curve is stronger for the longitudinal polarization). Even though the group velocity singularities are truncated at the finite v = c level in different fashions for the transverse and the longitudinal polarizations, the local narrow extrema give the same longrange propagation of closely located modes for both polarizations (about two orders of magnitude longer than for the nonsingular modes). Summarizing, one can state that in infinite metallic nanochains, a longrange propagation of plasmon–polariton selfmodes can be observed, due to the effectively ideal compensation of the Lorentz friction losses in a particular nanosphere by the energy income from other nanospheres in the chain; this takes place for both polarizations of the collective plasmon modes in a relatively large part of the wave vector k domain (diminishing with increasing d/a). In the case of an inho
9.6 Exact Solution of Eq. (9.20) for the Plasmon–Polariton SelfEnergy
209
mogeneous equation version of Eq. (9.20) (i.e., when a term of persistent external forcing is added to its righthand side, i.e., εa 3 ω21 E0α (k,ω), where ε is the dielectric permittivity of the chain surroundings and E0α (k,ω) is the external electric field Fourier component), one can expect the completely undamped propagation of the induced plasmon–polaritons corresponding to the forced oscillator properties. Both the low (only ohmic) attenuation of the selfoscillations and the possibility of exciting appropriately formed (by persistent excitation of some part of the chain) wave packets of plasmon–polariton modes in the chain may be responsible for the experimentally observed practically undamped propagation of the collective plasmon signal over relatively large distances in nanochains of lengths equal to several micrometres. It should be noted that the almost undamped propagation of surface plasmon– polaritons along metallic nanochains was first analysed by Markel and then developed by Citrin and, more recently, by other authors. They all tried to solve the problem of plasmon–polariton propagation within the dipole model of particle interactions. This makes the issue relatively simple and clearly formulated, i.e., the corresponding dynamic equation is a linear differential equation and it can be solved using various techniques. Nevertheless, some methods may not have been transparent and additionally may have complicated the solution and interpretation. In the present scheme, we have solved the linear differential equation by a standard technique, that of the Fourier transform (a continuous transform (CFT) in the time domain and a discrete transform (DFT) in the position domain, clearly linking with the problem definition for the periodic chain). All the analysis has been completely and transparently presented, mainly in an analytical manner. This is the basic value of this approach for a wave representation close to the experimental interpretation. Other approaches (e.g., the Z transformation method with the Green function method) give similar results. Unfortunately, none of the methods allowed for a full analytical solution and in each approach some numerical procedure had been applied. As is common in differential equation theory, some small uncertainties in a singular region can cause misleading conclusions. The effective numerical solution for the dispersion may thus have some inherently approximate character connected to the necessary procedure for cutting the infinite series in the numerical treatment. The solution for the Fourier transform of the initial differential equation is transparent in this regard and exhibits some singular points (corresponding to the constructive interference for transversely polarized plasmon–polaritons due to the farfield radiation on the light cone). This singularity is visible in all formulations because of the logarithmic divergence of the infinite sum of − cos(nx)/n. Various conclusions related to this singularity may be formulated, however, but not all are correct, especially if they use perturbative calculus, as directly demonstrated in the present discussion. The only way to resolve this problem is to solve the underlying equation exactly. An exact solution means here a solution of the nonlinear
210
Plasmon–Polaritons in Metallic Nanoparticle Chains
equation with respect to the Fourierargument algebraic equation point by point. For singularity points all methods agree, even approximate ones. Special attention must be given, however, to the group velocity, which in the framework of the Fourier transform above presented can be explicitly expressed and studied, revealing further sources of singularities: hyperbolic for the transverse polarization (caused by the farfieldzone dipole radiation) and an additional logarithmic singularity (caused by the mediumfieldzone radiation for both transverse and longitudinal polarizations). These singularities are hard to notice in numerical experiments, possibly owing to the slight confusion caused by the application of the unavoidable approximation methods of numerical calculus. Resolving the artefact is thus unclear and might cause doubt. The aim of our presentation is to demonstrate directly the character of the abovementioned singularities in a transparent and highly analytical manner. The singularities in the solution of the differential equation have been explicitly demonstrated as being caused by perturbation methods. Moreover, an exact solution of the problem has been described, free of all nonphysical singularities. It might be emphasized that such a level of transparency is not achieved with other techniques where the problem of singularities is not solved in a final manner. Therefore, a complete and transparent solution of the same initial problem is a novel and important contribution to the debate on plasmon–polaritons in metallic nanostructures.
9.7 Collective PlasmonWaveType Propagation along a NanoChain; NearFieldZone Approximation In the case of a metallic nanochain one has to take into account the mutual effects of the nanospheres in the chain. Assuming that in a sphere located at the point r we have a dipole D(t), then at a point r0 (where the vector r0 is drawn from the tip of r) this dipole causes electric and magnetic fields in the following form (including electromagnetic retardation) [55, 76]: for the ωFourier component of the electric field we have (ω/c)2 iω/c 1 + 2 − 3 eiωr0 /c Eω = Dω r0 r0 r0 (9.45) 2 (ω/c) i3ω/c 3 iωr0 /c + n0 (n0 · Dω ) − − + 3 e r0 r02 r0 and for the magnetic field Fourier component we have iω/c 1 Bω = (iω/c)(Dω × n0 ) − 2 eiωr0 /c, r0 r0
where n0 = r0 /r0 .
(9.46)
9.7 NearFieldZone Approximation
211
9.7.1 NearFieldZone Approximation of the Dipole Interaction in a Chain To examine the role of the terms corresponding to the nearfield zone (denominator with r03 ), the mediumfield zone (denominator with r02 ), and farfield zone (denominator with r0 ), let us first confine ourselves to the nearfieldzone dipoletype coupling. In this approximation there is only an electric field and its form is given by the static dipolefield formula: 2
3 E (r,r0,t) = r13 3n0 n0 · D r,t − rc0 − D r,t − rc0 . (9.47) 0 This allows us to write out a dynamical equation for plasmon oscillations for each nanosphere of the chain; the nanospheres will be numbered by integer l (d will denote the separation between nanospheres, d > 2a; the vectors r and r0 are collinear if the origin is associated with certain nanospheres in the chain). Note additionally that, as follows from numerical studies [41, 182], the dipole approximation for the plasmon interaction in the nanosphere chain is sufficiently accurate for d > 3a, when the multipole interaction contribution can be neglected. This dynamical equation attains the form,
∞ 3 Rα md,ω1 t − ω1 dl−m a c R¨ α (ld,ω1 t) + Rα (ld,ω1 t) = σα 3 d m=−∞,m=l l − m3 (9.48) 2 ˙ e Rα (ld,ω1 t) + − Eα (ld,ω1 t) , τ 0 ω1 maω1 2 where Rα (ω1 t) = Dα (ω1 t/ω1 )/(eNe a), the dots indicate derivatives with respect to dimensionless time t = ω1 t and −1 for α = x(y), σα = 2 for α = z, is introduced to distinguish the two oscillation polarizations. Thus the index α enumerates the polarizations, longitudinal and transverse, with respect to the chain orientation (the z axis). The first term of the righthand side in Eq. (9.48) describes the dipoletype coupling in the nearfield zone between nanospheres and the other two terms correspond to contributions due to plasmon attenuation (including the Lorentz friction linear term, which can be accounted for as described in the previous section). Note that a similar approach, but including only the nearfield dipole coupling in the chain, was utilized by the Atwater group [39, 24]. The summation in the first term on the righthand side of Eq. (9.48) can be explicitly performed in the manner presented in [185], if one changes to a wavevector picture, taking advantage of the chain periodicity in analogy to the Bloch states in crystals with the quasimomentum reciprocal lattice, i.e., Rα (ld,t) = Rα (k,t) e∓ikld ,
0≤k≤
2π , d
(9.49)
212
Plasmon–Polaritons in Metallic Nanoparticle Chains
where ∓k correspond to the two possible orientations of the phase velocity (the time factor is assumed to be e−iωt−t/τ ). Thus, Eq. (9.48) can be rewritten in the following form (the Lorentz friction term is represented in the same way as in Eq. (6.22)), R¨ α (kα,tω1 ) + ω˜ α2 Rα (kα,tω1 ) = −2R˙ α (kα,tω1 ) τα1ω1 ,
(9.50)
where 2
a3 ωp d = = 1 − 2σα 3 cos(kα d) cos √ , d c 3 3 1 ωp a 1 1 σα = + + √ τ α ω1 τ 0 ω1 3 12 c 3 2 a 3 ωp d π πkα d (kα d)2 . + σα 3 − + √ d 6 2 4 c 3
ω˜ α2
ωα ω1
(9.51)
(9.52)
Formula (9.52) expresses the attenuation rates for both polarizations. The two components of Eq. (9.52), for α = x(y) and z, give these damping rates explicitly and one notices a remarkable property, that the effective attenuation rates can change their sign depending on the values for d, a, and k. In Fig. 9.21 the regions of negative value for damping rates are marked for both polarizations. These regions shrink with the growth of d/a and with the growth of a itself. For a larger than some critical value, these regions disappear; the longitudinal modes for a > 35 nm and the transverse modes for a > 48 nm, for Au nanospheres.
d/a=3
d/a=4
Au chain
a (nm)
Figure 9.21 The regions with negative values of damping rates for plasmon– polaritons in a chain (for longitudinal polarization and also for transverse polarization) when only nearfield dipole coupling between the nanospheres is included. The regions shrink with growth in d/a, for the longitudinal (transverse) modes for d/a > 6 (7). The regions completely disappear for the longitudinal modes for 3.5 > a > 35 nm and for the transverse modes for 3.5 > a > 48 nm (for Au nanospheres).
9.7 NearFieldZone Approximation
213
Using Eqs. (9.51) one can calculate the group velocity of the plasmon–polariton mode wave packet in the nearfield coupling approximation: vα =
σα a 3 sin(kd) cos (ω1 d/c) dωα . = ω1 dk d 2 1 − 2σα (a 3 /d 3 ) cos(kd) cos (ω1 d/c)
(9.53)
From this formula it follows that the group velocity of the undamped or damped wavetype collective plasmon excitation may attain different values depending on a, d, and k, as is depicted in Fig. 9.22 (upper). With increasing a, this velocity grows Dispersion of plasmonpolaritons including only nearfield dipole coupling 5 5 3
(
(
)
)
3
d/a kd
d/a
kd
(
(
)
)
Dispersion of plasmon–polaritons including near, medium, and farfield coupling
5
kd
5
kd d/a
d/a 3
3
a = 10 nm Longitudinal
Transverse
Figure 9.22 The dispersion of plasmon–polaritons in a chain for both polarizations; upper) with the inclusion of only nearfield coupling, and (lower) with all near, medium, and farfield coupling.
214
Plasmon–Polaritons in Metallic Nanoparticle Chains
Group velocity (nearfield coupling) 5
5
3
(
(
)
)
3
kd
d/a
d/a
kd
Group velocity (near, medium, farfield coupling) 5
d/a
(
)
)
3
(
5
d/a kd L
a = 10 nm
kd
3
Transverse
Figure 9.23 The group velocity for both polarizations; with inclusion of only nearfield coupling (upper), and with all near, medium and farfield coupling (lower).
proportionally and diminishes with the separation of the nanospheres as (d/a)−2 . In Fig. 9.23 (upper) the dispersion of the collective plasmons in a chain in the same nearfield coupling approximation is plotted versus the wave vector and the separation of the nanospheres (for Au nanospheres with radius a = 10 nm). For positive attenuation rates one can expect ordinary damped plasmon– polariton propagation, while for negative damping rates the solution behaves differently, revealing the instability of the linear theory. A negative value of the damping rate, indicating an instability of the system, is, however, an unphysical artefact of the model, in view of energy conservation constraints. In other words, the continuous losses of plasmon oscillation energy due to scattering and radiation
9.7 NearFieldZone Approximation
215
is instantly recovered by the electromagnetic influence of the other nanospheres in the chain. When this income overcomes the losses then the wave packet for the corresponding modes would propagate without damping. The nearfield coupling model admits such an unphysical scenario for losses lower than a certain threshold. For nanospheres that are too small, with radii lower than about 3.5 nm for Au particles, depending on the constant C in the formula for the scattering damping rate, the scattering attenuation on the particle boundaries, ∼ CvF /(2aω1 ), is too √ 3
high; similarly, the radiation losses, ∼ 1/3 + σα /12 ωp a/c 3 , are above the required threshold, a > 35 (48) nm, for the longitudinal (transverse) modes. Thus, outside the regions 3.5 < a < 35 (48) nm, undamped longitudinal (transverse) modes in the nearfield coupling approximation do not occur regardless of the separation in the relative chain. The relative chain separation, d/a, also influences the range of undamped propagation; this is illustrated in Fig. 9.21. 9.7.2 Medium and FarField Corrections to the NearField Dipole Interaction The instability described above in the nearfield coupling approach indicates that other effects, essential for plasmon–polariton attenuation, have not been taken into account. The required correction can be linked with the dipole influence of other nanospheres assumed previously in the form (9.47). To rectify this instability of the nearfield zone approach, the mediumfieldzone and farfieldzone contributions must be taken into account. Thus, using formula (9.45), one arrives at an interdipole interaction contribution to the oscillator equation for the lth nanosphere: e∓ikld e−iωt e−τ t Rα (k)a 3
∞
e±iknd (F1 (n) + iF2 (n))einωd/c
(9.54)
cos(knd) (F1 (n) + iF2 (n))einωd/c,
(9.55)
n=−∞,n=l
or e∓ikld e−iωt e−τ t Rα (k)2a 3
∞ n=1,n=l
where
⎧ (ω/c)2 1 ⎪ ⎪ ⎪ ⎨ nd − n3 d 3 F1 = ⎪ 2 ⎪ ⎪ ⎩ n3 d 3
for α = x(y), (9.56) for α = z,
216
Plasmon–Polaritons in Metallic Nanoparticle Chains
and
⎧ ω/c ⎪ ⎪ ⎨ 2 2 n d F2 = 2ω/c ⎪ ⎪ ⎩− 2 2 n d
for α = x(y), (9.57) for α = z.
Employing the above formulae one can write out the contributions to the real and imaginary parts of the dynamical equation, which give corrections to the frequency ωα and to the damping rate τα , respectively, setting x = kd and ξ = ωd/c, 2a 3 n cos(nx) F1 cos(nξ ) − 2a 3 n cos(nx) F2 sin(nξ ), (9.58) −2a 3 n cos(nx) F1 sin(nξ ) − 2a 3 n cos(nx) F2 cos(nξ ). These contributions to the frequency of the plasmon–polariton oscillations and to the corresponding damping term have the following explicit forms: For the case of longitudinal polarization (α = z), the corrections to the frequency and to the damping rate are ! 2 2ω/c cos(nx) 3 3 cos(nξ ) + 2 cos(nx) 2 2 sin(nξ ) (9.59) a3 2 nd nd n n and a 3 −2
n
! 2 2ω/c cos(nx) 3 3 sin(nξ ) + 2 cos(nx) 2 2 cos(nξ ) . nd nd n
(9.60)
For the case of transverse polarization (α = x(y)), the corrections are ! (ω/c)2 ω/c 1 3 cos(nx) cos(nx) 2 2 sin(nξ ) a 2 − 3 3 cos(nξ ) − 2 nd nd nd n n (9.61) and a 3 −2
n
! (ω/c)2 ω/c 1 cos(nx) cos(nx) 2 2 cos(nξ ) . − 3 3 sin(nξ ) − 2 nd nd nd n
(9.62) To proceed with estimating these contributions to the oscillator equation, one can apply the iterative perturbation method of solution, which in the first step amounts to substituting ω by the free frequency ω1 on the righthand side of the osillatory equation. The sums in the formulae for the damping ratio contributions can be performed accurately [184] (for an arbitrary ω, including ω = ω1 ). As a result one obtains, for kd − ω1 d/c > 0 and kd + ω1 d/c < 2π , the following.
9.7 NearFieldZone Approximation
217
Table 9.2 Nanosphere parameters assumed for calculation Material is Au Bulk plasmon energy Bulk plasmon frequency Mie dipole plasmon energy Mie frequency Constant in Eq. (9.4) Fermi velocity Bulk mean free path
hω ¯ p ωp hω ¯ 1 √ ω1 = ωp / 3 C vF λb
8.57 eV 1.302 × 1016 /s 4.94 eV 0.752 × 1016 /s 1 1.396 × 106 m/s 53 nm
For the case of transverse polarization, ! a 2 ) ω1 a * π 2 a ) ω1 a *2 ω1 d (kd)2 1 ω1 d 2 + 2 − πkd + + d c c d c 3 2 6 c ! a 2 ) ω1 a * π 2 (kd)2 1 ω1 d 2 (9.63) − 2 − πkd + + d c 3 2 2 c ) ω a *3 1 ) * 3 2 ω1 a 1 = − (ω1 a/c)3 = . c 3 3 c For the case of longitudinal polarization, 2 a3 π ω1 d (kd)2 1 2 − 32 − πkd + + (ω1 d/c) d c 3 2 6
2 * 2 ) 2 ω1 a a π (kd) 1 2 (9.64) + 22 − πkd + + (ω1 d/c) d c 3 2 2 2 ) ω1 a *3 . = 3 c (Note again that in the above formulae substituting ω1 by ωα gives the accurate form.) We see that for both polarizations the instability has disappeared (i.e., the contribution to the damping rate does not change sign, in contrast with the case of the sole nearfieldzone contribution [185]). The imaginary term with denominator r 2 (for transverse polarization, a real term with denominator r also contributes) exactly cancels the previous unstable contribution of the real term with denominator r 3 . Simultaneously, the Lorentz friction 2/(τ ω1 ) = (2/3) (ω1 a/c)3 ) is completely cancelled by the contribution calculated above to the energy income from other nanospheres in the chain; this occurs for both polarizations but only when kd − ω1 d/c > 0 and kd + ω1 d/c < 2π , as illustrated in Fig. 9.24. In other words, plasmon–polaritons do not radiate energy and any dissipation of energy is due only to electron scattering – this confirms the previous numerical observations
218
Plasmon–Polaritons in Metallic Nanoparticle Chains
Longitudinal
Transverse
Figure 9.24 The region with completely quenched radiative losses of plasmon– polaritons (left), damping rates beyond the pure scattering contribution (i.e., 1 1 τα ω1 − τ0 ω1 ) for both polarizations (centre and right); near, medium, and farfield dipole coupling included. The small oscillations in the graph for transverse polarization are caused by the slowly convergent sum i sin(ix)/ i; 300 elements of this sum were taken. The sum also gives a discontinuous finite step on the radiatively undamped region border.
[41, 43, 168]. This cancellation of the radiation losses is exact in the first step of the iterative perturbation procedure, when in both terms, corresponding to Lorentz friction and to the energy income from other nanospheres, the frequency is taken as as ω1 . In order to answer the question whether this perfect quenching of radiation holds in general, i.e., for a resonance frequency in the chain ωα , it can be seen that the accurate energy income is still given by Eqs. (9.63) and (9.64), with ω1 changed for ωα . Simultaneously, the linear part of the Lorentz friction attains the exact form, (2/3) (ωα a/c)3 (due to the equality ∂ 3 Rα /∂t 3 = −ωα2 ∂Rα /∂t, which is satisfied for Rα ∼ e−iωα t ; the third cofactor with ωα in the expression for the Lorentz friction results from 1/τα = ωα /(τα ωα )). Thus one can argue that the cancellation is perfect in this case also. In this way the propagation of plasmon–polaritons along a discrete metallic nanostructure (the chain) resembles the wellknown phenomenon of plasmon– polariton propagation on the twodimensional interface between metal and dielectric [1, 5, 6]. The radiatively undamped propagation of plasmon–polaritons along a chain is a similar behaviour, associated with the concentration of electromagnetic energy along the chain and with group velocity about one order lower than c. All these properties are illustrated in Figs. 9.23–9.24, for the parameters listed in Table 9.2. The metallic nanochain thus behaves like an ideal wave guide for plasmon–polaritons in a way that is suitable for the arrangement of subdiffraction circuits. One can also calculate the group velocity for both polarization modes. In approximate form, taking only the first term of the quickly convergent sums with
9.7 NearFieldZone Approximation
219
denominators n3 and n2 but taking accurately the singular farfieldzone term, one can rewrite the dispersion relations in the perturbation approximation as follows; setting x = kd and ζ1 = ω1 d/c, 1/2 a3 a 2 ) ω1 a * , (9.65) cos(x) sin(ζ1 ) ωz = ω1 1 − 4 3 cos(x) cos(ζ1 ) − 4 2 d d c a3 a 2 ) ω1 a * ωx(y) = ω1 1 + 2 3 cos(x) cos(ζ1 ) + 2 2 cos(x) sin(ζ1 ) d d c 1/2 a 1 ) ω1 a *2 + ln[4(1 − cos(x + ζ1 ))(1 − cos(x − ζ1 )] . d2 c
(9.66)
The group velocities thus attain the forms vz =
∂ωz ∂k
= ω1
2(a 3 /d 2 ) sin(x) cos(ζ1 ) + (2a 2 /d) (ω1 a/c) sin(x) sin(ζ1 )
, 1 − (4a 3 /d 3 ) cos(x) cos(ζ1 ) − (4a 2 /d 2 ) (ω1 a/c) cos(x) sin(ζ1 ) (9.67) vx(y) =
E ∂ωx(y) = ω1 √ , ∂k F
where a3 a 2 ) ω1 a * sin(x) cos(ζ ) − sin(x) sin(ζ1 ) 1 d2 d c
a ) ω1 a *2 sin(x + ζ1 ) sin(x − ζ1 ) , + + 2 c 1 − cos(x + ζ1 ) 1 − cos(x − ζ1 ) a3 a 2 ) ω1 a * F = 1 + 2 3 cos(x) cos(ζ1 ) + 2 2 cos(x) sin(ζ1 ) d d c a 1 ) ω1 a *2 ln[4(1 − cos(x + ζ1 ))(1 − cos(x − ζ1 )]. + d2 c E =−
(9.68)
The above expressions are substituted for Eq. (9.53) when the nearfieldzone contribution, the medium and farfieldzone contributions are included. Worth noticing is the hyperbolic singularity in the group velocity formula for transverse polarization, induced by the logarithmic singularity due to the farfieldzone constructive interference of the fields of all particles in the chain. This local increase in the velocity is probably responsible for the longrange fainting mode of plasmon–polariton propagation, discussed previously, in a scenario when a selected single nanosphere is excited [43, 189, 182]. In that case the numerical analysis indicated a longrange signal. Remarkably, the damping
220
Plasmon–Polaritons in Metallic Nanoparticle Chains
rate was not small for this singular mode. According to our approach, at the singular point of dispersion the corresponding damping rate is not singular but grows rapidly (a discontinuous finite jump), see Fig. 9.23. Thus one may suspect that the longrange propagation of local modes noticed numerically corresponds to group velocity enhancement, as presented in Fig. 9.24 (the range of signal propagation is of the order of the damping time multiplied by the group velocity of a particular mode). As the singular point is isolated, the corresponding mode is decaying and is probably impossible to excite in practice, since for each realistic wave packet the summed contributions from both sides of the hyperbolic singularity will cancel, thus reducing the local increase in the wave packet velocity. This seems to be in agreement with experiment, where only wave packets that are not too sharply abrupt in wavevector space are attainable. The above analysis of the isolated logarithmic singularity in the transverse modes also explains the observation [43] that a finite length of the chain quenches the longrange propagating mode. It is clear why this is so, as the finite sum is not divergent and reduces the local increase in the group velocity. At the same time, all other details of the dispersion and of the damping rate for both polarizations are robust against any shortening of the chain, which agrees with other numerical studies [41, 168]. Nevertheless, again for the transverse mode, the exact quenching of radiation losses requires the contribution of an infinite number of farfieldzone terms. However, even for a relatively short chain of about 10 nanospheres only small discrepancies occur in the vicinity of boundaries of the nonradiative range defined by kd − ω1 d/c = 0 and kd + ω1 d/c = 2π . For other details the difference between an infinite number of terms and about 10 terms is negligible. With regard to the group velocity one can observe its dependence on the chain geometry – the nanosphere radius and chain separation. With increasing radius a the amplitude of the velocity also grows, while it diminishes with enhancement of the separation d. For d/a exceeding about 8 the energy dispersion is almost flat and in this band landscape the only features are singular lines for the transverse modes (in the coordinates kd and d/a) repeating owing to the periodicity, see Fig. 9.25. For such flat bands the group velocity is almost zero except in the vicinity of the singular points. This explains the numerical observation [43] that the longrange modes manifest themselves especially distinctly in the case of large separations in the chain. Finally let us note that in practice we are usually dealing with finite chains. However, the quick convergence of the sums relating to the interaction contribution to the dipole on a particular nanosphere caused by other nanospheres in the chain, even for a relatively small number of spheres (10) in the chain, gives almost the same result as that for an infinite number of spheres; see Figs. 9.26 and 9.27.
9.7 NearFieldZone Approximation
221
(
(
)
)
a = 15 nm
Figure 9.25 Flattening of energy dispersion with growth in chain separation; for d/a exceeding about 6, the only features are the singularity lines for the transverse band, repeating owing to the periodicity; for larger a the flattening begins at larger d/a.
–
–
–
–
–
–
– –
–
–
cos(nx)/n
sin(nx)/n
First 10 terms only
∞ 1 Figure 9.26 The sum n=1 cos (nx) / n = − 2 ln [ 2 ( 1 − cos (x)) ] (left), ∞ n=1 sin(nx)/n = (π − x)/2 for 0 < x < 2π (centre); the same sum with only the first 10 terms (right).
Furthermore, the singularities described above in the dynamic equation caused by the constructive interference of the dipole radiation in the far and mediumfield zones disappear for a finite chain. 9.7.3 Nonlinear Corrections to the Lorentz Friction Besides the main contribution to the Lorentz friction field (9.9), there are some small nonlinear corrections to this field, which turn out to be important for collective plasmon propagation in metallic arrays.
222
Plasmon–Polaritons in Metallic Nanoparticle Chains
– – –
–
–
–
–
–
–
3
sin(nx)/n –
2
2
cos(nx)/n –
3
x/6 + x /4 – x /12
2
/6 + x
x /4
– – –
–
–
–
–
–
–
First 2 terms only
First 2 terms only
∞ 3 2 2 3 Figure 9.27 The sums n=1 sin(nx)/n − π x/6 + π x /4 − x /12 (left), ∞ 2 2 2 n=1 cos(nx)/n − π /6 + π x/2 + x /4 (right); lower panels the same sums with only the first two terms included.
For a metallic nanosphere with its centre located at R0 , the electric dipole of the electrons (the fluctuation in electron density beyond the uniform distribution compensated by positive jellium) equals (9.69) D(R0,t) = e δρ(r,t)rd 3 r. V
This dipole√corresponds to surface plasmons and oscillates with the Mie frequency ω1 = ωp / 3, where ωp is the bulk plasmon frequency. These plasmons are not persisting excitations; they are damped owing to scattering phenomena, with damping rate 1/τ0 = vf /2λB + CvF /2a and also owing to radiation losses. For large nanospheres the most effective mechanism of plasmon damping is the radiation energy losses, which, as described above, for the case of radiation from the farfield zone can be expressed by the Lorentz friction [77, 55]. Assuming quasiclassically that electrons in the nanosphere have positions ri and e assuming a static jellium, the dipole of the nanosphere, D(R0,t) = e N i=1 ri = Ne eNe re (t); here re = i=1 ri /Ne is the mass centre of the electron system and Ne is
9.7 NearFieldZone Approximation
223
the number of electrons in the nanosphere. In the dynamic case, the velocity of the e mass centre ve = N i=1 vi /Ne . In order to determine the nonlinear corrections to Eq. (9.9) one can write down the Lorentz friction force acting on a charge eNe located at the mass centre re (t), expressed in an invariant form [55]: 2 ! 2 d u 2 dU j −u , j = 1, . . . ,4, (9.70) fL = (eNe )2 3 ds 2 ds where ds = cdt 1 − ve2 /c2 , ⎧ ve ⎪ ⎪ ⎨ u = (c1 − v 2 /c2 ) e Uj = , i ⎪ ⎪ ⎩ u4 = 1 − ve2 /c2
Uj2 = −1.
Up to terms of order ve2 /c2 with respect to the main term, one can write down an electric field equivalent to the Lorentz friction force: fL eNe
2 1 d 2 ve 1 3 d 2 ve 2 dve dve d 2 ve ve · + ve ve · . = (eNe ) 3 + 2 v +3 3 c dt 2 c 2 dt 2 e dt dt dt 2 (9.71)
EL (t) =
˙ ) = Next, using the dimensionless variables t = tω1 , R(t ) = re (t)/a,... R(t ¨ ) = d 2 re (t)/aω12 dt 2 = dve /aω12 dt, R (t ) = dre (t)/aω1 dt = ve /aω1 , R(t 3 2 2 d ve (t),aω1 dt (the dots indicate derivatives with respect to t ), one can write out the dynamical equation in a convenient form. Taking into account that the dipole corresponding to surface plasmons, D = eNe aR,
(9.72)
satisfies an equation of oscillatory type, one can write out that equation in the following form (incorporating also the Lorentz friction force), 0 .. 2 . 2 ωp a 3 ... ωp a 2 √ R+R+ R= R+ √ τ 0 ω1 3 3c 3c
.. . .. . . ... 3 ... . . × R (R · R) + 3 R (R · R)+ R (R · R) . 2 (9.73)
224
Plasmon–Polaritons in Metallic Nanoparticle Chains
The terms on the righthand side of the above equation describe the Lorentz friction including relativistic nonlinear corrections (in the square brackets) beyond the ... ordinary main linear term ∼ R, as previously given by (9.9). √ 3 For the case when 1/τ0 ω1, ωp a/c 3 1 (fulfilled for nanospheres with radii 5−50 nm for Au or Ag), one can apply the perturbation method of solution, ¨ + R = 0. In the next perturbation step one thus and at zero ..order one can... set R . substitutes R= − R and R= − R in the righthand side of Eq. (9.73). Nonlinear Correction to Plasmon Radiation Losses of Single Nanosphere Let us consider first a single metallic nanosphere with dipoletype surface oscillations with dipole D. The oscillatory dynamical equation for the dipole, Eq. (9.73), at the first order of perturbation attains the following form (it includes the damping of plasmons due to scattering at a rate 1/τ0 and due to radiation losses coming from the linear term of the Lorentz friction while the righthand side of Eq. (9.74) below expresses the nonlinear corrections): 3 ! 5
ω ω a a 5 2 2 2 p p ¨ +R+ ˙ R ˙ ·R ˙ + 3R R ˙ ·R . ˙ = − R + R R √ √ τ 0 ω1 3 3 2 3c 3c (9.74) The above nonlinear differential equation can be solved by application of the asymptotic method, as described in [190]. According to this method, one finds the solution of Eq. (9.74) in the following form (R = Rr/r): R(t) = √
A0 e−t/τ
1+ 98 γ A0 2 (1−e−2t/τ )
cos(ω1 t + θ0 ),
(9.75)
where A0 and θ0 are adjusted to the initial conditions, 1 1 ωp a 3 1 ωp a 3 1 = + ≈ √ √ τ ω1 τ 0 ω1 3 3 3c 3c ) √ *5 (which is satisfied for a larger than ∼ 15 nm) and γ = τ ω1 (1/3) ωp a/ 3c . From the form of the equation for 1/τ ω1 it follows that 1/τ ω1 is always positive. The scattering term, 1/τ0 = CvF /2a + vF /2λB , is negligible (for nanosphere radii beyond ∼ 15 nm) in comparison with the linear contribution of the Lorentz friction, as is demonstrated in Fig. 9.28. The scale of the nonlinear corrections is given by the coefficient γ ≈ 7.3 × −4 10 (a (nm))2 . As this coefficient is small, one can neglect the related contribution in the denominator of the solution (9.75), which results in an ordinary linear solution for damped oscillations. This means that the nonlinear corrections to the
9.7 NearFieldZone Approximation
225
Nanosphere radius a (nm)
Figure 9.28 Contributions to the damping rate of surface plasmon oscillations in the nanosphere versus nanosphere radius, including the scattering attenuation (∼ vF /(2λB ) + CvF /(2a)) (the dotted line) and the Lorentz friction damping, ∼ a 3 (dashed line). For radii greater than ∼ 15 nm the second channel dominates the overall damping (upper line). A logarithmic scale for the attenuation ratio has been used.
Lorentz friction have no significance in the case of plasmon oscillations of a single nanosphere. This situation changes, however, in the case of a collective plasmon excitation propagating along a metallic nanochain, as will be described in the following subsection. 9.7.4 Nonlinear Correction to the Radiation Losses of Plasmon–Polariton in a NanoChain In the case of the dynamics of plasmon–polaritons in a metallic nanochain, the inclusion of nonlinear correction to the Lorentz friction amounts to accounting for these nonlinear contributions in Eq. (9.48) via the formula for EL . Instead of Eq. (9.50) we then get the following equation (the Lorentz friction term is represented as in Eq. (9.74)): R¨ α (kα,tω1 ) + ω˜ α2 R0 α (kα ,tω1 ) 4 5
ω a 5 1 1 p = −2R˙ α (kα,tω1 ) + R˙ α (kα,tω1 )2 − 3Rα (kα,tω1 )2 , √ τ α ω1 3 c 3 2 (9.76) with the renormalized frequency and damping rate given respectively by Eqs. (9.77) and (9.78) below. To solve Eq. (9.76) one assumes that in the retardation terms on the righthand of solution. side of this equation, ω = ω1 , as in the iterative perturbation method ... This method was applied earlier to the Lorentz friction, obtaining R = −R˙ (note,
226
Plasmon–Polaritons in Metallic Nanoparticle Chains
however, that for R ∼ eiωt the accurate relation is ∂ 3 R/∂t 3 = −ω2 ∂R/∂t). Thus Eq. (9.76) corresponds to the first step of the iterative procedure, where ωα2 A, α = z, 2 3 ω˜ α = 2 = 1 − a B, α = x(y), ω1 and 2 2ω1 /c cos(nω d/c) + 2 cos(knd) 2 2 sin(nω1 d/c), 1 3 3 nd nd n n (ω1 /c)2 1 B=2 cos(nkd) − 3 3 cos(nω1 d/c) nd n d n ω1 /c −2 cos(knd) 2 2 sin(nω1 d/c). (9.77) nd n A=2
cos(nkd)
Furthermore, ⎧ 1 ω1 ω1 ⎪ ⎪ for kd − d > 0, kd + d < 2π, α = z,x(y), ⎨ 1 τ 0 ω1 c c 3 = ω a 1 1 C, α = z, p τ α ω1 ⎪ ⎪ + + a3 √ ⎩ D, α = x(y), τ 0 ω1 3 c 3 where C=−
cos(nkd)
n
D=−
2 2ω1 /c sin(nω d/c) + cos(nkd) 2 2 cos(nω1 d/c), 1 3 3 nd nd n
cos(nkd)
n
−
n
cos(nkd)
(ω1 /c)2 1 − 3 3 sin(nω1 d/c) nd nd
ω1 /c cos(nω1 d/c). n2 d 2
(9.78)
In Eq. (9.77) one can substitute the pointdivergent sum by an exact analytic form: a3
∞ cos(nkd)(ω1 /c)2 cos(nω1 d/c) n=1
nd
a ) ω1 a *2 1 ln[4(1 − cos(kd + ω1 d/c))(1 − cos(kd − ω1 d/c))], (9.79) d c 4 which displays explicitly the isolated logarithmic singularity in the dispersion formula for the transverse mode. The longitudinal modes are without this singularity; this is linked with the absence of the constructive interference of dipole radiation in the farfield zone, expressed by the term with denominator r0 , which is in a direction collinear with the dipole orientation in the case of the longitudinal polarization. =−
9.7 NearFieldZone Approximation
227
Applying the same asymptotic methods [190] for the solution of the nonlinear equation (9.76) as in the previous subsection, one can find the corresponding solutions for the regions with positive and negative damping rates, respectively. For the positive damping rate region, 1/τα ω1 > 0 (see [190]), we have Rα (k,t) =
Aα0 e−t/τα
cos(ωα t + θ0 ), 1 + γα A2α0 1 − e−2t/τα
(9.80)
Rα (k,t) →(t→∞) 0, where
) ω a *5 1 5 1 2 ω˜ − 1 , γα = τα ω1  c 4 2 α
θ0 = kld + φ0 .
Here φ0 and Aα0 are adjusted to the initial conditions. We note from the form of Eq. (9.80) that this is a damped mode vanishing at longer time scales. For the negative damping rate region, 1/τα ω1 < 0, the solution has a different form (see [190]): Rα (k,t) =
Aα0 et/τα 
cos(ωα t + θ0 ), 1 + γα A2α0 e2t/τα  − 1
Rα (k,t) →(t→∞)
(9.81)
1 √ cos(ωα t + θ0 ), γα
with θ0 = kld + φ0 . This solution is stable; it corresponds to an undamped mode √ which stabilizes at a fixed amplitude 1/ γα at longer time scales, independently of the initial condition, expressed by Aα0 . The corresponding dipole oscillations attain in the latter case the form of monochromatic waves propagating along the chain in both directions, eNe a 1 cos(ωα t ∓ kld + φ0 ). Dα = √ γα 2
(9.82)
From the above discussion it follows that for positive attenuation rates we are dealing with ordinary damped plasmon–polariton propagation, which is not strongly modified from the linear theory (owing to the small value of the factor γα ). However, in the case of a negative damping rate the solution behaves differently – on longer time scales this solution stabilizes at a constant amplitude independently of the initial conditions. This property characterizes the undamped propagation of plasmon–polaritons along the chain. It should be noted, however, that the existence of undamped modes in a system with scattering losses, and thus with energy dissipation, would contradict energy conservation. Nevertheless, if one assumes ˙ that the system is energetically supplied by an external source synchronic to R
228
Plasmon–Polaritons in Metallic Nanoparticle Chains
then, even if its strength were relatively small, it would prevail over the scattering losses and in the whole region of radiativelossquenching (the white region in Fig. 9.24 (left)) the total damping rate would be negative. In such a case we would be dealing with two types of plasmon–polariton: first, ordinary damped modes with a still positive overall attenuation rate (the shaded region in Fig. 9.24, slightly diminished close to its borders with the white region due to the shift caused by the external energy supply); second, undamped modes. The modes from the first region will be extinguished after a distance of the order of the attenuation time multiplied by the group velocity, but the modes from the second region will undergo stable propagation at a fixed amplitude independently of initial conditions. These latter modes express the instability (induced in this case) of the system; thus, the energy for this propagation is not the initial excitation energy but is the energy supplied by the pumping force. In other words, the continuous losses of plasmon oscillation energy due to scattering are instantly recovered by the external pumping. When this income equals the losses, the wave packets of the corresponding modes propagate without damping. This behaviour is typical for other nonlinear oscillation systems and its existence for plasmon–polaritons also would be of practical significance. Concluding this part of the discussion, the radiatively undamped modes of propagation of collective surface plasmons indicated above seem to match with the experimentally observed longrange propagation of plasmon excitations along finite metallic nanochains [116, 39, 24, 1]. We have demonstrated the use of the RPA semiclassical model of plasmon oscillations in metallic nanospheres for a description of collective surface plasmon–polariton propagation along a metallic nanochain. The oscillatory form of the dynamics both for volume and surface plasmons, rigorously described in the RPA semiclassical limit, fits well with the largenanosphere case, with radii of several nm to several tens of nm; this is confirmed by experimental observations. The most important property of plasmons on large nanospheres is the very strong electromagnetic radiation caused by these excitations, which results in the quick damping of oscillations. Attenuation effects for plasmons are not, however, included in the quantum RPA model. Nevertheless, they can be included in a phenomenological manner, taking advantage of the oscillatory form of the dynamical equations. Some information on plasmon damping can be taken from the microscopic analysis of smaller metallic clusters, with sizes of 1−2 nm (especially those made by the local density approximation (LDA) and timedependent LDA methods of numerical simulation, employing the Kohn–Sham equation). For larger nanospheres these effects, mainly of a scattering type (but also including Landau damping), are, however, of decreasing significance with growth in radius, since they depend on 1/a while the damping of plasmons starts to be dominated by radiation losses growing as a 3 .
9.7 NearFieldZone Approximation
229
The radiation effects overwhelming the other energy losses in the case of large nanospheres can be understood in terms of the Lorentz friction, which hampers the movement of charges. Two distinct situations are indicated: first, free radiation to the farfield zone in the dielectric (or vacuum) surroundings of a single nanoparticle; second, the location of an additional charged system in the nearfield zone of the plasmons. Such an additional system of charges, acting as an electromagnetic energy receiver in the vicinity of another metallic nanosphere with plasmons, strongly modifies the energy balance of the source and in this way modifies the energy emission in comparison with the free emission in vacuum or in dielectric surroundings. In particular, the Lorentz friction is modified in the presence of an energy receiver in the nearfield zone of plasmons, in comparison with simple free emission to the farfield zone. The electromagnetic energy receiver located close to an emitting nanosphere could be a semiconductor (as in the case of metallic modified solar cells) or other metallic nanospheres (as in the case of a metallic nanochain). The latter situation has been analysed above. We showed that, within the nearfield coupling approximation [185], collective plasmon–polaritons can propagate along an infinite nanochain (being collective surface plasmons coupled by the electromagnetic field in the nearfield zone); at certain values of nanosphere radius and separation in the chain, these modes are undamped. Moreover, the instability regions in the linear theory of plasmon–polariton dynamics occur, which shows that some corrections must be included to ensure energy conservation. We examined this artefact of nearfieldzone coupling and have demonstrated that inclusion of the mediumfield and farfield contributions removes the instability and leads to the exact quenching of radiative losses typical for plasmon–polaritons. We analysed the corrections due to the medium and farfieldzone contributions in full retarded form, including the isolated logarithmic singularity in the dispersion of the transverse modes due to the constructive interference effect in the farfield dipole term. The dispersion, damping rates, and group velocities for longitudinal and transverse polarizations with respect to the chain orientation were analysed with regard to their dependence on nanosphere size and separation in the chain. The results explain some previous, numericaltype observations related to the existence of a decaying mode of plasmon–polaritons due to farfield constructive interference. The wave packet due to a singlepoint excitation in the chain includes all wave vectors (as in the Fourier picture of a pointlike initial signal), even from the region of the hyperbolic singularity of the group velocity for transverse polarization. As this singularity is isolated and provides oppositesign contributions on both sides, the resulting farfield propagation (related to the growth in group velocity) may correspond to a decaying mode, though with higher velocity and thus a larger range in comparison with other wave packet components. The manifestation of this behaviour is more visible for larger nanosphere separation, when the group
230
Plasmon–Polaritons in Metallic Nanoparticle Chains
velocity away from the singularity is strongly lowered owing to the flattening of the spectrum, which also fits previous numerical observations. We examined also nonlinear corrections to the collective plasmon–polariton dynamics along the chain, including the nonlinear contribution to the Lorentz friction force. Even though the related nonlinearity is small, it suffices to regularize the unstable linear approach in the case of an external energy supply. We noted the presence, in this case, of undamped excitations which have a fixed amplitude independently of how small or large the initial conditions were.
10 Plasmon–Polariton Kinetics in a Metallic Nanochain Located in Absorbing Surroundings
The application of plasmon–polaritons in metallic nanoarrays frequently requires modification of the model concerning the metallic nanosystem surroundings. Plasmons and plasmon–polaritons easily couple with electrically active systems such as metals or semiconductors. This results in properties of plasmon–polaritons that are different from those in dielectric surroundings. In this chapter the theory of plasmon–polariton kinetics along a metallic chain with inclusion of energyabsorbing surroundings is formulated. Taking into account that the coupling channel of plasmon–polaritons with other systems may act in both directions, this opens a wide field of practical applications, e.g., of arbitrarily longrange plasmon–polariton kinetics if energy is supplemented to cover the electron scattering losses in metallic components via the coupling with an external subsystem.
Besides the strong plasmon photovoltaic effect, with growing applications in photovoltaics via the metallization of solar cells at the nanoscale [104, 32, 33, 105, 34, 35], other nanoplasmonic effects are also highly prospective for applications. Plasmon–polaritons propagating in linear arrays of metallic nanoparticles behave as information carriers that are almost lossless [3, 116, 4]. Such perfect wave guides for plasmon–polaritons in the form of metallic nanochains [166, 40, 38] are considered as promising for subdiffraction light circuits for the new generation of optoelectronics. The transformation of a light signal into a plasmon–polariton with the same frequency but a much shorter wavelength [1, 5, 6] can avoid the diffraction restrictions of conventional optoelectronics. The latter cannot be miniaturized below the light wavelength (of micrometre scale for visible light and higher for infrared) which does not match the nanometre scale of electronics miniaturization. Reducing the wavelength of the information carrier, when changing a photon into a plasmon–polariton, will constitute significant progress toward nanoscale optoplasmonelectronics. Plasmon–polaritons also have another exceptional property. They do not irradiate energy when travelling along a wave guide, thus are almost lossless. They do not have any external electromagnetic signature because they do not interact with photons owing to the large incommensurability in momentum for the same 231
232
Plasmon–Polariton Kinetics in Absorbing Surroundings
energy, and this prevents radiation loss from plasmon–polaritons. Also, they cannot be perturbed by any external electromagnetic field configurations. This property of plasmon–polaritons is of importance for metallic nanochains located in dielectric surroundings. When a metallic nanochain is placed on a semiconductor substrate or embedded in semiconductor surroundings, then the situation changes because of the strong coupling of plasmon oscillations in each metallic nanocomponent to the electron band system in the surrounding medium. This nearfieldzone coupling causes a plasmon–polariton energy outflow to the semiconductor, resulting in damping of the collective plasmon modes propagating in the chain. Note that the same nearfield coupling may be used in the opposite direction to supply energy to plasmon–polaritons in the chain from the semiconductor substrate, with the inverse electron occupation of semiconductor bands; this may be attained, e.g., by application of an appropriate lateral current in the semiconductor. Such an energy supplementation might be convenient to balance the generally small dissipation of plasmon–polariton energy caused by unavoidable ohmic losses. In this chapter we provide a description of the nearfield coupling of a plasmon–polariton in a metallic nanochain to the semiconductor substrate using an application of the Fermi golden rule in order to derive the related damping rate and to analyse the damped propagation of plasmonpolaritons. The longrange propagation of a plasmon–polariton signal along linear periodic metallic nanostructures has been described theoretically [41, 167, 168] and demonstrated experimentally [24, 170, 39, 171, 166, 169]. The undamped propagation of plasmon–polaritons modes in Au and Ag nanochains has been observed over distances ∼ 0.5 μm. Plasmon–polaritons are the hybridization of plasmons with photons and this results in a lowering of their group velocity below 0.1×c [170, 171, 166]. The related momentum incommensurability at the same energy of photons and plasmon–polaritons means that the latter do not radiate and so propagate along metallic nanochains over large distances [40, 169]. However, the residual ohmic losses cause an irreversible dissipation of the energy into Joule heat, limiting the propagation range of plasmon–polaritons. In the following sections of the present chapter we will describe the propagation of plasmon–polaritons in a metallic nanochain in close semiconductor surroundings including the coupling of propagating plasmon oscillations to the semiconductor band system in the nearfieldzone regime, as schematically presented in Fig. 10.1. This coupling causes an energy transfer between the plasmon–polaritons and the semiconductor electrons. The energy outflow from plasmon–polaritons to the semiconductor band system enhances the damping of the plasmon–polaritons, whereas an opposite direction of energy flow may be utilized to cover the plasmon–polariton Joule heating losses caused by electron scattering in the metallic components. First, we will recall the surface dipoletype
10.1 Plasmon Oscillations in a Single Metallic Nanosphere Including Damping 233 plasmon–polariton
Au
a > 5 nm
d > 2a
conduction band
Si electrons
forbiden gap
holes
valence band
Figure 10.1 When a metallic nanochain is deposited on or embedded in an absorbing medium (such as a semiconductor), a strong leakage of the plasmon– polariton energy takes place via the coupling in the nearfield zone of plasmon dipoles with the band electrons in the surrounding medium.
plasmons in a single metallic nanosphere (within the previously formulated RPA model [23, 77]) including damping effects. The damping of plasmons in a single nanoparticle is caused by the Lorentz friction of the plasmons, which is equivalent to radiation to the farfield zone. Additional damping arises via the channel of energy outflow in the nearfield zone due to the coupling of plasmon dipoles to the nearby electrons in the surrounding semiconductor. Next, we will describe the collective surface plasmon excitations in a nanochain of metallic particles, i.e., plasmon–polaritons, taking into account both channels for energy losses. The propagation of damped plasmon–polaritons in a metallic nanochain surrounded by an absorbing medium will be analysed for both longitudinal and transverse polarizations of the plasmon oscillations with respect to the propagation direction and for a variety of geometries, sizes, and material details of the whole system. 10.1 Plasmon Oscillations in a Single Metallic Nanosphere Including Damping A metallic nanosphere is conventionally modelled as a spherical static positive jellium together with an electrically balanced electron liquid which can locally fluctuate in density, resulting in regular charge oscillations. These are surface plasmons when the oscillations have a translational character, with the electrical local imbalance occurring on the sphere’s surface only, and they are volume plasmons when the oscillations have a compressional character along the radius
234
Plasmon–Polariton Kinetics in Absorbing Surroundings
of the nanosphere. It is interesting that the energy of nanosphere volume plasmons ¯ p = for a given mode is always greater than the bulk plasmon energy hω 2 h¯ e ne /(mε0 ) (m is the mass of an electron, e is the electron charge, ne is the density of free electrons in a metal, and ε0 is the dielectric constant), whereas the energy of the surface plasmon modes is lower than hω ¯ p [23]. The latter property makes noble metal (Au, Ag, Cu) nanoparticles attractive for applications as their reducedenergy surface plasmon resonances overlap with the visible light spectrum. The fluctuations in that local electron density in the nanosphere thus have surface and volume parts as follows: 0 for r < a, δρ1 (r,t) (10.1) δρ(r,t) = for r ≥ a (r → a+), δρ2 (r,t) These fluctuation modes satisfy equations derived in the framework of the random phase approximation (RPA) [23]: ∂ 2 δρ1 (r,t) 2 F 2 = ∇ δρ1 (r,t) − ωp2 δρ1 (r,t), 2 ∂t 3m and
r 3 F ne + F δρ2 (r,t) δ(r − a) 5 r ωp2 r 2 F r 1 − ∇δρ2 (r,t) + ∇ d 3 r1 3mr 4π r r − r1 
∂ 2 δρ2 (r,t) 2 =− ∇ ∂t 2 3m
(10.2)
× (δρ1 (r1,t)(a − r1 ) + δρ2 (r1,t)(r1 − a)) δ(r − a), (10.3) where is the Heaviside step function defining the static jellium, ne (r) = ne (a − r), and a is the nanosphere radius. The analysis and solution of the above equations has been performed in detail in previous chapters, resulting in the determination of the plasmon selfmode spectra for both the volume and surface modes. This RPA treatment does not account, however, for plasmon damping. The damping of plasmons can be included in a phenomenological manner, by adding the term −(2/τ0 )∂δρ(r,t)/∂t to the righthand side of both Eqs. (10.2) and (10.3), taking advantage of their oscillatory form. The damping ratio 1/τ0 accounts for electron scattering losses (eventually Joule heat losses in the metal of the nanosphere) [24]: vF CvF 1 + . τ0 2λb 2a
(10.4)
In Eq. (10.4), C is a constant of order unity, vF is the Fermi velocity in the metal, λb is the electron mean free path, which is the same as in the bulk metal; included
10.1 Plasmon Oscillations in a Single Metallic Nanosphere Including Damping 235
are the scattering of electrons on other electrons, on impurities, on phonons in the metallic nanoparticle, and on the nanoparticle boundary [24]. As previously discussed, the latter term in the formula (10.4) accounts for the scattering of electrons on the boundary of the nanoparticle, whereas the former term corresponds to scattering processes similar to those in bulk. Other scattering effects such as Landau damping are important for small nanoparticles [80, 79]) but are negligible for nanoparticle radii larger than 5 nm; here we consider such large nanospheres with radii ≥ 5 nm. The homogeneous equations (10.2) and (10.3) determine the selffrequencies of the plasmon modes. One can write out also dual inhomogeneous equations with an explicit driving factor. This factor would be the timedependent electric field, e.g., the electric component of the incident electromagnetic wave (of a laser beam or sunlight in photovoltaic applications [30]). The light wavelength in resonance with surface plasmons in the metallic nanosphere (Au, Ag, Cu) is of order 500 nm and greatly exceeds the nanosphere size (with radius 5−50 nm); thus dipoleapproximationregime conditions are satisfied. Hence, the driving field E(t) of the electromagnetic wave is almost homogeneous over the nanosphere (this corresponds to the dipole approximation) and can only excite the dipole surface mode in the electron liquid of the metallic nanosphere. The dipoletype mode may be described by a function Q1m (t), with l = 1 and m = −1,0,1 the angular momentum quantum numbers, related to the spherical symmetry of the metallic nanoparticle. The function Q1m (t) satisfies the equation ∂ 2 Q1m (t) 2 ∂Q1m (t) + + ω12 Q1m (t) ∂t 2 τ0 ∂t & √
( 4π ene ' = Ez (t)δm,0 + 2 Ex (t)δm,1 + Ey (t)δm,−1 , (10.5) 3 m √ where ω1 = ωp / 3ε (ω1 is the dipole surface plasmon Mietype frequency [18, 17] and ε is the dielectric constant for the nanosphere surroundings). The electron density fluctuations can be written as follows: ⎧ r < a, ⎨ 0, 1 (10.6) δρ(r,t) = Q1m (t)Y1m ( ), r ≥ a (r → a+), ⎩ m=−1
where Ylm ( ) is a spherical harmonic with l = 1. The plasmon oscillations given by Eq. (10.6) define a dipole D(t): & ⎧ 2π ⎪ 3 ⎪ eQ1,1 (t)a 3, Dx (t) = e d rxδρ(r,t) = ⎪ ⎪ ⎪ 3 ⎪ & ⎨ 2π (10.7) Dy (t) = e d 3 ryδρ(r,t) = eQ1,−1 (t)a 3, ⎪ 3 ⎪ & ⎪ ⎪ ⎪ ⎪ ⎩ Dz (t) = e d 3 rzδρ(r,t) = 4π eQ1,0 (t)a 3 . 3
236
Plasmon–Polariton Kinetics in Absorbing Surroundings
By virtue of Eq. (10.5), the dipole D(t) thus satisfies the equation
2 a 3 4πe2 ne 2 ∂ ∂ 2 D(t) = + + ω E(t) = εa 3 ω12 E(t). 1 2 ∂t τ0 ∂t 3m
(10.8)
The damping term in the above equation includes energy dissipation due to electron scattering in the metallic nanosphere, i.e., electron–electron, electron–phonon, and electron–admixture scattering, as well as a contribution from the boundary scattering [24]. There is, however, also an important channel of plasmon damping caused by radiation losses, not included in the formula for τ0 . The radiative losses of plasmon energy in the dielectric surroundings can be expressed by the Lorentz friction [55], i.e., by a fictitious electric field slowing down the motion of charges: √ 2 ε ∂ 3 D(t) . (10.9) EL = 3c3 ∂t 3 Thus, one can rewrite Eq. (10.8) including the Lorentz friction term as
2 2 ∂ ∂ 2 3 2 3 2 + (10.10) + ω 1 D(t) = εa ω1 E(t) + εa ω1 EL, ∂t 2 τ0 ∂t or for, the case when E = 0, !
2 2 ∂ ωp a 3 ∂ 2 ∂ 2 2 − D(t) + + ω1 D(t) = D(t) . √ ∂t 2 ∂t τ0 3ω1 c 3 ∂t 2
(10.11)
Now applying a perturbation procedure to solve Eq. (10.11) and treating the righthand side of this .equation as the / perturbation, one obtains, in the zeroth step of the perturbation, ∂ 2 /∂t 2 + ω12 D(t) = 0, from which (∂ 2 /∂t 2 )D(t) = −ω12 D(t). Therefore, in the first step of the perturbation, one includes the latter formula on the righthand side of Eq. (10.11), obtaining
2 2 ∂ ∂ 2 (10.12) + + ω1 D(t) = 0, ∂t 2 τ ∂t where 1 ω1 1 + = τ τ0 3
ωp a √ c 3
3 .
(10.13)
In this way we have included the Lorentz friction in the total attenuation rate 1/τ . This is justified for nanospheres that are not very large, i.e., when the second term in Eq. (10.13), proportional to a 3 , is sufficiently small to fulfil the perturbation procedure constraints. For nanospheres with radius 10−30 nm this approximation is fulfilled and has been verified experimentally for Au and Ag nanospheres [77, 45]. Inclusion of the Lorentz friction in this perturbative manner explains the experimentally observed redshift of the resonance surface
10.2 Radiative Properties of Plasmon–Polaritons
237
a∗
Table 10.1 Radius of the nanosphere corresponding to the minimal value of surface plasmon damping in dielectric surroundings a∗
√ n= ε
Au
Ag
Cu
n = 1 vacuum n = 1.4 water n=2
8.4 9.137 9.989
8.44 9.18 10.037
6.46 9.202 10.04
plasmon frequency with increasing a. Indeed, the solution of Eq. (10.12) is of the form D(t) = Ae−t/τ cos(ω1 t + φ), where ω1 = ω1 1 − 1/(ω1 τ )2 , which gives the experimentally observed redshift of the plasmon resonance due to the ∼ a 3 growth in the plasmon damping caused by radiation. The Lorentz friction term in Eq. (10.13) dominates the plasmon damping in dielectric surroundings for a ≥ 12 nm (for Au and Ag) owing to this a 3 dependence. Thus the plasmon damping grows rapidly with a and results in a pronounced redshift of the resonance frequency, in good agreement with the experimental data for 10 < a < 30 nm (Au and Ag) [77]. Taking into account that 1/τ0 scales as 1/a, while the Lorentz friction contribution scales as a 3 for 10 < a < 30 nm, in this size region one encounters a crossover of the attenuation rate with respect to a. The minimum damping is achieved at 1/4 3 √ 9 c v F ε 4 , (10.14) a∗ = 2 ωp and for a < a ∗ the damping ratio grows with decreasing a approximately as ∼ 1/a, while for a > a ∗ this ratio grows with increasing a in proportion to a 3 . The value of a ∗ can be estimated for Au, Ag, and Cu; see Table 10.1. 10.2 Radiative Properties of Plasmon–Polaritons in a Metallic NanoChain Embedded in a Dielectric Medium When a metallic nanosphere is an element of a chain of similar nanospheres equidistantly distributed along a line, one has to take into account that alongside the radiation losses from that nanosphere, a simultaneous income of energy takes place from the radiation of other nanospheres when a collective plasmon excitation (a plasmon–polariton) propagates along the chain. The interaction between nanospheres in the chain can be considered as dipoletype coupling. The minimal separation of the nanospheres in the chain is d = 2a
238
Plasmon–Polariton Kinetics in Absorbing Surroundings
(d is the distance between neighbouring sphere centres), and the dipole approximation of the plasmon interaction in the nanosphere chain is sufficiently accurate for d > 3a, because then the multipoleinteraction contribution can be neglected. Various numerical largescale calculations of the electromagnetic field distribution in such systems with the inclusion of dipole and also multipole interactions between the plasmonic oscillations in the metallic components have been carried out [41, 167, 168]. A model of interacting dipoles [177, 178] had been developed earlier for the investigation of stellar matter [179, 180] and it was then adopted for metal particle systems [181, 182]. Numerical studies beyond the dipole model [41, 168] indicated that the dipole model is sufficiently accurate when the particle separation is not lower than the particle dimensions, since the multipole contribution to the interaction is then small [183]. An oscillating dipole D(t) located at a point r causes an electric field at another point r0 (we assume that the vector r0 is drawn from the tip of r) that has the following form (including the relativistic retardation of the electromagnetic signals) [55, 76]: ) ∂2 1 r0 * 1 ∂ 1 1 − 2 2 − D r,t − − E(r,r0,t) = ε v ∂t r0 v∂t r02 r03 v (10.15) 2 ) ) ∂ 1 ∂ 3 3 r0 ** 1 n0 n0 · D r,t − + + + , ε v 2 ∂t 2 r0 v∂t r02 r03 v √ where n0 = r0 /r0 and v = c/ . The above formula includes terms corresponding to the nearfieldzone (denominator r03 ), mediumfieldzone (denominator r02 ), and farfieldzone (denominator r0 ) contributions to the dipole field. Equation (10.15) allows us to write out the dynamical equation for the plasmon oscillations at each nanosphere of the chain, numbered by an integer l. We denote by d the separation between nanospheres in the chain and by a the nanosphere radius. The vectors r and r0 are collinear if the origin of the coordinate system is associated with a nanosphere in the chain. Therefore the equation for the collective surface plasmon oscillation in the lth sphere of the chain is as follows,
2 m=∞ l − md 2 ∂ ∂ 2 2 3 + Eα md,t − + ω1 Dα (ld,t) = εω1 a ∂t 2 τ0 ∂t c m=−∞, m=l + εω12 a 3 ELα (ld,t) + εω12 a 3 Eα (ld,t). (10.16) The first term on the righthand side of Eq. (10.16) describes the dipole coupling between nanospheres in the chain and the next two terms correspond to the contribution to the plasmon attenuation due to Lorentz friction (as described in the
10.2 Radiative Properties of Plasmon–Polaritons
239
previous section) and to the driving electric field. The index α enumerates the polarizations: longitudinal for α = z and transverse for α = x(y), with respect to the chain orientation (assumed to be in the z direction). According to Eq. (10.15) we have: ∂ 1 d 2 d Dz md,t − m − l , + Ez (md,t) = 3 εd m − l3 vm − l2 ∂t v ∂2 ∂ 1 1 d d2 Ex(y) (md,t) = − 3 + + 2 εd m − l3 vm − l2 ∂t v l − d ∂t 2 d . × Dx(y) md,t − m − l v (10.17) Taking advantage of the chain periodicity one can assume in analogy to the Bloch states in onedimensional crystals, with a reciprocal quasimomentum lattice, Dα (ld,t) = Dα (k,t) e−ikld ,
0≤k≤
2π . d
(10.18)
The above can be asserted in a more formal manner by taking the Fourier picture of Eq. (10.16). As the dipoles are localized at the centres of the nanospheres, the system is discrete, as in the case of phonons in a onedimensional crystal. One can thus apply a discrete Fourier transform (DFT) with respect to the positions, and a continuous Fourier transform (CFT) with respect to time. A DFT is defined for a finite set of numbers, so one can consider a chain with 2N + 1 nanospheres, i.e., of length L = 2Nd. Thus for any discrete characteristics f (l), l = −N, . . . ,0, . . . ,N of the chain, such as the dipole distribution, one is dealing with the DFT picture: f (k) =
N
f (l)eikld ,
l=−N
where k = 2πn/(2Nd), n = 0, . . . ,2N. Hence, kd ∈ [0,2π ] owing to the periodicity of the chain. The Born–Karman boundary condition has been imposed, on the whole system, resulting in k = 2πn(2Nd). In order to account for the infinite length of the chain one can take the limit N → ∞, with the result that the variable k becomes quasicontinuous, but kd ∈ [0,2π ] still holds. The Fourier picture of Eq. (10.16), with a DFT for positions and a CFT for time, is as follows, a3 2 2 2 −ω − i ω + ω1 Dα (k,ω) = ω12 3 Fα (k,ω)Dα (k,ω) + εa 3 ω12 E0α (k,ω), τ0 d (10.19)
240
with
Plasmon–Polariton Kinetics in Absorbing Surroundings ∞ cos(mx)
cos(mx) Fz (k,ω) = 4 cos(mξ ) + ξ sin(mξ ) m3 m2 m=1 ! ∞ 1 3 cos(mx) cos(mx) sin(mξ ) − ξ cos(mξ ) , (ξ ) + 2 + 2i 3 2 3 m m m=1 ∞ cos(mx) cos(mx) cos(mξ ) + ξ sin(mξ ) Fx(y) (k,ω) = −2 3 m m2 m=1 2 cos(mx) −(ξ ) cos(mξ ) m ∞ cos(mx) cos(mx) 2 sin(mξ ) + ξ cos(mξ ) − i − (ξ )3 + 2 3 2 3 m m m=1 cos(mx) 2 −(ξ ) sin(mξ ) . m (10.20)
The direct calculation of the functions Im Fz (k,ω) and Im Fx(y) (k,ω) corresponding to radiative damping for the longitudinal and transverse plasmon– polariton polarizations, respectively, was done explicitly in the case of a dielectric medium in Eqs. (9.27) and (9.29), and holds also for an absorbing medium. We showed there that both these functions vanish when 0 < kd ± ωd/v < 0 (the corresponding region – the light cone – is indicated in Fig. 9.3). Outside this region the radiative damping expressed by the functions Im Fα (k,ω) is nonzero, which is illustrated in Figs. 9.4 and 9.5, respectively for the longitudinal and transverse modes. 10.3 Plasmon–Polariton SelfModes in a Chain in Dielectric Surroundings The real parts of the functions Fα give the renormalized selffrequency of the plasmon–polaritons in the chain, whereas the imaginary parts give the renormalized damping of these modes. Re Fα (k,ω) and Im Fα (k,ω) are functions of k and ω. Applying the perturbation method of solution, within the firstorder approximation one can put ω = ω1 in Re Fα and also in the residual nonzero Im Fα outside the region 0 < kd ± ω1 d/v < 2π . Let us emphasize, however, that the vanishing of Im Fα (k,ω) inside the region 0 < kd ± ωd/v < 2π holds for any value of ω [44], thus also for the exact (nonperturbative) solution, as shown numerically in Figs. 10.2–10.5.
10.3 Plasmon–Polariton SelfModes in a Chain in Dielectric Surroundings
241
Transverse plasmon–polariton mode 0.05
1/
1.02 0
5 10
1.01
0.03
1.00
0.02
x
x y
0.04
0 5 10
0.99
0.01 0.98
200
400 600 800 kd (2 /1000)
1000
0.08 x y
x y
1/ 0 +
0.07 0.06 0.05 0.04 0.03 0
200
400 600 800 kd (2 /1000)
0
200
400 600 800 kd (2 /1000)
1.020 1.015 1.010 1.005 1.000 0.995 0.990 0.985
200 400 600 800 1000 kd (2 /1000)
5 10 0 5 10
0
1000
0
1000
x
0
200
400
600
0
800 1000
kd (2 /1000)
200 400 600 800 1000 kd (2 /1000)
Figure 10.2 The damping rate Im ωx(y) (k), the selffrequency Re ωx(y) (k), and the group velocity vx(y) (k) of a plasmon–polariton for transverse polarization in an infinite chain of Au nanospheres with radius a = 10 nm and chain separation d = 4a for vacuum surroundings (upper) and semiconductor (Si) surroundings (lower).
Transverse plasmon–polariton mode 1.010 4 10
0
0.026
1.005
2 10
1.000
0.024
0
x
1/
0.028
x y
x y
0.030
2 10
0.022
0.995 0
200
400 600 800 1000 kd (2 /1000)
4 10
0
200
400 600 800 1000 kd (2 /1000)
0
200 400 600 800 1000 kd (2 /1000)
0
200 400 600 800 1000 kd (2 /1000)
0.148 4 10
0.142
0.995
2 10 x
1/ 1 +1/
0.144
x y
x y
0.146
0.990
0.140
0 2 10
0.138
0.985 0
200
400 600 800 1000 kd (2 /1000)
4 10 0
200
400 600 800 1000 kd (2 /1000)
Figure 10.3 The damping rate Im ωx(y) (k), the selffrequency Re ωx(y) (k), and the group velocity vx(y) (k) of a plasmon–polariton for transverse polarization in an infinite chain of Au nanospheres with radius a = 5 nm and chain separation d = 5a for vacuum surroundings (upper) and semiconductor (Si) surroundings (lower).
242
Plasmon–Polariton Kinetics in Absorbing Surroundings
Longitudinal plasmon–polariton mode
kd (2 /1000)
kd (2 /1000)
kd (2 /1000)
kd (2 /1000)
kd (2 /1000)
kd (2 /1000)
Figure 10.4 The damping rate Im ωx(y) (k), the selffrequency Re ωx(y) (k), and the group velocity vx(y) (k) of a plasmon–polariton for longitudinal polarization in an infinite chain of Au nanospheres with radius a = 10 nm and chain separation d = 4a, for vacuum surroundings (upper) and semiconductor (Si) surroundings (lower).
Longitudinal plasmon–polariton mode 0.0250
1/
0
1 10
1.01 z
0.0245
5 10
1.00
0
0.0240
5 10
0.99
0.0235
1 10
0.98
0.0230 0
200
400 600 800 1000 kd (2 /1000)
0
200
400 600 800 kd (2 /1000)
0
200 400 600 800 1000 kd (2 /1000)
0
200 400 600 800 1000 kd (2 /1000)
1000
0.0325
1 10 0
1.01 z
1/
0.0320 0.0315
1.00
0.0310
0.99
5 10 0 5 10 1 10
0.0305
0.98 0
200
400 600 800 1000 kd (2 /1000)
0
200
400 600 800 kd (2 /1000)
1000
Figure 10.5 The damping rate Im ωx(y) (k), the selffrequency Re ωx(y) (k), and the group velocity vx(y) (k) of a plasmon–polariton for longitudinal polarization in an infinite chain of Au nanospheres with radius a = 5 nm and chain separation d = 5a, for vacuum surroundings (upper) and semiconductor (Si) surroundings (lower).
In the perturbation scheme, one rewrites the dynamic equation (10.19) for plasmon–polariton modes in the chain in the following form: 2 2 2 (10.21) −ω − i ω + ωα (k) Dα (k,ω) = εa 3 ω12 E0α (k,ω), τα (k)
10.3 Plasmon–Polariton SelfModes in a Chain in Dielectric Surroundings
where the renormalized attenuation rate is given by ⎧ 1 ⎪ ⎪ for 0 < kd ± ω1 d/v < 2π, ⎪ ⎪ τ0 ⎪ ⎨ 1 1 a 3 ω1 = Im Fα (k,ω1 ) for kd − ω1 d/v < 0 ⎪ + τα (k) ⎪ ⎪ τ0 2d 3 ⎪ ⎪ ⎩ or kd + ω1 d/a > 2π .
243
(10.22)
The renormalized bare selffrequency (owing to damping, the true resonance is, however, redshifted, as for a damped oscillator, but this is not given here) is a3 2 2 ωα (k) = ω1 1 − 3 Re Fα (k,ω1 ) . (10.23) d Equation (10.21) can be easily solved for both the inhomogeneous case and the homogeneous case (when E0α = 0). The general solution of Eq. (10.21) is the sum of the general solution of the homogeneous equation and a single particular solution of the inhomogeneous equation. The first includes the initial conditions and describes damped selfoscillations with frequency 1 1 (10.24) ωα = ωα2 (k) − 2 , τα (k) i.e., for each k and α,
Dα (k,t) = Aα,k ei(ωα t+φα,k ) e−t/τα (k),
(10.25)
with constants Aα,k and φα,k determined by the initial conditions. For the inhomogeneous case the particular solution is as follows: Dα (k,t) = εa 3 ω12 E0α (k)ei(γ t+ηα,k )
1 (ωα2 (k)
−
γ 2 )2
+ 4γ 2 /τα2 (k)
,
(10.26)
given the assumed single Fourier time component E0α (k,t) = E0α (k)eiγ t , and tg(ηα,k ) =
2γ /τ (α,k) ω(α,k)2 − γ 2
as for a driven oscillator. Let us emphasize that E0α (k) is a real function: E0α (ld)∗ = E0α (ld) = E0α (−ld). An appropriate choice of this function, in practice the choice of the number of externally excited nanospheres in the chain (e.g., by a suitably focused laser beam), allows for the modelling of its Fourier picture E0α (k). This gives the envelope of the wave packet if one inverts the Fourier transform in the solution given by Eq. (10.26) back to the position variable. For the case of the external excitation of only a single nanosphere, the wave packet envelope includes homogeneously all wave vectors k ∈ [0,2π ]. The larger the number of nanospheres simultaneously excited, the narrower in k is the wave packet envelope. For E0α (ld)∗ = E0α (ld) = E0α (−ld) the Fourier transform has the same properties, i.e., E0α (k)∗ = E0α (k) = E0α (−k) and the latter equality can be
244
Plasmon–Polariton Kinetics in Absorbing Surroundings
rewritten, owing to the periodicity 2π of k, as E0α (−k) = E0α (2π /d −k) = E0α (k) d (this shifts k to the equivalent positively valued domain k ∈ [0,2π ]). The inverse Fourier picture of the real part of Eq. (10.26) is Dα (ld,t)
2π/d
=
dk cos(kld − γ t − ηα,k ) εa 3 ω12 E0α (k) 0
×
1 (ωα2 (k)
−
γ 2 )2
+ 4γ 2 /τα2 (k)
.
(10.27)
This integral can be rewritten, by virtue of the mean value theorem, in the form Dα (ld,t) =
2π cos(k ∗ ld − γ t − ηα,k∗ ) εa 3 ω12 E0α (k ∗ ) d 1 × . ∗ 2 2 (ωα (k ) − γ )2 + 4γ 2 /τα2 (k ∗ )
(10.28)
The above expression describes undamped wave motion with frequency γ and the velocity, amplitude, and phase shift determined by k ∗ . The energy losses are supplemented continuously by the driving force, as for any steady state of a damped and driven oscillator. The amplitude attains its maximal value at resonance, when 1 2 ∗ . (10.29) γ = ωα (k ) 1 − (τα (k ∗ )ωα (k ∗ ))2 If the chain is subject to a persistent driving force in the form of a timedependent external electric field applied to some number (even a small number) of the nanospheres, one is dealing with undamped wave packet propagation along the whole chain – the energy supply by the driving factor covers damping losses. These modes, depending on the shaping of the wave packet by the specific choice of chain excitation, may be responsible for the experimentally observed longrange practically undamped plasmon–polariton propagation [169, 171, 39, 40]. The selfmodes of Eq. (10.25) are damped and their propagation depends on appropriately prepared initial conditions admitting nonzero values of Aα,k . The resulting wave packet may embrace the wavenumbers k from some region of [0,2π]. If only the wave numbers k for which 0 < kd ± ω1 d/v < 2π contribute to the wave packet, its damping is only of ohmic type. The value of 1/τ0 decreases with increasing a (see Eq. (10.4)); thus, to achieve a longer range of these damped excitations in the chain, larger spheres are more suitable. The limiting value of 1/τ0 is vf /(2λB ) ∼ 1013 /s, which gives the maximum range of propagation for these modes of a plasmon–polariton as ∼ 0.1cτ0 ∼ 10−6 m. For the group velocity of the wave packet we assume ∼ 0.1c as its maximum value (though this depends on the radius and separation of the nanospheres in the chain). The group velocities
10.3 Plasmon–Polariton SelfModes in a Chain in Dielectric Surroundings
245
calculated for both polarizations are presented in the righthand panels of Figs. 10.2–10.5 (which give an accurate solution). Though the analysis presented above is addressed to chains consisting of ideal nanospheres, the conclusions also hold for chains of other shapes of particle and agree with experimental observations at least qualitatively. In [171] the propagation of a plasmon–polariton in a nanochain of Ag rodshaped particles (90 : 30 : 30 nm, oriented with the longer axis perpendicular to the chain in order to enhance the nearfield coupling [39], with facetoface separation, 70 nm) is evidenced by observing the luminescence of dye particles located in proximity to the transmitting electromagnetic signal but distant from the pointlike excitation source by about 0.5 μm. The observed behaviour has been supported by FDTD numerical simulations. Several samples of the chain were fabricated by electron beam lithography in the form of a twodimensional matrix with sufficiently wellseparated individual chains. The energy blueshift of the plasmon resonance for the nanorods in the chain, in comparison with the single particle case is observed to be about 0.1 eV [171]. This agrees with our estimation of the reduction in radiation losses in the chain in comparison with the strong Lorentz friction for a single metallic nanoparticle and the related smaller redshift of damped oscillations. The position of the resonance maximum in the chain is located at a higher energy for the transverse mode than for the longitudinal mode [170], which also agrees with theoretical predictions. In [39] it was indicated that FDTD simulations give lower values of the group velocities for both polarizations and higher attenuation rates in comparison with these quantities as previously estimated [170, 24] using a simplified pointdipole model with nearfield–zone interaction only and neglecting retardation effects. Let us note, however, that the simplified approach including only the nearfield contribution to the electric field of the interacting dipoles leads to an artefact, i.e., for some values of the chain parameters d and a an instability of the collective dynamics occurs [185]. This instability is completely removed by the inclusion of the medium and farfield contributions to the electric field of the dipole, including relativistic retardation [44]. Nevertheless, the dipole interaction model even if it includes, besides the nearfield contribution, the medium and farfield contributions and all retardation effects, still suffers from the absence of the magnetic field component needed for a complete description of the farfieldzone and mediumfieldzone wave propagation. As it is demonstrated in [186, 187], for large separations in a chain, the scattering of electromagnetic radiation dominates the signal behaviour in metallic nanochains, which then act as a Bragg grating for plasmon–polaritons. For ellipsoidal Au nanoparticles (210 : 80 nm) deposited on the top of an Si wave guide, the change of regime from collective plasmon–polariton guiding to the Bragg scattering scenario takes place at distances
246
Plasmon–Polariton Kinetics in Absorbing Surroundings
between nanoparticles exceeding about 1 μm [186]. This proves that the model of dipole coupling in the nanochain works quite well for a wide region of chain parameters, in practice up to the order of microns for the distance between the metallic elements in the chain. This supports the qualitative argument that the Bragg grating regime is not efficient for subwavelength distances and justifies the applicability of the model considered. The SNOM measurements of nearfield coupled plasmon modes in a metallic nanochain [166], interpreted within the classical fieldsusceptibility formalism in [188], also support the sufficiency of the dipole approximation for interactions in the chain for the scale considered here, with nanosphere radii a of the order of 10−30 nm and chain separation d not exceeding ∼ 10a. 10.4 Damping of Surface Plasmons in a Single Metallic Nanoparticle Deposited on a Semiconductor Substrate The interaction of band electrons with surface plasmons in a metallic nanoparticle deposited on the top surface of a semiconductor (or embedded in a semiconductor medium) causes an energy transfer resulting in an additional damping of the plasmons. The perturbation of the electron band system in the substrate semiconductor due to the presence of dipole surface plasmon oscillations in a metallic nanosphere with radius a deposited on the semiconductor surface (or embedded in it) has the form of the electromagnetic field of an oscillating dipole. The Fourier components of the electric field Eω (the Fourier component of Eq. (9.45)) and the magnetic field Bω produced at a distance R from the centre of a nanosphere having a surface plasmon dipole with frequency ω have the form [55] 2 2 k 1 1 k 3 ik 3ik ˆ nˆ · D0 ) − − 2 + 3 D0 eikR (10.30) + 2 − 3 + n( Eω = ε R R R R R R and ik ik 1 ˆ Bω = √ [D0 × n] − 2 eikR R R ε
(10.31)
(ε is the dielectric constant). In the case of spherical symmetry, the plasmon dipole is considered as pinned to the centre of the nanosphere, D = D0 e−iωt . In Eqs. (10.30) and (10.31) we have used the notation for a retarded argument: iω (t − R/c) = iωt − ikR, nˆ = R/R, ω = ck, and momentum p = h¯ k. Because we are considering the interaction with a closely adjacent layer of the substrate semiconductor, we can neglect the terms with denominators R 2 and R as small in comparison with the term with denominator R 3 – this is the nearfieldzone approximation (in which the magnetic field disappears and the electric field is that
10.4 Damping of Surface Plasmons for Single Metallic Nanoparticle
247
of a static dipole [55]). Therefore the related perturbation potential added to the system Hamiltonian attains the form e nˆ · D0 sin(ωt + α) = w + eiωt + w − e−iωt . (10.32) w = eψ(R,t) = εR 2 For the first term we can write ∗ e eiα w+ = w− = nˆ · D0 . εR 2 2i This describes emission, i.e., the case of interest. According to the Fermi golden rule scheme, the interband transition probability is proportional to 2 2π k1 w + k2 δ(Ep (k1 ) − En (k2 ) + hω), (10.33) w(k1,k2 ) = ¯ h¯ where the Bloch states in the conduction and valence bands are assumed to be plane waves for simplicity, 1 eik·R−iEn(p) (k)t/h¯ , (2π)3/2 h¯ 2 k2 h¯ 2 k2 Ep (k) = − ∗ − Eg, En (k) = 2mp 2m∗n k =
(the indices n,p refer to electrons from the conduction and valence bands, respectively; Eg is the forbidden gap). The matrix element 1 1 e iα d 3R k1 w + k2 = (10.34) e nˆ · D0 2 e−i(k1 −k2 )·R (2π)3 ε2i R can be found analytically by direct integration, which gives the formula (setting q = k1 − k2 ), ∞ −1 eeiα 1 d sin qR cos (2π) dR k1 w + k2 = D 0 (2π)3 ε q dR qR a (10.35) iα 1 ee D0 · q sin qa = . (2π)2 ε q2 qa Next we must sum over all initial and final states in both bands. Thus, for the total interband transition probability we have . / 3 δw = d k1 d 3 k2 f1 (1 − f2 )w(k1,k2 ) − f2 (1 − f1 )w(k2,k1 ) , (10.36) where f1,f2 are the temperaturedependent Fermi–Dirac distribution functions for the initial and final states, respectively. At room temperature, f2 0 and f1 1, which leads to (10.37) δw = d 3 k1 d 3 k2 w(k1,k2 ).
248
Plasmon–Polariton Kinetics in Absorbing Surroundings
After some also analytical integration in the above formula, we arrive at the expression, 4 μ2 (m∗n + m∗p )2(h¯ ω − Eg )e2 D02 1 sin2 (xaξ ) δw = dx 1 − x2 ∗ ∗ 2 3 (xaξ ) mn mp 2π h¯ 5 ε2 0 1 2 2 2 2 e D0 2 4 μ sin (xaξ ) = ∗ ∗ ξ dx 1 − x 2, (10.38) 3 mn mp 2π h¯ 3 ε2 (xaξ )2 0 according to assumed band dispersions; m∗n and m∗p denote the effective masses of electrons and holes, μ = m∗n m∗p /(m∗n + m∗p ) is the reduced mass, and the parameter ξ is given by 2(h¯ ω − Eg )(m∗n + m∗p )/h¯ . In the limiting cases, for a nanoparticle of radius a we finally obtain ⎧ μ m∗n m∗p (h¯ ω − Eg )e2 D02 4 ⎪ ⎪ for aξ 1, ⎨ 5 2 δw = 3 3/2 √ h¯ ε (10.39) ⎪ μ 2 h¯ ω − Eg e2 D02 ⎪ ⎩4 for aξ 1. 3 a h¯ 4 ε2 In the latter case the following approximation has been applied: ∞ 1 sin2 (xaξ ) 1 sin2 (xaξ ) π 2 ≈ (for aξ 1) dx 1 − x d(xaξ ) = , 2 2 (xaξ ) aξ (xaξ ) 2aξ 0 0 1 √ whereas in the former case we have 0 dx 1 − x 2 = π/4. With regard to these two limiting cases, aξ 1 and aξ 1, where ξ = 2(h¯ ω − Eg )(m∗n + m∗p )/h¯ , we have already noted in previous chapters that for larger nanospheres, e.g., with a > 10 nm, the second regime holds. Assuming that the energy acquired by the semiconductor band system, A, is equal to the plasmon oscillation energy output (corresponding to plasmon damping), one can estimate the corresponding damping rate of plasmon oscillations. Namely, for a plasmon amplitude decaying in time according to D0 (t) = D0 e−t/τ , one finds, for the total transmitted energy, ∞ A=β 0
δw h¯ ω dt = β h¯ ω δw τ /2 ⎧ 2 2 2 βωτ μ m∗n m∗p (h¯ ω − Eg )e D0 ⎪ ⎪ ⎨ h¯ 4 ε2 √ = 3 3/2 ⎪ 2 h¯ ω − Eg e2 D02 βωτ μ ⎪ ⎩2 3 a h¯ 3 ε2
for aξ 1, for aξ 1, (10.40)
where τ is the damping time rate and β accounts for losses not included in the model, especially those that reduce the energy transfer for the case of a realistic
10.5 Plasmon–Polariton Dynamics for Metallic Chain
249
deposition type on the top of the semiconductor layer instead of the fully embedded case. Comparing the value of A given by Eq. (10.40) with the plasmon energy loss by damping estimated in [23] (the initial energy of the plasmon oscillations which has been transferred step by step to the semiconductor, A = D02 /(2εa 3 )), one finds that ∗ ∗ ⎧ ¯ − Eg )e2 a 3 ⎪ 4βωμ mn mp (hω ⎪ for aξ 1, ⎨ 1 3h¯ 4 ε √ (10.41) = − Eg e 2 a 2 4βωμ3/2 2 hω τ ⎪ ¯ ⎪ ⎩ for aξ 1. 3h¯ 3 ε By τ we denote here the large damping of plasmons due to energy transfer to the semiconductor, which greatly exceeds the internal damping, characterized by τ0 , due to the scattering of electrons inside the metallic nanoparticle [23] (1/τ0 1/τ ). For example, for nanospheres of Au deposited on an Si layer we obtain for the Mie selffrequency ω = ω1 , ⎧ 3 3 μ m∗n m∗p ⎪ ⎨ 44.092β a , for aξ 1, 1 m *m (10.42) = ) τ (ω1 ) ⎪ ⎩13.648β a 2 2 μ 3/2 for aξ 1, m where a is in nanometres. For light (heavy) carriers in Si, m∗n = 0.19m (0.98m), m∗p = 0.16m (0.52)m, m is the bare electron mass, μ = m∗n m∗p /(m∗n + m∗p ), Eg = 1.14 eV, and hω ¯ 1 = 2.72 eV. For these parameters and for nanospheres with radius a in the range 5−50 nm, the lower case of Eq. (10.42) applies (at ω = ω1 ). The parameter β fitted from the experimental data [33, 23] equals about 0.001. 10.5 Plasmon–Polariton Dynamics in a Metallic Chain Deposited on a Semiconductor For a metallic nanochain deposited on (or embedded in) a semiconductor medium, the plasmon oscillations at each nanoparticle of the chain are additionally damped owing to energy transfer to the semiconductor band system as described above. Thus Eq. (10.19) should be generalized to the form: 2 2 2 2 ω + ω1 Dα (k,ω) + −ω − i τ0 τ a3 (10.43) = ω12 3 Fα (k,ω)Dα (k,ω) + εa 3 ω12 E0α (k,ω), d where τ is given by Eq. (10.41). Equations (10.20) still hold however. The damping rate in the case of a chain completely embedded in the semiconductor medium does not depend on the polarization of the plasmon oscillations; let us consider first this simple case. Using a perturbation scheme for the solution of
250
Plasmon–Polariton Kinetics in Absorbing Surroundings
Eq. (10.43) we can consider the real part of the righthand side of this equation as a correction to the frequency of the plasmon–polariton and the imaginary part as a correction to the damping rate. In an explicit form one thus deals with a perturbative solution, 1 2 a3 1 1 a3 + − 3 Im Fα (k,ω1 ) , ω(k) = ω12 (1 − 3 Re Fα (k,ω1 )) − d τ0 τ (ω1 ) 2d 1 1 1 a3 + = − 3 Im Fα (k,ω1 ), τ τ0 τ (ω1 ) 2d (10.44) where τ (ω1 ) is given by Eq. (10.42). The exact solution of Eq. (10.43) is presented in Figs. 10.2–10.5 and exhibits rather minor corrections to the perturbative solution, though the singular points need an exact solution to avoid the singularity misbehaviour of the perturbative solution. Thus in Figs. 10.2–10.5 we present the numerical solution of Eq. (10.43) for the full domain of k and for the real and imaginary parts of ω(k) which correspond to the perturbation solution given by Eq. (10.44). The numerical solution of the nonlinear equation (10.43) was obtained by a Newtontype highaccuracy method applied at 1000 points of the domain kd ∈ [0,2π ] point by point (the derivative of Re ω(k) with respect to k, needed in order to find the group velocity, was taken from the interpolated Re ω(k) function). Because Im Fα (k,ω) = 0 in the majority of the domain for k, one can expect that the damping of the plasmon–polariton kmode will go via the channels τ0 and τ (ω1 ) only and not via the Lorentz friction, which is perfectly balanced by the radiation income of energy from other nanoparticles in the chain. The comparison of the contributions of both active channels for plasmon–polariton damping is presented in Figs. 10.2–10.5 for different geometries and size parameters of the chain and for longitudinal and transverse polarizations of the plasmon–polariton oscillations with respect to propagation direction. For the nonhomogeneous equation (10.43) the stationary solution for the kmode corresponds to the usual damped driven oscillations, when the energy of the driving incident light is transferred to the semiconductor substrate in part whereas the rest is dissipated in Joule heat in the metal material of the chain. The energy transferred to the semiconductor may be transformed eventually into photocurrent, reemitted as light via exciton recombination, and also partly converted into Joule heat via the scattering of band electrons with phonons, defects, and admixtures (impurities) in the semiconductor medium. If we are dealing with two channels of plasmon damping, the energy dissipation per time unit for these channels is equal to T T dt 2 ∂Dα 2 dt 2 ∂Dα 2 and , T τ0 ∂t T τ ∂t 0 0
10.5 Plasmon–Polariton Dynamics for Metallic Chain
251
respectively. After averaging over the period of the stationary solution for the driven and damped oscillator, we arrive at the energy loss per time unit, (1/τ0 )ω2 A2 and (1/τ )ω2 A2 , respectively, where ω is the frequency of the driving force and A=
εa 3 ω12 E0
.
(ω12 − ω2 )2 + 4ω2 (1/τ0 + 1/τ )2
This outflow of energy is compensated during each period T of the driving force by the power of this force averaged over the period. Therefore the ratio of energy losses via the two channels equals (1/τ0 )/(1/τ ). Because the energy transferred to the semiconductor surroundings (the substrate) may not be converted into Joule heat or radiation, some deficit in energy balance might occur, not exceeding, however, the ratio indicated above. When this ratio is of order 1/3 (for a realistic value of the parameter β; see Figs. 10.2–10.5) one could observe, e.g., an ostensible shortage in the energy balance at the level of about 75% of the incoming energy. We have focused attention on the energy losses of plasmon–polaritons caused by the coupling of collective plasmons with another charged system in the nearfield zone. The coupling of dipole plasmon modes with closely located band electrons in a semiconductor opens a very quick, and thus effective, channel for energy transfer, which results in the strong damping of plasmon–polaritons in metallic nanochains deposited on or embedded in semiconductor surroundings. It should be emphasized that this channel of plasmon–polariton energy leakage is not of a radiative type because it happens on a subdiffraction scale with regard to the wavelength of the plasmon resonance. Depending on the nanosphere radii in the chain, different regimes for nearfield coupling with the semicoductor substrate occur. For ultrasmall nanoparticles with radii 2−3 nm the dipole coupling with the substrate electrons breaks the translation invariance and lifts the momentum conservation constraints imposed on interband electron transitions in the semiconductor. This greatly enhances the indirect (nonmomentumconserving) interband transition probability, resulting in the strong damping of plasmon–polaritons in the nanochain. With increasing nanoparticle size this effect gradually weakens but at about 5 nm nanoparticle radius (for Au or Ag) the interband transition probability again grows owing to the increase in the dipole amplitude in proportion to the number of oscillating electrons. Again plasmon–polaritons are strongly damped at this nanoparticle size scale. The damping of plasmon–polaritons due to nearfield coupling with the semiconductor surroundings typically exceeds by a factor 3 the Joule heat losses due to electron scattering in metallic nanoparticles, which means that, relatively easily, the latter energy dissipation can be balanced by inverted energy transfer from the surrounding or substrate semiconductor to the metallic nanochain, resulting in arbitrary longrange plasmon–polariton propagation in such a system.
11 Plasmons in Finite Spherical Ionic Systems
In this chapter the topic of soft plasmonics in finite electrolyte liquid systems bounded by insulating membranes is considered. Such systems can be encountered at the biocell organization level, taking into account that the characteristics of ion plasmons fall into the micrometre scale rather than the nanometre scale in metals because the masses of ions are at least three orders of magnitude larger than the mass of an electron. The lower density of ions in electrolytes compared with the density of electrons in metals may reduce the energy of plasmons by several orders of magnitude. Here a fully analytical description of surface and volume plasmons in a finite ionic microsystem is provided, allowing further applications.
In view of the plasmons and plasmon–polaritons found in metallic nanostructures, one can question whether there are similar charge fluctuations in other electrical systems such as electrolytes. A challenging problem that we will discuss here is the possibility of the occurrence of plasmon effects for ionic carriers similar to those for electrons. Many finite ionic systems in the form of an electrolyte closed by membranes are encountered in biological structures and questions arise of to what degree would plasmonic phenomena play a role in them and whether the radiative properties of plasmon fluctuations would also be as significant in ionic systems as they are in metals. It is reasonable that ionic plasmon effects would be found in other regions of energy and wavelength scale compared with those of metallic systems. One could expect that the energy of ionic plasmons would be much lower than that of electrons in metals and that the typical size of plasmonic finite systems would be of micrometre scale. Such ‘soft’ plasmonics would be linked with the functionality of biological systems, where the electricity is of ionic rather than electronic character. Cell signalling, membrane transfer, and nerve cell conductivity would serve as examples. For a theoretical model for ions we will adopt, as far as possible, an analogy to metallic nanospheres with plasmon excitations. Ionic systems are much more complicated than a metal crystal structure with free electrons. Therefore, the 252
11.1 Fluctuations of the Charge Density in a Spherical Electrolyte System
+ + + +A + +


B 

253
l = 1, m = 0, 1
l = 2, m = 0, 1, 2
l = 3, m = 0, 1, 2, 3 l=3,m=2
Figure 11.1 Dipole D(t) creation in a single sphere by the simplest surface plasmon oscillations, due to the symmetrical separation of ions A+ and B − (left); more complicated patterns of oscillation of surface plasmon charge distributions can be assigned, in the case of spherical symmetry, with various multipole numbers, l, m. The different greyscale intensities indicate distinct values of local charge density from negative to positive (right) (given in colour in [48]).
identification of an appropriate simplification of the approach to ionic systems is of primary significance. The model must be, however, efficient in repeating for ions in electrolytes the plasmon scenario known from metal electrons. Let us consider a finite spherical ionic system (e.g., a liquid electrolyte artificially enclosed with a membrane) and identify the plasmon excitations of ions in this system. We will determine their energies for various parameters of the ionic system with special attention paid to the radiation properties of the ionic plasmons. We will analyse ionic plasmon–polariton propagation in electrolytesphere chains with a prospective relationship to signalling in biological systems. Bearing in mind that metallic nanochains serve as very efficient wave guides for electromagnetic signals in the form of collective surface plasmon excitations of wave type called plasmon–polaritons, we will try to model similar phenomena in ionicsphere chains. For an initial model we will study a spherical or prolate spheroidal ionic conducting system with balanced charges, in analogy to the jellium model in a metal. In this model the positivecharge background is static and local fluctuations in electron liquid density, negative or positive against the background of the positive jellium, form plasmons in the nanoparticles [23]. In the case of an electrolyte we are dealing, however, with a different situation – in a binary electrolyte both the oppositely charged ions are similarly dynamical as they have similar masses; here there is no rigid jellium. 11.1 Fluctuations of the Charge Density in a Spherical Electrolyte System The problem of how to establish an adequate model for a multiionic system in order to grasp the essential properties of ionic plasmons is challenging. For a simple
254
Plasmons in Finite Spherical Ionic Systems
twocomponent ionic system (a binary electrolyte) we are dealing with an electrolyte with balanced negative and positive total charges. In equilibrium the charge cancellation is also local, corresponding to a uniform charge distribution of both signs. As there are two kinds of carrier, both carriers form density fluctuations, resulting in the violation of local electric equilibrium. The total compensation of both charge signs requires, however, that any density fluctuation in the negative charge must be accompanied by an in general distant, but ideally equivalent, positive ion fluctuation, and conversely. This means that effectively we have charge density fluctuations of both ion subsystems with respect to an equilibrium homogeneous neutral state. One can thus consider the local effective fluctuations of, let us say, the negative ions as positive or negative in charge value with respect to the uniform charge distribution assumed as ideally cancelled by a positive uniform background – a fictitious jellium in analogy to the case of a metal. In this way we can model a twocomponent ionic system by two singlecomponent ion systems with double jelliums of opposite sign. These oppositesign fictitious jelliums cancel each other. However, the oppositely charged ion fluctuations will mutually interact. For simplicity we will assume that the absolute values of the charges and the masses of the oppositely charged ions are the same, but the generalization to different ion characteristics is straightforward. To simplify the model along the lines described above let us consider a spherical system with radius a with balanced total charge consisting of ions with both sign and with uniform equilibrium density distributions n+(−) (r) = n(a − r) ((r) is the Heaviside step function and a is the sphere radius). We assume, for simplicity, the same absolute value of the charge of each plus or minuscharged ion. By m+(−) we denote the mass of a positive (negative) ion. Both masses are of the order of 104−5 me , where me = 9.1 × 10−31 kg is the mass of the electron. The reduction of the twocomponent system to two systems each with a fictitious jellium is an approximation, but it may serve for a tentative recognition of the ionic dynamics of the system and an assessment of the scales of its quantitative characteristics, at least. The advantage of such an approach is its close analogy to the description of plasmons in metals where the rigid shape of the system is imposed by the shape of a ‘real’ jellium – the crystal lattice. Given the abovementioned model assumptions we will consider ionic carriers with density oscillating around the zerovalued equilibrium density and balanced by a fictitious charged background of oppositesign ions (the effect of the simultaneous presence of the oppositesign ions). Thus the electrolyte is regarded as the sum of two subsystems corresponding to ions of each sign and each with own fictitious jellium. These jelliums mutually cancel. The uniform charge distributions of the ions of each sign also mutually cancel and an approximation is the assumption of the independence of the fluctuations in the two subsystems. In this way, an
11.2 Model Definition
255
approximate correspondence with the electron liquid in a metal within the jellium model is established. Hence, the description of fluctuations in the local density of electrons in a metallic nanosphere can be directly used to model fluctuations in the effective ion density, substituting the electron mass by the ion mass and the electronic charge by the ion charge. The dynamical equation for the charged fluid in the spherical ion system can be thus repeated from the case of the metal nanosphere with electrons. The equilibrium density of the effective charged liquid, denoted by n, will be treated as a parameter and will be assumed equal to ηN0 , where η is the molarity of the electrolyte in the sphere and N0 is the molar electrolyte concentration of ions. The equilibrium density determines the bulk plasmon frequency for the ion system according to the formula, ωp2 = 4πnq 2 /m, where m is the mass of an ion with charge q. As m is much larger than me and the concentration of the ions is usually smaller than that for electrons in metals, ωp can be considerably reduced, even by several orders of magnitude. Note that for electrons in metals h¯ ωp 10 eV and ωp typically falls into the ultraviolet region with corresponding photon energy. In an ionic system the plasmon frequency ωp can be much lower and is found in the infrared or even lowerenergy part of the electromagnetic spectrum. 11.2 Model Definition The Hamiltonian for a binary ion system has the form −
Hˆ ion = −
N h¯ 2 ∇ 2 i=1
i 2m−
+
−
N h¯ 2 ∇j2 j =1
2m+
−
−,N + N
i,j
−
q −q + εri − rj 
+
N N (q − )2 (q + )2 1 1 + + , 2 εri − ri  2 εrj − rj  i,i ,i=i
(11.1)
j,j j =j
where q −(+) , M −(+) , and N −(+) are the charges, masses, and number of −(+) ions, respectively. To analyse this complicated system we propose the following approximation, assuming, for simplicity, q − = −q + = q, N − = N + = N, m− = m+ = m. We next add and subtract the same terms, as written below: Hˆ ion = −
N h¯ 2 ∇ 2 i
i=1
+
2m
−
N h¯ 2 ∇j2 j =1
2m
−
i,j
q2 εri − rj 
N N q2 q2 1 1 + 2 εri − ri  2 εrj − rj  i,i ,i=i
j,j j =j
256
Plasmons in Finite Spherical Ionic Systems
n(r)d 3 r − q2 εrj − r j i n(r)d 3 r + q2 + q2 εr − r j j i
− q2
n(r)d 3 r εri − r n(r)d 3 r , εri − r
(11.2)
where we have introduced formally the fictitious jellium of spherical shape for both types of ions, with density n ideally compensating the opposite charges of the uniformly distributed ions, so that n(r) = n(a − r) where a is the sphere radius (the positive and negative jelliums mutually cancel). Assuming that n(r)d 3 r n(r)d 3 r q2 2 2 +q − 0, (11.3) q εrj − r εri − r εri − rj  j i i,j which is fulfilled for ion fluctuations that are not too far beyond the uniform distribution (in dilute ion systems), we can separate the original Hamiltonian into a sum, Hˆ ions = Hˆ − + Hˆ + , where ! 3 h¯ 2 ∇j2 r q2 n(r)d 1 −(+) 2 = −q + . (11.4) − Hˆ 2m εrj − r 2 εrj − rj  j j =j
The last term on the righthand side of Eq. (11.4) corresponds to the interaction between ions of the same sign, whereas the second term in the first sum describes the interaction of these ions with the jellium (of opposite sign); ε is the dielectric permittivity of the electrolyte medium. The confined electrolyte system can be shaped by an appropriately formed membrane, as frequently happens in biological systems. Because of the separation of the Hamiltonian (11.1) one can consider the single Hamiltonians (11.4). We will denote by ion (t) the ion wave function corresponding to the Hamiltonian (11.4). The form of (11.4) allows for further discussion according to the scheme applied to electrons in metals [23], which we recall below for the sake of completeness. The local density of the chosen type of ion can be written, in analogy to the semiclassical Pines–Bohm RPA approach to electrons in a metal [16, 14], in the following form: δ(r − rj ) ion (t) , (11.5) ρ(r,t) = ion (t) j where rj denotes the coordinate of the j th ion. The Fourier picture of the above density has the form, ˆ (11.6) ρ(k,t) ˜ = ρ(r,t)e−ik·r d 3 r = ion (t)ρ(k) ion (t), where the operator ρ(k) ˆ =
j
e−ik·rj .
11.2 Model Definition
257
Using the above notation one can rewrite Hˆ ion , (11.1), in the following form, in analogy to the metallic plasmon description presented in previous chapters [16, 23]: ! N * h¯ 2 ∇j2 2π ) ˆ+ q2 3 ˆ d k n(k) ˜ (k) + ρ(k) ˆ ρ − − Hion = 2m (2π)3 k2 j =1 ( ' q2 3 2π ˆ+ (k)ρ(k) d k ˆ − N , (11.7) ρ + (2π)3 k2 3 where n(k) ˜ = d r n(r)e−ik·r (we have taken into account that 4π /k 2 = 3 −ik·r/r 2 ), q = q 2 /ε. d re Utilizing this form of the effectiveion Hamiltonian one can write down the dynamic equation for the ion density fluctuations in the Heisenberg representation, ( ( d 2 ρ(k) ˆ 1 '' ˆ ion , Hˆ ion , = ρ(k), ˆ H dt 2 (i h) ¯ 2
(11.8)
in the following form:
2 h¯ 2 k 2 h¯ 2 h¯ 2 k 4 ˆ d 2 ρ(k) −ik·rj k · ∇ − = − e + ik · ∇ + j j dt 2 m2 m2 4m2 j 4πq 2 k·p d 3 p n(p) − ˜ ρ(k ˆ − p) 3 m(2π) p2 4πq 2 k·p d 3 p ρ(k − ˆ − p) 2 ρ(p). ˆ 3 m(2π) p
(11.9)
If one takes into account that ρ(k ˆ − p)ρ(p) ˆ = δ ρ(k ˆ − p)δ ρ(p) ˆ + n(k ˜ − p)δ ρ(p) ˆ + δ ρ(k ˆ − p)n(p) ˜ + n(k ˜ − p)n(p) ˜ and n(p) ˜ ρ(k ˆ − p) = n(p)δ ˜ ρ(k ˆ − p) + n(p) ˜ n(k ˜ − p), where δ ρ(k) ˆ = ρ(k) ˆ − n(k) ˜ describes the operator for local ion density fluctuations above the uniform distribution, one can rewrite Eq. (11.9) as follows,
2 h¯ 2 k 2 h¯ 2 h¯ 2 k 4 d 2 δ ρ(k) ˆ −ik·rj − 2 k · ∇j + 2 ik · ∇j + =− e dt 2 m m 4m2 j 4πq 2 k·p d 3 p n(k − ˜ − p) 2 δ ρ(p) ˆ 3 m(2π) p k·p 4πq 2 d 3 p δ ρ(k ˆ − p) 2 δ ρ(p). ˆ (11.10) − 3 m(2π) p
258
Plasmons in Finite Spherical Ionic Systems
Hence, for the ion density fluctuation, δ ρ(k,t) ˜ = ion δ ρ(k,t) ˆ ion = ρ(k,t) ˜ − n(k), ˜ one finds 2 2 2 2 4 −ik·r
h h h ˜ k k ∂ 2 δ ρ(k,t) 2 ¯ ¯ ¯ j − 2 k · ∇j + 2 ik · ∇j + = − ion e 2 ion ∂t 2 m m 4m j 2 4πq k·p d 3 p n(k − ˜ − p) 2 δ ρ(p,t) ˜ 3 m(2π) p k·p 4πq 2 d 3 p 2 ion δ ρ(k ˆ − p)δ ρ(p) ˆ (11.11) − ion . 3 m(2π) p For small k, in analogy to the semiclassical approximation for electrons [23, 16], the contributions of the second and third components to the first term on the righthand side of Eq. (11.11) can be neglected as being small in comparison with the first component. The third term on the righthand side of Eq. (11.11) is also negligible as it involves a product of two δ ρ˜ (which we assume to be small, δ ρ/n ˜ 1). This approach corresponds to the RPA formulated for the bulk metal [16, 14] (note that δ ρ(0) ˆ = 0 and the coherent RPA contribution of the interaction comprises the last but one term in Eq. (11.11)). Within the RPA, Eq. (11.11) thus attains the following shape: 2 2 h ∇ ¯ ˜ 2k ∂ δ ρ(k,t) j −ik·r j vion ion = e ∂t 2 3m 2m j 4πq 2 k·p d 3 pn(k − ˜ − p) 2 δ ρ(p,t). ˜ 3 m(2π) p 2
2
(11.12)
Owing to the spherical symmetry, 2 −ik·r h¯ 2 −ik·r h¯ 2 ∇j2
2 2k j j ion . ion ion k · ∇j ion e e m2 3m 2m j j
Thus one can rewrite Eq. (11.12) in the position representation as 2 2 h¯ ∇j ˜ ∂ δ ρ(r,t) 2 2 ion = − ∇ ion δ(r − rj ) ∂t 2 3m 2m j ωp2 1 3 ∇ (a − r)∇ d r1 δ ρ(r ˜ 1,t) . + 4π r − r1  2
(11.13)
11.2 Model Definition
259
In the case of metals the Thomas–Fermi formula is then used to obtain the average kinetic energy [16]: 2 2 2 h¯ ∇j ion 3 (3π 2 )2/3 h¯ (ρ(r,t))5/3 ion − δ(r − rj ) 2m 5 2m j (11.14) 2 δ ρ(r,t) ˜ h 3 5 ¯ = (3π 2 )2/3 n5/3 (a − r) 1 + + ··· . 5 2m 3 n The Thomas–Fermi formula applies, however, to fermionic and degenerate quantum systems such as electrons in metals. For ionic systems, such an estimation of the kinetic energy is inappropriate because the ion concentration is usually much lower than that of electrons in metals and the system is not degenerate even if the ions are fermions; the Maxwell–Boltzmann distribution should be applied instead of the Fermi–Dirac or Bose–Einstein distributions. Independently of whether the statistics of the ions are fermionic or bosonic, the Maxwell–Boltzmann distribution allows the estimation of the average kinetic energy of the ions located inside the spherical electrolyte with the radius a in the following form: 2 2 h¯ ∇j ion (n + δρ(r,t))(a − r) 3kB T , (11.15) δ(r − rj ) ion − 2m 2 j where kB is the Boltzmann constant and T is the temperature. For ions of an extended threedimensional or linear shape, inclusion of the rotational degrees of freedom results in a factor 6kB T /2 or 5kB T /2, respectively, instead of 3kB T /2 for the pointlike ion model. Using Eq. (11.15) and taking into account that ∇(a − r) = −(r/r)δ(a − r), one can rewrite Eq. (11.13) in the following manner:
∂ 2 δ ρ(r,t) ˜ kB T 2 2 = ˜ − ωp δ ρ(r,t) ˜ (a − r) ∇ δ ρ(r,t) ∂t 2 m 6 /r k B T 5. − ∇ n + δ ρ(r,t) ˜ δ(a − r) m r ! 2 ωp r 1 kT r − ∇δ ρ(r,t) ˜ + ∇ d 3 r1 δ ρ(r ˜ 1,t) δ(a − r). m r 4π r r − r1  (11.16)
In the above formula ωp is the bulkion plasmon frequency, ωp2 = 4πnq 2 /m. The solution of Eq. (11.16) can be decomposed into two parts relating to distinct domains, inside the sphere and on its surface: for r < a, δ ρ˜1 (r,t) (11.17) δ ρ(r,t) ˜ = for r ≥ a (r → a+) δ ρ˜2 (r,t)
260
Plasmons in Finite Spherical Ionic Systems
The two parts of Eq. (11.17) correspond to volume and surface excitations, respectively. They satisfy equations derived from Eq. (11.16)): kB T 2 ∂ 2 δ ρ˜1 (r,t) = ∇ δ ρ˜1 (r,t) − ωp2 δ ρ˜1 (r,t) 2 ∂t m
(11.18)
and (here = 0+) 6 /r kB T 5. ∂ 2 δ ρ˜2 (r,t) = − (r,t) ∇ n + δ ρ ˜ δ(a + − r) 2 ∂t 2 m r 2 ωp r kB T r 1 ∇δ ρ˜2 (r,t) + ∇ d 3 r1 − (δ ρ˜1 (r1,t)(a − r1 ) m r 4π r r − r1  +δ ρ˜2 (r1,t)(r1 − a)) δ(a + − r). (11.19) The Dirac delta in Eq. (11.19) results from the derivative of the Heaviside step function describing the fictitious jellium distribution shape. In Eq. (11.19) an infinitesimal shift, = 0+, is introduced to fulfil requirements of the Dirac delta definition (its singular point has to be an inner point of an open subset of the domain). This shift is only of a formal character and does not reflect any asymmetry. Some kind of asymmetry is, however, caused by the last term in Eq. (11.16), the gradienttype term, which describes the electric field induced by iondensity fluctuations. The electric field due to the surface charges is zero inside the sphere, and therefore cannot influence the volume excitations. Conversely, the volumechargefluctuationinduced electric field can excite surface fluctuations. This asymmetry is visible by comparison of Eqs. (11.18) and (11.19) for the volume and surface plasmons, respectively. The equation for the volume plasmons is completely independent of the surface plasmons, whereas the volume plasmons contribute to the equation for the surface plasmons. The problem of separating the surface and volume plasmons has been thoroughly analysed for metal. For very small nanoparticles the effect of spillout of electrons beyond the jellium edge, significant at this size scale, makes the surface fuzzy, resulting in coupling of the volume and surface plasmon oscillations. By direct numerical simulations using the timedependent local density approximation (TDLDA) [19, 20], it has been proved that the coupling of the volume and surface excitations gradually disappears in larger nanoparticles (with the number of electrons exceeding about 60) [19, 20], which supports the accuracy of the semiclassical RPA description, within which volume plasmons can be separated from the surface plasmons (even though, as mentioned above, the latter can be excited by the former owing to the last term in Eq. (11.19)). This volume–surface coupling, important for ultrasmallradii metallic nanoparticles, when the shell effects and
11.3 Solution of RPA Plasmon Equation
261
quantum spillout are significant, completely disappears, however, with growth in the sphere dimension to several nanometres in the case of metals. We consider here a binary electrolyte system with radius of order a micrometre, when quantum effects specific for ultrasmall clusters are negligible. This gives us the opportunity to formulate an analytical RPA semiclassical description in the form of an oscillator equation, allowing for the phenomenological inclusion of damping effects. The energy dissipation effects, though going beyond the RPA model, turn out to be the overwhelming physical property in the case of larger metallic nanospheres [23, 77] (with a > 10 nm for Au or Ag) and also for much larger ionic systems, as we will demonstrate below. 11.3 Solution of RPA Plasmon Equation: Volume and Surface Plasmon Frequencies in a Spherical Finite Ion System Equations (11.18) and (11.19) have been solved for metallic nanospheres [23] and these solutions can be directly applied to ionic systems. To summarize briefly this analysis, the two parts of the plasma fluctuation can be represented as follows: . / for r < a, δ ρ˜1 (r,t) = n f1 (r) + F (r,t) for r ≥ a (r → a+), δ ρ˜2 (r,t) = nf2 (r) + σ ( ,t)δ(r + − a), = 0 + , (11.20) with initial conditions F (r,t)t=0 = 0 and σ ( ,t)t=0 = 0 ( represents the spherical coordinate angles) and also the continuity condition (1 + f1 (r))r=a = f 2 (r)r=a ,3 the boundary condition F (r,t)r=a = 0, and the neutrality condition ρ(r,t)d r = N . Neglecting the static contributions f1,2 describing the spillout effect, which decreases sharply with growth in the system size [23], one can write out the timedependent parts of the ion concentration fluctuations in the form ∞ ∞ l Almn jl (knl r)Ylm ( ) sin(ωli t), (11.21) F (r,t) = l=1 m=−l i=1
and σ ( ,t) =
∞ l Blm Y ( ) sin(ω0l t) 2 lm a l=1 m=−l
+ ×
∞ ∞ l
Almn
(l + 1)ωp2
lωp2 − (2l + l=1 m=−l i=1 a r l+2 dr1 1l+2 jl (kli r1 ) sin(ωli t), a
0
1)ωli2
Ylm ( )ne
(11.22)
262
Plasmons in Finite Spherical Ionic Systems Spherical Bessel functions Jl
a
1.0
1.0 × 108
0 l
1
0.4 l
0.2
2
0.0
(1/s)
l
0.6
8.0 × 107
li
0.8
l
50 m ionic sphere
1.2 × 108
6.0 × 107 4.0 × 10
− 0.2 0
5
10 r
15
20
l= 1,i= 2 l= 2,i= 1
7
2.0 × 107 200
l= 1,i= 1
220
240
260
280
300
Temperature (K)
Figure 11.2 The spherical Bessel functions Jl (r) for l = 0,1,2 displaying charge density fluctuations in a nanosphere along the sphere radius r (arbitrary units) for volume plasmon modes; the angular distribution for these modes is governed by the spherical harmonics Ylm ( ) in the same way as for the surface plasmon modes (see Fig. 11.1 (right)). The exemplary temperature dependence of the selffrequencies of the volume plasmon modes ωli , li = 11, 12, 21, for a dilute electrolyte with n 1014 /m3 and ion mass ∼ 104 me , a ∼ 50 μm (right).
√ π/2ξ Il+1/2 (ξ ) is a spherical Bessel function, Ylm ( ) is a spherical harmonic, ωli = ωp 1 + kB T xli2 /(ωp2 a 2 m) are the frequencies of the ion volume selfoscillations (the volume plasmon frequencies), xli are the nodes of the Bessel function jl (ξ ) enumerated by i = 1,2,3, . . . (see Fig. 11.2), kli = xli /a, √ and ωl0 = ωp l/(2l + 1) are the frequencies of the ion surface selfoscillations (the surface plasmon frequencies). The derivation of the selffrequencies for ionic plasmon oscillations is presented in full detail in the final section of this chapter. The amplitudes Almi and Blm are arbitrary in the homogeneous problem and are determined by the initial conditions. The function F (r,t) describes volume plasmon oscillations, whereas σ ( ,t) describes the surface plasmon oscillations. Let us emphasize that the first term in Eq. (11.22) corresponds to surface selfoscillations, while the second term describes the surface oscillations induced by the volume plasmons. The frequencies of the surface selfoscillations are equal to & l , (11.23) ω0l = ωp 2l + 1 where jl (ξ ) =
which, for l = 1, is the dipoletype surface √ oscillation frequency, described for a metallic nanosphere by Mie [18], ω01 = ωp / 3. 11.3.1 Ionic Surface Ion Plasmon Frequencies for an Electrolyte Nanosphere Embedded in a Dielectric Medium with ε1 > 1 One can now include the influence of dielectric surroundings (in general, distinct from the inner medium of the ionic system under consideration) on the plasmons in
11.4 Damping of Plasmon Oscillations in Ionic Systems
263
this system. In order to do this let us assume that the ions on the surface (r = a+, i.e., r ≥ a, r → a) interact via Coulomb forces renormalized by the relative dielectric permittivity ε1 > 1 (which is distinct from the dielectric permittivity ε for the inner medium). Thus a small modification of Eq. (11.19) is in order:
2 r ∂ 2 δ ρ˜2 (r) 3 =− ∇ F n + F δ ρ˜2 (r,t) δ(a + − r) ∂t 2 3m 5 r 2 ωp r 2 F r 1 3 δ ρ˜1 (r1,t)(a − r1 ) ∇δ ρ˜2 (r,t) + ∇ d r1 − 3mr 4π r r − r1  1 (11.24) + δ ρ˜2 (r1,t)(r1 − a) δ(a + − r) ε1 (note that Eq. (11.18) is not affected by the outer medium). The solution of the above equation is of the same form as that for Eq. (11.19) but with renormalized surface plasmon frequencies 1 1 l . (11.25) ω0l = ωp 2l + 1 ε1 11.4 Damping of Plasmon Oscillations in Ionic Systems The semiclassical RPA treatment of plasmon excitations in finite ion systems as presented above does not account for plasmon damping. The damping of plasmon oscillations can be included, however, in a phenomenological manner, by the addition of an attenuation term to the plasmon dynamic equations; i.e., the term −(2/τ0 )∂δρ(r,t)/∂t is added to the righthand sides of both Eqs. (11.18) and (11.19), taking advantage of their oscillatory form. The damping rate 1/τ0 accounts for ion scattering losses and can be approximated, in analogy to metallic systems, by the inclusion of energy dissipation caused by its irreversible transformation into heat via various microscopic channels similar to those for ohmic resistivity [24], v Cv 1 + , τ0 2λb 2a
(11.26)
√ where a is the sphere radius, v is the mean velocity of the ions, v = 4kB T /(3m), and λb is the ion mean free path in the bulk electrolyte material (it includes the scattering of ions on other ions and on solvent particles and admixtures). The second term in Eq. (11.26) accounts for the scattering of ions at the boundary of the finite ionic system, for a sphere with radius a; the constant C is of the order of unity [24]. In order to express a forcing field which moves ions in the system, an inhomogeneous timedependent term should be added to the homogeneous equations (11.18)
264
Plasmons in Finite Spherical Ionic Systems
and (11.19). The forcing field may be a timedependent electric field. If one considers it to be the electric component of the incident electromagnetic wave then a comparison of the resonance wavelength with the system size is in order. As for metallic nanospheres, for finite ionic systems also the surface plasmon resonance wavelength greatly exceeds the system dimension and thus the forcing field is practically uniform across the whole system. Such a perturbation can excite only surface dipole plasmons, i.e., the mode with l = 1, which can be described by the function Q1m (t) (l = 1 and m are the angular momentum quantum numbers relating to the assumed spherical symmetry of the system). The corresponding dynamical equation for surface plasmons reduced to only the mode Q1m (t) has the following form: 2 ∂Q1m (t) ∂ 2 Q1m (t) + + ω12 Q1m (t) ∂t 2 τ0 ∂t & √
( 4π qn ' Ez (t)δm,0 + 2 Ex (t)δm,1 + Ey (t)δm,−1 , = (11.27) 3 m √ where ω1 = ωp / 3ε1 for a dipole surface plasmon frequency, i.e., the Mie frequency [18] and ε1 is the relative dielectric permittivity of the system surroundings. Because only the Q1m contribute to the plasmon response to the homogeneous electric field, the effective iondensity fluctuation has the form [23] ⎧ r < a, ⎨ 0, 1 (11.28) δρ(r,t) = Q1m (t)Y1m ( ), r ≥ a, r → a + , ⎩ m=−1
where Ylm ( ) is a spherical harmonic with l = 1. One can also explicitly calculate the dipole D(t) corresponding to the surface plasmon oscillations given by Eq. (11.28): ⎧ 3 2π ⎪ (t) = q d rxδρ(r,t) = eQ1,1 (t)a 3, D ⎪ ⎪ 3 ⎨ x (11.29) eQ1,−1 (t)a 3, Dy (t) = q d 3 ryδρ(r,t) = 2π 3 ⎪ ⎪ ⎪ ⎩ D (t) = q d 3 rzδρ(r,t) = 4π eQ (t)a 3 . z 1,0 3 The dipole D(t) satisfies the equation (if one rewrites Eq. (11.27)),
2 a 3 4πq 2 n 2 ∂ ∂ 2 D(t) = + + ω E(t) = εa 3 ω12 E(t). 1 ∂t 2 τ0 ∂t 3m
(11.30)
Notice that the dipole (11.29) scales as the system volume, i.e., as a 3 , which may be interpreted as indicating that all ions actually contribute to the surface plasmon oscillations. This is connected with the fact that the surface modes correspond
11.4 Damping of Plasmon Oscillations in Ionic Systems 4
2
0.006 0.005 0.004 0.003 0.002 0.001 0.000
m=104m , q=3e, n=103 N , T=300K
0.015
radiation losses ~a3 1
1
m=10 me, q=3e, n=10 N0, T=300K
265
radiation losses ~a3
0.010 ion scattering ~1/a
ion scattering ~1/a
0.005 0.000
0
20 40 60 80 100 120 140 a (10 nm)
0
100
200 300 a (10 nm)
400
500
Figure 11.3 The crossover in the ionic system size dependence of the damping rate for surface plasmons, for T = 300K, m = 104 me , q = 3e, for n = 10−2 N0 (N0 is the molar concentration of the electrolyte) (left) and for n = 10−3 N0 (right); the ion scattering losses, ∼ 1/a, are of decreasing importance with increasing electrolytesphere size (a is the sphere radius), whereas the radiation losses dominate at larger sizes as they initially grow as a 3 ; in the size region close to the crossover a perturbative treatment for the Lorentz friction agrees with the exact approach.
to uniformtranslationtype oscillations of ions in the system, for which, inside the sphere, the charges of the ions are exactly compensated by oppositely signed ions, whereas an unbalanced charge density occurs only on the surface despite the fact that all the ions oscillate. For the volume plasmons, noncompensated chargedensity fluctuation are present also inside the sphere as the volumeplasmon modes have a compressional character with unbalanced charge fluctuations along the sphere radius. The scattering effects accounted for by the approximate formula (11.26) cause especially strong damping of plasmons for a small system, owing to the nanosphereedge scattering contribution, proportional to 1/a. This term is, however, of less significance with increase in radius. We will show that the radiation losses due to the accelerated movement of ions scale as a 3 and, for increasing a, these radiative energy losses quickly dominate the overall plasmon attenuation. The opposite size dependences of the scattering and radiation contributions to the plasmon damping one observes a crossover in damping with respect to size dependence, as is depicted in Fig. 11.3. One can also determine the radius a ∗ for which the total attenuation rate for surface plasmons is minimal: 1/4 3/2 3 3 Cc v . a∗ = 2ω1 ωp3 The minimal sizes a ∗ for two distinct ionic system arrangements are listed in Table 11.1.
266
Plasmons in Finite Spherical Ionic Systems
Table 11.1 The ionsystem parameters assumed for the calculation of damping rates and selffrequency for dipole surface plasmons Material
Ionic system
Sample 1
Sample 2
ion concentration effective ion mass charge of effective ion temperature mean velocity of ions bulk plasmon frequency dielectric permittivity of surroundings Mie frequency constant in Eq. (11.26) bulk mean free path (room temperature)
n (N0 is one mole of electr.) m (m √ e electron mass) q/ ε T √ v = 3kT /m ωp ε1
10−2 N0 104 me 3e 300 K 1168 m/s 9.3 × 1013 /s 2
10−3 N0 104 me 3e 300 K 1168 m/s 2.93 × 1012 /s 2
√ ω1 = ωp / 3ε1 C λb
3.8 × 1013 /s 2 0.5 μm
1.2 × 1012 /s 2 0.1 μm
radius for minimal damping
a∗
2.7 × 10−7 m
8.6 × 10−7 m
=
33/2 Cc3 v 2ω1 ωp3
1/4
The radiation of energy from an oscillating dipole is expressed by the socalled Lorentz friction [55], viewed as an effective electric field slowing down the motion of charges: √ 2 ε ∂ 3 D(t) . (11.31) EL = 3c3 ∂t 3 Hence, we can rewrite Eq. (11.30) including the Lorentz friction term as
2 2 ∂ ∂ 2 + + ω1 D(t) = εa 3 ω12 E(t) + εa 3 ω12 EL, ∂t 2 τ0 ∂t or, for E = 0, !
2 3 2 ∂ a ∂ ∂ ω 2 2 p + ω12 D(t) = D(t) . − D(t) + √ ∂t 2 ∂t τ0 3ω1 c 3 ∂t 2
(11.32)
(11.33)
Now one can apply the perturbation method for the solution of Eq. (11.33), treating the righthand side.of this equation zeroth step of the per/ as the perturbation. In the 2 2 2 2 turbation we have ∂ /∂t + ω1 D(t) = 0, from which (∂ /∂t 2 )D(t) = −ω12 D(t). Hence, for the first step of the perturbation, we insert the latter formula into the righthand side of Eq. (11.33), obtaining
2 2 ∂ ∂ 2 (11.34) + + ω1 D(t) = 0, ∂t 2 τ ∂t
11.4 Damping of Plasmon Oscillations in Ionic Systems
where
267
ωp a 3 . (11.35) √ c 3 Within the first perturbation step, the Lorentz friction can be included in the total attenuation rate 1/τ . Nevertheless, this approximation is justified only for sufficiently small perturbations, i.e., when the second term in Eq. (11.35), proportional to a 3 , is small enough to fulfil the perturbation restrictions. The related limiting value, a, ˜ of the ionic system size depends on the ion concentration, charge, mass, and dielectric permittivity, as is exemplified in the next subsection. The solution of Eq. (11.34) is of the form D(t) = Ae−t/τ cos(ω1 t + φ), where ω1 = ω1 1 − 1/(ω1 τ )2 , which gives the redshift of the plasmon resonance due to the strong, ∼ a 3 , growth of the attenuation caused by radiation. The Lorentz friction term in Eq. (11.35) dominates the plasmon damping for a ≤ a˜ owing to this a 3 dependence; see Fig. 11.3. The plasmon damping grows rapidly with a and this results in a pronounced redshift of the resonance frequency. ω1 1 1 + = τ τ0 3
11.4.1 Exact Inclusion of the Lorentz Damping Now we will consider the dynamic equation for surface plasmons in the ionic spherical system in Eq. (11.33) with the Lorentz friction term, but without using the perturbation method of solution, which results in the substitution of the Lorentz friction term ωp a 3 ∂ 3 D(t) 2 √ 3ω1 v 3 ∂t 3 with the approximate formula,
ωp a 3 ∂D(t) ; √ ∂t v 3 this was the result of taking on the righthand side of Eq. (11.33) the zeroth order 2 = −ω12 D(t). To compare the various contributions to solution, for which ∂ ∂tD(t) 2 Eq. (11.33) we change to a dimensionless variable: t → t = ω1 t. Then Eq. (11.33) attains the form ∂ 2 D(t ) 2 ∂D(t ) 2 ωp a 3 ∂ 3 D(t ) + + D(t ) = . (11.36) √ τ0 ω1 ∂t 3 v 3 ∂t 2 ∂t 3 2ω1 − 3
If we solve Eq. (11.36) by the perturbation method we get a renormalized attenuation rate for the effective damping term, 1 ωp a 3 1 + . √ ω1 τ 0 3 v 3
268
Plasmons in Finite Spherical Ionic Systems
This term quickly achieves the value 1, for which the oscillator falls into the overdamped regime. For the system parameters assumed for Fig. 11.3, the atten−3 uation rate reaches 1 at radii 25.5 μm and 8 μm for n = 10 N0 and for −2 n = 10 N0 , respectively. At these values the frequency ω1 = ω1 1 − 1/(ω1 τ )2 goes to zero, which indicates an artefact of the perturbation method. To verify how the exact damped frequency behaves in the system under consideration one needs to solve the dynamical equation without any approximations. As this equation is a thirdorder linear differential equation, one finds that its solution is in the form ∼ ei t , with analytical expressions for three possible values of the exponent,
1 = −
−
i21/3 (1 + 6gu) ) *1/3 3g 2 + 27g 2 +18gu + 4( − 1 − 6gu)3 + (2 + 27g 2 +18gu)2 ) *1/3 i 2 + 27g 2 + 18gu + 4( − 1 − 6gu)3 + (2 + 27g 2 + 18gu)2 i − 3g
∈ Im(= iα), i
2 = − 3g
3 × 21/3 g
√ i(1 + i 3)(1 + 6gu) + ) *1/3 3 × 22/3 g 2 + 27g 2 + 18gu + 4( − 1−6gu)3 + (2 + 27g 2 +18gu)2 *1/3 √ ) i(1 − i 3) 2 + 27g 2 +18gu + 4( − 1−6gu)3 + (2 + 27g 2 +18gu)2 + 6 × 21/3 g 1 = ω+i , τ i
3 = − 3g √ i(1 − i 3)(1 + 6gu) + ) *1/3 3 × 22/3 g 2 + 27g 2 + 18gu + 4( − 1−6gu)3 + (2 + 27g 2 +18gu)2 *1/3 √ ) i(1 + i 3) 2 + 27g 2 +18gu + 4( − 1−6gu)3 + (2 + 27g 2 +18gu)2 + 6 × 21/3 g 1 = −ω+i , τ (11.37)
11.4 Damping of Plasmon Oscillations in Ionic Systems 4
269
3
0.8
0.8 1)
0.6
( )
1.0
0.6
(
(
1)
m=10 me, q=3e, n=10 N0, T=300K 1.0
0.4
0.4
0.2
0.2
0.0 0
0.0
1000 2000 3000 4000 5000 a (10 nm)
0
0.00045 0.00040 0.00035 0.00030 0.00025 0.00020 0.00015 0
1000 2000 3000 4000 5000 a (10 nm)
1000 2000 3000 4000 5000 a (10 nm)
0.8 0.6
(
0.6
0.00014 0.00012 ( )
0.8 1)
1.0
(
1
)
m=104me, q=3e, n=102 N0, T=300K 1.0
0.4
0.4
0.2
0.2
0.00008 0.00006 0
0.0
0.0 0
200 400 600 800 1000 1200 a (10 nm)
0.00010
0
200 400 600 800 1000 1200 a (10 nm)
200 400 600 800 10001200 a (10 nm)
Figure 11.4 For comparison, the damping rate and the resonance frequency (transformed to the resonance wavelength in the righthand panels). The damping rate and frequency or wavelength of the oscillating solution of Eq. (11.36) are given: exact values (solid line) and approximate values from the perturbation approach (dashed line), both as functions of the ionic finite system radius a.
where 1 u= τ 0 ω1
and
2 g= 3
aωp √ c 3ε1
3 .
In Fig. 11.4 the damping rate (Im ) is plotted and the selffrequency (Re ) (in terms of the resonance wavelength with righthand panels) in terms of the system radius a. For comparison, the approximate perturbative solutions are plotted as dashed lines, whereas the exact solutions of Eq. (11.36) are plotted as solid lines. The dashed lines finish at alimit , when the attenuation rate within the perturbation approach reaches the critical value 1 (then λ → ∞). For the accurate solution of Eq. (11.36) this singular behaviour completely disappears and the oscillating solution, ei t , exists for larger a as well. We notice that the redshift of the plasmon resonance is strongly overestimated in the framework of the perturbative approach to the Lorentz friction unless a < a, ˜ where a˜ is sensitive to the ionic system parameters and especially to the ion concentration (as is demonstrated in Fig. 11.4). Let us emphasize that Eq. (11.36) has in general two types of particular solu tions ei t , with complex selffrequencies . The solutions given by 2 and 3 (see Eq. (11.37)) are of oscillating type with damping (i 2 and i 3 are mutually conjugate: 2 and 3 have real parts of opposite sign but the same imaginary parts;
270
Plasmons in Finite Spherical Ionic Systems
the latter is positive, giving the damping rate). The second type of solution is given by 1 , which turns out to be an unstable exponentially rising solution (a negative imaginary solution). This unstable solution is the wellknown artefact in Maxwell electrodynamics (see, e.g., Section 75 in [55]) and corresponds to the infinite selfacceleration of the free charge due to the Lorentz friction force (i.e., to the singular solution of the equation m˙v = const. × v¨ , which is associated with a formal renormalization of the fieldmass of the charge – infinite for a pointlike charge and cancelled in an artificial manner by an arbitrary assumed negative infinite nonfield mass, resulting in the ordinary mass of, e.g., an electron, which is, however, not defined mathematically in a proper way). This unphysical singular particular solution should be thus discarded. The other, oscillatorytype, solution resembles the solution for an ordinary damped harmonic oscillator, though with a distinct attenuation rate and frequency. The latter are expressed by the analytical formulae for 2 and 3 in Eqs. (11.37) and can be calculated for various a and compared with the corresponding quantities found within the perturbation approach. This comparison is presented in Fig. 11.4. It can be clearly seen that the perturbation approach leads to considerable overestimation of the damping rate for a > a. ˜ Therefore, we can conclude that the use of the approximate formula for the Lorentz friction damping in the form (11.35) is justified only up to a a, ˜ while for a > a, ˜ these approximate values strongly differ from the exact ones. The value a˜ < alimit depends sharply on the ionic system parameters; approximately, a˜ alimit /2. 11.5 Derivation of Plasmon Frequencies for a Finite Electrolyte System 11.5.1 Volume Ionic Plasmons In order to determine the selffrequencies of the volume ionic plasmon in the nansphere we must solve Eq. (11.18), the form of the relevant solution being given by Eq. (11.20). For the initial conditions listed below Eq. (11.20) we also assume that F (r,t) = Fω (r) sin(ωt) and, by substitution of this function into Eq. (11.18), we get Fω (r) + k 2 Fω (r) = 0,
(11.38)
where k 2 = (ω2 − ωp2 )m/(kB T ). This is a wellknown Helmholtz differential equation, of which solutions (finite at the origin) can be expressed in terms of the spherical Bessel functions (for the radial dependence of Fω (r)), Fω (r) = Ajl (kr)Ylm ( ), (11.39) √ where jl (x) = π/(2x)Il+1/2 (x) is the lth spherical Bessel function, linked to the Bessel function of first kind. The boundary condition, F (a) = 0, gives the
11.5 Derivation of Plasmon Frequencies for a Finite Electrolyte System
271
quantization of k, kli = xli /a, where xli is the ith zero of the lth Bessel function (see Fig. 11.2 (left)). Following this quantization one arrives at the corresponding selffrequency quantization, kB T xli 2 2 (11.40) ωli = ωp 1 + 2 2 . ωp ma Thus, the volume ionic plasmons in the sphere are described by the functions δρ1 (r,t) = n
∞ ∞ m=l
Almi jl (kli r)Ylm ( ) sin(ωli t),
(11.41)
l=1 m=−l i=1
where the Almi are arbitraryconstants. The component with l = 0 vanishes √ because a 2 of the neutrality condition, 0 r drd F (r,t) = 0 (as d Ylm ( ) = 4πδl0 δm0 , d = sin ddφ). Note that in ionic systems, the selffrequencies of the volume plasmons in the sphere are temperature dependent – see Eq. (11.40) and Fig. 11.2 (right).
11.5.2 Surface Ionic Plasmons In order to determine the selffrequencies for surface plasmons, one has to consider Eq. (11.19) and the solution for it given by Eq. (11.20). The first term on the righthand side of Eq. (11.19) can be rewritten in the form kB T kT ∇(n + δρ2 )∇(a − r) + (n + δρ2 ) m m kB T kB T 1 ∂ ∂ =− δ(a − r) (n + δρ2 ) − (n + δρ2 ) 2 [r 2 δ(a − r)] m ∂r m r ∂r / kB T 1 ∂ . =− (11.42) (n + δρ2 )r 2 δ(a − r) , m r 2 ∂r where we have used the formulae ∇(a − r) = (−r/r)δ(a − r), (r/r)∇ = ∂/∂r. The next term on the righthand side of Eq. (11.19) can be transformed into 3 ωp2 r r d r1 δρ(r1 ) kB T δ(a − r) ∇δρ2 − δ(a − r) ∇ − m r 4π r r − r1  3 2 ωp d r1 δρ(r1 ) kB T ∂ ∂ =− δ(a − r) δρ2 − δ(a − r) . (11.43) m ∂r 4π ∂r r − r1  Equation (11.19) thus attains the form / kB T 1 ∂ . ∂ 2 ρ2 2 (n + δρ = − )r δ(a − r) 2 ∂t 2 m r 2 ∂r 3 ωp2 d r1 δρ(r1 ) kB T ∂ ∂ − δ(a − r) δρ2 − δ(a − r) . m ∂r 4π ∂r r − r1 
(11.44)
272
Plasmons in Finite Spherical Ionic Systems
We suppose the solution of the above equation to be in the form δρ2 = σ ( ,t)δ(a + of Eq. (11.44) by r 2 , and integrate with respect to r in 0+ − r), multiply both Lsides arbitrary limits, i.e., l r 2 dr · · · , such that a ∈ (l,L) (this integration removes the Dirac deltas), which leads to the equation a
2∂
2
L
σ ( ,t) kB T =− 2 ∂t m
dr
/ ∂ . (n + δρ2 )r 2 δ(a − r) ∂r
l
kB T − σ ( ,t) m
L r 2 drδ(a − r)
∂ δ(a − r) ∂r
l
−
−
ωp2
L
4π ωp2
∂ r 2 drδ(a − r) ∂r
∞
l
a
L
a
∂ r drδ(a − r) ∂r 2
4π l
r12 dr1
d
δρ2 (r2 ) r − r1 
d
δρ1 (r1 ) . r − r1 
r12 dr1
0
(11.45)
The two first terms on the righthand side of the above equation vanish because kB T − m
L dr
/ / ∂ . kB T . (n + δρ2 )r 2 δ(a − r) = − (n + δρ2 )r 2 δ(r − a) Ll = 0 ∂r m
l
(11.46) and L
∂ r drδ(a − r) δ(a − r) = a 2 ∂r
L
2
l
dr
1 ∂ 2 δ (a − r) 2 ∂r
l 2
a 2 δ (a − r)Ll 2 μ 1 a2 = δ(a − r)Ll = 0. (11.47) lim 2 2 μ→0 π μ + (a − r)2
=
The last two terms on the righthand side of Eq. (11.45) can be transformed using the formula [72] 1
= 1 + z2 − 2z cos γ
∞ l=0
Pl (cos γ )zl
for z < 1,
11.5 Derivation of Plasmon Frequencies for a Finite Electrolyte System
273
l
∗ where Pl (cos γ ) = 4π/(2l + 1) m=−l Ylm ( )Ylm ( ) are Legendre polynomials. This formula leads to the following: ⎧ ∞ la l−1 ⎪ ⎪ P (cos γ ) for a < r1, ⎨ r l+1 l 1 ∂ l=0 1 (11.48) = ∞ (l+1)r1l ∂a a − r1  ⎪ ⎪ Pl (cos γ ) for a > r1, ⎩ − a l+2 l=0
where a = ar/r, cos γ = a · r1 /(ar1 ). Employing Eq. (11.48), the last two terms in Eq. (11.45) can be transformed as follows: −
L
ωp2 4π
∂ r 2 drδ(a − r) ∂r
∞
d 1
a
l
=−
r12 dr1
ωp2 4π
a2
∞ r12 dr1 δρ2 (r1 )
d 1 a
=−
ωp2 4π
a
2
δρ2 (r1 ) r − r1 
1 ∂ ∂a a 2 + r 2 − 2ar cos γ 1 1
∞ r12 dr1 σ ( 1 )δ(a
d 1
+ 0 + −r1 )
l=0
a
∞ la l−1
r1l+1
Pl (cos γ )
∞ l 1 4πl ∗ Ylm ( )Ylm ( 1 ) 4π a 2 l=0 2l + 1 m=−l ∞ l l 2 2 ∗ ( 1 ) = −ωp a Ylm ( ) d 1 σ ( 1 )Ylm 2l + 1 l=0 m=−l
=−
ωp2
a2
d 1 σ ( 1 )
and −
ωp2
L
4π
∂ r 2 drδ(a − r) ∂r
l
=−
=
a
r12 dr1
d 1
0
ωp2 4π
ωp2 4π
a2
a
= ωp2 n
2
a r12 dr1 nF (r1,t)
d 1 0
d 1 nF (r1,t)
∞ l+1 Ylm ( ) 2l + 1 l=0
1 ∂ ∂a a 2 + r 2 − 2ar cos γ 1 1
∞ (l + 1)r l
1
l=0 a
a l+2
r12 dr1 0
δρ1 (r1 ) r − r1 
r1l al
Pl (cos γ )
(11.49)
274
Plasmons in Finite Spherical Ionic Systems
×
l1 ∞ l1 =1 m1 =−l1
= ωp2 n
∞ l=0
Almi jl1 (kl1 i r1 ) sin(ωl1 i t)
∗ d 1 Ylm ( 1 )Yl1 m1 ( 1 )
i
l+2 l+1 r1 dr1 jl (kli r1 ) sin(ωli t). (11.50) Ylm ( )Almi 2l + 1 al m=−l i a
l
0
Equation (11.45) thus attains the form ∞ l ∂ 2 σ ( ,t) l 2 2 ∗ = −ωp a ( 1 ) Ylm ( ) d 1 σ ( 1 )Ylm 2 ∂t 2l + 1 l=0 m=−l l+2 ∞ l l+1 r1 dr1 2 jl (kli r1 ) sin(ωli t). + ωp n Ylm ( )Almi 2l + 1 al l=0 m=−l i a
0
(11.51) Assuming now that σ ( ,t) = the above equation, we obtain
∞ l l=0
m=−l
qlm (t)Ylm ( ) and inserting this into
∞ l l=0
∞ l ωp2 l ∂ 2 qlm (t) Ylm ( ) =− Ylm ( )qlm (t) ∂t 2 2l + 1 m=−l l=0 m=−l
+ ωp2 a ×
∞ l l+1 Ylm ( )Alm 2l + 1 l=1 m=−l i
r1l+2 dr1 jl (kli r1 ) sin(ωli t). a l+2
(11.52)
0
From the above equation we notice that for l = 0 we get ∂ 2 q00 /∂t 2 = 0 and thus q00 (t) = 0 (as q(0) = 0 and limt→∞ q(t) < ∞). For l ≥ 1 we obtain ωp2 l ∂ 2 qlm (t) l+1 = − (t) + ωp2 q Alm n lm 2 ∂t 2l + 1 2l + 1 i
a
r1l+2 dr1 jl (kli r1 ) sin(ωli t), a l+2
0
(11.53) which induces the following solution form: & l Blm 2 qlm (t) = sin ωp t a 2l + 1 +
i
Alm
(l + 1)ωp2
a n 2
ωp2 − (2l + 1)ωli
0
r1l+2 dr1 jl (kli r1 ) sin(ωli t). a l+2
(11.54)
11.5 Derivation of Plasmon Frequencies for a Finite Electrolyte System
∞ l
275
Finally, δρ2 (r,t) = l=1 m=−l qlm (t)Ylm ( )δ(a−r). The first term in Eq. (11.54) describes the selffrequencies of surface plasmons, whereas the second corresponds to the surface plasmon oscillations induced by the volume plasmons. This induced part of the surface oscillations is nonzero only when the volume modes are excited and thus their amplitudes Almi are nonzero. The frequencies of selfoscillation √ of the surface plasmons equal ωl0 = ωp l/(2l + 1), corresponding to various multipole modes (numbered with l). are lower than Note that these frequencies the bulk plasmon frequency (ωp = nq 2 4π/m in Gauss units or nq 2 /(ε0 m) in SI), whereas the volume plasmon modes oscillate with frequencies higher than ωp . Worth noting also is the absence of any temperature dependence of the surface ionic plasmon resonances, in contrast to the volume plasmon selffrequencies. Concluding, we can state that in ionic finite systems we may observe plasmons similar to those in metallic nanoparticles. The structure of the surface and volume plasmons for ions repeats the properties of electronic plasmons in metallic spherical systems with, however, a significant shift of the resonance energy towards lower values, corresponding to the much larger mass of the ions in comparison with the electron mass and the different concentration of ions in the electrolyte. Thus, corresponding to the resonance energy, the electromagnetic wavelength is shifted to the deep infrared or even longer wavelengths, depending on the ion concentration. Typical for metal clusters is the crossover in the size dependence of plasmon damping between on the one hand the scattering losses, leading to ohmictype energy dissipation, and on the other hand the radiation losses. This crossover is also observable in ionic spherical systems with a similar size dependence, though it is shifted toward the micrometre scale for ions whereas for metals it is at the nanometre scale. Of particular interest is the high radiation regime for dipole plasmons in ionic systems with prospective applications in signalling and energy transfer in such systems. An initial strong enhancement in efficiency of the Lorentz friction with the radius growth of an electrolyte sphere is observed on the micrometre scale with typical a 3 radius dependence above some threshold radius whose value depends on the electrolyte parameters. At a certain value of the radius (varying over a wide range and depending on the ion system parameters) this enhancement saturates and then slowly diminishes, which allows definition of the most convenient sizes of finite electrolyte systems for optimizing radiationmediated transport efficiency.
12 Plasmon–Polaritons in a Chain of Finite Ionic Systems; Model of Saltatory Conduction in Myelinated Axons
In this chapter we apply the theory of ionic plasmons described in the previous chapter to plasmon–polaritons in periodic ionic systems. The complete theory of ionic plasmon– polariton kinetics in a chain of micrometresize electrolyte spheres confined by a dielectric membrane is formulated and solved. The latter theory is then applied to a problem that has been unclear for several decades, the socalled saltatory conduction of the action potential in the myelinated axons of nerve cells. Contrary to conventional nerve signalling models, the plasmon–polariton model fits well with the unusual properties of saltatory conduction. Moreover, the soft plasmonics application presented regarding signalling in myelinated axons allows for the identification of different informationprocessing roles of the white and grey matter in the brain and spinal cord. The proposed model of saltatory conduction defines the role of the insulating myelin differently from previous models, which may be helpful in the development of a better understanding of demyelination diseases.
The effective and quick transduction of the action potential through long myelinated axons in the neurons of the peripheral nervous system and in the white matter of the central nervous system undeniably lies behind the motorics and other communication functions of the body. The acceleration of the signal transduction is associated here with jumping of the signal between consecutive socalled Ranvier nodes separated by myelinated sectors approximately 100 μm long. The nature of this signal jumping, called saltatory conduction, has not yet been explained as the timing of the signal jumping exceeds conventional models of electrical signalling in neurons. Despite the indepth current recognition of nerve function mechanisms, including the action potential spikeformation mechanism on Ranvier nodes [50] and the model of the diffusionlike conduction of ion current in dendrites and nonmyelinated axons according to the cable theory originated by W. Thomson (1854) [52], see Fig. 12.1 (with various modifications [191, 51]), the mechanism of saltatory conduction observed in myelinated axons [192] is still unclear, since it cannot be explained by cable theory, and other possible mechanisms are still being researched [53, 50]. 276
Model of Saltatory Conduction in Myelinated Axons
277
r0 rm a
im
cm ii
ri
Figure 12.1 Schematic presentation of the cable model of nervous signal transduction in dendrites and in nonmyelinated axons [50, 51]. The capacitor across the neuron membrane, cm , together with the acrossmembrane resistivity, rm , creates a series of coupled RC circuits; the consecutive local charging and discharging of the capacitors cm results in diffusiontype [52, 192] transduction of the ion current ii inside the dendrite or nonmyelinated axon. Because of the relatively large longitudinal resistivities ri(o) of the inside and outside cytosol and the values of cm and rm across the cell membrane, the velocity of the diffusive current is limited to 1−3 m/s [50–52].
In order to solve the problem of saltatory conduction, a new and original model for this mysterious conduction was developed, on the basis of the kinetic properties of collective plasmon–polariton modes propagating along linear and periodically modified electrolyte systems. For an axon this system is the thin cord of the nerve cell periodically wrapped by Schwann cells creating a periodic and relatively thick myelin sheath (Schwann cells myelinate axons in the peripheral system, whereas in the central neural system axons are myelinated by oligodendrocyte cells [191, 50, 51]). These plasmon–polaritons have been investigated and understood using the welldeveloped domain of plasmonics [1, 5], especially nanoplasmonics applied to the longrange lowdamped propagation of plasmon–polaritons along metallic nanochains [40], as presented in previous chapters. The main properties of these collective excitations occurring on the conductor–insulator interface [116, 4] owing to the hybridization of the surface plasmons (i.e., the electron density fluctuations on the metal surface) with an electromagnetic wave are as follows: (1) a plasmon–polariton velocity much lower than the velocity of light, corresponding to plasmon–polaritons with wavelengths much shorter than the wavelength of light at the same frequency; (2) the related strong discrepancy between the momenta of plasmon–polaritons and photons with the same energies means that the external electromagnetic waves do not interact with the plasmon–polaritons, i.e., photons cannot be excited or absorbed by plasmon–polaritons owing to momentum conservation constraints; (3) all the electromagnetic field associated with the propagation of plasmon–polaritons is compressed into the tunnelvolume of the chain, especially the spaces between chain elements; (4) all the radiative
278
Model of Saltatory Conduction in Myelinated Axons
losses are quenched, and plasmon–polariton attenuation occurs only because of ohmic losses due to oscillating charged carriers (electrons in a metal), which makes metallic nanochains almost perfect wave guides for plasmon–polaritons; and (5) the longrange and practically undamped propagation of plasmon–polaritons is experimentally observed in metallic nanochains [40, 39]. The plasmon–polaritons in metallic nanostructures are likely to be exploited for future applications in optoelectronics where the conversion of light signals into plasmon–polariton signals circumvents the diffraction constraints that greatly limit the miniaturization of conventional optoelectronic devices (as the nanoscale of electron confinement inconveniently conflicts with the severalordersofmagnitude larger scale of the wavelength of light at an energy similar to that of nanoconfined electrons) [4, 41]. Some unique properties of plasmon–polaritons in metallic nanochains are of great interest, as these properties can be repeated in periodic linear arrangements of electrolyte systems with ions instead of electrons as charge carriers. According to the much larger mass of ions compared with that of electrons and the lower concentration of ions in electrolytes compared with that of electrons in metals, plasmon resonances in finite ionic systems (e.g., in a liquid electrolyte confined to a finite volume by appropriately formed membranes, frequently found in biological cell structures) occur on the scale of micrometres rather than nanometres, as for metals, and at frequencies several orders of magnitude lower (depending on the ion concentration). For a spherical electrolyte system, the surface and volume plasmons are handled analogously to those of the metallic nanospheres, described in the previous chapter. The ionic surface plasmon frequencies are given for the multipole lth mode by the formula 1 l ε(2l + 1) and the bulk plasmon frequency is ωp = 4πq 2 n/m (n is the ion concentration, q and m are the ion charge and mass, respectively, and ε is the relative permittivity of the surroundings). For dipole surface plasmons (l = 1), this equation resolves into √ a Mietype formula [18, 23], ω1 = ωp / 3ε. The plasmon oscillations intensively radiate their own energy and are quickly damped due to Lorentz friction losses (i.e., due to the radiation of electromagnetic waves by oscillating charges [55, 76]). For large systems with a large number of ions participating in the plasmon oscillations (thus strengthening the Lorentz friction) these losses are much greater than the ohmic losses due to carrier scattering (the scattering of ions on other ions, solvent and admixture atoms, and the boundary of the system), as illustrated in Fig. 11.3, where a crossover in the size dependence of the plasmon damping rate is visible (similar to that for metal nanospheres [48, 27]). ωl = ωp
12.1 Plasmon–Polariton Propagation in Linear Periodic Ionic Systems
279
Surprisingly, for a linear chain of spherical ionic systems, the radiation losses reduce to zero in exactly the same manner as in metallic chains [193, 43, 44]. The radiation energy losses expressed by the Lorentz friction [55, 76] are ideally compensated by the energy income due to radiation from the other spheres in the chain. As a result, the radiative losses are ideally balanced, and only a relatively small irreversible ohmic energy dissipation remains due to ion scattering. Thus, collective surface dipole plasmon–polaritons can propagate in the chain with strongly reduced damping and, if energy is permanently supplemented to balance the small ohmic losses, this propagation could occur over arbitrarily long distances without any damping. 12.1 Plasmon–Polariton Propagation in Linear Periodic Ionic Systems We will apply the model of dipole plasmon–polariton excitations in a linear chain of electrolyte spheres to an axon cord periodically wrapped with myelin sheaths, as schematically depicted in Figs. 12.2 and 12.3. The periodicity makes the chain similar to a onedimensional crystal. Although the cord of an axon is a continuous ion tube, the modelling of an axon by a chain of segments defined by the periodic myelin sheath meets well with plasmon–polariton kinetics, which maintains the same character in discrete chains and in continuous but periodically corrugated wires. The interaction between the chain elements (or segments defined by the myelin sheath) can be regarded as dipoletype coupling. For chains of ionic spheres, the results of the corresponding analysis for metallic chains can be adopted; these results support a dipole model of interaction between the spheres [41, 167, 168]. Note that the model of interacting dipoles [177, 178] was originally developed for the description of ion stellar matter [179, 180] and was then utilized for metal particle systems [181, 182]. The dipole interaction can be understood in terms of the electric and magnetic fields created by an oscillating dipole D(r,t) at any distant point. If this point is represented by the vector r0 (with one end fixed at the end of r, where the dipole is placed), then the electric field produced by the dipole D(r,t) takes the following form, which also includes the relativistic retardation [55, 76]: ) ∂2 1 r0 * 1 ∂ 1 1 − 2 2 − D r,t − − E(r,r0,t) = ε v ∂t r0 v∂t r02 r03 v 2 ) ) ∂ 1 ∂ 3 3 r0 ** 1 n + + · D r,t − + n , (12.1) 0 0 ε v 2 ∂t 2 r0 v∂t r02 r03 v √ with n0 = r0 /r0 and v = c/ ε. The terms with denominators r03 , r02 , and r0 are usually referred to as the nearfield, mediumfield, and farfield components of the
280
Model of Saltatory Conduction in Myelinated Axons
Chain of ionic spheres Transverse polarization
Longitudinal polarization
x
z y
Dendrit e
Scheme of myelinated axon structure Axon terminal Cell body Ranvier node h Myelin sheat
Schwann cell
2r diameter of an axon cord
Myelinated sector Schwann cell
100 m Nucleus
Ranvier interval Fictitious spheres for the model
Axon
Figure 12.2 In analogy to metallic nanochains, microchains of finite ionic segments enclosed by dielectric membranes are considered; in these ionic microchains, the plasmon–polarion modes can propagate similarly to those in metallic nanochains. A myelinated corrugated axon can be modelled as a chain of separated ion segments because the plamon–polaritons can traverse both continuous and discrete linear plasmonic system alignments.
interaction, respectively. Equation (12.1) describes the mutual interactions of the plasmon dipoles at each sphere in the chain. The spheres in the chain are numbered by integers l, and the equation for the surface plasmon oscillation of the lth sphere can be written as follows (where d denotes the separation between the centres of the spheres):
m=∞ l − md 2 ∂ ∂2 2 2 3 + Eα md,t − + ω1 Dα (ld,t) = εω1 a ∂t 2 τ0 ∂t v m=−∞, m=l + εω12 a 3 ELα (ld,t) + εω12 a 3 Eα (ld,t).
(12.2)
Here α = z indicates the longitudinal polarization, whereas α = x(y) indicates a transverse polarization (the chain orientation is assumed to be along the z direction, as illustrated in Fig. 12.2). The first term on the righthand side of Eq. (12.2) describes the dipole coupling between the spheres, and the other two terms correspond to the plasmon attenuation due to Lorentz friction radiation losses and to the force field arising from an external electric field, respectively;
12.1 Plasmon–Polariton Propagation in Linear Periodic Ionic Systems Dendrite
(a)
281 (b)
Action potential +40
Schwann cell
n zatio
0
55
Failed initiations
Threshold
Resting state
70
Nucleus
Stimulus
Refractory period
Axon 0
Scheme of myelinated axon structure
Myelinated sector Schwann cell
4
2 3 Time (ms)
+
5
+ 16
n ~ 2.1 10 /m
100 m
1
Dipoles in Ranvier nodes equivalent to longitudinal surface plasmons on myelinated sectors
(c) 2r diameter of an axon cord
ation
D ep olari
Ranvier node
Myelin sheath
Repolariz
Cell body
Voltage (mV)
Axon terminal
+
3
+
(d)
Ranvier interval
n’ ~ 10mM~6 1024/m3 Fictitious spheres for the model
Figure 12.3 (a) Schematic illustration of a long axon, with a chain of periodically repeated myelinated sectors of approximately 100 μm in length separated by unmyelinated Ranvier nodes, corresponding to a number of segments of order 10,000 per metre of axon length; (b) time pattern of the action potential forming on a Ranvier node; (c) periodic fragments of a myelinated axon with a fictitious periodic chain of spherical ionic systems proposed as an effective model; (d) the equivalence of polarized Ranvier nodes and longitudinal surface plasmons on myelinated sectors (the effective concentration of ions n in an auxiliary sphere corresponds to the actual ion concentration n ).
√ ω1 = ωp / 3ε is the frequency of the dipole surface plasmons. Ohmic losses are included via the term 2/τ0 , as for metals [171] but with the Fermi velocity of electrons in metals substituted by the mean velocity of ions for a nondegenerate classical Boltzmann distribution, regardless of the quantum statistics of the ions, i.e., v Cv 1 = + , (12.3) τ0 2λB 2a where λB is the mean free path of the carriers (ions) in the bulk electrolyte, v is the √ mean velocity of the carriers at temperature T , v = 3kB T /m, m is the mass of an ion, kB is the Boltzmann constant, C is a constant of the order of unity (to account for scattering of carriers by the system boundary), and a is the radius of a sphere. The first term in the expression for 1/τ0 approximates ion scattering losses such as those occurring in the bulk electrolyte (collisions with other ions, solvent, and admixture atoms), whereas the second term describes losses due to the scattering of ions on the boundary of a sphere of radius a. According to Eq. (12.1), we can
282
Model of Saltatory Conduction in Myelinated Axons
write the quantities that appear in Eq. (12.2) as follows: ∂ 1 d 2 d × Dz md,t − m − l , + Ez (md,t) = 3 εd m − l3 vm − l2 ∂t v ∂2 ∂ 1 1 d d2 Ex(y) (md,t) = − 3 (12.4) + + 2 εd m − l3 vm − l2 ∂t v l − d ∂t 2 d . × Dx(y) md,t − m − l v Because of the periodicity of the chain, a wavetype collective solution of the dynamical equation in the form of a Fourier component can be assumed for (12.2): Dα (ld,t) = Dα (k,t) e−ikld ,
0≤k≤
2π . d
(12.5)
In the Fourier version of Eq. (12.2) (i.e., a discrete Fourier transform (DFT) with respect to position and a continuous Fourier transform (CFT) with respect to time) this solution takes a form similar to that of the solution for phonons in onedimensional crystals. Note that a DFT is defined for a finite set of numbers; therefore, we will consider a chain with 2N + 1 spheres, i.e., a chain of finite length L = 2Nd. Then, for any discrete characteristic f (l), l = −N, . . . ,0, . . . ,N, of the chain, such as a selected polarization of the dipole distribution, we must consider the DFT picture, f (k) =
N l=−N
f (l)eikld ,
k=
2π n, n = 0, . . . ,2N . 2Nd
This means that kd ∈ [0,2π) because of the periodicity of the equidistant chain. The Born–Karman periodic boundary condition f (l + L) = f (l) is imposed on the entire system, resulting in the form of k given above. For a chain of infinite length, we can take the limit N → ∞, which causes the variable k to become quasicontinuous, although kd ∈ [0,2π) still holds. The Fourier representation of Eq. (12.2) takes the following form, a3 2 2 2 −ω − i ω + ω1 Dα (k,ω) = ω12 3 Fα (k,ω)Dα (k,ω) + εa 3 ω12 E0α (k,ω), τ0 d (12.6) with, settling as before x = kd and ξ = ωd/v,
12.1 Plasmon–Polariton Propagation in Linear Periodic Ionic Systems
Fz (k,ω) = 4
∞ m=1
cos(mx) cos(mx) cos(mξ ) + ξ sin(mξ ) 3 m m2
283
! ∞ cos(mx) cos(mx) 1 3 sin(mξ ) − ξ cos(mξ ) , ξ +2 + 2i 3 m3 m2 m=1 ∞ cos(mx) cos(mx) cos(mξ ) + ξ sin(mξ ) Fx(y) (k,ω) = −2 3 2 m m m=1 2 cos(mx) −ξ cos(mξ ) m ∞ cos(mx) 2 sin(mξ ) − i − ξ3 + 2 3 3 m m=1 cos(mx) 2 cos(mx) +ξ cos(mξ ) − ξ sin(mξ ) . m2 m (12.7) As for metallic nanochains, Im Fα (k,ω) ≡ 0 (for α = z,x(y)), which indicates perfect quenching of the radiation losses at any sphere in the chain (meaning that, for each sphere, the amount of energy that comes in from the other spheres is the same as the energy outflow due to Lorentz friction). We can easily verify this property, as the related infinite sums in Eq. (12.7) can be found analytically [72]. Equation (12.6) is highly nonlinear with respect to the complex frequency ω and can be solved both perturbatively in an analytical manner [44] or numerically, which is more accurate. The solutions determined for Re ω and Im ω (i.e., for the selffrequency and damping of the plasmon– polaritons, respectively) can be applied to the axon model as an effective chain of electrolyte spheres with ion concentrations adjusted to the actual neuron parameters. The problem of the propagation of plasmon–polaritons along metallic nanochains was addressed by, among others, Citrin [42, 193] in order to obtain an explanation for the radiative losses of plasmon–polaritons in metallic nanochains in agreement with observations relating to radiation losses in onedimensional and twodimensional crystals [194]. Plotted in Fig. 12.4 are the resonance frequency (Re ω(k)), its kderivative, i.e., the group velocity, and the attenuation rate (Im ω(k)) of the dipole plasmon–polariton modes numbered by the wave vector k, derived by the solution of Eq. (12.6) [44, 45] for ionic chains with typical concentration, chain size, and ion parameters.
284
Model of Saltatory Conduction in Myelinated Axons a = 5 m (ion)
a = 20 m (ion) d = 4a
a = 20 m (ion) d = 4a 1.03
4
[m/s]
1.00 0.99
z
Re
z
1.01
0.98 0.97
1 2 4
106 106 106 0 106 106 106
0.96 0
200
400
600
800
3 d 3a
Im Fz
1.02
3 2 1
200
a = 20 m (ion) d = 4a
1.000 0.995 0.990 600
800
1000
1
800
4
106
2
106
4
106
1000
2
3
4
200
400
600
kd [2 /1000]
3
d 3a
2
d 4a
1
d 6a
800
1000
1
0
1
2
3
4
kd
Figure 12.4 Exact solutions for the selffrequencies of the longitudinally and transversely polarized modes of the plasmon–polaritons in an ionic chain (ω in units of ω1 ) obtained by solving Eq. (12.6) exactly at 1000 points in the region kd ∈ [0,2π) (left); the corresponding group velocities for both types of polarization (centre); the functions Im Fz (k;ω = ω1 ) and Im Fx(y) (k;ω = ω1 ) for infinite chains of electrolyte spheres of radius a at separations d = 3a, 4a, and 6a; the shift of the singularities towards the band edges with decreasing d/a is noticeable (right) ([49]).
12.2 Plasmon–Polariton Model of Saltatory Conduction: Fitting the Kinetics to the Axon Parameters The bulk plasmon frequency is ωp = q 2 n4π/m (it is assumed for the model that the ion charge is q = 1.6 × 10−19 C and the ion mass is m = 104 me , where me = 9.1 × 10−31 kg is the mass of an electron). For a concentration n = 2.1 × 1016 /m3 , we obtain a Mietype frequency for ionic dipole oscillations, √ ω1 0.1ωp / 3ε1 4 × 106 /s, where the relative permittivity of water is ε1 80 for frequencies in the MHz range [195] (although for higher frequencies, beginning at approximately 10 GHz, this value decreases to approximately 1.7, corresponding √ to the optical refractive index of water, η ε1 = 1.33). For a thin axon cord and thus, in the discrete model, for a strongly prolate inner ionic cord segment, the longitudinal Mietype frequency is reduced by a factor 0.1 [196, 197] compared with the isotropic spherical case. The axon consists of a cord with a small value of the diameter 2r, and this thin cord is wrapped with a myelin sheath of length 2a per segment; however, for the effective model we consider fictitious electrolyte spheres of radius a. Thus, the auxiliary concentration n of ions in the fictitious spheres corresponds to an ion concentration in the cord of n =
5
6
5
6
0 0
kd [2 /1000]
1
a = 5 m (ion)
6
10
0
4
0 2
d 6a
kd
Im Fx(y)
[m/s]
1.005
x(y)
x(y)
Re
1.010
400
600
a = 20 m (ion) d = 4a
1.015
200
400
kd [2 /1000]
kd [2 /1000]
0
d 4a
1 0
0
1000
2
n4/3πa 3 , 2aπr 2
12.2 Fitting the Kinetics to the Axon Parameters
285
which yields a typical concentration of ions in a nerve cell of n ∼ 10 mM (i.e., ∼ 6×1024 /m3 ). The reason is that in the sphere model all the ions participating in the dipole oscillation correspond to a much smaller volume in the real system, that of the thin cord portion (the insulating myelin sheath consists of a lipid substance without any ions). The insulating, relatively thick, myelin coverage creates the periodically broken channel (a corrugated conductor–insulator structure) required for plasmon–polariton formation and propagation. To reduce the coupling with the surrounding intercellular electrolyte and protect against any leakage of plasmon–polaritons, the myelin sheath must be sufficiently thick, much thicker than what is required merely for electrical insulation. Moreover, to accommodate the conductivity parameters calculated for a spherical geometry to the highly prolate geometry of the real oscillating ionic system, the Mietype frequency of the longitudinal oscillations must be significantly lower than that for a sphere with a diameter equal to the elongation axis. As a rough estimate, a correction factor of 0.1 was assumed [196, 197]; see Fig. 12.7. For the resulting Mietype frequency, ω1 4 × 106 /s, one can determine the plasmon–polariton selffrequencies in a chain of spheres of radius a = 50 μm (for a Schwann cell length of 2a) and for small chain separations such that d/a = 2.01, 2.1, and 2.2 (corresponding to Ranvier node lengths of 0.5, 5, and 10 μm, respectively) within the approach presented above, via the solution of Eq. (12.6). The derivatives of the obtained selffrequencies with respect to the wave vector k determine the group velocities of the plasmon–polariton modes. The results are presented in Fig. 12.5. We observe that for the ionic system parameters listed above, the group velocity of the plasmon–polaritons reaches 100 m/s for the longitudinal mode with polarization suitable for the prolate geometry, assuming that
a = 50 m (ionic spheres)
a = 50 m (ionic spheres)
1.2
100
(m/s)
1.0
2.01 2.1
0.9
50
2.01 2.1
0
2.2
z
z
/
1
1.1
2.2
50
0.8
100
0.7 0
1
2
3 kd
4
5
6
0
1
2
3
4
5
6
kd
Figure 12.5 Solutions for the selffrequencies and group velocities of the longitudinal mode of a plasmon–polariton in a model ionic chain; ω is presented in units of ω1 ; here ω1 = 4 × 106 /s for a chain of spheres with radius a = 50 μm and Ranvier separation d, such that d/a = 2.01, 2.1, or 2.2, for an equivalent ion concentration in the inner ionic cord of the axon of n ∼ 10 mM = 6 × 1024 /m3 .
286
Model of Saltatory Conduction in Myelinated Axons
the initial postsynaptic action potential, or that from the cell hillock, predominantly excites longitudinal ion oscillations. Note that, for ω1 = 4 × 106 /s and a = 50 μm, the light cone interference conditions kd − ω1 d/c = 0 and kd + ω1 d/c = 2π are fulfilled only for extremely small values of kd and 2π − kd, respectively (of the order of 10−6 for d/a ∈ [2,2.5]). Thus these interference conditions are negligible with regard to the plasmon–polariton ion kinetics (though they are important for metals, as discussed in Chapter 9); the related singularities on the light cone induced by the far and mediumfield contributions to the dipole interaction are pushed to the borders of the k wave vector domain and thus are unimportant for the ionic system considered. Hence, the quenching of the radiative losses (i.e., the perfect balance of the Lorentz friction in each sphere by the radiation income from the other spheres in the chain) for the plasmon–polariton modes in the axon model occurs practically throughout the entire kd ∈ [0,2π) region. Additionally, the aforementioned singularities [45] are characteristic of infinite chains and therefore cannot fully develop because in the model the nerve electrolyte chains are of a finite length, whereas other effects, such as the quenching of radiation losses, occur for finite chains owing to the very fast convergence of the sums in Eq. (12.7) with denominators m2 and m3 ; in practice, a chain consisting of only 10 elements exhibits almost the same properties as an infinite chain, as was noted in Chapter 9; see Figs. 9.26 and 9.27. Although the ionicsystem chain model for a myelinated axon appears to be a crude approximation to the real axon structure, it can serve for a comparison of the energy and time scales of plasmon–polariton propagation implied by a model with the observed kinetic parameters of nerve signals. In the model, the propagation of a plasmon–polariton through the axon chain, excited by an initial action potential on the first Ranvier node after the synapse or, for the reverse signal direction, in the neuron cell hillock, sequentially ignites the consecutive Ranvier node blocks of Na+ and K+ ion gates. The resulting firing of the action potential traverses the axon with a model velocity of approximately 100 m/s, consistent with the velocity actually observed in myelinated axons (and not possible for an ionic diffusive current in the cable model [50, 51]). The plasmon–polariton ignition of consecutive Ranvier nodes enables the creation of the same activation potential pattern, aided by the external energy supply at each Ranvier node block. Because of the nonlinearity of the ionchannel block mechanism, the signal growth saturates at a constant level, and the overall timing of each action potential spike has the stable shape of the local polarization/depolarization scheme in the short fragment of cell membrane that corresponds to the nonmyelinated Ranvier node. The permanent supply of energy associated with the creation of action potential spikes at sequentially firing Ranvier nodes also contributes to the plasmon–
12.2 Fitting the Kinetics to the Axon Parameters
287
polariton dynamics, ensuring that the amplitude of each Ranvier block dipole excitation is beyond the activation threshold. The external energy supply (through the conventional ATP/ADP cell mechanism) assists the renovation of the action potential pattern at each Ranvier node. This energy supply residually compensates the ohmic thermal losses of the plasmon–polariton mode propagating along the axon and ensures undamped propagation over an unlimited range. Although the entire signal cycle of the action potential on a single Ranvier node block requires several milliseconds (or even longer when one includes the time required to restore steadystate conditions, which, however, on the other hand conveniently blocks the reversing of the signal), subsequent nodes are ignited more rapidly. This occurs because the velocity of the plasmon–polariton wave packet triggers the ignition of consecutive Ranvier nodes, as illustrated in Fig. 12.8. Thus, we are dealing with the firing of the axon, which propagates with the velocity of the ionic plasmon–polariton wave packet. The direction of the velocity of this wave packet corresponds to the semiinfinite geometry of the chain, though in fact the chain is finite and is excited at one of its ends. The firing of the action potential triggered by the plasmon–polariton traverses along the axon in only one direction because the nodes that have already fired have had their Na+ , K+ gates inactivated (discharged) and require a relatively long time to restore these gates to their original status (the entire Na/K block requires a time of the order of as much as a second and a sufficient energy supply to bring the concentrations to their normal values via crossmembrane active ion pumps against the iondensity gradient). The plasmon–polariton scheme described above for the ignition of the action potential spikes in the ordered chain of Ranvier nodes along an axon is thus consistent with the saltatory conduction observed in myelinated axons. The observation that the firing of the action potential can simultaneously move in two opposite directions if a certain central Ranvier node of a passive axon is ignited, as well as the observation that the maintenance of the firing persists despite small breaks in the axon cord or a few damaged Ranvier nodes, also agrees with the collective wavetype plasmon–polariton model of saltatory conduction, in contrast wth the lack of satisfactory explanations in models based on the cable theory. The maintenance of plasmon–polariton kinetics despite discontinuities in the axon cord agrees well with the discrete chain model of a cord corrugated by the periodic myelin sheath. In Fig. 12.6 the group velocity of the action potential traversing a firing myelinated axon, in the plasmon–polariton model, is plotted for various diameters of the axon internal cord and for a length of 100 μm for each myelinated sector wrapped by Schwann cells and Ranvier intervals of 0.5 μm, 5 μm, and 10 μm. The dependence of the group velocity on the length of the Ranvier interval is weak (i.e., negligible at the scale considered, which is consistent with the
288
Model of Saltatory Conduction in Myelinated Axons r = 20 nm
r = 50 nm
r = 100 nm
a = 50 m (ionic spheres)
a = 50 m (ionic spheres)
a = 50 m (ionic spheres)
100
20
200
50 z
z
2.1
0
100
2.01 2.1
2.01 0 50
100
100
40 1
2
3
kd
2.1 2.2
0
2.2
2.2 20
0
2.01
z
40
4
5
6
200 0
1
2
3
kd
4
5
6
0
1
2
3
4
5
6
kd
Figure 12.6 For comparison, the group velocities, in m/s, of the longitudinal plasmon–polariton mode with respect to the wave vector k ∈ [0,2π/d) within the axon model, for Schwanncell myelinated sectors with length 100 μm. The plots shown are for Ranvier separations 0.5 μm, 5 μm, and 10 μm (represented by d/a = 2.01, 2.1, and 2.2 in the figure, respectively) and axon cord radii r = 20, 50, and 100 nm.
equivalence of the discrete model for the continuous system if one considers wavetype plasmon–polariton propagation), but the increase in the velocity with increasing internal cord thickness is significant, and is similar to that for real axons with increasing diameters. To comment on the appropriateness of the chain model for axons, let us note that even though the thin core of the axon is a continuous ionconducting fibre, the surface electromagnetic field can be closely pinned to the linear conductor in the same way as for the Goubau line (well known in microwave technology) [37, 198]. If periodically wrapped by dielectric sheaths, plasmons resonantly coupled with the electromagnetic field propagate as concentrated plasmon–polaritons along the chain of periodic segments despite the continuity of the fibre. For plasmon– polariton kinetics, the continuity of the conducting fibre is unimportant because here we are dealing with the wave packet of the plasma oscillations and not with the charge carriers themselves. The situation is similar to that for Goubau microwave lines, which also have discontinuous segments; the Goubau lines maintain their transmittance via discrete disconnected elements. The fragments of the thin axon cord wrapped with thick myelin shells with an ion concentration that is typical for neurons of n 10 mM 6 × 1024 /m3 inside the cell can be equivalently modelled by a sphere with diameter equal to the length of the cord fragment and an ion concentration of n 2 × 1016 /m3 , for an assumed axon cord diameter of 100 nm, conserving the number of ions in the segment participating in the dipole oscillations. Such a model is justified since it has the same dynamical equation structure as that for dipole plasmon fluctuations in a chain of spheres, i.e., Eq. (12.2), and as the modification of this equation for prolate spheroid or elongated cylindrical rod chains. This modification amounts to the substitution of the isotropic ω1 frequency in Eq. (12.2) by frequencies that are different for each polarization ωα1 , i.e.,
12.2 Fitting the Kinetics to the Axon Parameters
289
m=∞
∂2 l − md 2 ∂ 2 Dα (ld,t) = A + Eα md,t − + ωα1 2 ∂t τα0 ∂t v m=−∞, m=l
+ AELα (ld,t) + AEα (ld,t), where A = V nq 2 /m is a shapeindependent factor proportional to the number of ion carriers with concentration n in the volume of the spheroid with semiaxes a,b,c, V = (4π /3)abc = (4π /3)a 3 (the latter for a sphere); see Fig. 12.7. Taking into account that the plasmon frequency in a bulk electrolyte with ion concentration n equals ωp = nq 2 4π /m, one can rewrite A as follows: A = abcωp2 /3 = εa 3 ω12 √ (the latter for a sphere, for which ω1 = ωp / 3ε). The ohmic losses can be included via the anisotropic term, v Cv 1 = + α, τα0 2λB 2a where a α is the dimension (semiaxis) of the spheroid in the direction α (α = a,b,c for a spheroid). The first isotropic term in the expression for 1/τα0 approximates ion scattering losses such as those occurring in the bulk electrolyte (isotropic losses), whereas the second term describes the losses due to the scattering of ions on the anisotropic boundary of the spheroid. This term can be neglected for longitudinal polarization because the neuron cord is continuous along the z direction. The dipole Dipoles in Ranvier nodes equivalent to longitudinal surface plasmons on myelinated sectors
Scheme of myelinated axon structure
Myelinated sector Schwann cell
+
+
n = 2.1 1016/m3
2r diameter of an axon cord

+
+
Ranvier interval
100 m
n’ = 10 mM = 6 1024/m3 Fictitious spheres for the model
l y
r
x z
y
b c
x
a
z
Figure 12.7 The effectivechain model of a continuous axon corrugated by periodic myelin sectors corresponds to a series of rods or prolate spheroids; because of the linearity of the dynamics equation with respect to the dipole field, it is possible to renormalize the equations for both polarizations without changing their structure.
290
Model of Saltatory Conduction in Myelinated Axons plasmon–polariton vg =100 m/s 1 ms
Ranvier node axon cord
10 cm (1000 segments)
100 m
Schwann cell action potential
0
55 70
Threshold
0
0
55 Resting state
Stimulus
1
2 3 Time (ms)
1st node
4
5
+40
phase of the action potential
Voltage (mV)
+40 Voltage (mV)
Voltage (mV)
+40
70
Threshold
55 Resting state
Stimulus
0
0
1
2 3 Time (ms)
400th node
4
5
70
Threshold Resting state Stimulus
0
1
2 3 Time (ms)
4
5
800th node
Figure 12.8 Schematic presentation of the firing of a nerve cell triggered by the propagation of a plasmon–polariton wave packet along the periodic structure of a myelinated axon. For a group velocity of the plasmon–polariton wave packet of the order of 100 m/s, within 1 ms the packet traverses 10 cm distance and initiates one by one the formation of the action potential on 1000 Ranvier nodes in sequence. The various time phases are indicated by black dots for exemplary nodes. The lefthand parts of the action potential spikes refer to the depolarization phase, and the righthand parts to the repolarization phase. The very small peaks are failed initiations and the trough that follows the spike is the refractory period.
coupling is independent of the shape of the chain elements. The mutual independence of dipole oscillations with distinct polarizations described above follows from the linearity of the dynamics equation regardless of the metal or electrolyte conducting elements. Because the dynamics equation is not affected by the anisotropy of the situation the solutions of the equation for each polarization have the same form as for the spherical case, except that the related frequencies of the dipole oscillations in each direction are modified and that there is a small correction to the orientationdependent contribution of the scattering ratio (this part is related to the scattering of carriers by the boundaries and is not important for longitudinal polarization when the axon cord is continuous). Thus, we can independently renormalize the equation for the dipole oscillations for each polarization direction, introducing the resonance oscillation frequency for each direction ωα1 in a phenomenological manner. These √ frequencies can be estimated numerically, whereas for a sphere, ω1 = ωp / 3ε; in general, the longer the semiaxis, the lower is the related dipole oscillation frequency. Moreover, the size correction of the boundary scattering term must be taken into account as described above (favourably reducing the longitudinal plasmon–polariton damping for a prolate geometry. This renormalization was done for the model of the axon segment chain considered. The periodic structure of a myelinated axon does not form a chain of electrolyte spheres but rather is a thin electrolyte cord with periodically distributed
12.2 Fitting the Kinetics to the Axon Parameters
291
sectors that are wrapped in myelin sheath separated by very short unmyelinated intervals, the Ranvier nodes. The periodic corrugated structure of the dielectric insulation allows, however, for collective plasmon wavetype oscillations, ∼ eiqz , with q governed by the periodicity, propagating along the cord; these oscillations are wavetype synchronic dipole polarized consecutive Ranvier intervals. Taking into account that the Ranvier nodes are short, these polarized dipoles are equivalent to the synchronically oscillating dipoles of the myelinated sectors. The latter can thus be treated as dipole surface plasmon oscillations propagating along a chain of prolate spheroids with small separations and longitudinal dipole polarization despite the continuous character of the cord, as shown in Fig. 12.3 (righthand panels). To estimate the characteristics of such collective dipole wavetype excitations along the cord sectors, one can use the model of a chain of spherical electrolyte systems with suitably diluted ion concentration (resulting in the same total ion number as that in the cord fragments) and with decreased resonance frequency similar to that for the longitudinal polarization for highly prolate spheroids (or elongated cylinders). The model allows for the quantitative estimation of the relevant propagation characteristics and verification of whether plasmon–polariton dynamics fit the observed features of saltatory conduction in myelinated axons. At consecutive Ranvier nodes, the plasmon–polariton wave packet triggers the release of ions through the nonmyelinated membrane and the formation of the action potential (renewed at each Ranvier node). The relatively low polarization induced by the plasmon–polariton initiates the opening of the Na+ and K+ acrossmembrane ion channels at a Ranvier node, which results in a characteristically large action signal due to the transfer of ions through these open channels, caused by the difference in the ion concentrations on opposite sides of the membrane. The entire cycle requires several milliseconds, but the initial increase in polarization caused by the rapid opening of the Na+ channel occurs on the time scale of a single millisecond. Because the myelin layer wrapped by the Schwann cell prohibits crossmembrane ion transfer, the local polarization/depolarization of the internal cytoplasm of the axon occurs only at the Ranvier nodes, thus strengthening dipole formation in the axon fragment wrapped by the Schwann cell and the amplitude of the wavetype collective dipole oscillations in the whole chain. Each Ranvier node activity consecutively triggered by a plasmon– polariton increases the plasmon–polariton amplitude to a constant value despite the ohmic losses. The plasmon–polariton mode that traverses the axon structure, consisting of periodically polarized electrolyte segments wrapped with myelin sheaths, causes consecutive individual ignitions of the Ranvier nodes in sequence along the axon. This triggering role of the plasmon–polariton thus elucidates how the action signal jumps between neighbouring active Ranvier nodes.
292
Model of Saltatory Conduction in Myelinated Axons
The plasmon–polariton scenario in an ionic chain, even in this simplified version, could share certain features with the ability of nerve systems to achieve efficient and energetically economical electric signalling despite the rather poor ordinary electric conductivity of axons. The plasmon–polariton kinetics in the periodic structure of the axon may provide a convenient explanation for highperformance nerve signalling, providing quick signal propagation despite low ordinary conductivity over a practically unlimited range as energy is continuously supplied to cover the relatively small plasmon–polariton ohmic losses (which are lower than for an ordinary current). Moreover, plasmon–polaritons do not radiate any energy. The energy supply is residually provided by the ATP/ADP mechanism in neuron cells, which energetically contributes to the signaldependent opening and closing of the Na+ and K+ channels in the Ranvier nodes and then to the restoration of steadystate conditions, via the active transport of ions across the membrane against the ionic concentration gradient, which requires an external energy supply. Moreover, the coincidence of the micrometre scale of the periodic structure of the Schwann cells in an axon (approximately 100 μm in length) with the typical requirements for the size of ionic chains supports the plasmon–polariton concept as the explanation for the transduction of the action potential along an axon, in agreement with the tentative quantitative fitting of the model. It must be emphasized that plasmon–polaritons do not interact with external electromagnetic waves or, equivalently, with photons (even with frequencies adjusted to the plasmon–polariton frequency), as a consequence of the large difference between the group velocity of plasmon–polaritons and the velocity of photons √ (c/ ε). The resulting large discrepancy between the wavelengths of photons and plasmon–polaritons of the same energy prohibits mutual transformation of these two types of excitations because of momentum and energy conservation constraints. Therefore, signalling by means of collective wavetype dipole plasmon oscillations along a chain, i.e., plasmon–polaritons, can be neither detected nor perturbed by external electromagnetic radiation. This also fits well with neural signalling properties in the peripheral nervous system and in the white myelinated matter in the central nervous system. The ionic surface plasmon frequencies are independent of temperature, although the ionic volume plasmon frequencies are temperature dependent, as has been described in the previous chapter. However, √ temperature does influence the mean velocity of the ions, v = 3kT /m, thereby enhancing the ohmic losses with increasing temperature (see Eq. (12.3)), which in turn strengthens plasmon–polariton damping. Hence, at higher temperatures, higher external energy supplementation is required to maintain the same longrange propagation of plasmon–polaritons with a constant amplitude. This property is also consistent with experimental observations. However, the energy cost is the active ion transport through the membrane to recover the steady state of each
12.3
The Roles of Grey and White Matter in Information Processing
293
Ranvier node. Only a residual part of this energy is needed to support and maintain undamped plasmon–polariton propagation, which can be included in the scheme for a steady solution of the forced and damped oscillator, applied here to plasmon– polariton dynamics in a way similar to that for a metallic chain activated by a coupled external source (e.g., a coupled quantum dot system [199]). The energy supply from consecutively excited Ranvier nodes continuously covers plasmon–polariton ohmic losses, which ensures that the amplitude of the action potential spike is renewed at each conscutive Ranvier node. This results, however, in a convenient narrowing of the plasmon–polariton k wave packet, strengthened step by step at the Ranvier nodes. This narrowing shifts the packet towards the longwave limit (smaller k), which follows from the Fourier picture of the Dirac delta (a narrower plasmon–polariton k wave packet is formed as a larger number of chain segments contribute). This favourable property allows for the precise ignition of sequential Ranvier nodes: unlimited propagation of a relatively narrow plasmon–polariton wave packet accurately triggers consecutive Ranvier nodes, which in turn strengthen the packet. The utilization of radiatively undamped plasmon–polariton propagation in a chain of electrolyte subsystems may explain the efficient and longrange saltatory conduction in myelinated axons in the peripheral neural system and in the white matter of the brain and spinal cord. A plasmon–polariton model of the triggering of action potential firing along an axon myelinated by Schwann cells separated by Ranvier nodes in the peripheral nervous system fits well with the high conduction velocity observed and with the temperature and size dependence of the conduction velocity. This agreement, together with the immunity of plasmon–polaritons to external electromagnetic perturbations and detection, supports the reliability of this new model for saltatory conduction of the action potential, which is very efficient and energyfrugal despite the poor ordinary conductivity of axons. 12.3 Soft Plasmonics Application: The Role of Grey and White Matter in Information Processing in the Brain The electrical activity of the nervous system refers to the transduction of a series of action potential spikes along the axons and dendrites of neuron cells connected together by electrochemical synapses into a highly entangled web. Not all trajectories for signal travel are accessible (they can be blocked by passive synapses or by their absence). The activation of selected synapses makes paths available for communication for longer or shorter time periods depending on the intensity and repetition of the synapse activation. Via the activation of selected (even in a random manner) synapses, the nervous system creates an entangled pattern or a braided web of trajectories. The role of the braids seems to be more important than the
294
Model of Saltatory Conduction in Myelinated Axons
simple connections (the addressing) in the activated neuron network. Classification of the resulting entanglement patterns may be achieved in topological terms using socalled pure braid groups [200], as will be demonstrated in the next paragraph. Elements of these groups display various inequivalent patterns of entanglement of threads (neuron filaments), allowing the distinguishing and precise comparison of complicated filament muddles in a mathematically rigorous topological homotopy way. Two braids are homotopic if one can be transformed into the other by continuous deformation without cutting. For N threads, the number of various topologically inequivalent braid patterns is infinite, though countable [200]; in practice it is limited only by size restrictions such as the finite filament diameter and length. The various braid patterns greatly exceed ordinary addressing limits, for which N filaments give only N ! opportunities; this is low in comparison with the infinite number of N filament braids. If one electrically activates an entangled network by pushing an alternating charge current along the threads, the unique pattern of braiding with a specific number of loops might serve as a multiloop electromagnetic active circuit such as a distributed coil. The alternating current in this braid coil could generate an individual unique spatially local electromagnetic field configuration that could fall into resonance with another, even a distant, part of the web. Thus, we could associate information messages (elements of memory) imprinted in distinct elements of the pure braid group implemented in a nonlocal manner in fragments of the large neuron web of the brain via previous activation (ceation) and temporal consolidation of a certain subset of synapses. A message could be temporarily stored in the neuron braid corresponding to a certain mathematical braid from the pure braid group, as long as the selected engaged synapses are still active (or are ready to be active). This information can be next invoked by electromagnetic resonance with a similar braid within the brain and temporarily created in another brain structure (e.g., in the hippocampus) as the result of an influx of neuron signals from the surroundings via the senses. The new message tentatively imprinted in a temporary braid in the hippocampus might excite the same braid as was recorded in the past in the cortex via electromagnetic resonance and, in this way, may cause the identification of a new message in the mind. Let us note here that the dendrites in the grey matter prepare thousands of lateral spikes ready to create new synapses between neurons. To utilize the braids in the proposed electromagnetic recognition process, alternating electric currents are necessary to initiate the resonance response. Such AC electricity may generate the brain waves that are constantly observed via EEG in the grey matter of the cerebral cortex. For the transduction of neuron signals in nonmyelinated axons and in all dendrites in the cortex, the diffusive movement of ions is employed in elongated and branched neuron cells. This electric current
12.3
The Roles of Grey and White Matter in Information Processing
295
type communication is described very well by the cable theory originated by W. Thomson (1854) [52] and is widely applied to explain the neural electrophysiology of dendrites and nonmyelinated axons. Hence, one can expect that the storage and identification of information occurs in the cerebral cortex, taking advantage of the huge information capacity of the entangled neuron filaments, which creates various braid structures enumerated by pure braidgroup elements. The topologically precise homotopy resolution and quick and complex access to the stored messages in entangled braids [200–203] via electromagnetic resonance, additionally using a few distinct frequencies of brain waves, might help to understand the functionality of memory and pattern recognition by a mind. All these phenomena occur in the grey matter of the cortex, where signal transduction is accomplished by the diffusion of ions equivalent to an ordinary alternating current, which induces a local electromagnetic field in a coil. Different types of brain wave frequencies might conveniently implement simultaneous independent resonance channels for identification of the multiloop coils created by neuron filament braids [203]. As mentioned above, braid groups were introduced to describe entangled bundles of the classical trajectories of N particle systems [200]. Two types of braid groups have been investigated and applied; for the first type, full braid groups, the indistinguishability of identical particles is assumed and is applied to characterize the quantum statistics of particles [202]; the second type comprises the socalled pure braid groups for distinguishable particles [200, 202]. The latter are suitable for describing and classifying highly entangled multifilament webs. Both full and pure braid groups are infinite for N particles moving on a plane but are finite when the particles move in three dimensions (3D). In 3D there is room to disentangle the lines representing the particle trajectories, which is impossible in 2D (in 2D, particles must twist around each other and cannot hop beyond or beneath each other). The pure braid group of N distinguishable particles on a plane (in 2D) may be presented as a set of N threads in 3D with their ends fixed to steady points but braided in between in an arbitrary manner. Thus, the 3D web of entangled threads such as neurons in a brain can be mapped onto a 2D pure braid group. The patterns of such braids are unique and cannot be transformed into each other without cutting threads. However, the patterns can be precisely enumerated by pure braid group elements. If we imagine that the N initial and N final points of the threads are fixed in 3D space, then a structure linking them into braids – the 2D Nelement pure braidgroup elements – reproduces in a onetoone fashion 3D webs of arbitrary entangled nets of filaments, such as a web of neurons linked via selected synapses in the brain.
296
Model of Saltatory Conduction in Myelinated Axons
12.3.1 Possible Link with the Topological Model of a Neuron Web The topological characteristics of entangled filament webs, such as neuron webs, may be described in terms of homotopy, reflecting the complexity of the trajectories of manyparticle systems [204]. The first homotopy group of the space D, labelled π1 (D), is the collection of topologically nonequivalent classes of closed trajectories (i.e., they are nonhomotopic; one class cannot be continuously deformed into another) in the space D. If this space is the configuration space of a system of N particles, each of which has its own trajectory on a manifold M, then the first homotopy group π1 is called a braid group [204, 201]. The configuration space for N identical particles located on a manifold M (e.g., R n ) is defined as follows: FN (M) = M N \ , for distinguishable identical particles, where M N is an N fold normal product of the manifold M and is a set of diagonal points such that the coordinates of two or more particles coincide, which has to be subtracted in order to conserve the number of particles in the system (particles cannot hide behind one another). The braid groups represent the topologically different available trajectories of a system of N particles (without reference to any specific dynamics). Thus, the pure braid group which we will utilize to describe a neuron web is defined as π1 (FN (M)) = π1 (M N \ ).
(12.8)
When trajectories (representing the neuron filaments) are mutually entangled in multiline braid form, the initial ordering of the particles must be unchanged. The elementary generators of the pure braid group are assigned as lij (Fig. 12.9) [200]; they correspond to the simplest entanglement of two trajectories of a particle pair, the ith and j th, while the rest of the particle trajectories remain untangled. The generators lij can be expressed by σi (an exchange of neighbouring particles, say the ith and (i + 1)th, that does not conserve their positions [200]): −1 −1 · · · σj−1 lij = σj −1 σj −2 · · · σi+1 σi2 σi+1 −2 σj −1,
1 ≥ i ≥ j ≥ N − 1.
(12.9)
The pure braid group can be considered as an abstract mathematical group generated by lij defined by the following relations [200, 202] (see Fig. 12.10): ⎧ ⎪ i < r < s < j, lij , ⎪ ⎪ ⎪ ⎪ r < s < i < j, ⎨ lij , −1 −1 , r < i = s < j, lrj lij lrj lrs (12.10) lij lrs = ⎪ −1 −1 ⎪ ⎪ i = r < s < j, ⎪ lrj lsj lij lsj lrj , ⎪ ⎩ l l l −1 l −1 l l l l −1 l −1, r < i < s < j . rj sj rj sj ij sj rj sj rj We propose to identify a fragment of the neuron web, connected via active synapses predefined by a prior record of certain information in the filament web, as a certain pattern from the pure braid group. In particular, one can use binary
12.3 (a)
The Roles of Grey and White Matter in Information Processing
i
297
j (b)
(c)
(d)
i i+1
i i+1
i i+1
i i+1
l ij
Figure 12.9 (a) Generator lij of the pure braid group; (b) the exchange of neighbouring particles, σi ; (c) its inverse, σi−1 ; (d) and the reason why braids on a plane are complicated. (a)
(c)
(d)
When ion current is pushed in opposite directions through two tangled threads, a loop of an electrical coil is created (b)
(e)
When ion current is pushed in same directions through two tangled threads, the loop is not active
Figure 12.10 (a) Generator lij and (b) its inverse lij−1 of the pure braid group; (c) an example of the N = 11 pure braid; (d) the creation of an electromagnetic active loop of coil by entanglement of threads in a pure braid; (e) the creation of a nonactive loop.
code to record any message in a threefilament bundle (two of the generators of the corresponding N = 3 pure braid group serve to code the 0 and 1 bits, and the third generator encodes the end of a word). It is possible to code an N letter alphabet message in an N thorder pure braid group [203]. It has been demonstrated that the ratio of the information efficiency of an Nthorder pure braid group to the resources needed to organize a physical web (such as a neuron web with N entangled filaments) attains a maximum at N = 20−30, which agrees with the number of phonics in the majority of phonic languages [202]. This result may suggest that ordinary words in a language are coded in a relatively small number of filaments in entangled bunches.
298
Model of Saltatory Conduction in Myelinated Axons
In the braid scenario it was proposed that information is coded in the brain in entanglement patterns in pieces of the neuron web selected by the activation of certain synapses. This coding is a topologically nonlocal type of coding and is more efficient than the conventional addressing of synapse registers (N synapse addressing offers only N! various connections with another N synapse register, whereas the number of distinct braids of threads linking these registers is infinite, limited only by the physical constraints of finite size, diameter, and length of the threads). To identify neuron braids we propose electromagnetic resonance utilizing the ion currents that flow in the neuron filaments of the grey matter. A different role is played by the white matter, with axon cords corrugated by the periodic myelin sheaths. The effective and fast saltatory transduction of action potentials through the long myelinated axons of the peripheral nerves and in the white matter of the central nervous system undeniably lies behind the motorics and other communication functions of the body. This saltatory transduction requires at least 100 times faster signalling than that offered by diffusiontype ion flows, according to the cable theory. This highspeed signalling is observed in myelinated axons and is described as saltatory conduction of the action potential [192]. As mentioned above in myelinated axons, the action potential spikes occur at the Ranvier nodes, small unmyelinated breaks periodically distributed along a myelinated axon [50]. The spikes are renewed on the subsequent series of these nodes according to the wellknown Hodgkin–Huxley membrane model [50]. However, the signal rapidly hops in between the Ranvier nodes, along the myelinated sectors of an axon; this strongly accelerates the transduction of the action signal along the periodically myelinated axon. The velocity of this saltatory conduction is at least two orders faster than the diffusion ion current. Such an acceleration in transduction is certainly required for longdistance signalling in the peripheral nervous system but is also required for quick communication in the white matter of the brain and spinal cord. In the brain, the white matter is located in inner structures beneath the cortex, but in the spinal cord the reverse is the case. This difference might be connected to the different roles of the grey matter in the cerebral cortex and in the spinal cord. The cortex is the place where memory is stored and where new messages from the surroundings accessed via the senses are identified or compared with the memory, whereas the grey matter in the spinal cord serves to identify the internal body information necessary to control body functions. The latter must be precise and errorless; thus, the grey matter in the spinal cord should be isolated from the surroundings in the best possible way, here by an outer white matter layer. It has been demonstrated that an external electromagnetic field, especially the magnetic field component, can influence and transcranially perturb the identification process in the brain cortex; this would be, however, very dangerous in the spinal cord, thus in the latter the grey structure must be better isolated than the cortex in the brain.
12.3
The Roles of Grey and White Matter in Information Processing
299
The white matter participates in communication but is not used in the recognition of braids with stored information, which is the role of the grey matter. Signal transduction in myelinated axons is not achieved by any electrical current and thus cannot participate in the electromagnetic identification of braids. This scenario is consistent with the plasmon–polariton wavetype character of saltatory conduction in myelinated axons presented above. Saltatory conduction is apparently of a wave type because conduction is maintained even if a myelinated axon is divided into two disjoint pieces with the ends separated slightly by an insulating barrier that would be impossible for a diffusive ion current to cross. We have discussed a model for saltatory conduction based on the kinetic properties of collective plasmon–polariton modes propagating along linear and periodically myelinated electrolyte systems, which, for axons, is the thin cord of the nerve cell periodically wrapped by Schwann cells creating thick myelin sheaths (Schwann cells myelinate axons in the peripheral nervous system, whereas in the central nervous system the white matter is built from axons myelinated by oligodendrocyte cells). Plasmon–polaritons were previously investigated and understood based on the welldeveloped nanoplasmonics of metal chains [1, 5]. The longrange lowdamped propagation of plasmon–polaritons has been demonstrated along a metallic nanochain [40]. Let us recall the main properties of these collective excitations occurring in metallic nanochains on a conductor–insulator interface [116, 4] by the hybridization of surface plasmons (i.e., fluctuations of the charge density of the electron fluid on the metal surface) with the electromagnetic wave. 1. The much lower velocity of plasmon–polaritons in comparison to the velocity of light gives a much shorter plasmon–polariton wavelength than the wavelength of light for a given frequency; this causes a strong discrepancy in the momenta of plasmon–polaritons and photons with the same energy. Thus, plasmon– polaritons do not interact with electromagnetic waves, i.e., photons cannot be excited or absorbed by plasmon–polaritons. 2. There are no radiative losses of plasmon–polaritons; plasmon–polariton attenuation is due only to ohmic losses, which makes metallic nanochains almost perfect wave guides for plasmon–polaritons, 3. The longrange and practically undamped propagation of plasmon–polaritons is observed experimentally [40, 39]. Certain unique properties of plasmon–polaritons in metallic nanochains are of special interest, as these properties can be repeated in periodic linear alignments of electrolyte systems with ions instead of electrons as the charged carriers. Owing to the larger mass of ions compared with that of electrons and the lower concentration of ions in electrolytes compared with that of electrons in metals, plasmon resonances in finite ionic systems (e.g., in liquid electrolytes confined
300
Model of Saltatory Conduction in Myelinated Axons
to a finite volume by appropriately formed membranes, which are frequently found in biological cell organization) occur on the scale of micrometres rather than nanometres and at frequencies or energies several orders of magnitude lower (depending on the ion concentration). For spherical electrolyte microsystems, the surface and volume plasmons are handled analogously to those in metallic nanospheres, as demonstrated in the previous chapter. The ionic surface plasmon frequencies are given for the lth multipole √ mode by the formula ωl = ωp l/(ε(2l + 1)), where the bulk plasmon frequency ωp = 4πq 2 n/m (n is the ion concentration, q and m are the ion charge and mass, respectively, and ε is the relative dielectric permittivity of the surroundings). For dipoletype surface plasmons (for√which l = 1), the frequency is given by a Mietype formula, [18, 23] ω1 = ωp / 3ε. In a linear chain of ionic systems, the radiation losses are reduced to zero in exactly the same manner as in metallic nanochains [193, 43, 44]. The high radiation energy losses expressed by the Lorentz friction at each chain element [55, 76] are ideally compensated by the radiation from the rest of the chain. Since the radiative losses are ideally balanced by mutual radiation exchange, only the relatively low irreversible ohmic energy dissipation remains. The collective plasmon–polaritons can thus propagate in the ionic chain with strongly reduced damping as in an almost perfect wave guide. If energy is slightly supplemented to compensate the ohmic losses, the propagation can reach arbitrarily long distances without any damping, which is observed in saltatory conduction in myelinated axons; moreover, the plasmon–polaritons in these axons can be neither detected nor perturbed by an external electromagnetic field. The advantages of plasmon–polariton kinetics that benefit the myelinated neuron signalling properties observed are listed as follows. • Plasmon–polaritons cannot be perturbed nor detected by electromagnetic waves (EEG signals are related to grey matter activity with ordinary conduction, according to the cable theory, which produces weak electromagnetic fields, whereas myelinated white matter does not generate EEG signals). • Immunity to electromagnetic perturbation is convenient in the long links of myelinated neurons in the peripheral nervous system (motorics and sensing cannot be disturbed by an external electromagnetic field). • The electromagnetic field of plasmon–polaritons is compressed along the tight tunnel around the axon cord. • The myelin sheath must be sufficiently thick, not for insulation but for the creation of a dielectric tunnel in the surrounding intercellular electrolyte that allows for plasmon–polariton formation (reducing the myelin sheath thickness perturbs the formation of plasmon–polaritons and lowers the plasmon–polariton group velocity, resulting e.g., in multiple sclerosis).
12.3
The Roles of Grey and White Matter in Information Processing
301
• Increasing temperature causes increasing ohmic losses but does not reduce the plasmon–polariton group velocity (however, more energy ADP/ATP, residual to the action potential spike formation, is needed to compensate the increased ohmic losses at higher temperatures). • No radiative losses occur for plasmon–polaritons; if plasmon–polaritons are residually aided by spike formation (renovation) at consecutive Ranvier nodes, an arbitrary longrange plasmon–polariton kinetics is possible with constant dipolesignal amplitude. • The plasmon–polariton group velocity increases with the cross section of the axon cord. • The plasmon–polariton group velocity for real neuron electrolytes and size parameters fits the observed velocity of saltatory conduction. • Wavetype plasmon–polariton kinetics explains the maintenance of signal transduction despite small breaks and gaps in the neuron cord or damage of some Ranvier nodes (these observations cannot be explained within the cable theory or by the compressionsoliton model). • Onedirection kinetics occurs if propagation starts from one end of an axon, but twodirection kinetics occurs if a plasmon–polariton is ignited from a certain central point of a passive axon. Taking into account the properties listed above of plasmon–polariton conduction, one might thus propose a nonlocal topological braidgrouptype approach to information processing in the brain, considering the specific and different electricity of the grey and white matter of neurons. The web of neuron filaments in grey matter would serve to encode the information in the entanglement of filaments selected by the activation of certain synapses, because the electricity of dendrites and of nonmyelinated axons (in the grey matter) is of an electrical current type, providing an electromagnetic signature when an AC signal is transduced through the neuron network. The method of electromagnetic resonance identification of the information stored in braided segments of the neuron web can be thus suggested. This method favours the grey matter with ordinary ion currents of the diffusive type (as in the cable model) but excludes the myelinated white matter, which has wavetype plasmon–polariton signalling without any electromagnetic signature. The saltatory conduction in myelinated axons in the white matter is not active with respect to electromagnetic resonance, as is typical for plasmon–polaritons. A model of ionic plasmon–polariton propagation to explain saltatory conduction in myelinated axons has thus been proposed. This wavetype propagation of the action potential is actually passive with respect to the electromagnetic response and cannot contribute to the braid information processing in the grey matter, though it conveniently fulfils a communication role in the peripheral and central nervous systems. The plasmon–polariton model explains the efficient, very fast, and
302
Model of Saltatory Conduction in Myelinated Axons
longrange saltatory conduction in myelinated axons in the peripheral neural system and in the white matter of the brain and spinal cord, where the velocity and energyefficiency of communication are of the most significance. The coincidence with observations supports the appropriateness of this new model proposed for saltatory conduction of the action potential, which, on the other hand, fits in a complementary way the different role and functioning of the grey matter. Both myelinated and nonmyelinated structures share between them different but complementary roles in the whole nervous system.
References
[1] W. L. Barnes, A. Dereux, and T. W. Ebbesen, ‘Surface plasmon subwavelength optics’, Nature 424, 824, 2003. [2] H. A. Atwater and A. Polman, ‘Plasmonics for improved photovoltaic devices’, Nat. Materi. 9, 205, 2010. [3] S. A. Maier, Plasmonics: Fundamentals and Applications, Springer, Berlin, 2007. [4] F. J. G. de Abajo, ‘Optical excitations in electron microscopy’, Rev. Mod. Phys. 82, 209, 2010. [5] J. M. Pitarke, V. M. Silkin, E. V. Chulkov, and P. M. Echenique, ‘Theory of surface plasmons and surfaceplasmon polaritons’, Rep. Prog. Phys. 70, 1, 2007. [6] P. Berini, ‘Longrange surface plasmon polaritons’, Adv. Opt. Photonics 1, 484, 2009. [7] L. Jacak, A. Wojs, and P. Hawrylak, Quantum Dots, Springer, Berlin, 1998. [8] W. Jacak, J. Krasnyj, L. Jacak, and R. Gonczarek, Decoherence of Orbital and Spin Degrees of Freedom in QDs, WUT University Press, Wrocław, 2009. [9] A. A. Abrikosov, L. P. Gorkov, and I. E. Dzialoshinskii, Methods of Quantum Field Theory in Statistical Physics, Dover Publications, New York, 1975. [10] E. M. Lifshitz and L. P. Pitaevskii, Statisticeskaja fizika, czast 2, Nauka, Mascow, 1978. [11] A. L. Fetter and J. D. Walecka, Quantum Theory of MultiParticle Systems, PWN, Warsaw, 1988. [12] A. A. Abrikosov, Wvedenie w Teoriu Normalnych Metalov, Nauka, Moscow, 1972. [13] D. Pines and P. Nozi`eres, The Theory of Quantum Liquids, W. A. Benjamin, New York, 1966. [14] D. Pines and D. Bohm, ‘A collective description of electron interactions: II. Collective vs. individual particle aspects of the interactions’, Phys. Rev. 85, 338, 1952. [15] D. Pines and D. Bohm, ‘A collective description of electron interactions: III. Coulomb interactions in a degenerate electron gas’, Phys. Rev. 92, 609, 1953. [16] D. Pines, Elementary Excitations in Solids, ABP Perseus Books, Massachusetts, 1999. [17] C. F. Bohren and D. R. Huffman, Absorption and Scattering of Light by Small Particles, Wiley, New York, 1983. [18] G. Mie, ‘Beitr¨age zur Optik tr¨uber medien, speziell kolloidaler Metall¨osungen’, Ann. Phys. 330(3), 377–445, 1908. [19] M. Brack, ‘The physics of simple metal clusters: selfconsistent jellium model and semiclassical approaches’, Rev. Mod. Phys. 65, 667, 1993. 303
304
References
[20] W. Ekardt, ‘Sizedependent photoabsorption and photoemission of small metal particles’, Phys. Rev. B 31, 6360, 1985. [21] V. V. Kresin, ‘Collective resonances and response properties of electrons in metal clusters’, Phys. Rep. 220, 1, 1992. [22] S. Link and M. A. ElSayed, ‘Size and temperature dependence of the plasmon absorption of colloidal gold nanoparticles’, J. Phys. Chem. B 103, 4212, 1999. [23] J. Jacak, J. Krasnyj, W. Jacak, R. Gonczarek, A. Chepok, and L. Jacak, ‘Surface and volume plasmons in metallic nanospheres in semiclassical RPAtype approach; nearfield coupling of surface plasmons with semiconductor substrate’, Phys. Rev. B 82, 035418, 2010. [24] M. L. Brongersma, J. W. Hartman, and H. A. Atwater, ‘Electromagnetic energy transfer and switching in nanoparticle chain arrays below the diffraction limit’, Phys. Rev. B 62, R16356, 2000. [25] M. Vollmer and U. Kreibig, ‘Optical properties of metal clusters’, Springer Ser. Mat. Sci. 25, 1995. [26] W. A. Jacak, ‘Lorentz friction for surface plasmons in metallic nanospheres’, J. Phys. Chem. C 119(12), 6749–6759, 2015. [27] W. A. Jacak, ‘Sizedependence of the Lorentz friction for surface plasmons in metallic nanospheres’, Opt. Express 23, 4472–4481, 2015. [28] K. Kluczyk and W. Jacak, ‘Dampinginduced size effect in surface plasmon resonance in metallic nanoparticles: comparison of RPA microscopic model with numerical finite element simulation (COMSOL) and Mie approach’, J. Quant. Spectrosc. Radiat. Transfer 78, 168, 2016. [29] K. Kolwas, A. Derkachova, and M. Shopa, ‘Size characteristics of surface plasmons and their manifestation in scattering properties of metal particles’, J. Quant. Spectrosc. Radiat. Transfer 110(14), 1490–1501, 2009. [30] W. Jacak, E. Popko, A. Henrykowski, E. Zielony, G. Luka, R. Pietruszka et al., ‘On the size dependence and the spatial range for the plasmon effect in photovoltaic efficiency enhancement’, Sol. Energy Mater. Sol. Cells 147, 1, 2016. [31] M. Jeng, Z. Chen, Y. Xiao, L. Chang, J. Ao, Y. Sun et al., ‘Improving efficiency of multicrystalline silicon and CIGS solar cells by incorporating metal nanoparticles’, Materials 8(10), 6761–6771, 2015. [32] S. Pillai, K. R. Catchpole, T. Trupke, G. Zhang, J. Zhao, and M. A. Green, ‘Enhanced emission from Sibased lightemitting diodes using surface plasmons’, Appl. Phys. Lett. 88, 161102, 2006. [33] D. M. Schaadt, B. Feng, and E. T. Yu, ‘Enhanced semiconductor optical absorption via surface plasmon excitation in metal nanoparticles’, Appl. Phys. Lett. 86, 063106, 2005. [34] M. Westphalen, U. Kreibig, J. Rostalski, H. L¨uth, and D. Meissner, ‘Metal cluster enhanced organic solar cells’, Sol. Energy Mater. Sol. Cells 61, 97, 2000. [35] A. J. Morfa, K. L. Rowlen, T. H. Reilly, M. J. Romero, and J. Lagemaat, ‘Plasmonenhanced solar energy conversion in organic bulk heterojunction photovoltaics’, Appl. Phys. Lett. 92, 013504, 2008. [36] M. A. Green and S. Pillai, ‘Harnessing plasmonics for solar cells’, Nat. Photon 6, 130–132, 2012. [37] G. Goubau, ‘Surface waves and their application to transmission lines’, J. Appl. Phys. 21, 119, 1950. [38] P. A. Huidobro, M. L. Nesterov, L. MartinMoreno, and F. J. GarciaVidal, ‘Transformation optics for plasmonics’, Nano Lett. 10, 1985, 2010.
References
305
[39] S. A. Maier, P. G. Kik, and H. A. Atwater, ‘Optical pulse propagation in metal nanoparticle chain waveguides’, Phys. Rev. B 67, 205402, 2003. [40] S. A. Maier and H. A. Atwater, ‘Plasmonics: localization and guiding of electromagnetic energy in metal/dielectric structures’, J. Appl. Phys. 98, 011101, 2005. [41] D. S. Citrin, ‘Plasmon polaritons in finitelength metalnanoparticle chains: the role of chain length unravelled’, Nano Lett. 5, 985, 2005. [42] D. Citrin, ‘Coherent excitation transport in metalnanoparticle chains’, Nano. Lett. 4, 1561, 2004. [43] V. A. Markel and A. K. Sarychev, ‘Propagation of surface plasmons in ordered and disordered chains of metal nanospheres’, Phys. Rev. B 75, 085426, 2007. [44] W. Jacak, ‘On plasmon polariton propagation along metallic nanochain’, Plasmonics 8, 1317, 2013. DOI: 10.1007/s1146801395288. [45] W. Jacak, ‘Exact solution for velocity of plasmon–polariton in metallic nanochain’, Optics Express 22, 18958, 2014. [46] W. Jacak, J. Krasnyj, and A. Chepok, ‘Plasmon–polariton properties in metallic nanosphere chains’, Materials 8, 3910, 2015. [47] W. Jacak, ‘On plasmon polariton propagation along metallic nanochain’, Plasmonics 8, 1317, 2013. [48] W. Jacak, ‘Plasmons in finite spherical electrolyte systems: RPA effective jellium model for ionic plasma excitations’, Plasmonics, 11, 637–651, 2016. Epub 2015, DOI: 10.1007/s1146801500646. [49] W. Jacak, ‘Propagation of collective surface plasmons in linear periodic ionic structures: plasmon polariton mechanism of saltatory conduction in axons’, J. Phys. Chem. C 119(18), 10015, 2015. [50] D. Debanne, E. Campanac, A. Bia?owa¸s, E. Carlier, and G. Alcaraz, ‘Axon physiology’, Physiol. Rev. 91, 555, 2011. [51] S. Brzychczy and R. Poznaski, Mathematical Neuroscience, Academic Press, San Diego, 2011. [52] W. Thomson, ‘On the theory of the electric telegraph’, Proc. R. Soc. London 7, 382, 1854. [53] T. Heimburg and A. D. Jackson, ‘On soliton propagation in biomembranes and nerves’, Proc. Natl Acad. Sci. USA 102, 9790, 2005. [54] N. W. Ashcroft and N. D. Mermin, Solid State Theory, Holt, Rinehart, and Winston, New York, 1976. [55] L. D. Landau and E. M. Lifshitz, Field Theory, Nauka, Moscow, 1973. [56] L. D. Landau, Zh. Eksp. Teor. Fiz. 30, 1058, 1956. [57] W. P. Silin, Zh. Eksp. Teor. Fiz. 33, 495, 1957. [58] P. Nozi`eres, Theory of Interacting Fermi Systems, W. A. Benjamin, New York, 1964. [59] P. S. Kiriejew, Physics of Semiconductors, PWN, Warsaw, 1969. [60] L. D. Landau, Zh. Eksp. Teor. Fiz. 32, 59, 1957. [61] L. D. Landau, Zh. Eksp. Teor. Fiz. 84, 262, 1958. [62] I. Y. Pomeranchuck, Zh. Eksp. Teor. Fiz. 35, 524, 1958. [63] P. Nozi`eres and J. M. Luttinger, Phys. Rev. 127, 1423, 1962. [64] P. Nozi`eres and J. M. Luttinger, Phys. Rev. 127, 1431, 1962. [65] L. Jacak, Nonlinear Topics in the Theory of Fermi Liquids, vol. 11 of Monografie, Oficyna Wydawnicza PWr, Wrocław, 1987. [66] G. N. Eliashberg, Zh. Eksp. Teor. Fiz. 42, 1658, 1962. [67] A. I. Larkin and A. N. Migdal, Zh. Eksp. Teor. Fiz. 44, 1703, 1963. [68] J. Czerwonko, Acta Phys. Polon. 37, 335, 1967. [69] J. Czerwonko, Zh. Eksp. Teor. Fiz. 71, 1099, 1976.
306
References
[70] N. F. Mott and H. Jones, The Theory of Metals and Alloys, Oxford University Press, New York, 1936. [71] M. Brack, ‘Multipole vibration of small alkalimetal spheres in a semiclassical description’, Phys. Rev. B 39, 3533, 1989. [72] I. S. Gradshteyn and I. M. Ryzhik, Table of Integrals, Series and Products, Academic Press, Boston MA, 1994. [73] J. Wu, S. C. Mangham, V. Reddy, M. Manasreh, and B. Weaver, ‘Surface plasmon enhanced intermediate band based quantum dots solar cell’, Sol. Energy Mater. Sol. Cells 102, 44–49, 2012. [74] N. Kalfagiannis, P. Karagiannidis, C. Pitsalidis, N. Panagiotopoulos, C. Gravalidis, S. Kassavetis et al., ‘Plasmonic silver nanoparticles for improved organic solar cells’, Sol. Energy Mater. Sol. Cells 104, 165–174, 2012. [75] L. D. Landau and L. M. Lifshitz, Quantum Mechanics. Nonrelativistic Theory, Pergamon Press, New York, 1965. [76] J. D. Jackson, Classical Electrodynamics, John Wiley and Sons, New York, 1998. [77] W. Jacak, J. Krasnyj, J. Jacak, R. Gonczarek, A. Chepok, L. Jacak et al., ‘Radius dependent shift of surface plasmon frequency in large metallic nanospheres: theory and experiment’, J. Appl. Phys. 107, 124317, 2010. [78] P. J. Compaijen, V. A. Malyshev, and J. Knoester, ‘Surfacemediated light transmission in metal nanoparticle chains’, Phys. Rev. B 87, 205437, 2013. [79] W. Ekardt, ‘Anomalous inelastic electron scattering from small metal particles’, Phys. Rev. B 33, 8803, 1986. [80] C. Yannouleas, R. A. Broglia, M. Brack, and P. F. Bortignon, ‘Fragmentation of the photoabsorption strength in neutral and charged metal microclusters’, Phys. Rev. Lett. 63, 255, 1989. [81] A. Rubio and L. Serra, ‘Dielectric screening effects on the photoabsorption cross section of embedded metallic clusters’, Phys. Rev. B 48, 18222, 1993. [82] C. S¨onnichsen, T. Franzl, T. Wilk, G. von Plessen, and J. Feldmann, ‘Plasmon resonances in large noblemetal clusters’, New J. Phys. 4, 93, 2002. [83] S. Link and M. A. ElSayed, ‘Shape and size dependence of radiative, nonradiative and photothermal properties of gold nanocrystals’, Int. Rev. Phys. Chem. 19, 409, 2000. [84] K. Kolwas and A. Derkachova, ‘Damping rates of surface plasmons for particles of size from nano to micrometers; reduction of the nonradiative decay’, J. Quant. Spectrosc. Radiat. Transfer 114, 45, 2013. [85] J. Mock, M. Barbic, D. Smith, D. Schultz, and S. Schultz, ‘Shape effects in plasmon resonance of individual colloidal silver nanoparticles’, J. Chem. Phys. 116(15), 6755–6759, 2002. [86] C. Noguez, ‘Surface plasmons on metal nanoparticles: the influence of shape and physical environment’, J. Phys. Chem. C 111(10), 3806–3819, 2007. [87] S. Dickreuter, J. Gleixner, A. Kolloch, J. Boneberg, E. Scheer, and P. Leiderer, ‘Mapping of plasmonic resonances in nanotriangles’, Beilstein J. Nanotechnol. 4(1), 588–602, 2013. [88] V. E. Ferry, J. N. Munday, and H. A. Atwater, ‘Design considerations for plasmonic photovoltaics’, Advanced Mat. 22(43), 4794–4808, 2010. [89] J. A. Schuller, E. S. Barnard, W. Cai, Y. C. Jun, J. S. White, and M. L. Brongersma, ‘Plasmonics for extreme light concentration and manipulation’, Nature Mat. 9(3), 193–204, 2010. ¨ [90] R. Gans, ‘Uber die Form ultramikroskopischer Goldteilchen’, Ann. Phys. 342(5), 881–900, 1912.
References
307
[91] A. Taflove and S. C. Hagness, ‘Computational electrodynamics’, Artech House, 2000. [92] J. M. Montgomery, T.W. Lee, and S. K. Gray, ‘Theory and modeling of light interactions with metallic nanostructures’, J. Phys.: Condensed Matter 20(32), 323201, 2008. [93] F. G. de Abajo and A. Howie, ‘Retarded field calculation of electron energy loss in inhomogeneous dielectrics’, Phys. Rev. B 65(11), 115418, 2002. [94] C. G. Khoury, S. J. Norton, and T. VoDinh, ‘Investigating the plasmonics of a dipoleexcited silver nanoshell: Mie theory versus finite element method’, Nanotechnology 21(31), 315203, 2010. [95] V. Myroshnychenko, J. Rodr´ıguezFern´andez, I. PastorizaSantos, A. M. Funston, C. Novo, P. Mulvaney et al., ‘Modelling the optical response of gold nanoparticles’, Chem. Soc. Rev. 37(9), 1792–1805, 2008. [96] P. K. Jain, K. S. Lee, I. H. ElSayed, and M. A. ElSayed, ‘Calculated absorption and scattering properties of gold nanoparticles of different size, shape, and composition: applications in biological imaging and biomedicine’, J. Phys. Chem. B 110(14), 7238–7248, 2006. [97] J. Jin, The Finite Element Method in Electromagnetics, John Wiley & Sons, New York, 2014. [98] C. G. Khoury, S. J. Norton, and T. VoDinh, ‘Plasmonics of 3D nanoshell dimers using multipole expansion and finite element method’, ACS Nano. 3(9), 2776–2788, 2009. [99] X. Cui and D. Erni, ‘Enhanced propagation in a plasmonic chain waveguide with nanoshell structures based on low and highorder mode coupling’, JOSA A 25(7), 1783–1789, 2008. [100] P. B. Johnson and R.W. Christy, ‘Optical constants of the noble metals’, Phy. Rev. B 6(12), 4370, 1972. [101] W. Haiss, N. T. Thanh, J. Aveyard, and D. G. Fernig, ‘Determination of size and concentration of gold nanoparticles from uvvis spectra’, Anal. Chem. 79(11), 4215–4221, 2007. [102] P. N. Njoki, I.I. S. Lim, D. Mott, H.Y. Park, B. Khan, S. Mishra et al., ‘Size correlation of optical and spectroscopic properties for gold nanoparticles’, J. Phys. Chem. C 111(40), 14664–14669, 2007. [103] A. L. Koh, K. Bao, I. Khan, W. E. Smith, G. Kothleitner, P. Nordlander et al., ‘Electron energyloss spectroscopy (EELS) of surface plasmons in single silver nanoparticles and dimers: influence of beam damage and mapping of dark modes’, ACS Nano. 3(10), 3015–3022, 2009. [104] K. Okamoto, I. Niki, A. Scherer, Y. Narukawa, and Y. Kawakami, ‘Surface plasmon enhanced spontaneous emission rate of InGaN/ GaN quantum wells probed by timeresolved photoluminescence spectroscopy’, Appl. Phys. Lett. 87, 071102, 2005. [105] S. P. Sundararajan, N. K. Grandy, N. Mirin, and N. J. Halas, ‘Nanoparticleinduced enhancement and suppression of photocurrent in a silicon photodiode’, Nano. Lett. 8, 624, 2008. [106] L. Hong, X. Rusli, H. Wang, L. Zheng, X. He, H. Xu et al., ‘Design principles for plasmonic thin film GaAs solar cells with high absorption enhancement’, J. Appl. Phys. 112, 054326, 2012. [107] D. Derkacs, S. H. Lim, P. Matheu, W. Mar, and E. T. Yu, ‘Improved performance of amorphous silicon solar cells via scattering from surface plasmon polaritons in nearby metallic nanoparticles’, Appl. Phys. Lett. 89, 093103, 2006.
308
References
[108] S. Kim, S. Na, J. Jo, D. Kim, and Y. Nah, ‘Plasmon enhanced performance of organic solar cells using electrodeposited Ag nanoparticles’, Appl. Phys. Lett. 93, 073307, 2008. [109] M. Kirkengen, J. Bergli, and Y. M. Galperin, ‘Direct generation of charge carriers in cSi solar cells due to embedded nanoparticles’, J. Appl. Phys. 102(9), 093713, 2007. [110] J. Lee and P. Peumans, ‘The origin of enhanced optical absorption in solar cells with metal nanoparticles embedded in the active layer’, Opt. Express 18, 10078, 2010. [111] M. Losurdo, M. M. Giangregorio, G. V. Bianco, A. Sacchetti, P. Capezzuto, and G. Bruno, ‘Enhanced absorption in Au nanoparticles/aSi:H/cSi heterojunction solar cells exploiting Au surface plasmon resonance’, Sol. Energy Mater. Sol. Cells 93, 1749, 2009. [112] K. R. Catchpole, S. Mokkapati, F. Beck, E. Wang, A. McKinley, A. Basch et al., ‘Plasmonics and nanophotonics for photovoltaics’, MRS Bulletin 36, 461–467, 2011. [113] N. Guillot and M. L. de la Chapelle, ‘The electromagnetic effect in surface enhanced Raman scattering: enhancement optimization using precisely controlled nanostructures’, J. Quant. Spectrosc. Radiat. Transfer 113(18), 2321, 2012. [114] E. L. Ru, E. Blackie, M. Meyer, and P. Etchegoin, ‘Surface enhanced Raman scattering enhancement factors: a comprehensive study’, J. Phys. Chem. C 111, 13794, 2007. [115] I. Smolyaninov, A. A. Zayats, and O. Keller, ‘The effect of the surface enhanced polariton field on the tunneling current of an STM’, Phys Lett. A 200, 438, 1995. [116] A. V. Zayats, I. I. Smolyaninov, and A. A. Maradudin, ‘Nanooptics of surface plasmon polaritons’, Phys. Rep. 408, 131, 2005. [117] H. R. Stuart and D. G. Hall, ‘Enhanced dipole–dipole interaction between elementary radiators near a surface’, Phys. Rev. Lett. 80, 5663, 1998. [118] K. Okamoto, I. Niki, A. Shvartser, Y. Narukawa, T. Mukai, and A. Scherer, ‘Surface plasmon enhanced spontaneous emission rate of InGaN/GaN QW probed by timeresolved photolumimnescence spectroscopy’, Nat. Mater. 3, 601, 2004. [119] C. Wen, K. Ishikawa, M. Kishima, and K. Yamada, ‘Effects of silver particles on the photovoltaic properties of dyesensitized TiO2 thin films’, Sol. Cells 61, 339, 2000. [120] F. Masia, W. Langbein, and P. Borri, ‘Measurement of the dynamics of plasmons inside individual gold nanoparticles using a femtosecond phaseresolved microscope’, Phys. Rev. B 85, 235403, 2012. [121] T. L. Temple and D. M. Bagnall, ‘Optical properties of gold and aluminium nanoparticles for silicon solar cell applications’, J. Appl. Phys. 109, 084343, 2011. [122] M. L. Trolle and T. G. Pedersen, ‘Indirect optical absorption in silicon via thinfilm surface plasmon’, J. Appl. Phys. 112, 043103, 2012. [123] W. Ekardt, ‘Dynamical polarizability of small metal particles: selfconsistent spherical jellium model’, Phys. Rev. Lett. 52, 1925, 1984. [124] W. Jacak, J. Krasnyj, J. Jacak, W. Donderowicz, and L. Jacak, ‘Mechanism of plasmon mediated enhancement of PV efficiency’, J. Phys. D: Appl. Phys. 44, 055301, 2011. [125] M. Kauranen and A. Zayats, ‘Nonlinear plasmonics’, Nat. Photonics 6, 737, 2012. [126] K. Tsia, S. Fathpour, and B. Jalali, ‘Energy harvesting in silicon wavelength converters’, Opt. Express 14, 12327, 2006. [127] I. Volovichev, ‘New nonlinear photovoltaic effect in uniform bipolar semiconductor’, J. Appl. Phys. 116, 193701, 2014.
References
309
[128] Y. Chen, D. M. Bagnall, H. Koh, K. Park, K. Hiraga, Z. Zhu et al., ‘Plasma assisted molecular beam epitaxy of ZnO on cplane sapphire: growth and characterization’, J. Appl. Phys. 84, 39128, 1998. [129] R. Yousefi, F. JamaliSheini, and A. K. Zak, ‘A comparative study of the properties of ZnO nano/microstructures grown using two types of thermal evaporation setup conditions’, Chem. Vapor Depos. 18, 215–220, 2012. [130] E. Guziewicz, I. A. Kowalik, M. Godlewski, K. Kopalko, V. Osinniy, A. W´ojcik et al., ‘Extremely low temperature growth of ZnO by atomic layer deposition’, J. Appl. Phys. 103, 033515, 2008. [131] L. Chen, ‘Photodiodes – from fundamentals to applications’, in: SiBased ZnO Ultraviolet Photodiodes, ISBN 9789535108955. [132] H. S. Bae and S. Im, ‘Ultraviolet detecting properties of ZnObased thin film transistors’, Thin Solid Films 75, 469, 2004. [133] M. Dutta and D. Basak, ‘pZnO/nSi heterojunction: solgel fabrication, photoresponse properties, and transport mechanism’, Appl. Phys. Lett. 92, 21212, 2008. [134] D. B. S. Mridha and M. Dutta, ‘Photoresponse of nZnO/pSi heterojunction towards ultraviolet/visible lights: thickness dependent behavior’, J. Mater. Sci. Mater. Electron. 20, 376, 2009. [135] A. Djuri˘si´c and Y. H. Leung, ‘Optical properties of ZnO nanostructures’, Small 2, 944, 2006. [136] K. Bhandari, J. Collier, R. Ellingson, and D. Apul, ‘Energy payback time (EPBT) and energy return on energy invested (EROI) of solar photovoltaic systems: a systematic review and metaanalysis’, Ren. Sust. Energy Rev. 47, 133, 2015. [137] H. R. Stuart and D. G. Hall, ‘Island size effect in nanoparticles photodetectors’, Appl. Phys. Lett. 73, 3815, 1998. [138] P. Matheu, S. Lim, D. Derkacs, C. McPheeters, and E. Yu, ‘Metal and dielectric nanoparticle scattering for improved optical absorption in photovoltaic devices’, Appl. Phys. Lett. 93(11), 113108, 2008. [139] S. Lim, W. Mar, P. Matheu, D. Derkacs, and E. Yu, ‘Photocurrent spectroscopy of optical absorption enhancement in silicon photodiodes via scattering from surface plasmon polaritons in gold nanoparticles’, J. Appl. Phys. 101(10), 104309, 2007. [140] L. Luo, C. Xie, X. Wang, Y. Yu, C. Wu, H. Hu et al., ‘Surface plasmon resonance enhanced highly efficient planar silicon solar cell’, Nano Energy 9, 112–120, 2014. [141] S. Pillai, K. Catchpole, T. Trupke, and M. Green, ‘Surface plasmon enhanced silicon solar cells’, J. Appl. Phys. 101(9), 093105, 2007. [142] T. Temple, G. Mahanama, H. Reehal, and D. Bagnall, ‘Influence of localized surface plasmon excitation in silver nanoparticles on the performance of silicon solar cells’, Solar Energy Mater. Solar Cells 93(11), 1978–1985, 2009. [143] C. Uhrenfeldt, T. Villesen, A. Tˆetu, B. Johansen, and A. Nylandsted Larsen, ‘Broadband photocurrent enhancement and lighttrapping in thin film Si solar cells with periodic Al nanoparticle arrays on the front’, Opt. Express 23(11), A525, 2015. [144] W. Ho, C. Hu, C. Yeh, and Y. Lee, ‘External quantum efficiency and photovoltaic performance of silicon cells deposited with aluminum, indium, and silver nanoparticles’, Japanese J. Appl. Phys. 55(8S3), 08RG03, 2016. [145] K. Kluczyk, C. David, J. Jacak, and W. Jacak, ‘On modeling of plasmoninduced enhancement of the efficiency of solar cells modified by metallic nanoparticles’, Nanomaterials 9, 3, 2019. DOI:10.3390/nano9010003. [146] D. Aspnes and A. Studna, ‘Dielectric functions and optical parameters of Si, Ge, GaP, GaAs, GaSb, InP, InAs, and InSb from 1.5 to 6.0 eV’, Phys. Rev. B 27(2), 985–1009, 1982.
310
References
[147] M. Ghidelli, L. Mascaretti, B. Bricchi, A. Zapelli, V. Russo, C. Casari et al., ‘Engineering plasmonic nanostructured surfaces by pulsed laser deposition’, Appl. Surface Sci. 434, 1064–1073, 2018. [148] B. Bricchi, M. Ghidelli, L. Mascaretti, A. Zapelli, V. Russo, C. Casari et al., ‘Integration of plasmonic Au nanoparticles in TiO2 hierarchical structures in a singlestep pulsed laser codeposition’, Mater. Design 156, 311–319, 2018. [149] J. Borges, T. Kubart, S. Kumar, K. Leifer, M. Rodrigues, N. Duarte et al., ‘Microstructural evolution of Au/TiO2 nanocomposite films: the influence of Au concentration and thermal annealing’, Thin Solid Films 580, 77–88, 2015. [150] P. Tonui, E. Arbab, and G. Mola, ‘Metal nanocomposite as charge transport cobuffer layer in perovskite based solar cell’, J. Phys. Chem. Solids 126, 124–130, 2019. [151] E. Arbab and G. Mola, ‘Metals decorated nanocomposite assisted charge transport in polymer solar cell’, Mater. Sci. Semiconductor Proc. 91, 1–8, 2019. [152] F. Bella, P. Renzi, C. Cavallo, and C. Gerbaldi, ‘Caesium for perovskite solar cells: an overview’, Chemistry – A European J. 24, 12183–12205, 2018. [153] J. Hao, H. Hao, J. Li, L. Shi, T. Zhong, C. Zhang et al., ‘Light trapping effect in perovskite solar cells by the addition of Ag nanoparticles, using textured substrates’, Nanomaterials 8(10), 815, 2019. [154] S. Galliano, F. Bella, G. Piana, G. Giacona, G. Viscardi, C. Gerbaldi et al., ‘Finely tuning electrolytes and photoanodes in aqueous solar cells by experimental design’, Sol. Energy 163, 251–255, 2018. [155] D. Pintossi, G. Iannaccone, A. Colombo, F. Bella, M. V¨alim¨aki, K. V¨ais¨anen et al., ‘Luminescent downshifting by photoninduced solar–gel hybrid coatings: accessing multifunctionality on flexible organic photovoltaics via ambient temperature material processing’, Adv. Electron. Mater. 2, 1600288, 2016. [156] P. Pearce, A. Mellor, and N. EkinsDaukes, ‘The importance of accurate determination of optical constants for the design of nanometallic lighttrapping structures’, Sol. Energy Mater. Sol. Cells 191, 133–140, 2019. [157] Y. Zhang, B. Cai, and B. Jia, ‘Ultraviolet plasmonic aluminium nanoparticles for highly efficient light incoupling on silicon solar cells’, Nanomaterials 6, 95, 2016, DOI:10.3390/nano6060095. [158] D. Song, H. Kim, J. Suh, B. Jun, and W. Rho, ‘Multishaped Ag nanoparticles in the plasmonic layer of dyesensitized solar cells for increased power conversion efficiency’, Nanomaterials 7(6), 136, 2017. [159] K. Kluczyk, C. David, and W. Jacak, ‘On quantum approach to modeling of plasmon photovoltaic effect’, J. Optical Soc. America B 34, 2115, 2017. [160] E. Runge and E. K. U. Gross, ‘Densityfunctional theory for timedependent systems’, Phys. Rev. Lett. 52, 997, 1984. [161] P. Hohenberg and W. Kohn, ‘Inhomogeneous electron gas’, Phys. Rev. Lett. 136, 864, 1964. [162] R. Esteban, A. Zugarramurdi, P. Zhang, P. Nordlander, F. J. G. Vidal, A. G. Borisov et al., ‘A classical treatment of optical tunneling in plasmonic gaps: extending the quantum corrected model to practical situations’, Faraday Discuss. 178, 151, 2015. [163] T. V. Teperik, P. Nordlander, J. Aizpurua, and A. G. Borisov, ‘Quantum effects and nonlocality in strongly coupled plasmonic nanowire dimers’, Opt. Express 21, 27306, 2013. [164] F. J. G. de Abajo, ‘Nonlocal effects in the plasmons of strongly interacting nanoparticles, dimers, and waveguides’, J. Phys. Chem. C 112, 17983, 2008. [165] K. Kluczyk, L. Jacak, C. David, and W. Jacak, ‘Microscopic electron dynamics in metal nanoparticles for photovoltaic systems’, Materials 11, 1077, 2018.
References
311
[166] S. A. Maier, P. G. Kik, H. A. Atwater, S. Meltzer, E. Harel, B. E. Koel et al., ‘Local detection of electromagnetic energy transport below the diffraction limit in metal nanoparticle plasmon waveguides’, Nat. Mater. 2, 229, 2003. [167] L. L. Zhao, K. L. Kelly, and G. C. Schatz, ‘The extinction spectra of silver nanoparticle arrays: influence of array structure on plasmon resonance wavelength and width’, J. Phys. Chem. B 107, 7343, 2003. [168] S. Zou, N. Janel, and G. C. Schatz, ‘Silver nanoparticle array structures that produce remarkably narrow plasmon lineshapes’, J. Chem. Phys. 120, 10871, 2004. [169] J. R. Krenn, A. Dereux, J. C. Weeber, E. Bourillot, Y. Lacroute, J. P. Goudonnet et al., ‘Squeezing the optical nearfield zone by plasmon coupling of metallic nanoparticles’, Phys. Rev. Lett. 82, 2590, 1999. [170] S. A. Maier, M. L. Brongersma, P. G. Kik, and H. A. Atwater, ‘Observation of nearfield coupling in metal nanoparticle chains using farfield polarization spectroscopy’, Phys. Rev. B 65, 193408, 2002. [171] S. A. Maier, P. G. Kik, L. A. Sweatlock, H. A. Atwater, J. J. Penninkhof, A. Polman et al., ‘Energy transport in metal nanoparticle plasmon waveguides’, Mat. Res. Soc. Symp. Proc. 777, T7.1.1, 2003. [172] H. Ditlbacher, A. Hohenau, D. Wagner, U. Kreibig, M. Rogers, F. Hofer et al., ‘Silver nanowires as surface plasmon resonators’, Phys. Rev. Lett. 95, 257403, 2005. [173] I. L. Rasskazov, S. V. Karpov, and V. A. Markel, ‘Nondecaying surface plasmon polaritons in linear chains of silver nanospheroids’, Opt. Lett. 38, 4743, 2013. [174] A. A. Govyadinov and V. A. Markel, ‘From slow to superluminal propagation: dispersive properties of surface plasmon polaritons in linear chains of metallic nanospheroids’, Phys. Rev. B 78, 035403, 2008. [175] Y. Hadad and B. Z. Steinberg, ‘Green’s function theory for infinite and semiinfinite particle chains’, Phys. Rev. B 84, 125402, 2011. [176] V. A. Markel and A. K. Sarychev, ‘Comment on Green’s function theory for infinite and semiinfinite particle chains’, Phys. Rev. B 86, 037401, 2012. [177] S. B. Singham and C. F. Bohren, ‘Light scattering by an arbitrary particle: a physical reformulation of the coupled dipole method’, Opt. Lett. 12, 10, 1987. [178] T. Jensen, L. Kelly, A. Lazarides, and G. C. Schatz, ‘Electrodynamics of noble metal nanoparticles and nanoparticle clusters’, J. Cluster Sci. 10, 295, 1999. [179] B. T. Draine, ‘The discretedipole approximation and its application to interstellar graphite grains’, Astrophys. J. 333, 848, 1988. [180] E. M. Purcell and C. R. Pennypacker, ‘Scattering and absorption of light by nanospherical dielectric grains’, Astrophys. J. 186, 705, 1973. [181] B. T. Draine and P. J. Flatau, ‘Discretedipole approximation for scattering calculations’, J. Opt. Soc. America A 11, 1491, 1994. [182] V. A. Markel, ‘Coupleddipole approach to scattering of light from a one dimensional periodic dipole structure’, J. Mod. Opt. 40, 2281, 1993. [183] P. Anger, P. Bharadwaj, and L. Novotny, ‘Enhancement and quenching of singlemolecule fluorescence’, Phys. Rev. Lett. 96, 113002, 2006. [184] I. S. Gradstein and I. M. Rizik, Tables of Integrals, Fizmatizdat, Moscow, 1962. [185] W. Jacak, J. Krasnyj, J. Jacak, A. Chepok, L. Jacak, W. Donderowicz et al., ‘Undamped energy transport by collective surface plasmon oscillations along metallic nanosphere chain’, J. Appl. Phys. 108, 084304, 2010. [186] M. Fevrier, P. Gogol, J.M. Lourtioz, and B. Dagens, ‘Metallic nanoparticle chains on dielectric waveguides: coupled and uncoupled situations compared’, Opt. Express 21, 24505, 2013. DOI:10.1364/OE.21.024504. [187] A. Apuzzo, M. Fevrier, R. SalasMontiel, A. Bruyant, A. Chelnokov, G. Lerondel et al., ‘Observation of nearfield dipolar interactions involved in a metal nanoparticle chain waveguide’, Nano Lett. 13, 1000, 2013. doi: 10.1021/nl304164y.
312
References
[188] C. Girard and R. Quidant, ‘Nearfield optical transmittance of metal particle chain waveguides’, Opt. Express 12, 6141, 2004. [189] V. A. Markel, ‘Divergence of dipole sums and the nature of nonLorentzian exponentially narrow resonances in onedimensional periodic arrays of nanospheres’, J. Phys. B: Atom., Mol. Opt. Phys. 38, L115, 2005. [190] N. N. Bogolubov and J. A.Mitropolkyj, Asymptotical Methods in the Theory of Nonlinear Oscillations, Nauka, Moscow, 2005. [191] I. A. Lazarevich and V. B. Kazantsev, ‘Dendritic signal transmission induced by intracellular charge inhomogeneities’, Phys. Rev. E. 88, 062718, 2013. [192] R. S. Lillie, ‘Factors affecting transmission and recovery in passive iron nerve model’, J. Gen. Physiol. 7, 473, 1925. [193] D. Citrin, ‘Plasmon–polariton transport in metalnanoparticle chains embedded in a gain medium’, Opt. Letters 31, 98, 2006. [194] V. M. Agranovich and O. A. Dubovskii, ‘Effect of retarded interaction on the exciton spectrum in onedimensional and twodimensional crystals’, JETP Lett. 3, 223, 1966. [195] T. Meissner and F. Wentz, ‘The complex dielectric constant of pure and sea water from microwave satellite observations’, IEEE THRS 42, 1836, 2004. [196] T. A. ElBrolossy, T. Abdallah, M. B. Mohamed, S. Abdallah, K. Easawi, S. Negm et al., ‘Shape and size dependence of the surface plasmon resonance of gold nanoparticles studied by photoacoustic technique’, Eur. Phys. J. Special Topics 153, 361, 2008. [197] L. M. LizMarzan, ‘Tuning nanorod surface plasmon resonances’, SPIE Newsroom (10.1117/2.1200707.0798), 2007. ¨ [198] A. Sommerfeld, ‘Uber die fortpflanzung elektrodynamischer Wellen langs eines Drahts’, Ann. Phys. Chem. 67, 233, 1899. [199] E. Andrianov, A. A. Pukhov, A. V. Dorofeenko, A. P. Vinogradov, and A. A. Lisyansky, ‘Stationary behavior of a chain of interacting spasers’, Phys. Rev. B 85, 165419, 2012. [200] J. S. Birman, Braids, Links and Mapping Class Groups, Princeton University Press, 1974. [201] D. Mermin, ‘The topological theory of defects in ordered media’, Rev. Mod. Phys. 51, 591, 1979. [202] J. Jacak, R. Gonczarek, L. Jacak, and I. J´oz´ wiak, Application of Braid Groups in 2D Hall System Physics, World Scientific, Singapore, 2012. [203] H. Stokowski and J. Jacak, ‘Multicharacter alphabet coding using braid group formalism’, Comput. Math. Appl., submitted. [204] E. Spanier, Algebraic Topology, Springer, Berlin, 1966.
Index
acoustic sound, 26 Avogadro number, 21, 39 Bethe–Salpeter equation, 29, 31, 32 binary electrolyte, 12, 253, 254, 261 Bloch theory, 17, 19, 111, 187, 239 Bohm, 2, 3, 35, 64, 100, 101, 256 Boltzmann constant, 20, 21, 281 Born–Karman conditions, 18, 239, 282 Bravais webs, 17–20 bulk metal, 3, 4, 35, 43, 49, 58, 65, 98, 155 cable model, 13, 286, 301 CIGS cells, 9, 133, 143, 145, 148, 162 collective excitations, 25, 32 commutator for Heisenberg equation, 37, 45 COMSOL, ix, 3, 85, 87, 90, 96, 151, 154, 157, 163, 172 Cooper pair, 30, 34 crystal lattice cell, 1, 2, 9, 12, 17 dephasing, 1 dielectric function, 3, 67, 79, 82, 86, 93, 154 Drude–Lorentz model, 3, 67, 86, 150, 166 effective mass, 26, 28, 32, 110 extinction cross section, 3, 82, 87, 96 Fermi energy, 2, 21, 33, 39, 98 Fermi liquid, 22, 25, 26, 30, 32 Fermi sea, 2, 21 Fermi surface, 2, 21, 23, 24, 26, 27, 29, 33, 98 Fermi velocity, 12, 13, 67, 104, 206 fourmomentum, 29, 31 Fourier transform, 36, 40, 43, 47, 49, 188, 190, 196, 209, 239 Fresnel–Maxwell electrodynamics equations, 3, 155
Goubau transmission lines, 9, 288 Green functions for metal, 2, 80 group velocity of plasmon–polariton, 10, 24, 179, 181, 197, 200, 204, 213, 220, 244 Hamiltonian for plasmons, 34, 35, 37, 43, 44, 46, 135, 255, 256 harmonic damped oscillator (plasmons), 6, 71, 83 Heisenberg equation, 4, 46 hyperbolic singularity (plasmon–polariton), 10, 201, 202, 219, 229 jellium, 4, 36, 38, 40, 42, 43, 45, 48, 99, 102, 222, 234, 254, 256 Joule heat, 10, 14, 61, 232, 234, 250, 278 kinetical energy, 4, 5, 12, 45 Kohn–Sham approach, 43, 48, 63, 98, 155 Landau damping, 24, 25, 30, 67 Landau interaction, 26, 29, 32 light cone, 10, 11, 201 linear response theory of Kubo, 32 logarithmic singularity, plasmon–polariton, 10, 11, 181, 200–202, 204 longitudinal polarization, 192, 202, 205, 208, 216, 226, 280 Lorentz friction, 6, 60–62, 70, 71, 75, 77, 81, 84, 95, 105, 151, 155, 192, 211, 223, 229, 237, 270, 300 Lorentz invariance, 11 Luttinger theorem, 21, 28 Matsubara Green functions, 27, 29 metallic clusters, 3, 4, 42, 43, 62, 69, 80, 178, 180, 253 metallic nanoparticles, 1, 62–64, 69, 71, 76, 79, 83, 85, 87, 95, 96, 99, 101, 109, 119, 137, 198, 235, 275 metamaterials, 3, 98 Mie energy, 4, 134 Mietype calculation, 6, 80, 85, 300
313
314
Index
momentum conservation, 39, 100, 131, 134, 151 multipole modes of plasmons, 4, 84, 91, 275, 276 myelinated axons, 13, 301 nanochains, 9–11, 61 nanosphere, 5, 62, 69, 77, 81, 101, 109, 187, 192 nearfield zone, 7, 8, 198, 211, 215, 229, 245, 251 neurons, 13, 276, 288, 295, 301 Newtontype procedure, 10, 202, 205, 250 ordinary photoeffect, 7, 8, 100, 112, 113, 118, 131, 137, 154 overdamped regime, 6, 73, 108, 114, 115, 143 peripheral nervous system, 13 perturbative solution, 10, 61, 71, 76, 84, 107, 185, 250 phonon, 1 photodiode, 8, 118, 123, 149 Pines, 2–4, 35, 256 plasmon–polariton, 9, 283, 285, 286, 288, 290, 292, 300, 301 plasmonoptoelectronics, 9, 10 plasmonic effect, 9, 119, 122, 163 plasmons, 2, 6, 34, 96, 109, 137, 229, 252, 260 Pomeranchuck instability, 25 pseudomomentum, 19
Schr¨odinger equation, 17 semimetal, 20 semiconductor quantum dots, 1 semiconductor substrate, 6, 97, 100, 110, 113, 120, 131, 140, 155, 173, 232 singlet spin state, 34 solar cell, 7, 9, 59, 97, 120, 133, 147, 154 spillout, 4, 62, 80, 94, 99, 178 spin waves, 27, 32 stellar kernels, 2 subdiffraction, 1, 12, 60 superfluid He3 , 34 superluminal propagation, 10, 179 surface plasmons, 4, 5, 8, 11, 53, 59, 66, 68, 71, 77, 79, 87, 95, 99, 106, 109, 115, 119, 124, 148, 153, 160, 187, 229, 237, 246, 264, 291 Thomas–Fermi 5/3 formula, 5, 12 Thomas–Fermi wave vector, 4, 40, 66, 99, 101 Thomson, 13, 276, 295 timedependent local density approximation (TDLDA) method, 48, 51, 63, 101, 180, 260 transverse polarization, 10, 91, 93, 181, 189, 194, 198, 200, 203, 205, 216, 240, 280 triplet superfluid, 34 ultraviolet radiation, 2, 34, 139
quasiparticles, 2, 5, 23 random phase approximation (RPA) approach to plasmons, 3, 5, 38, 51, 64, 66, 67, 82, 99, 181 Ranvier nodes, 15, 276, 286, 291, 293 retarded or advanced Green function, 27, 115 Ritchie frequency, 4 saltatory conduction, 4, 14, 276, 287, 298, 302 scattering, 3, 29, 39, 61, 69, 79, 83, 88, 151, 178, 224, 245, 278
vertical interband transitions, 8, 100, 118, 131, 133, 151, 158 vibrational and rotational excitations, 13, 259 volume plasmons, 41, 51, 52, 66, 68, 103, 234, 260, 262, 265, 275 wave function, 18, 64, 102, 111, 124, 256 zero sound, 25, 27, 32